Chemical Thermodynamics of Materials Macroscopic and Microscopic Aspects Svein StĂ¸len Department of Chemistry, University of Oslo, Norway
Tor Grande Department of Materials Technology, Norwegian University of Science and Technology, Norway with a chapter on Thermodynamics and Materials Modelling by Neil L. Allan School of Chemistry, Bristol University, UK
Chemical Thermodynamics of Materials
Chemical Thermodynamics of Materials Macroscopic and Microscopic Aspects Svein StĂ¸len Department of Chemistry, University of Oslo, Norway
Tor Grande Department of Materials Technology, Norwegian University of Science and Technology, Norway with a chapter on Thermodynamics and Materials Modelling by Neil L. Allan School of Chemistry, Bristol University, UK
Copyright © 2004 by
John Wiley & Sons Ltd, The Atrium, Southern Gate, Chichester West Sussex PO19 8SQ, England Telephone (+44) 1243 779777
Email (for orders and customer service enquiries): cdbooks@wiley.co.uk Visit our Home Page on www.wileyeurope.com or www.wiley.com All Rights Reserved. No part of this publication may be reproduced, stored in a retrieval system or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning or otherwise, except under the terms of the Copyright, Designs and Patents Act 1988 or under the terms of a licence issued by the Copyright Licensing Agency Ltd, 90 Tottenham Court Road, London W1T 4LP, UK, without the permission in writing of the Publisher, with the exception of any material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the publication. Requests to the publisher should be addressed to the Permissions Department, John Wiley & Sons Ltd, The Atrium, Southern Gate, Chichester, West Sussex PO19 8SQ, England, or emailed to permreq@wiley.co.uk, or faxed to (+44) 1243 770571. This publication is designed to provide accurate and authoritative information in regard to the subject matter covered. It is sold on the understanding that the publisher is not engaged in rendering professional services. If professional advice or other expert assistamce is required, the services of a competent professional should be sought. Other Wiley Editorial Offices John Wiley & Sons Inc., 111 River Street, Hoboken, NJ 07030, USA JosseyBass, 989 Market Street, San Francisco, CA 941031741, USA WileyVCH Verlag GmbH, Boschstr. 12, D69469 Weinheim, Germany John Wiley & Sons Australia Ltd, 33 Park Road, Milton, Queensland 4064, Australia John Wiley & Sons (Asia) Pte Ltd, 2 Clementi Loop # 0201, Jin Xing Distripark, Singapore 129809 John Wiley & Sons Canada Ltd, 22 Worcester Road, Etobicoke, Ontario, Canada M9W 1L1
Library of Congress CataloginginPublication Data Stølen, Svein. Chemical thermodynamics of materials : macroscopic and microscopic aspects / Svein Stølen, Tor Grande. p. cm. Includes bibliographical references and index. ISBN 0471492302 (cloth : alk. paper) 1. Thermodynamics. I. Grande, Tor. II. Title. QD504 .S76 2003 541'.369dc22 2003021826 British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library ISBN 0 471 49230 2 Typeset in 10/12 pt Times by Ian Kingston Editorial Services, Nottingham, UK Printed and bound in Great Britain by Antony Rowe, Ltd, Chippenham, Wiltshire This book is printed on acidfree paper responsibly manufactured from sustainable forestry in which at least two trees are planted for each one used for paper production.
Contents
Preface
xi
1 Thermodynamic foundations
1
1.1 Basic concepts Thermodynamic systems Thermodynamic variables Thermodynamic processes and equilibrium
1.2 The first law of thermodynamics Conservation of energy Heat capacity and definition of enthalpy Reference and standard states Enthalpy of physical transformations and chemical reactions
1.3 The second and third laws of thermodynamics The second law and the definition of entropy Reversible and nonreversible processes Conditions for equilibrium and the definition of Helmholtz and Gibbs energies Maximum work and maximum nonexpansion work The variation of entropy with temperature The third law of thermodynamics The Maxwell relations Properties of the Gibbs energy
1.4 Open systems Definition of the chemical potential Conditions for equilibrium in a heterogeneous system Partial molar properties The Gibbsâ€“Duhem equation
References Further reading
2 Singlecomponent systems 2.1 Phases, phase transitions and phase diagrams Phases and phase transitions Slopes of the phase boundaries Phase diagrams and Gibbs phase rule
1 1 2 3
4 4 5 8 9
12 12 12 13 15 16 17 18 20
24 24 25 25 26
27 27
29 29 29 33 36
v
vi
Contents Fieldinduced phase transitions
2.2 The gas phase Ideal gases Real gases and the definition of fugacity Equations of state of real gases
2.3 Condensed phases Variation of the standard chemical potential with temperature Representation of transitions Equations of state
References Further reading
37
39 39 40 42
44 44 47 52
54 55
3 Solution thermodynamics
57
3.1 Fundamental definitions
58
Measures of composition Mixtures of gases Solid and liquid solutions – the definition of chemical activity
3.2 Thermodynamics of solutions Definition of mixing properties Ideal solutions Excess functions and deviation from ideality
3.3 Standard states Henry’s and Raoult’s laws Raoultian and Henrian standard states
3.4 Analytical solution models Dilute solutions Solution models Derivation of partial molar properties
3.5 Integration of the Gibbs–Duhem equation References Further reading
4 Phase diagrams 4.1 Binary phase diagrams from thermodynamics Gibbs phase rule Conditions for equilibrium Ideal and nearly ideal binary systems Simple eutectic systems Regular solution modelling Invariant phase equilibria Formation of intermediate phases Melting temperature: depression or elevation? Minimization of Gibbs energy and heterogeneous phase equilibria
4.2 Multicomponent systems Ternary phase diagrams Quaternary systems Ternary reciprocal systems
4.3 Predominance diagrams References Further reading
58 59 60
60 60 63 64
67 68 70
73 73 74 77
79 83 83
85 85 85 88 90 96 98 102 103 106 109
109 109 115 116
117 125 125
Contents
5 Phase stability 5.1 Supercooling of liquids – superheating of crystals 5.2 Fluctuations and instability The driving force for chemical reactions: definition of affinity Stability with regard to infinitesimal fluctuations Compositional fluctuations and instability The van der Waals theory of liquid–gas transitions Pressureinduced amorphization and mechanical instability
5.3 Metastable phase equilibria and kinetics Phase diagrams reflecting metastability Thermal evolution of metastable phases Materials in thermodynamic potential gradients
References Further reading
6 Surfaces, interfaces and adsorption 6.1 Thermodynamics of interfaces Gibbs surface model and definition of surface tension Equilibrium conditions for curved interfaces The surface energy of solids Anisotropy and crystal morphology Trends in surface tension and surface energy Morphology of interfaces
6.2 Surface effects on heterogeneous phase equilibria Effect of particle size on vapour pressure Effect of bubble size on the boiling temperature of pure substances Solubility and nucleation Ostwald ripening Effect of particle size on melting temperature Particle sizeinduced phase transitions
6.3 Adsorption and segregation Gibbs adsorption equation Relative adsorption and surface segregation Adsorption isotherms
References Further reading
7 Trends in enthalpy of formation 7.1 Compound energetics: trends Prelude on the energetics of compound formation Periodic trends in the enthalpy of formation of binary compounds Intermetallic compounds and alloys
7.2 Compound energetics: rationalization schemes Acid–base rationalization Atomic size considerations Electron count rationalization Volume effects in microporous materials
7.3 Solution energetics: trends and rationalization schemes Solid solutions: strain versus electron transfer Solubility of gases in metals Nonstoichiometry and redox energetics Liquid solutions
vii
127 128 132 132 133 135 140 143
149 149 150 152
153 155
157 159 159 163 164 165 167 171
175 176 177 179 180 181 185
186 186 189 191
193 195
197 199 199 202 210
211 211 214 215 216
218 218 220 221 223
viii
Contents
References Further reading
8 Heat capacity and entropy 8.1 Simple models for molecules and crystals 8.2 Lattice heat capacity The Einstein model Collective modes of vibration The Debye model The relationship between elastic properties and heat capacity Dilational contributions to the heat capacity Estimates of heat capacity from crystallographic, elastic and vibrational characteristics
8.3 Vibrational entropy The Einstein and Debye models revisited Effect of volume and coordination
8.4 Heat capacity contributions of electronic origin
226 227
229 230 233 233 235 241 244 245 247
248 248 250
252
Electronic and magnetic heat capacity Electronic and magnetic transitions
252 256
8.5 Heat capacity of disordered systems
260
Crystal defects Fast ion conductors, liquids and glasses
References Further reading
9 Atomistic solution models 9.1 Lattice models for solutions
260 261
264 266
267 268
Partition function Ideal solution model Regular solution model Quasichemical model Flory model for molecules of different sizes
268 269 271 276 279
9.2 Solutions with more than one sublattice
285
Ideal solution model for a two sublattice system Regular solution model for a two sublattice system Reciprocal ionic solution
9.3 Orderâ€“disorder Braggâ€“Williams treatment of convergent ordering in solid solutions Nonconvergent disordering in spinels
9.4 Nonstoichiometric compounds Mass action law treatment of defect equilibria Solid solution approach
References Further reading
10 Experimental thermodynamics 10.1 Determination of temperature and pressure 10.2 Phase equilibria 10.3 Energetic properties Thermophysical calorimetry Thermochemical calorimetry Electrochemical methods
285 286 288
292 292 294
296 296 297
300 301
303 303 305 308 309 313 319
ix
Contents Vapour pressure methods Some words on measurement uncertainty
10.4 Volumetric techniques References Further reading
11 Thermodynamics and materials modelling by Neil L. Allan 11.1 Interatomic potentials and energy minimization Intermolecular potentials Energy minimization, molecular mechanics and lattice statics High pressure Elevated temperatures and thermal expansion: Helmholtz, Gibbs energies and lattice dynamics Negative thermal expansion Configurational averaging â€“ solid solutions and grossly nonstoichiometric oxides
11.2 Monte Carlo and molecular dynamics Monte Carlo Molecular dynamics Thermodynamic perturbation Thermodynamic integration
323 326
328 330 335
337 339 339 343 347 347 350 353
356 356 359 361 362
11.3 Quantum mechanical methods
363
Hartreeâ€“Fock theory Density functional theory
364 366
11.4 Applications of quantum mechanical methods Carbon nitride Nanostructures Lithium batteries Ab initio molecular dynamics Surfaces and defects Quantum Monte Carlo
11.5 Discussion Structure prediction
References Further reading
367 367 367 369 369 370 372
373 373
374 375
Symbols and data
377
Index
385
1
Thermodynamic foundations
1.1 Basic concepts Thermodynamic systems A thermodynamic description of a process needs a welldefined system. A thermodynamic system contains everything of thermodynamic interest for a particular chemical process within a boundary. The boundary is either a real or hypothetical enclosure or surface that confines the system and separates it from its surroundings. In order to describe the thermodynamic behaviour of a physical system, the interaction between the system and its surroundings must be understood. Thermodynamic systems are thus classified into three main types according to the way they interact with the surroundings: isolated systems do not exchange energy or matter with their surroundings; closed systems exchange energy with the surroundings but not matter; and open systems exchange both energy and matter with their surroundings. The system may be homogeneous or heterogeneous. An exact definition is difficult, but it is convenient to define a homogeneous system as one whose properties are the same in all parts, or at least their spatial variation is continuous. A heterogeneous system consists of two or more distinct homogeneous regions or phases, which are separated from one another by surfaces of discontinuity. The boundaries between phases are not strictly abrupt, but rather regions in which the properties change abruptly from the properties of one homogeneous phase to those of the other. For example, Portland cement consists of a mixture of the phases bCa2SiO4, Ca3SiO5, Ca3Al2O6 and Ca4Al2Fe2O10. The different homogeneous phases are readily distinguished from each
Chemical Thermodynamics of Materials by Svein StĂ¸len and Tor Grande ÂŠ 2004 John Wiley & Sons, Ltd ISBN 0 471 492320 2 1
2
1 Thermodynamic foundations
other macroscopically and the thermodynamics of the system can be treated based on the sum of the thermodynamics of each single homogeneous phase. In colloids, on the other hand, the different phases are not easily distinguished macroscopically due to the small particle size that characterizes these systems. So although a colloid also is a heterogeneous system, the effect of the surface thermodynamics must be taken into consideration in addition to the thermodynamics of each homogeneous phase. In the following, when we speak about heterogeneous systems, it must be understood (if not stated otherwise) that the system is one in which each homogeneous phase is spatially sufficiently large to neglect surface energy contributions. The contributions from surfaces become important in systems where the dimensions of the homogeneous regions are about 1 mm or less in size. The thermodynamics of surfaces will be considered in Chapter 6. A homogeneous system â€“ solid, liquid or gas â€“ is called a solution if the composition of the system can be varied. The components of the solution are the substances of fixed composition that can be mixed in varying amounts to form the solution. The choice of the components is often arbitrary and depends on the purpose of the problem that is considered. The solid solution LaCr1â€“yFeyO3 can be treated as a quasibinary system with LaCrO3 and LaFeO3 as components. Alternatively, the compound may be regarded as forming from La2O3, Fe2O3 and Cr2O3 or from the elements La, Fe, Cr and O2 (g). In La2O3 or LaCrO3, for example, the elements are present in a definite ratio, and independent variation is not allowed. La2O3 can thus be treated as a single component system. We will come back to this important topic in discussing the Gibbs phase rule in Chapter 4. Thermodynamic variables In thermodynamics the state of a system is specified in terms of macroscopic state variables such as volume, V, temperature, T, pressure, p, and the number of moles of the chemical constituents i, ni. The laws of thermodynamics are founded on the concepts of internal energy (U), and entropy (S), which are functions of the state variables. Thermodynamic variables are categorized as intensive or extensive. Variables that are proportional to the size of the system (e.g. volume and internal energy) are called extensive variables, whereas variables that specify a property that is independent of the size of the system (e.g. temperature and pressure) are called intensive variables. A state function is a property of a system that has a value that depends on the conditions (state) of the system and not on how the system has arrived at those conditions (the thermal history of the system). For example, the temperature in a room at a given time does not depend on whether the room was heated up to that temperature or cooled down to it. The difference in any state function is identical for every process that takes the system from the same given initial state to the same given final state: it is independent of the path or process connecting the two states. Whereas the internal energy of a system is a state function, work and heat are not. Work and heat are not associated with one given state of the system, but are defined only in a transformation of the system. Hence the work performed and the heat
1.1 Basic concepts
3
adsorbed by the system between the initial and final states depend on the choice of the transformation path linking these two states. Thermodynamic processes and equilibrium The state of a physical system evolves irreversibly towards a timeindependent state in which we see no further macroscopic physical or chemical changes. This is the state of thermodynamic equilibrium, characterized for example by a uniform temperature throughout the system but also by other features. A nonequilibrium state can be defined as a state where irreversible processes drive the system towards the state of equilibrium. The rates at which the system is driven towards equilibrium range from extremely fast to extremely slow. In the latter case the isolated system may appear to have reached equilibrium. Such a system, which fulfils the characteristics of an equilibrium system but is not the true equilibrium state, is called a metastable state. Carbon in the form of diamond is stable for extremely long periods of time at ambient pressure and temperature, but transforms to the more stable form, graphite, if given energy sufficient to climb the activation energy barrier. Buckminsterfullerene, C60, and the related C70 and carbon nanotubes, are other metastable modifications of carbon. The enthalpies of three modifications of carbon relative to graphite are given in Figure 1.1 [1, 2]. Glasses are a particular type of material that is neither stable nor metastable. Glasses are usually prepared by rapid cooling of liquids. Below the melting point the liquid become supercooled and is therefore metastable with respect to the equilibrium crystalline solid state. At the glass transition the supercooled liquid transforms to a glass. The properties of the glass depend on the quenching rate (thermal history) and do not fulfil the requirements of an equilibrium phase. Glasses represent nonergodic states, which means that they are not able to explore their entire phase space, and glasses are thus not in internal equilibrium. Both stable states (such as liquids above the melting temperature) and metastable states (such as supercooled liquids between the melting and glass transition temperatures) are in internal equilibrium and thus ergodic. Frozenin degrees of freedom are frequently present, even in crystalline compounds. Glassy crystals exhibit translational periodicity of the molecular
o Df Hm / kJ mol C 1
40 C60
C70
30 20
graphite
diamond
10 0
Figure 1.1 Standard enthalpy of formation per mol C of C60 [1], C70 [2] and diamond relative to graphite at 298 K and 1 bar.
4
1 Thermodynamic foundations
centre of mass, whereas the molecular orientation is frozen either in completely random directions or randomly among a preferred set of orientations. Strictly spoken, only ergodic states can be treated in terms of classical thermodynamics.
1.2 The first law of thermodynamics Conservation of energy The first law of thermodynamics may be expressed as: Whenever any process occurs, the sum of all changes in energy, taken over all the systems participating in the process, is zero. The important consequence of the first law is that energy is always conserved. This law governs the transfer of energy from one place to another, in one form or another: as heat energy, mechanical energy, electrical energy, radiation energy, etc. The energy contained within a thermodynamic system is termed the internal energy or simply the energy of the system, U. In all processes, reversible or irreversible, the change in internal energy must be in accord with the first law of thermodynamics. Work is done when an object is moved against an opposing force. It is equivalent to a change in height of a body in a gravimetric field. The energy of a system is its capacity to do work. When work is done on an otherwise isolated system, its capacity to do work is increased, and hence the energy of the system is increased. When the system does work its energy is reduced because it can do less work than before. When the energy of a system changes as a result of temperature differences between the system and its surroundings, the energy has been transferred as heat. Not all boundaries permit transfer of heat, even when there is a temperature difference between the system and its surroundings. A boundary that does not allow heat transfer is called adiabatic. Processes that release energy as heat are called exothermic, whereas processes that absorb energy as heat are called endothermic. The mathematical expression of the first law is
책 dU = 책 dq + 책 dw = 0
(1.1)
where U, q and w are the internal energy, the heat and the work, and each summation covers all systems participating in the process. Applications of the first law involve merely accounting processes. Whenever any process occurs, the net energy taken up by the given system will be exactly equal to the energy lost by the surroundings and vice versa, i.e. simply the principle of conservation of energy. In the present book we are primarily concerned with the work arising from a change in volume. In the simplest example, work is done when a gas expands and drives back the surrounding atmosphere. The work done when a system expands its volume by an infinitesimal small amount dV against a constant external pressure is dw =  pext dV
(1.2)
1.2 The first law of thermodynamics
5
Table 1.1 Conjugate pairs of variables in work terms for the fundamental equation for the internal energy U. Here f is force of elongation, l is length in the direction of the force, s is surface tension, As is surface area, Fi is the electric potential of the phase containing species i, qi is the contribution of species i to the electric charge of a phase, E is electric field strength, p is the electric dipole moment of the system, B is magnetic field strength (magnetic flux density), and m is the magnetic moment of the system. The dots indicate scalar products of vectors. Type of work Mechanical Pressure–volume Elastic Surface Electromagnetic Charge transfer Electric polarization Magnetic polarization
Intensive variable
Extensive variable
Differential work in dU
–p f s
V l AS
–pdV fdl sdAS
Fi E B
qi p m
Fidqi E×dp B×dm
The negative sign shows that the internal energy of the system doing the work decreases. In general, dw is written in the form (intensive variable)◊d(extensive variable) or as a product of a force times a displacement of some kind. Several types of work terms may be involved in a single thermodynamic system, and electrical, mechanical, magnetic and gravitational fields are of special importance in certain applications of materials. A number of types of work that may be involved in a thermodynamic system are summed up in Table 1.1. The last column gives the form of work in the equation for the internal energy. Heat capacity and definition of enthalpy In general, the change in internal energy or simply the energy of a system U may now be written as dU = dq + dw pV + dw non e
(1.3)
where dw pV and dw non e are the expansion (or pV) work and the additional nonexpansion (or nonpV) work, respectively. A system kept at constant volume cannot do expansion work; hence in this case dw pV = 0. If the system also does not do any other kind of work, then dw non e = 0. So here the first law yields dU = dqV
(1.4)
where the subscript denotes a change at constant volume. For a measurable change, the increase in the internal energy of a substance is
6
1 Thermodynamic foundations
DU = qV
(1.5)
The temperature dependence of the internal energy is given by the heat capacity at constant volume at a given temperature, formally defined by æ ¶U ö CV = ç ÷ è ¶T øV
(1.6)
For a constantvolume system, an infinitesimal change in temperature gives an infinitesimal change in internal energy and the constant of proportionality is the heat capacity at constant volume dU = C V dT
(1.7)
The change in internal energy is equal to the heat supplied only when the system is confined to a constant volume. When the system is free to change its volume, some of the energy supplied as heat is returned to the surroundings as expansion work. Work due to the expansion of a system against a constant external pressure, pext, gives the following change in internal energy: dU = dq + dw = dq  pext dV
(1.8)
For processes taking place at constant pressure it is convenient to introduce the enthalpy function, H, defined as H = U + pV
(1.9)
Differentiation gives dH = d(U + pV ) = dq + dw + Vdp + pdV
(1.10)
When only work against a constant external pressure is done: dw =  pext dV
(1.11)
and eq. (1.10) becomes dH = dq + Vdp
(1.12)
Since dp = 0 (constant pressure), dH = dq p
(1.13)
1.2 The first law of thermodynamics
7
and DH = qp
(1.14)
The enthalpy of a substance increases when its temperature is raised. The temperature dependence of the enthalpy is given by the heat capacity at constant pressure at a given temperature, formally defined by æ ¶H ö Cp = ç ÷ è ¶T ø p
(1.15)
Hence, for a constant pressure system, an infinitesimal change in temperature gives an infinitesimal change in enthalpy and the constant of proportionality is the heat capacity at constant pressure. dH = C p dT
(1.16)
The heat capacity at constant volume and constant pressure at a given temperature are related through Cp  CV =
a 2 VT kT
(1.17)
where a and k T are the isobaric expansivity and the isothermal compressibility respectively, defined by a=
1 æ ¶V ö ÷ ç V è ¶T ø p
(1.18)
and kT =
1 æ ¶V ç V çè ¶p
ö ÷÷ øT
(1.19)
Typical values of the isobaric expansivity and the isothermal compressibility are given in Table 1.2. The difference between the heat capacities at constant volume and constant pressure is generally negligible for solids at low temperatures where the thermal expansivity becomes very small, but the difference increases with temperature; see for example the data for Al2O3 in Figure 1.2. Since the heat absorbed or released by a system at constant pressure is equal to its change in enthalpy, enthalpy is often called heat content. If a phase transformation (i.e. melting or transformation to another solid polymorph) takes place within
8
1 Thermodynamic foundations
Table 1.2 The isobaric expansivity and isothermal compressibility of selected compounds at 300 K. Compound
a /10–5 K–1
kT/10–12 Pa
MgO Al2O3 MnO Fe3O4 NaCl C (diamond) C (graphite) Al
3.12 1.62 3.46 3.56 11.8 0.54 2.49 6.9
6.17 3.97 6.80 4.52 41.7 1.70 17.9 13.2
5
C / J K –1mol –1
130
Cp,m CV,m
120
–12
kT / 10
–1
Pa
4
110 3
100
–5
a / 10 K 90
–1
Al 2O3
2
80 500
1000 1500 500 T/K
1000 1500
Figure 1.2 Molar heat capacity at constant pressure and at constant volume, isobaric expansivity and isothermal compressibility of Al2O3 as a function of temperature.
the system, heat may be adsorbed or released without a change in temperature. At constant pressure the heat merely transforms a portion of the substance (e.g. from solid to liquid – ice–water). Such a change is called a firstorder phase transition and will be defined formally in Chapter 2. The standard enthalpy of aluminium relative to 0 K is given as a function of temperature in Figure 1.3. The standard enthalpy of fusion and in particular the standard enthalpy of vaporization contribute significantly to the total enthalpy increment. Reference and standard states Thermodynamics deals with processes and reactions and is rarely concerned with the absolute values of the internal energy or enthalpy of a system, for example, only with the changes in these quantities. Hence the energy changes must be well defined. It is often convenient to choose a reference state as an arbitrary zero. Often the reference state of a condensed element/compound is chosen to be at a pressure of 1 bar and in the most stable polymorph of that element/compound at the
1.2 The first law of thermodynamics
9
400 o DT0 Hm / kJ mol 1
Al 300
Dvap Hmo = 294 kJ mol –1
200 100 0 0
DfusHmo = 10.8 kJ mol –1
500 1000 1500 2000 2500 3000 T/K
Figure 1.3 Standard enthalpy of aluminium relative to 0 K. The standard enthalpy of fusion o o ) is significantly smaller than the standard enthalpy of vaporization (D vap H m ). (D fus H m
temperature at which the reaction or process is taking place. This reference state is called a standard state due to its large practical importance. The term standard state and the symbol o are reserved for p = 1 bar. The term reference state will be used for states obtained from standard states by a change of pressure. It is important to note that the standard state chosen should be specified explicitly, since it is indeed possible to choose different standard states. The standard state may even be a virtual state, one that cannot be obtained physically. Let us give an example of a standard state that not involves the most stable polymorph of the compound at the temperature at which the system is considered. Cubic zirconia, ZrO2, is a fastion conductor stable only above 2300 °C. Cubic zirconia can, however, be stabilized to lower temperatures by forming a solid solution with for example Y2O3 or CaO. The composition–temperature stability field of this important phase is marked by Css in the ZrO2–CaZrO3 phase diagram shown in Figure 1.4 (phase diagrams are treated formally in Chapter 4). In order to describe the thermodynamics of this solid solution phase at, for example, 1500 °C, it is convenient to define the metastable cubic hightemperature modification of zirconia as the standard state instead of the tetragonal modification that is stable at 1500 °C. The standard state of pure ZrO2 (used as a component of the solid solution) and the investigated solid solution thus take the same crystal structure. The standard state for gases is discussed in Chapter 2. Enthalpy of physical transformations and chemical reactions The enthalpy that accompanies a change of physical state at standard conditions is called the standard enthalpy of transition and is denoted D trs H o . Enthalpy changes accompanying chemical reactions at standard conditions are in general termed standard enthalpies of reaction and denoted D r H o . Two simple examples are given in Table 1.3. In general, from the first law, the standard enthalpy of a reaction is given by
10
1 Thermodynamic foundations 2500
Css + Css
T / °C
2000
Css + CaZrO3
Tss 1500 Tss + Css 1000 500
liq. liq. + CaZrO3 liq.
Tss + CaZr4O9
Mss + CaZr4O9 Mss
0 ZrO2
10
Css + CaZr4O9 CaZr4O9 + CaZrO 3
20
30 xCaO
40
50 CaZrO3
Figure 1.4 The ZrO2–CaZrO3 phase diagram. Mss, Tss and Css denote monoclinic, tetragonal and cubic solid solutions. Table 1.3 Examples of a physical transformation and a chemical reaction and their respeco denotes the standard molar enthalpy of fusion. tive enthalpy changes. Here D fus H m Reaction
Enthalpy change
Al (s) = Al (liq) 3SiO2 (s) + 2N2 (g) = Si3N4 (s) + 3O2 (g)
o o = D fus Hm = 10789 J mol–1 at Tfus D trs Hm o D r H = 1987.8 kJ mol–1 at 298.15 K
o o DrH o = åvjHm ( j)  å v i H m (i) j
(1.20)
i
where the sum is over the standard molar enthalpy of the reactants i and products j (vi and vj are the stoichiometric coefficients of reactants and products in the chemical reaction). o Of particular importance is the standard molar enthalpy of formation, D f H m , which corresponds to the standard reaction enthalpy for the formation of one mole of a compound from its elements in their standard states. The standard enthalpies of formation of three different modifications of Al2SiO5 are given as examples in Table 1.4 [3]. Compounds like these, which are formed by combination of electropositive and electronegative elements, generally have large negative enthalpies of formation due to the formation of strong covalent or ionic bonds. In contrast, the difference in enthalpy of formation between the different modifications is small. This is more easily seen by consideration of the enthalpies of formation of these ternary oxides from their binary constituent oxides, often termed the o standard molar enthalpy of formation from oxides, D f ,ox H m , which correspond o to D r H m for the reaction SiO2 (s) + Al2O3 (s) = Al2SiO5 (s)
(1.21)
1.2 The first law of thermodynamics
11
Table 1.4 The enthalpy of formation of the three polymorphs of Al2SiO5, kyanite, andalusite and sillimanite at 298.15 K [3]. Reaction
o / kJ mol–1 D f Hm
2 Al (s) + Si (s) + 5/2 O2 (g) = Al2SiO5 (kyanite) 2 Al (s) + Si (s) + 5/2 O2 (g) = Al2SiO5 (andalusite) 2 Al (s) + Si (s) + 5/2 O2 (g) = Al2SiO5 (sillimanite)
–2596.0 –2591.7 –2587.8
These are derived by subtraction of the standard molar enthalpy of formation of the binary oxides, since standard enthalpies of individual reactions can be combined to obtain the standard enthalpy of another reaction. Thus, o o o ( Al2 SiO 5 ) = D f H m ( Al2 SiO 5 )  D f H m ( Al2 O 3 ) D f,ox H m
(1.22)
o ( SiO2 )  DfHm
This use of the first law of thermodynamics is called Hess’s law: The standard enthalpy of an overall reaction is the sum of the standard enthalpies of the individual reactions that can be used to describe the overall reaction of Al2SiO5. Whereas the enthalpy of formation of Al2SiO5 from the elements is large and negative, the enthalpy of formation from the binary oxides is much less so. D f,ox H m is furthermore comparable to the enthalpy of transition between the different polymorphs, as shown for Al2SiO5 in Table 1.5 [3]. The enthalpy of fusion is also of similar magnitude. The temperature dependence of reaction enthalpies can be determined from the heat capacity of the reactants and products. When a substance is heated from T1 to T2 at a particular pressure p, assuming no phase transition is taking place, its molar enthalpy change from DH m (T 1 ) to DH m (T 2 ) is
Table 1.5 The enthalpy of formation of kyanite, andalusite and sillimanite from the binary constituent oxides [3]. The enthalpy of transition between the different polymorphs is also given. All enthalpies are given for T = 298.15 K. Reaction Al2O3 (s) + SiO2 (s) = Al2SiO5 (kyanite) Al2O3 (s) + SiO2 (s) = Al2SiO5 (andalusite) Al2O3 (s) + SiO2 (s) = Al2SiO5 (sillimanite) Al2SiO5 (kyanite) = Al2SiO5 (andalusite) Al2SiO5 (andalusite) = Al2SiO5 (sillimanite)
o o / kJ mol–1 D r Hm = D f,ox Hm
–9.6 –5.3 –1.4 4.3 3.9
12
1 Thermodynamic foundations T2
DH m (T 2 ) = DH m (T 1 ) + ò C p ,m dT
(1.23)
T1
This equation applies to each substance in a reaction and a change in the standard reaction enthalpy (i.e. p is now po = 1 bar) going from T1 to T2 is given by D r H o (T 2 ) = D r H o (T 1 ) +
T2
ò D r C p , m dT o
(1.24)
T1
o where D r C p,m is the difference in the standard molar heat capacities at constant pressure of the products and reactants under standard conditions taking the stoichiometric coefficients that appear in the chemical equation into consideration:
D r C op ,m = å v j C op ,m ( j)  å v i C po ,m (i) j
(1.25)
i
The heat capacity difference is in general small for a reaction involving condensed phases only.
1.3 The second and third laws of thermodynamics The second law and the definition of entropy A system can in principle undergo an indefinite number of processes under the constraint that energy is conserved. While the first law of thermodynamics identifies the allowed changes, a new state function, the entropy S, is needed to identify the spontaneous changes among the allowed changes. The second law of thermodynamics may be expressed as The entropy of a system and its surroundings increases in the course of a spontaneous change, DS tot > 0. The law implies that for a reversible process, the sum of all changes in entropy, taken over all the systems participating in the process, DS tot , is zero. Reversible and nonreversible processes Any change in state of a system in thermal and mechanical contact with its surroundings at a given temperature is accompanied by a change in entropy of the system, dS, and of the surroundings, dSsur: dS + dS sur ³ 0
(1.26)
1.3 The second and third laws of thermodynamics
13
The sum is equal to zero for reversible processes, where the system is always under equilibrium conditions, and larger than zero for irreversible processes. The entropy change of the surroundings is defined as dS sur = 
dq T
(1.27)
where dq is the heat supplied to the system during the process. It follows that for any change: dS ³
dq T
(1.28)
which is known as the Clausius inequality. If we are looking at an isolated system dS ³ 0
(1.29)
Hence, for an isolated system, the entropy of the system alone must increase when a spontaneous process takes place. The second law identifies the spontaneous changes, but in terms of both the system and the surroundings. However, it is possible to consider the specific system only. This is the topic of the next section. Conditions for equilibrium and the definition of Helmholtz and Gibbs energies Let us consider a closed system in thermal equilibrium with its surroundings at a given temperature T, where no nonexpansion work is possible. Imagine a change in the system and that the energy change is taking place as a heat exchange between the system and the surroundings. The Clausius inequality (eq. 1.28) may then be expressed as dS 
dq ³0 T
(1.30)
If the heat is transferred at constant volume and no nonexpansion work is done, dS 
dU ³0 T
(1.31)
The combination of the Clausius inequality (eq. 1.30) and the first law of thermodynamics for a system at constant volume thus gives TdS ³ dU
(1.32)
14
1 Thermodynamic foundations
Correspondingly, when heat is transferred at constant pressure (pV work only), TdS 続 dH
(1.33)
For convenience, two new thermodynamic functions are defined, the Helmholtz (A) and Gibbs (G) energies: A = U  TS
(1.34)
G = H  TS
(1.35)
and
For an infinitesimal change in the system dA = dU  TdS  SdT
(1.36)
dG = dH  TdS  SdT
(1.37)
and
At constant temperature eqs. (1.36) and (1.37) reduce to dA = dU  TdS
(1.38)
dG = dH  TdS
(1.39)
and
Thus for a system at constant temperature and volume, the equilibrium condition is dA T ,V = 0
(1.40)
In a process at constant T and V in a closed system doing only expansion work it follows from eq. (1.32) that the spontaneous direction of change is in the direction of decreasing A. At equilibrium the value of A is at a minimum. For a system at constant temperature and pressure, the equilibrium condition is dG T , p = 0
(1.41)
In a process at constant T and p in a closed system doing only expansion work it follows from eq. (1.33) that the spontaneous direction of change is in the direction of decreasing G. At equilibrium the value of G is at a minimum.
1.3 The second and third laws of thermodynamics
15
Equilibrium conditions in terms of internal energy and enthalpy are less applicable since these correspond to systems at constant entropy and volume and at constant entropy and pressure, respectively dU S ,V = 0
(1.42)
dH S , p = 0
(1.43)
The Helmholtz and Gibbs energies on the other hand involve constant temperature and volume and constant temperature and pressure, respectively. Most experiments are done at constant T and p, and most simulations at constant T and V. Thus, we have now defined two functions of great practical use. In a spontaneous process at constant p and T or constant p and V, the Gibbs or Helmholtz energies, respectively, of the system decrease. These are, however, only other measures of the second law and imply that the total entropy of the system and the surroundings increases. Maximum work and maximum nonexpansion work The Helmholtz and Gibbs energies are useful also in that they define the maximum work and the maximum nonexpansion work a system can do, respectively. The combination of the Clausius inequality TdS ³ dq and the first law of thermodynamics dU = dq + dw gives dw ³ dU  TdS
(1.44)
Thus the maximum work (the most negative value of dw) that can be done by a system is dw max = dU  TdS
(1.45)
At constant temperature dA = dU – TdS and w max = DA
(1.46)
If the entropy of the system decreases some of the energy must escape as heat in order to produce enough entropy in the surroundings to satisfy the second law of thermodynamics. Hence the maximum work is less than  DU . DA is the part of the change in internal energy that is free to use for work. Hence the Helmholtz energy is in some older books termed the (isothermal) work content. The total amount of work is conveniently separated into expansion (or pV) work and nonexpansion work. dw = dw non e  pdV
(1.47)
16
1 Thermodynamic foundations
For a system at constant pressure it can be shown that dw non e,max = dH  TdS
(1.48)
At constant temperature dG = dH – TdS and w non e,max = DG
(1.49)
Hence, while the change in Helmholtz energy relates to the total work, the change in Gibbs energy at constant temperature and pressure represents the maximum nonexpansion work a system can do. Since D r G o for the formation of 1 mol of water from hydrogen and oxygen gas at 298 K and 1 bar is –237 kJ mol–1, up to 237 kJ mol–1 of ‘chemical energy’ can be converted into electrical energy in a fuel cell working at these conditions using H2(g) as fuel. Since the Gibbs energy relates to the energy free for nonexpansion work, it has in previous years been called the free energy. The variation of entropy with temperature For a reversible change the entropy increment is dS = dq / T . The variation of the entropy from T1 to T2 is therefore given by S (T 2 ) = S (T 1 ) +
T2
ò
T1
dq rev T
(1.50)
For a process taking place at constant pressure and that does not involve any nonpV work dq rev = dH = C p dT
(1.51)
and S (T 2 ) = S (T 1 ) +
T2
ò
T1
C p dT
(1.52)
T
The entropy of a particular compound at a specific temperature can be determined through measurements of the heat capacity as a function of temperature, adding entropy increments connected with firstorder phase transitions of the compound: S (T ) = S (0) +
Ttrs
ò
0
C p (T ) T
T
dT + D trs S m +
ò
Ttrs
C p (T ) T
dT
(1.53)
1.3 The second and third laws of thermodynamics
200
Dvap Smo =
–1
Al
–1
105.3 J K mol
150
–1
S mo / J K mol
17
–1
Dfus Smo =
100
–1
11.56 J K mol
–1
50 0
0
500
1000
1500
2000
2500
3000
T/K
Figure 1.5 Standard entropy of aluminium relative to 0 K. The standard entropy of fusion o o ) is significantly smaller than the standard entropy of boiling (D vap S m ). (D fus S m
The variation of the standard entropy of aluminium from 0 K to the melt at 3000 K is given in Figure 1.5. The standard entropy of fusion and in particular the standard entropy of vaporization contribute significantly to the total entropy increment. Equation (1.53) applies to each substance in a reaction and a change in the standard entropy of a reaction (p is now po = 1 bar) going from T1 to T2 is given by (neglecting for simplicity firstorder phase transitions in reactants and products) D r S o (T 2 ) = D r S o (T 1 ) +
T2
ò
T1
D r C po ,m (T ) T
dT
(1.54)
where D r C op,m (T ) is given by eq. (1.25). The third law of thermodynamics The third law of thermodynamics may be formulated as: If the entropy of each element in some perfect crystalline state at T = 0 K is taken as zero, then every substance has a finite positive entropy which at T = 0 K become zero for all perfect crystalline substances. In a perfect crystal at 0 K all atoms are ordered in a regular uniform way and the translational symmetry is therefore perfect. The entropy is thus zero. In order to become perfectly crystalline at absolute zero, the system in question must be able to explore its entire phase space: the system must be in internal thermodynamic equilibrium. Thus the third law of thermodynamics does not apply to substances that are not in internal thermodynamic equilibrium, such as glasses and glassy crystals. Such nonergodic states do have a finite entropy at the absolute zero, called zeropoint entropy or residual entropy at 0 K.
18
1 Thermodynamic foundations 1.5
25
C p,m / J K 1 mol 1
S
rhombic
20
1.2
15
0.9
10
0.6
5
0.3 0
100
200 T/K
300
D trs S / J K 1 mol 1
monoclinic
0.0 400
Figure 1.6 Heat capacity of rhombic and monoclinic sulfur [4,5] and the derived entropy of transition between the two polymorphs.
The third law of thermodynamics can be verified experimentally. The stable rhombic lowtemperature modification of sulfur transforms to monoclinic sulfur at 368.5 K (p = 1 bar). At that temperature, Ttrs, the two polymorphs are in equilibrium and the standard molar Gibbs energies of the two modifications are equal. We therefore have o o o D trs G m = D trs H m  T trs D trs S m =0
(1.55)
It follows that the standard molar entropy of the transition can be derived from the measured standard molar enthalpy of transition through the relationship o o = D trs H m / T trs D trs S m
(1.56)
o o Calorimetric experiments give D trs H m = 401.66 J molâ€“1 and thus D trs S m = 1.09 J Kâ€“1 molâ€“1 [4]. The entropies of the two modifications can alternatively be derived through integration of the heat capacities for rhombic and monoclinic sulfur given in Figure 1.6 [4,5]. The entropy difference between the two modifications, also shown in the figure, increases with temperature and at the transition temperature (368.5 K) it is in agreement with the standard entropy of transition derived from the standard enthalpy of melting. The third law of thermodynamics is thereby confirmed. The entropies of both modifications are zero at 0 K.
The Maxwell relations Maxwell used the mathematical properties of state functions to derive a set of useful relationships. These are often referred to as the Maxwell relations. Recall the first law of thermodynamics, which may be written as dU = dq + dw
(1.57)
1.3 The second and third laws of thermodynamics
19
For a reversible change in a closed system and in the absence of any nonexpansion work this equation transforms into dU = TdS  pdV
(1.58)
Since dU is an exact differential, its value is independent of the path. The same value of dU is obtained whether the change is reversible or irreversible, and eq. (1.58) applies to any change for a closed system that only does pV work. Equation (1.58) is often called the fundamental equation. The equation shows that the internal energy of a closed system changes in a simple way when S and V are changed, and U can be regarded as a function of S and V. We therefore have æ ¶U ö æ ¶U ö dU = ç ÷ dV ÷ dS + ç è ¶V ø S è ¶S øV
(1.59)
It follows from eqs. (1.58) and (1.59) that æ ¶U ö ÷ =T ç è ¶S øV
(1.60)
and that æ ¶U ö ÷ = p ç è ¶V ø S
(1.61)
Generally, a function f(x,y) for which an infinitesimal change may be expressed as df = gdx + hdy
(1.62)
is exact if æ ¶g ö æ ¶h ö çç ÷÷ = ç ÷ y ¶ è ø x è ¶x ø y
(1.63)
Thus since the internal energy, U, is a state function, one of the Maxwell relations may be deduced from (eq. 1.58): æ ¶p ö æ ¶T ö ÷ ÷ = ç ç V ¶ øS è è ¶S øV
(1.64)
20
1 Thermodynamic foundations
Table 1.6 The Maxwell relations. Thermodynamic function
Differential
Equilibrium condition
Maxwell’s relations
U (S, V)
dU = TdS – pdV
(dU)S,V = 0
æ ¶p ö æ ¶T ö ÷ = ç ÷ ç è ¶S ø V è ¶V ø S
H (S, p)
dH = TdS + Vdp
(dH)S,p = 0
æ ¶T ö ¶V ö çç ÷÷ = æç ÷ è ¶p ø S è ¶S ø p
A (T, V)
dA = –SdT – pdV
(dA)T,V = 0
æ ¶S ö æ ¶p ö ç ÷ =ç ÷ è ¶V ø T è ¶T ø V
G (T, p)
dG = –SdT + Vdp
(dG)T,p = 0
æ ¶S ö ¶V ö çç ÷÷ =  æç ÷ ¶ p è ¶T ø p è øT
V
A
G
U
S
T
H
p
Figure 1.7 The thermodynamic square. Note that the two arrows enable one to get the right sign in the equations given in the second column in Table 1.6.
Using H = U + pV , A = U  TS and G = H  TS the remaining three Maxwell relations given in Table 1.6 are easily derived starting with the fundamental equation (eq. 1.58). A convenient method to recall these equations is the thermodynamic square shown in Figure 1.7. On each side of the square appears one of the state functions with the two natural independent variables given next to it. A change in the internal energy dU, for example, is thus described in terms of dS and dV. The arrow from S to T implies that TdS is a positive contribution to dU, while the arrow from p to V implies that pdV is a negative contribution. Hence dU = TdS  pdV follows. Properties of the Gibbs energy Thermodynamics applied to real material systems often involves the Gibbs energy, since this is the most convenient choice for systems at constant pressure and temperature. We will thus consider briefly the properties of the Gibbs energy. As the natural variables for the Gibbs energy are T and p, an infinitesimal change, dG, can be expressed in terms of infinitesimal changes in pressure, dp, and temperature, dT. æ ¶G dG = çç è ¶p
ö æ ¶G ö ÷÷ dp + ç ÷ dT è ¶T ø p øT
(1.65)
1.3 The second and third laws of thermodynamics
21
The Gibbs energy is related to enthalpy and entropy through G = H – TS. For an infinitesimal change in the system dG = dH  TdS  SdT
(1.66)
Similarly, H = U + pV gives dH = dU + pdV + Vdp
(1.67)
Thus in the absence of nonexpansion work for a closed system, the following important equation dG = Vdp  SdT
(1.68)
is easily derived using also eq. (1.58). Equations (1.65) and (1.68) implies that the temperature derivative of the Gibbs energy at constant pressure is –S: æ ¶G ö ÷ = S ç è ¶T ø p
(1.69)
and thus that G (T f ) = G (T i ) 
Tf
ò SdT
(1.70)
Ti
where i and f denote the initial and final p and T conditions. Since S is positive for a compound, the Gibbs energy of a compound decreases when temperature is increased at constant pressure. G decreases most rapidly with temperature when S is large and this fact leads to entropydriven melting and vaporization of compounds when the temperature is raised. The standard molar Gibbs energy of solid, liquid and gaseous aluminium is shown as a function of temperature in Figure 1.8. The corresponding enthalpy and entropy is given in Figures 1.2 and 1.5. The melting (vaporization) temperature is given by the temperature at which the Gibbs energy of the solid (gas) and the liquid crosses, as marked in Figure 1.8. Equation (1.70) applies to each substance in a reaction and a change in the standard Gibbs energy of a reaction (p is now po = 1 bar) going from Ti to Tf is given by D r G o (T f ) = D r G o (T i ) 
Tf
ò Dr S
o
dT
(1.71)
Ti
D r S o is not necessarily positive and the Gibbs energy of a reaction may increase with temperature.
22
1 Thermodynamic foundations 0 o – o Gm Gm (s, 0 K)/kJ mol–1
sol. –50 Tfus = 933.47 K –100
gas liq.
–150 –200
Al Tvap = 2790.8 K
–250
0
1000
2000
3000
T /K
Figure 1.8 Standard Gibbs energy of solid, liquid and gaseous aluminium relative to the standard Gibbs energy of solid aluminium at T = 0 K as a function of temperature (at p = 1 bar).
The pressure derivative of the Gibbs energy (eq. 1.68) at constant temperature is V: æ ¶G çç è ¶p
ö ÷÷ = V øT
(1.72)
and the pressure variation of the Gibbs energy is given as pf
G ( p f ) = G ( p i ) + ò V dp
(1.73)
pi
Since V is positive for a compound, the Gibbs energy of a compound increases when pressure is increased at constant temperature. Thus, while disordered phases are stabilized by temperature, highdensity polymorphs (lower molar volumes) are stabilized by pressure. Figure 1.9 show that the Gibbs energy of graphite due to its open structure increases much faster with pressure than that for diamond. Graphite thus transforms to the much denser diamond modification of carbon at 1.5 GPa at 298 K. Equation (1.73) applies to each substance in a reaction and a change in the Gibbs energy of a reaction going from pi to pf is given by D r G ( pf ) = D r G ( pi ) +
pf
ò D r V dp
pi
(1.74)
o Gm  Gm (graphite, 1 bar) / kJ mol 1
1.3 The second and third laws of thermodynamics
23
12 C 9 6
Diamond Ttrs
3 Graphite 0 0.0
0.5
1.0 p / GPa
1.5
2.0
Figure 1.9 Standard Gibbs energy of graphite and diamond at T = 298 K relative to the standard Gibbs energy of graphite at 1 bar as a function of pressure.
Df,oxGm / kJ mol 1
0 –1 Kyanite –2
Sillimanite
–3 –4 Andalusite –5 0.0
0.5
Al 2SiO5 1.0 p / GPa
1.5
2.0
Figure 1.10 The standard Gibbs energy of formation from the binary constitutent oxides of the kyanite, sillimanite and andalusite modifications of Al2SiO5 as a function of pressure at 800 K. Data are taken from [3]. All three oxides are treated as incompressible.
DrV is not necessarily positive, and to compare the relative stability of the different modifications of a ternary compound like Al 2SiO5 the volume of formation of the ternary oxide from the binary constituent oxides is considered for convenience. The pressure dependence of the Gibbs energies of formation from the binary constituent oxides of kyanite, sillimanite and andalusite polymorphs of Al2SiO5 are shown in Figure 1.10. Whereas sillimanite and andalusite have positive volumes of formation and are destabilized by pressure relative to the binary oxides, kyanite has a negative volume of formation and becomes the stable highpressure phase. The thermodynamic data used in the calculations are given in Table 1.7 [3].1 1 Note that these three minerals, which are common in the Earth’s crust, are not stable at ambient pressure at high temperatures. At ambient pressure, mullite (3Al2O3◊2SiO2), is usually found in refractory materials based on these minerals.
24
1 Thermodynamic foundations
Table 1.7 Thermodynamic properties of the kyanite, sillimanite and andalusite polymorphs of Al2SiO5 at 800 K [3]. o Compound D f Hm kJ mol–1
o Sm J K–1 mol–1
o Vmo D f,ox Hm 3 –1 –1 cm mol kJ mol
o D f,ox S m –1 JK mol–1
o D f,oxGm –1 J mol
D f,oxVmo cm3 mol–1
Sillimanite Kyanite Andalusite Al2O3 SiO2
252.4 240.1 248.8 152.2 100.1
50.4 44.8 52.2 25.8 23.3
0.1 –12.2 –3.5
–3400 –1050 –4030
1.3 –4.3 3.1
–2505.57 –2513.06 –2509.08 –1622.62 –879.63
–3.32 –10.81 –6.83
1.4 Open systems Definition of the chemical potential A homogeneous open system consists of a single phase and allows mass transfer across its boundaries. The thermodynamic functions depend not only on temperature and pressure but also on the variables necessary to describe the size of the system and its composition. The Gibbs energy of the system is therefore a function of T, p and the number of moles of the chemical components i, ni: G = G (T , p, n i )
(1.75)
The exact differential of G may be written æ ¶G æ ¶G ö dG = ç dT + çç ÷ è ¶T ø p , n i è ¶p
æ ¶G ö dp + çç ÷÷ ø T ,n i è ¶n i
ö ÷÷ dn i ø T , p ,n j ¹ i
(1.76)
The partial derivatives of G with respect to T and p, respectively, we recall are –S and V. The partial derivative of G with respect to ni is the chemical potential of component i, m i æ ¶G m i = çç è ¶n i
ö ÷÷ ø T , p ,n j ¹ i
(1.77)
Equation (1.68) can for an open system be expressed as dG =  SdT + Vdp + å m i dn i
(1.78)
i
The internal energy, enthalpy and Helmholtz energy can be expressed in an analogous manner:
1.4 Open systems
25
dU = TdS  pdV + å m i dn i
(1.79)
dH = TdS + Vdp + å m i dn i
(1.80)
dA =  SdT  pdV + å m i dn i
(1.81)
i
i
i
The chemical potential is thus defined by any of the following partial derivatives: æ ¶G m i = çç è ¶n i
æ ¶A ö ÷÷ = çç ø T , p , n j ¹ i è ¶n i
æ ¶H ö ÷÷ = çç ø T ,V ,n j ¹i è ¶n i
ö æ ¶U ÷÷ = çç ø S , p , n j ¹ i è ¶n i
ö (1.82) ÷÷ ø S ,V ,n j ¹i
Conditions for equilibrium in a heterogeneous system Recall that the equilibrium condition for a closed system at constant T and p was given by eq. (1.41). For an open system the corresponding equation is (dG ) T , p ,n i = 0
(1.83)
For such a system, which allows transfer of both heat and mass, the chemical potential of each species must be the same in all phases present in equilibrium; hence m ai = m ib = m gi =…
(1.84)
Here a, b and g denote different phases in the system, whereas i denotes the different components of the system. Partial molar properties In open systems consisting of several components the thermodynamic properties of each component depend on the overall composition in addition to T and p. Chemical thermodynamics in such systems relies on the partial molar properties of the components. The partial molar Gibbs energy at constant p, T and nj (eq. 1.77) has been given a special name due to its great importance: the chemical potential. The corresponding partial molar enthalpy, entropy and volume under the same conditions are defined as æ ¶H H i = çç è ¶n i
ö ÷÷ ø T , p ,n j ¹ i
(1.85)
æ ¶S S i = çç è ¶n i
ö ÷÷ ø T , p ,n j ¹ i
(1.86)
26
1 Thermodynamic foundations
æ ¶V V i = çç è ¶n i
ö ÷÷ ø T , p ,n j ¹ i
(1.87)
Note that the partial molar derivatives may also be taken under conditions other than constant p and T. The Gibbs–Duhem equation In the absence of non pVwork, an extensive property such as the Gibbs energy of a system can be shown to be a function of the partial derivatives: æ ¶G G = å n i çç è ¶n i i
ö ÷÷ = å n iG i = å n i m i ø T , p ,n j ¹ i i i
(1.88)
In this context G itself is often referred to as the integral Gibbs energy. For a binary system consisting of the two components A and B the integral Gibbs energy eq. (1.88) is G = n A m A + n Bm B
(1.89)
Differentiation of eq. (1.89) gives dG = n A dm A + dn A m A + n B dm B + dn B m B
(1.90)
By using eq. (1.78) at constant T and p, G is also given by dG = m A dn A + m B dn B
(1.91)
By combining the two last equations, the Gibbs–Duhem equation for a binary system at constant T and p is obtained: n A dm A + n B dm B = 0 i.e.
å n i dm i = 0
(1.92)
i
In general, for an arbitrary system with i components, the Gibbs–Duhem equation is obtained by combining eq. (1.78) and eq. (1.90): SdT  Vdp + å n i dm i = 0
(1.93)
i
Expressions for the other intensive parameters such as V, S and H can also be derived:
å n i dV i = 0 i
(1.94)
1.4 Open systems
27
å n i dS i = 0
(1.95)
å n i dH i = 0
(1.96)
i i
The physical significance of the Gibbs–Duhem equation is that the chemical potential of one component in a solution cannot be varied independently of the chemical potentials of the other components of the solution. This relation will be further discussed and used in Chapter 3.
References [1] [2] [3] [4] [5]
H. D. Beckhaus, T. Ruchardt, M. Kao, F. Diederich and C. S. Foote, Angew. Chem. Int. Ed., 1992, 31, 63. H. P. Diogo, M. E. M. da Piedade, A. D. Darwish and T. J. S. Dennis, J. Phys. Chem. Solids, 1997, 58, 1965. S. K. Saxena, N. Chatterjee, Y. Fei and G. Shen, Thermodynamic Data on Oxides and Silicates. Berlin: SpringerVerlag, 1993. E. D. West, J. Am. Chem. Soc., 1959, 81, 29. E. D. Eastman and W. C. McGavock, J. Am. Chem. Soc., 1937, 59, 145.
Further reading P. W. Atkins and J. de Paula, Physical Chemistry, 7th edn. Oxford: Oxford University Press, 2001. E. A. Guggenheim, Thermodynamics: An Advanced Treatment for Chemists and Physicists, 7th edn. Amsterdam: NorthHolland, 1985. K. S. Pitzer, Thermodynamics. New York: McGrawHill, 1995. (Based on G. N. Lewis and M. Randall, Thermodynamics and the free energy of chemical substances. New York: McGrawHill, 1923.) D. Kondepudi and I. Prigogine, Modern Thermodynamics: from Heat Engines to Dissipative Structures. Chichester: John Wiley & Sons, 1998. F. D. Rossini, Chemical Thermodynamics. Chichester: John Wiley & Sons, 1950.
2
Singlecomponent systems
This chapter introduces additional central concepts of thermodynamics and gives an overview of the formal methods that are used to describe singlecomponent systems. The thermodynamic relationships between different phases of a singlecomponent system are described and the basics of phase transitions and phase diagrams are discussed. Formal mathematical descriptions of the properties of ideal and real gases are given in the second part of the chapter, while the last part is devoted to the thermodynamic description of condensed phases.
2.1 Phases, phase transitions and phase diagrams Phases and phase transitions In Chapter 1 we introduced the term phase. A phase is a state that has a particular composition and also definite, characteristic physical and chemical properties. We may have several different phases that are identical in composition but different in physical properties. A phase can be in the solid, liquid or gas state. In addition, there may exist more than one distinct crystalline phase. This is termed polymorphism, and each crystalline phase represents a distinct polymorph of the substance. A transition between two phases of the same substance at equilibrium is called a firstorder phase transition. At the equilibrium phase transition temperature the equilibrium condition eq. (1.84) yields m ai = m ib
(2.1)
where a and b denote the two coexisting phases. In this chapter we are only considering single component systems (i = 1) and for simplicity eq. (2.1) is expressed as Chemical Thermodynamics of Materials by Svein StĂ¸len and Tor Grande ÂŠ 2004 John Wiley & Sons, Ltd ISBN 0 471 492320 2 29
30
2 Singlecomponent systems
ma = m b
(2.2)
Thus the molar Gibbs energies of the two phases are the same at equilibrium. Typical firstorder phase transitions are for example melting of ice and vaporization of water at p = 1 bar and at 0° and 99.999 °C, respectively. Firstorder phase transitions are accompanied by discontinuous changes in enthalpy, entropy and volume. H, S and V are thermodynamically given through the first derivatives of the chemical potential with regard to temperature or pressure, and transitions showing discontinuities in these functions are for that reason termed firstorder. By using the first derivatives of the Gibbs energy with respect to p and T, defined in eqs. (1.69) and (1.72), the changes in the slopes of the chemical potential at the transition temperature are given as æ ¶m b ç ç ¶p è
ö æ a ÷  ç ¶m ç ÷ ø T è ¶p
ö ÷ = V mb  V ma = D trs V m ÷ øT
(2.3)
æ ¶m b ç ç ¶T è
ö æ a ÷  ç ¶m ç ÷ ø p è ¶T
ö D trs H m b ÷ = S m + Sa m =  D trs S m = ÷ T trs øp
(2.4)
Here D trs V m , D trs S m and D trs H m are the changes in the molar volume, entropy and enthalpy connected with the phase transition. Phases separated by a firstorder transition can be present together with a distinct interface, and the phases are thus coexistent under certain conditions. For a single component system like H2O, ice and water are coexistent at the melting temperature. The same is true at the firstorder transition between two crystalline polymorphs of a given compound. The changes in heat capacity at constant pressure, enthalpy, entropy and Gibbs energy at the firstorder semiconductor–metal transition in NiS [1] are shown in Figure 2.1. The heat capacity at constant pressure is the second derivative of the Gibbs energy and is given macroscopically by the temperature increment caused by an enthalpy increment; Cp = DH/DT. Since the firstorder transition takes place at constant temperature, the heat capacity in theory should be infinite at the transition temperature. This is obviously not observed experimentally, but heat capacities of the order of 107–108 J K–1 mol–1 are observed on melting of pure metals [2]. Transformations that involve discontinuous changes in the second derivatives of the Gibbs energy with regard to temperature and pressure are correspondingly termed secondorder transitions. For these transitions we have discontinuities in the heat capacity, isothermal compressibility and isobaric expansivity: æ ¶2 m b ç ç ¶T 2 è
ö æ 2 a ÷ ç¶ m 2 ç ÷ ø p è ¶T
æ b ö ÷ =  ç ¶S m ÷ ç ¶T øp è
ö æ a ÷ + ç ¶S m ç ¶T ÷ øp è
ö ÷ ÷ øp
=  (C bp ,m  C ap ,m ) / T = D trs C p ,m / T
(2.5)
2.1 Phases, phase transitions and phase diagrams
31
3000 49 2000 48 1000 47
o DT260 Hm / J mol 1
C op,m / J K 1 mol 1
50
9
–100
6 –200
3 0 260
270
280
290
300 T/ K
270
280
290
o DT260Gm / J mol 1
o DT260 Sm / J K 1 mol 1
0
–300 300
Figure 2.1 The temperature variation of the heat capacity, enthalpy, entropy, and Gibbs energy close to the firstorder semiconductor to metal transition in NiS [1].
æ ¶2 m b ç ç ¶ p2 è
ö æ 2 a ÷ ç¶ m 2 ç ÷ ø T è ¶p
b æ ö ÷ = ç ¶V m ÷ ç ø T è ¶p
ö æ a ÷  ç ¶V m ç ¶p ÷ øT è
ö ÷ ÷ øT
(2.6)
b
= V (k T  k aT ) = VD trsk T æ ¶2 m b ç ç ¶T¶p è
ö æ ¶2 ma ÷ç ÷ ç ¶T¶p ø è
ö æ ¶V mb ÷=ç ÷ ç ¶T ø è
ö æ a ÷  ç ¶V m ç ¶T ÷ øp è
ö ÷ ÷ øp
(2.7)
= V (a b  a a ) = VD trs a where kT and a are the isothermal compressibility (eq. 1.19) and isobaric expansivity (eq. 1.18). Modifications separated by a secondorder transition can never be coexistent. One typical secondorder transition, the displacive structural transition, is characterized by the distortion of bonds rather than their breaking, and the structural changes that occur are usually small. Typically, there is continuous variation in the positional parameters and the unit cell dimensions as a function of temperature. The structural changes in the system occur gradually as the system moves away from the transition point. As well as a structural similarity, a symmetry relationship
32
2 Singlecomponent systems (a)
(b)
118
–50
117
–60
Vunit cell / Å3
–40
116
50
85
45
80 75
40 Ttrs
35 800
850
900
70 950
800 T/K
900
C op,m / J K 1 mol 1
o o o DT0 Hm / kJ mol 1 DT0 Gm / kJ mol 1  D o0 Gm
Figure 2.2 Crystal structure of a (low) and b (high) quartz (SiO2).
1000
Figure 2.3 The temperature variation of the Gibbs energy [5], unitcell volume [4] enthalpy and heat capacity [5] at the secondorder a to bquartz transition of SiO2. Secondorder derivatives of the Gibbs energy like the heat capacity have discontinuities at the transition temperature.
exists between the two modifications.1 The a to bquartz transition may serve as an example, and the two modifications of SiO2 are illustrated in Figure 2.2. aquartz is most easily considered as a distorted version of hightemperature bquartz. When bquartz is cooled below 573 °C at 1 bar the framework of the structure collapses to the denser aconfiguration. The mean Si–O bond distances hardly change, but the Si–O–Si bond angle decreases from 150.9° at 590 °C to 143.61° at room temperature [3]. The variations of the unit cell volume [4], heat capacity, enthalpy, and Gibbs energy with temperature in the transition region [5] are given in Figure 2.3. While the 1 Secondorder transitions have certain restrictions concerning the symmetry of the space group for each of the two modifications. A secondorder transition can only occur between two modifications where the space group of the first is a subgroup of the space group of the second. Firstorder phase transitions do not have any restrictions concerning the symmetries of the two phases.
2.1 Phases, phase transitions and phase diagrams
33
transition is barely seen in the Gibbs energy, it gives rise to a change of slope in enthalpy and volume and to a discontinuity in the heat capacity. It is possible that both the first and second derivatives of the Gibbs energy are continuous, and that the discontinuous changes occur in the thirdorder derivatives of the Gibbs energy. The corresponding transition would be of third order. In practice, it is difficult to decide experimentally whether or not there is a discontinuity in the heat capacity, thermal expansivity or isothermal compressibility at the transition temperature. Even small jumps in these properties, which are difficult to verify experimentally, will signify a secondorder transition. Hence it is common to call all transitions with continuous firstorder derivatives secondorder transitions. Similarly, it may be difficult to distinguish some firstorder transitions from secondorder transitions due to kinetics. Slopes of the phase boundaries A phase boundary for a singlecomponent system shows the conditions at which two phases coexist in equilibrium. Recall the equilibrium condition for the phase equilibrium (eq. 2.2). Let p and T change infinitesimally but in a way that leaves the two phases a and b in equilibrium. The changes in chemical potential must be identical, and hence dm a = dm b
(2.8)
An infinitesimal change in the Gibbs energy can be expressed as dG = Vdp â€“ SdT (eq. 1.68) and eq. (2.8) becomes b b a S a m dT + V m dp =  S m dT + V m dp
(2.9)
Equation (2.9) can be rearranged to the Clapeyron equation: dp D trs S m = dT D trs V m
(2.10)
At equilibrium D trs S m = D trs H m / T trs and the Clapeyron equation may be written D trs H m dp = dT T trs D trs V m
(2.11)
The variation of the phase transition temperature with pressure can be calculated from the knowledge of the volume and enthalpy change of the transition. Most often both the entropy and volume changes are positive and the transition temperature increases with pressure. In other cases, notably melting of ice, the density of the liquid phase is larger than of the solid, and the transition temperature decreases
34
2 Singlecomponent systems Tfus(In)
1.01
Tfus(Al)
Ttrs / Ttrso
1.00 0.99
Tfus(H2O)
0.98 0.97
a to bAgI
0.96 0.00
0.04 p / GPa
0.08
Figure 2.4 The initial dT/dp slope of selected firstorder phase transitions relative to the transition temperature at p = 1 bar. Data taken from [6,7].
with pressure. The slope of the pT boundary for some firstorder transitions is shown in Figure 2.4. It should be noted that the boiling temperature of all substances varies more rapidly with pressure than their melting temperature since the large volume change during vaporization gives a small dp/dT. For a liquid–vapour or solid–vapour boundary the volume of gas is much larger than the volume of the condensed phase, and D vapV m » V mgas is a reasonable approximation. For an ideal gas (see eq. 2.23), V mgas = RT / p and equation (2.11) rearrange to the Clausius–Clapeyron equation: d ln p D vap H m = dT RT 2
(2.12)
The vapour pressure of Zn as a function of temperature, which implicitly also shows the variation of the boiling temperature with pressure, is shown in Figure 2.5.
log pZn / bar
0
–2 Zn –4
800
1000
1200
1400
T/K
Figure 2.5 The vapour pressure of pure Zn as a function of temperature. The standard boiling (or vaporization) temperature is defined by the temperature at which the pressure of Zn is 1 bar.
2.1 Phases, phase transitions and phase diagrams
35
Secondorder transitions do not involve coexisting phases but are transitions in which the structural properties gradually change within a single phase. The lowand hightemperature modifications are here two modifications of the same phase. Hence, although these transitions often are represented in phase diagrams, they are not heterogeneous phases and do not obey Gibbs’ phase rule (see below). There is no discontinuous change in the first derivatives of the Gibbs energy at the transition temperature for a secondorder transition, and the volumes of the two phases are thus equal. The change in volume, dV, must be equal for both modifications if the transition is to remain continuous. Taking into account that V is a function of temperature and pressure and by using the definitions of the isobaric expansivity and the isothermal compressibility: æ ¶V ö æ ¶V ö dV = ç ÷÷ dp = VadT  Vk T dp ÷ dT + çç è ¶T ø p è ¶p ø T
(2.13)
Thus the pT slope is for a secondorder transition is given as D a dp = trs dT D trsk T
(2.14)
Some selected examples of the variation with pressure of the transition temperatures of secondorder transitions are shown in Figure 2.6. Phase diagrams and Gibbs phase rule A phase diagram displays the regions of the potential space where the various phases of the system are stable. The potential space is given by the variables of the 1.02 a to bquartz 1.01 o Ttrs / Ttrs
TN (La 0.7Sr0.3MnO3) TN (Fe1–y O)
1.00
0.99 0.00
0.04
0.08
p / GPa
Figure 2.6 The initial dT/dp slope of selected secondorder transitions relative to the transition temperature at p = 1 bar; a to bquartz (SiO2) [8], the Néel temperature (TN) of Fe1–yO [9] and the Néel temperature of La0.7Ca0.3MnO3 [10].
36
2 Singlecomponent systems p / kPa
Tc at 647.6 K 22.1 MPa
100 kPa or 1 bar liquid solid H 2O
0.611 kPa
gas
273.15 273.16
373.15
T/K
Figure 2.7 The p,T phase diagram of H2O (the diagram is not drawn to scale).
system: pressure, temperature, composition and, if applicable, other variables such as electric or magnetic field strengths. In this chapter we are considering single component systems only. For a singlecomponent system the phase diagram displays the regions of pressure and temperature where the various phases of this component are stable. The lines separating the regions – the phase boundaries – define the p,T conditions at which two phases of the component coexist in equilibrium. Let us initially consider a singlecomponent phase diagram involving a solid, a liquid and a gaseous phase. The p,T phase diagram of H2O is given as an example in Figure 2.7. The transformations between the different phases are of first order. The liquid–vapour phase boundary shows how the vapour pressure of the liquid varies with temperature. Similarly, the solid–vapour phase boundary gives the temperature variation of the sublimation vapour pressure of the solid. The temperature at which the vapour pressure of a liquid is equal to the external pressure is called the boiling temperature at that pressure. The standard boiling temperature is the boiling temperature at 1 bar. Correspondingly, the standard melting temperature is the melting temperature at 1 bar. Boiling is not observed when a liquid is heated in a closed vessel. Instead, the vapour pressure increases continuously as temperature is raised. The density of the vapour phase increases while the density of the liquid decreases. At the temperature where the densities of the liquid and the vapour become equal, the interface between the liquid and the gas disappears and we have reached the critical temperature of the substance, Tc. This is visualized by using volume (or if preferred, density) as a third variable in a threedimensional (p,T,V) phase diagram – see Figure 2.8. The vapour pressure at the critical temperature is called the critical pressure. A single uniform phase, the supercritical fluid, exists above the critical temperature. For a singlecomponent system p and T can be varied independently when only one phase is present. When two phases are present in equilibrium, pressure and temperature are not independent variables. At a certain pressure there is only one temperature at which the two phases coexist, e.g. the standard melting temperature of water. Hence at a chosen pressure, the temperature is given implicitly. A point
2.1 Phases, phase transitions and phase diagrams
37
sol.–liq.
Pressure
Critical point liq.
sol.
Supercritical fluid liq.–gas gas
Vol um
sol.–gas e
ure
erat
p Tem
Figure 2.8 Threedimensional p,T,V representation of a single component phase diagram visualizing the critical point.
where three phases coexist in equilibrium is termed a triple point; three phases are in equilibrium at a given temperature and pressure. Ice, water and water vapour are in equilibrium at T = 273.16 K and p = 611 Pa. None of the intensive parameters can be changed. The observer cannot affect the triple point. The relationship between the number of degrees of freedom, F, defined as the number of intensive parameters that can be changed without changing the number phases in equilibrium, and the number of phases, Ph, and components, C, in the system is expressed through Gibbs phase rule: F = C – Ph + 2
(2.15)
In Chapter 4 the determination of the number of components in complex systems will be discussed in some detail. In this chapter we shall only consider singlecomponent systems. For a singlecomponent system, such as pure H2O, C = 1 and F = 3 – Ph. Thus, a single phase (Ph = 1) is represented by an area in the p,T diagram and the number of degrees of freedom F is 2. A line in the phase diagram represents a heterogeneous equilibrium between two coexisting phases (Ph = 2) and F = 1, while three phases (Ph = 3) in equilibrium are located at a point, F = 0. Fieldinduced phase transitions Various types of work in addition to pV work are frequently involved in experimental studies. Research on chemical equilibria for example may involve surfaces or phases at different electric or magnetic potentials [11]. We will here look briefly at fieldinduced transitions, a topic of considerable interest in materials science. Examples are stressinduced formation of piezoelectric phases, electric polarizationinduced formation of dielectrica and fieldinduced order–disorder transitions, such as for environmentally friendly magnetic refrigeration. Magnetic contributions to the Gibbs energy due to an internal magnetic field are present in all magnetically ordered materials. An additional energetic contribution
38
2 Singlecomponent systems
arises in a magnetic field with field strength or magnetic flux density B. This contribution is proportional to the magnetic moment, m, of the system and thus is B◊dm. An important additional complexity of external fields is that the field has a direction; the field can be applied parallel to any of the three principal axes of a single crystal. The magnetic moment and the magnetic field are thus vectors and represented by bold symbols. The fundamental equation for the internal energy for a system involving magnetic polarization is when the pV work is negligible (constant volume): dU = TdS + B◊dm
(2.16)
The corresponding equation for the Helmholtz energy is dA = –SdT + B◊dm
(2.17)
In order to focus on the driving force for phase transitions induced by a magnetic field it is advantageous to use the magnetic flux density as an intensive variable. This can be achieved through what is called a Legendre transform [12]. A transformed Helmholtz energy is defined as A ¢ = A – B◊m = 0
(2.18)
Taking the differential of A ¢ and substituting for dA in eq. (2.17): d A ¢ = dA – B◊dm – m◊dB = –SdT – m◊dB
(2.19)
Assuming an isotropic system, the following Maxwell relation can be derived from eq. (2.19), since d A ¢ is an exact differential: æ ¶m ö æ ¶S ö =ç ÷ ÷ ç è ¶B ø T ,V è ¶T ø B ,V
(2.20)
The entropy of a ferromagnetically ordered phase decreases with increasing magnetic field strength. The decrease is equal to the change in the magnetic moment with temperature and hence is large close to the order–disorder temperature. This implies that a larger change in the magnetic moment with temperature at constant field strength gives a higher entropy change connected with a field change at constant temperature. The effect of a magnetic field on the Helmholtz energy of a magnetic order–disorder transition thus clearly affects phase stability. The application of n additional thermodynamic potentials (of electric, magnetic or other origin) implies that the Gibbs phase rule must be rewritten to take these new potentials into account: F + Ph = C + 2 + n
(2.21)
2.2 The gas phase
39 40 MnP B  b
30
B(T)
para 20 fan 10 0 screw 0
ferro 100
200
300
T/K
Figure 2.9 The Bâ€“T phase diagram of MnP [13] with the magnetic field along the baxis. Three different magnetically ordered phases â€“ ferro, fan and screw â€“ are separated by firstorder phase transitions. The transitions to the disordered paramagnetic state are of second order and given by a dashed line.
The isobaric (1 bar) T,Bphase diagram of MnP with magnetic field parallel to the crystallographic baxis [13] is given in Figure 2.9. At isobaric conditions, where one degree of freedom is lost, the number of phases and the number of degrees of freedom are related by F + Ph = 3. Thus areas in the T,B diagram correspond to a single phase; a line corresponds to two phases in equilibrium; and three phases may exist in equilibrium at an invariant point, the triple point. It should be noted that the fact that a magnetic field can be applied parallel to any of the three principal axes of a single crystal implies that different phase diagrams will result in each case for a noncubic crystal.
2.2 The gas phase Ideal gases The thermodynamic properties of gases are given through equations of state (EoS) which in general may be given as p = f (T,V,n)
(2.22)
For an ideal gas the equation of state is known as the ideal gas law: p=
nRT V
(2.23)
where R is the gas constant and n is the number of moles of gas. The Gibbs energy of a gas at one pressure (pf) relative to that at another pressure (pi) is at constant temperature given through
40
2 Singlecomponent systems pf
G ( p f ) = G ( p i ) + ò V dp
(2.24)
pi
Using the ideal gas law the Gibbs energy expression becomes G ( pf ) = G ( pi ) + nRT
pf
æp ö dp = G ( pi ) + nRT lnçç f ÷÷ p è pi ø pi
ò
(2.25)
For any singlecomponent system such as a pure gas the molar Gibbs energy is identical to the chemical potential, and the chemical potential for an ideal gas is thus expressed as æ p ö ÷ = m o + RT ln p m( p) = m o ( p o ) + RT lnç ç po ÷ è ø
(2.26)
where the standard chemical potential (m o ) is the standard molar Gibbs energy of the pure ideal gas at the standard pressure 1 bar (p o ). The value of this standard molar Gibbs energy, m o (T ), found in data compilations, is obtained by integration from 0 K of the heat capacity determined by the translational, rotational, vibrational and electronic energy levels of the gas. These are determined experimentally by spectroscopic methods [14]. However, contrary to what we shall see for condensed phases, the effect of pressure often exceeds the effect of temperature. Hence for gases most attention is given to the equations of state. Real gases and the definition of fugacity Real gases do not obey the ideal gas law, but the ideal gas law is often a very good approximation. The largest deviation from ideal gas behaviour is observed at high pressures and low temperatures. Figure 2.10 displays schematically the pressure dependence of the chemical potential. For practical reasons, it is advantageous to have an expression for the chemical potential of the real gas, which resembles that used for perfect gases. In order to obtain a simple expression for the chemical potential we replace the ideal pressure in the expression for the chemical potential (eq. 2.26) with the effective pressure, the fugacity, f, and we have æ f ö ÷ = m o + RT ln f m( p) = m o ( p o ) + RT lnç ç po ÷ è ø
(2.27)
The standard state for a real gas is thus a hypothetical state in which the gas is at a pressure of po = 1 bar and behaving ideally.
2.2 The gas phase
41
m ideal gas
mo real gas
p
po
Figure 2.10 Schematic illustration of the pressure dependence of the chemical potential of a real gas showing deviations from ideal gas behaviour at high pressures. 1.04 N2(g) at 273.15 K Fugacity, f
1.02 1.00 0.98 0.96
0
1
2
3 ln(p/po)
4
5
6
Figure 2.11 Fugacity of N2(g) at 273.15 K as a function of pressure [15].
Most applications in materials science are carried out under pressures which do not greatly exceed 1 bar and the difference between f and p is small, as can be seen from the fugacity of N2(g) at 273.15 K [15] given in Figure 2.11. Hence, the fugacity is often set equal to the partial pressure of the gas, i.e. f » p. More accurate descriptions of the relationship between fugacity and pressure are needed in other cases and here equations of state of real, nonideal gases are used. Equations of state of real gases Purely phenomenological as well as physically based equations of state are used to represent real gases. The deviation from perfect gas behaviour is often small, and the perfect gas law is a natural choice for the first term in a serial expression of the properties of real gases. The most common representation is the virial equation of state: pV m = RT (1 + B¢ p + C ¢ p2 +… )
(2.28)
42
2 Singlecomponent systems
An alternative formulation is æ ö B C pV m = RT ç 1 + + + ... ÷ ç Vm V 2 ÷ m è ø
(2.29)
The coefficients B and C are the second and third virial coefficients, respectively, the first virial coefficient being 1. The compressibility factor of a gas is defined as Z=
pV m RT
(2.30)
For an ideal gas Z = 1. Departures from the value of unity indicate nonideal behaviour. Z < 1 can be related to dominating attractive forces, whereas Z > 1 relates to repulsive forces being dominant. The simplest physically based equation of state for real gases, the van der Waals equation, is based on two assumptions. As pressure is increased, the number of atoms per unit volume also increases and the volume available to the molecules in total is reduced, since the molecules themselves take up some space. The volume taken up by the molecules is assumed to be proportional to the number of molecules, n, and the volume occupied per atom, b. The equation of state is accordingly modified initially to p=
nRT V  nb
(2.31)
Secondly, since the frequency and force of the collisions with the walls of the container give the pressure, the change in these two factors with concentration must be taken into account. The attractive forces working between the molecules reduce both factors, the reduction being approximately proportional to the molar concentration (n/V). The pressure is hence reduced by a factor proportional to the square of this concentration and is then given as 2
p=
nRT ænö  aç ÷ V  nb èV ø
(2.32)
The equation can be written in a form resembling the ideal gas law (eq. 2.23): 2 é ænö ù ê p + aç ÷ ú (V  nb) = nRT è V ø úû êë
(2.33)
2.2 The gas phase
43
For 1 mol of gas, n = 1: æ a çç p + V2 è
ö ÷÷ (V  b) = RT ø
(2.34)
The constants a and b can be related to the pressure (pc) temperature (Tc) and volume (Vc) at the critical point by noting that at the critical point, by definition (see Section 5.2) æ ¶2 p æ ¶p ö ç ÷ =ç 2 è ¶V ø Tc çè ¶V
ö ÷ =0 ÷ ø Tc
(2.35)
The following three equations are obtained: RT c =
8a 27b
pc =
a 27b 2
V c = 3b
(2.36)
(2.37)
(2.38)
Hence there must be one relation involving pc, Tc and Vc which is independent of the parameters a and b. This relation defines the critical compressibility factor Zc: Zc =
pc V c ( a / 27b 2 )(3b) = =3/ 8 RT c (8a / 27b)
(2.39)
If p, T and V are measured in units of pc, Tc and Vc, the van der Waals equation becomes æ 3 çç p + V2 è
ö ÷÷ (3V  1) = 8T ø
(2.40)
where p = p/ pc , T = T / T c and V = V / V c . This is a remarkable equation because it does not explicitly contain any free parameter characteristic of the substance and illustrates the law of corresponding states. All real gases should, according to this equation, behave in the same manner. The van der Waals equation of state evidently represents an approximation only, and although it works reasonably well for gases composed of spherical molecules it fails in many other cases.
44
2 Singlecomponent systems
Even though the van der Waals equation is not as accurate for describing the properties of real gases as empirical models such as the virial equation, it has been and still is a fundamental and important model in statistical mechanics and chemical thermodynamics. In this book, the van der Waals equation of state will be used further to discuss the stability of fluid phases in Chapter 5.
2.3 Condensed phases For condensed phases (liquids and solids) the molar volume is much smaller than for gases and also varies much less with pressure. Consequently the effect of pressure on the chemical potential of a condensed phase is much smaller than for a gas and often negligible. This implies that while for gases more attention is given to the volumetric properties than to the variation of the standard chemical potential with temperature, the opposite is the case for condensed phases. Variation of the standard chemical potential with temperature The thermodynamic properties of singlecomponent condensed phases are traditionally given in tabulated form in large data monographs. Separate tables are given for each solid phase as well as for the liquid and for the gas. In recent years analytical representations have been increasingly used to ease the implementation of the data in computations. These polynomial representations typically describe the thermodynamic properties above room temperature (or 200 K) only. Polynomial expressions are conveniently used to represent a condensed phase which is stable in the whole temperature range of interest and which does not undergo any structural, electronic or magnetic transformations. The Gibbs energy of a compound is in the CALPHAD approach represented relative to the elements in their defined standard state at 298.15 K as a power series in terms of temperature in the form of [16]: o SER Gm (T )  H m = a + bT + cT ln(T ) +
i
책 dn T n
(2.41)
n =2
SER Here H m is the sum (in the stoichiometric ratio of the compound in question) of 298.15 o H m of the elements in their defined standard state. a, b, c and dn are coeffiD0 cients and n integers. This form of expression is useful for storing thermodynamic information in databases. A number of such expressions are often required for a given phase to cover the whole temperature range of interest. From eq. (2.41) all other thermodynamic functions can be derived, e.g. o Sm (T ) = b  c  c ln(T )  책 nd n T n
n 1
(2.42)
2.3 Condensed phases
45
Table 2.1 Thermodynamic properties of AlN at selected temperatures (data are taken from NISTJANAF tables [17]). Enthalpy reference temperature = T = 298.15 K; po = 1 bar. T K
JK
0 100 200 298.15 300 400 500 600 700 800 900 1000 2000
0. 5.678 19.332 30.097 30.254 36.692 40.799 43.538 45.434 46.791 47.792 48.550 51.290
o Sm
C p ,m 1
mol
1
JK
1
mol
1
0. 2.164 10.267 20.142 20.329 29.987 38.647 46.341 53.201 59.361 64.932 70.008 104.790
o DT298.15Hm
kJ mol –3.871 –3.711 –2.463 0. 0.056 3.428 7.317 11.541 15.994 20.608 25.339 30.158 80.490
o Hm (T ) = a  cT  å ( n  1)d n T
n
1
o D f Hm
kJ mol
1
–312.980 –314.756 –316.764 –317.984 –318.000 –318.594 –318.808 –318.811 –318.727 –318.648 –318.647 –329.363 –328.119
o D f Gm
kJ mol
log Kf
1
–312.980 –306.283 –296.990 –286.995 –286.803 –276.301 –265.697 –255.072 –244.455 –233.850 –223.252 –211.887 –94.810
INFINITE 159.986 77.566 50.280 49.937 36.081 27.757 22.206 18.241 15.269 12.957 11.068 2.476
(2.43)
n
C po ,m (T ) = c  å n( n  1) d n T
n 1
(2.44)
n
These thermodynamic functions implicitly given in analytical representations are given numerically at selected temperatures in monographs, as shown for AlN in Table 2.1 [17]. The analytical approach is exemplified by descriptions of three modifications of aluminium in Table 2.2 [18]. The stable facecentred cubic modification of crystalline aluminium (FCCAl) melts at 933.473 K. Hexagonal closepacked aluminium is unstable at all temperatures, as evident from the graphical representation of the Gibbs energy relatively to FCCAl in Figure 2.12. The thermodynamic properties may still be needed to describe alloys with hexagonal closedpacked structure where aluminium is a solute. Representation of transitions Thermodynamic representation of transitions often represents a challenge. Firstorder phase transitions are more easily handled numerically than secondorder transitions. The enthalpy and entropy of firstorder phase transitions can be calculated at any temperature using the heat capacity of the two phases and the enthalpy and entropy of transition at the equilibrium transition temperature. Small pretransitional contributions to the heat capacity, often observed experimentally, are most often not included in the polynomial representations since the contribution to the
46
2 Singlecomponent systems
Table 2.2 CALPHADtype representation of the thermodynamic properties of facecentred cubic (FCC), liquid and hexagonal closepacked (HCP) aluminium of the form (after Dinsdale [18]): o ( T )  H SER . K) = a + bT + cT ln( T ) + å d n T n Gm m ( 29815 n
.15 o with H SER . K) = D298 H m (FCC_ Al) = 4540 J mol–1. m ( 29815 0
FCC_Al (298.15 < T/K < 700) –7976.15 + 137.093038 T – 24.3671976T ln(T) – 1.884662E–3 T2 – 0.877664E–6 T3 + 74092 T–1 (700 < T/K < 933.473) –11276.24 + 223.048446 T – 38.5844296 T ln (T) + 18.531982E–3 T2 – 5.764227E–6 T3 + 74092 T–1 (933.473 < T/K < 2900) –11278.378 + 188.684153 T – 31.748192 T ln (T) – 1.231E28 T–9 Liquid relatively to FCC_Al (298.15 < T/K < 933.473) 11005.029 – 11.841867 T + 7.934E–20 T7 (933.473 < T/K < 2900) 10482.382 – 11.253974 T + 1.231E28 T–9
o o Gm  Gm (FCC_Al) / kJ mol 1
HCP_Al relative to FCC_Al (298.15 < T/K < 2900) 5481 – 1.8 T 10 5
HCP
0 FCC 5 10 –15
Al 500
liquid 1000
1500
2000
T/K o o Figure 2.12 G m Gm ( Al_ FCC) of hexagonal closedpacked (HCP) aluminium and aluminium melt relative to that of facecentred cubic aluminium [18].
Gibbs energy is small. This contribution is instead incorporated empirically in the enthalpy and entropy of transition. It is more difficult to describe secondorder transitions. Considerable shortrange order is in general present far above the transition temperature. Correspondingly,
2.3 Condensed phases
47
Fe0.99O Fe0.947 O Fe0.938 O Fe0.925 O
C p,m / J K 1 mol 1
150
100
50 160
200 T/K
240
Figure 2.13 Heat capacity of wüstite around the Néel temperature [19]. ¡: Fe0.99O; l: Fe0.947O; Ñ: Fe0.938O; +: Fe0.925O. Reproduced by permission of the Mineralogical Society of America.
considerable disordering has taken place already far below the disordering temperature. The magnetic order–disorder transition in nonstoichiometric wüstite, Fe1–yO, may serve as an example. The magnetic transition is largely dependent on the stoichiometry of the compound (see Figure 2.13), and is for the oxygenrich compositions spread over a considerable temperature range [19]. The disordering is far from abrupt. The Inden model [20] is frequently used to describe secondorder magnetic order–disorder transitions. Inden assumed that the heat capacity varied as a logarithmic function of temperature and used separate expressions above and below the magnetic order–disorder transition temperature (Ttrs) in order to treat the effects of both long and shortrange order. Thus for t = (T/Ttrs) < 1: C mag = K LR p
ln(1 + t 3 ) ln(1  t 3 )
(2.45)
For t > 1 C mag = K SR p
ln(1 + t 5 ) ln(1  t 5 )
(2.46)
The two coefficients KL and KS are derived empirically. They are related through the entropy of transition and constrained to reproduce the total enthalpy and entropy increments accompanying the phase transition. Since, the Inden model demands a series expansion in order to calculate the entropy, a simpler related equation by Hillert and Jarl [21] is used in many computer programs. Secondorder structural transitions are less frequently represented in applied thermodynamic calculations. Still, the Landau approach for determination of
48
2 Singlecomponent systems
Gibbs energy changes connected with secondorder transitions has a long tradition. The central concept of the Landau theory is the order parameter, G, which describes the course of the transition. The order parameter is related to the change in some macroscopic property like strain, average site occupancy or crystallographic distortion through the phase transition. The measured physical property is, however, not necessarily directly proportional to G, but most often scales as either G or G 2 . The relationship between the order parameter and the measured physical property is defined by the differences in symmetry between the high and lowtemperature polymorphs [22]. We will consider a phase transition between two crystal structures with different symmetry and where the space group of the lowsymmetry structure is a subgroup of the space group of the highsymmetry structure. Hence all symmetry elements of the highsymmetry structure are present in the lowsymmetry structure. An order parameter, G, is used to describe the thermodynamic state of the lowsymmetry phase. The contribution from the phase transition to the total Gibbs energy, here termed the transitional Gibbs energy DtrsG, is now given as a function of T, p and G as D trs G = D trs G (T , p, G )
(2.47)
G is scaled such that it is assigned the value 0 in the hightemperature modification and 1 in the lowtemperature form at 0 K. Thus, DtrsG = 0 for the hightemperature polymorph. The variation of the order parameter with temperature describes the transition thermodynamically. In general [23]: D trs G = aG +
1 1 1 bG 2 + cG 3 + dG 4 +… 2 3 4
(2.48)
Here a, b, c, d etc. are coefficients that in general are functions of temperature and pressure. The equilibrium behaviour of G through the phase transition is determined by minimizing DtrsG with respect to G. Furthermore, at equilibrium the DtrsG(G) surface is concave upwards (discussed thoroughly in Section 5.2), hence ¶D trs G = 0 and ¶G
¶ 2 D trs G ¶G 2
>0
(2.49)
These criteria can be used to get information on the coefficients of eq. (2.48). In the highsymmetry phase, stable above the transition temperature, the order parameter G = 0 and the equilibrium conditions imply that the two first constants in the polynomial expansion are restricted to a = 0 and b > 0. If we assume that b < 0, the lowsymmetry phase is stable since G 2 > 0 then implies that DtrsG < 0. The transitional Gibbs energy is thus reduced to
2.3 Condensed phases
D trs G =
49
1 1 1 bG 2 + cG 3 + dG 4 +… 2 3 4
(2.50)
The Landau theory predicts the symmetry conditions necessary for a transition to be thermodynamically of second order. The order parameter must in this case vary continuously from 0 to 1. The presence of oddorder coefficients in the expansion gives rise to two values of the transitional Gibbs energy that satisfy the equilibrium conditions. This is not consistent with a continuous change in G and thus corresponds to firstorder phase transitions. For this reason all oddorder coefficients must be zero. Furthermore, the sign of b must change from positive to negative at the transition temperature. It is customary to express the temperature dependence of b as a linear function of temperature: b = B(T  T trs )
(2.51)
Here B is a constant independent of temperature and pressure. The transitional Gibbs energy is thus D trs G =
1 1 1 B(T  T trs )G 2 + dG 4 + fG 6 +… 2 4 6
(2.52)
where d, f and higherorder coefficients all are assumed to be independent of temperature and pressure. Normally two or three terms of this expression give a satisfactory description of the transitional Gibbs energy using experimentally determined values for the temperature variation of the order parameter. When d > 0 the expansion describes a thermodynamic secondorder transition. The equilibrium condition neglecting higher order terms is ¶D trs G = B(T  T trs ) G + dG 3 = 0 ¶G
(2.53)
which gives G2 =
B (T  T trs ) for d
T < Ttrs
(2.54)
The form of the order parameter is given implicitly since by definition G =1 at 0 K and hence 1 B = d T trs and thus
(2.55)
50
2 Singlecomponent systems
éT  T ù G = ê trs ú ë T trs û
1/2
(2.56)
The transitional Gibbs energy is for T £ Ttrs D trs G = 
B2 B2 B2 (T  T trs )2 + (T  T trs )2 = (T  T trs )2 2d 4d 4d
(2.57)
The transitional entropy and heat capacity are readily derived by differentiation with respect to temperature. For T £ Ttrs D trs S =
C trs p =
B2 1 (T  T trs ) =  B × G 2 2d 2
B2 T 2d
(2.58)
(2.59)
The contribution of the transition to the thermodynamic functions can be evaluated once the coefficients B and d have been determined. Experimental determination of the transition temperature and one additional thermodynamic quantity at one specific temperature is sufficient to describe the transition thermodynamically using this model. It is easily shown that a firstorder phase transition is obtained for cases were d < 0, whereas behaviour at the borderline between first and secondorder transitions, tricritical behaviour, is obtained for d = 0. In the latter case the transitional Gibbs energy is D trs G =
1 1 B(T  T trs )G 2 + fG 6 +… 2 6
(2.60)
Minimization of the transitional Gibbs energy with respect to G gives éT  T ù G = ê trs ú ë T trs û
1/ 4
(2.61)
The variation of the order parameter with temperature thus distinguishes secondorder transitions from tricritical behaviour. In general the variation of the order parameter with temperature for a continuous transition is described as éT  T ù G = ê trs ú ë T trs û
b
(2.62)
2.3 Condensed phases
51
where b is the critical exponent. For our two ideal cases, secondorder and tricritical transitions, b = 1 (eq. 2.56) and 1 (eq. 2.61), respectively. 2 4 The transitional entropy, enthalpy and heat capacity for a tricritical transition is for T £ Ttrs: 1 D trs S =  B × G 2 2
(2.63)
1 1 D trs H =  B × T trs × G 2 + f × G 6 2 6
(2.64)
C trs p =
BT 4 T trs
(T trs  T ) 1/2
(2.65)
Orientational disordering of the carbonate groups in CaCO3 above 1260 K may serve as an example of application of Landau theory. Below the transition temperature, alternate layers of planar CO3 groups point in opposite directions. In the hightemperature modification they are free to rotate and become equivalent. The symmetry reduction on ordering is from space group R 3 m to R 3c with doubling of the caxis length. Thus the transition gives rise to superlattice reflections in the diffraction patterns of the lowtemperature phase. The intensities of these reflections are according to symmetry considerations proportional to G2. It has been shown by neutron diffraction that the order parameter is proportional to (T trs  T )1/ 4 and thus that the transition is tricritical [24]. Ttrs and the excess enthalpy determined by drop calorimetry characterize the transition thermodynamically [25]. The contribution from the transition to the total Gibbs energy and entropy (using B = 24 J mol–1 K–1 and f = 30 kJ mol–1) are given in Figure 2.14.
D trsG / kJ mol 1
–3 –3
CaCO3 –6
–6 –9
–9
300
600
900 1200 300
600
900 1200
D trs S / J K 1 mol 1
0
0
–12
T/K
Figure 2.14 The contribution from the order–disorder transition of CaCO3(s) to the total Gibbs energy and entropy [25].
52
2 Singlecomponent systems
Equations of state Equations of state of condensed materials are seldom used in materials science but are frequently used in geophysics and to an increasing degree also in solid state sciences for highpressure studies of phase transitions. A considerable amount of work on equations of state of minerals has been reported in the geophysical and geochemical literature. In the Earth’s mantle the pressure is several orders of magnitude higher than ambient since pressure and temperature increase with increasing depth within the Earth. Thus equation of state data is essential for thermodynamic calculations of phase equilibria in the Earth’s interior. Equations of state for solids are often cast in terms of the bulk modulus, KT, which is the inverse of the isothermal compressibility, kT, and thus defined as KT =
1 æ ¶p ö = V ç ÷ kT è ¶V ø T
(2.66)
The two most usual equations of state for representation of experimental data at high pressure are the Murnaghan and Birch–Murnaghan equations of state. Both models are based on finite strain theory, the Birch–Murnaghan or Eulerian strain [26]. The main assumption in finite strain theory is the formal relationship between compression and strain [27]: V = (1 + 2e ) 3/2 V0
(2.67)
The Murnaghan equation of state is given by p=
ù K T ,0 éæ V 0 ö K ¢T , 0 êç  1ú ÷ K ¢ T ,0 êè V ø úû ë
(2.68)
while what is termed the thirdorder Birch–Murnaghan equation of state is given by p=
ù éæ V ö2 / 3 ù éæ V ö 7/ 3 æ V ö 5/ 3 ù é 3 3  ç 0 ÷ ú × ê1  (4  K ¢ T ,0 ) × êç 0 ÷  1ú +…ú K T ,0 êç 0 ÷ 2 ú êëè V ø êëè V ø úû è V ø úû ê 4 û ë (2.69)
where K T ,0 and K ¢T ,0 are the isothermal bulk modulus and its pressure derivative at T = 298 K at zero pressure, respectively. The thirdorder Birch–Murnaghan EoS reduces to second order when K T¢ ,0 = 4 and
2.3 Condensed phases
53
1.00
Diamond: 588 GPa
0.95 Stishovite: 313 GPa SiO2
V / V0
0.90
MgSiO3: 107 GPa
0.85
Quartz: 39 GPa SiO2
0.80 0.75
0
10
20 30 p / GPa
40
50
Figure 2.15 Pressure–volume data for diamond, SiO2stishovite, MgSiO3 and SiO2quartz based on third order Birch–Murnaghan equation of state descriptions. The isothermal bulk modulus at 1 bar and 298 K are given in the figure.
p=
éæ V ö 7/ 3 æ V ö 5/ 3 ù 3 K T ,0 êç 0 ÷ ç 0 ÷ ú 2 êëè V ø è V ø úû
(2.70)
Volumetric data for four different substances represented by the thirdorder Birch–Murnaghan equation of state are shown in Figure 2.15. The equations discussed above are reliable for phases where the compressibility does not change too fast with pressure, more specifically for 3.4 < K ¢T ,0 < 7. The equations are thus suitable for a large range of crystalline substances but not for liquids or lowdimensional materials, where K ¢T ,0 is often larger than 7. In the latter cases the universal Vinet equation of state seems more appropriate [28]. The effect of temperature on the equation of state is introduced through the isobaric thermal expansivity. It is generally assumed that isobaric expansivity and isobaric compressibility work independently of each order and the volume as a function of T and p is then expressed as o V ( p, T ) = V298 f ( p)f (T )
(2.71)
Finally, it should be noted that the effect of the compressibility on the thermodymanics of solids is small even at relatively high pressures. The molar volume of magnetite, Fe3O4, at 1000 K is 46.0 cm3 mol–1 and VDp at p = 1 GPa is 46 kJ mol–1 if the compressibility of the compound is neglected. Taking compressibility into account reduces this contribution to 45.88 kJ mol–1 [29].
54
2 Singlecomponent systems
References [1] [2] [3] [4] [5] [6] [7] [8]
[9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29]
F. Grønvold and S. Stølen, Thermochim. Acta. 1995, 266, 213. F. Grønvold, Pure Appl. Chem. 1993, 65, 927. A. F. Wright and M. S. Lehmann, J. Solid State Chem. 1981, 36, 371. M. A. Carpenter, E. K. H. Salje, A. GraemeBarber, B. Wruck, M. T. Dove and K. S. Knight, Am. Mineral. 1998, 83, 2. F. Grønvold, S. Stølen and S. R. Svendsen, Thermochim. Acta. 1989, 139, 225. Supplementary Information for the International Temperature Scale of 1990. Bureau International des Poids et Mesures: Paris. 1990. C. N. R. Rao and J. Gopalakrishnan New Directions in Solid State Chemistry, 2nd edn. Cambridge: Cambridge University Press, 1997. See e.g. Silica: physical behaviour, geochemistry and materials applications (P. J. Heaney, C. T. Prewitt and G. V. Gibbs, eds), Reviews in Mineralogy, vol. 29, Mineralogical Society of America, 1994. T. Okamoto, H. Fujii, Y. Hidaka and E. Tatsumoto, J. Phys. Soc. Japan 1967, 23, 1174. Ulyanov, A. N., Maksimov, I. S., Nyeanchi, E. B., Medvedev, Yu. V., Yu, S. C., Starostyuk, N. Yu. and Sundquist, B. J. Appl. Phys. 2002, 91, 7739. K. S. Pitzer, Thermodynamics. New York: McGrawHill, 1995. R. A. Alberty, J. Chem. Thermodyn. 2002, 34, 1787. C. C. Becerra, Y. Shapira, N. F. Oliveira Jr. and T. S. Chang, Phys. Rev. Lett. 1980, 44, 1692. J. E. Meyer and M. G. Meyer, Statistical Mechanics, 2nd edn. New York: Wiley, 1977. J. Otto, A. Michels and H. Wouters, Physik. Z. 1934, 35, 97. N. Saunders and A. P. Miodownik, CALPHAD: Calculation of Phase Diagrams: a Comprehensive Guide. Oxford: Pergamon, Elsevier Science, 1998. NISTJANAF Thermochemical Tables, 4th edn (M. W. Chase Jr, ed.) J. Phys. Chem. Ref. Data Monograph No. 9, 1998. A. T. Dinsdale, CALPHAD 1991, 15, 317. S. Stølen, R. Glöckner, F. Grønvold, T. Atake and S. Izumisawa, Am. Mineral. 1996, 81, 973. G. Inden, Proceedings of the Fifth conference on Calculation of Phase Diagrams, CALPHAD V (Dusseldorf) III(4)1. M. Hillert and M. Jarl, CALPHAD 1978, 2, 227. E. K. H. Salje, Phase Transitions in Ferroelastic and Coelastic Crystals. Cambridge: Cambridge University Press, 1990. A. Putnis, Introduction to Mineral Sciences. Cambridge: Cambridge University Press, 1992. M. T. Dove and B. M. Powell, Phys. Chem. Mineral. 1989, 16, 503. S. A. T. Redfern, E. Salje and A. Navrotsky, Contrib. Mineral. Petrol. 1989, 101, 479. F. Birch, J. Geophys. Res. 1952, 57, 227. F. D. Stacey, B. J. Brennan and R. D. Irvine, Geophys. Surv. 1981, 4, 189. P. Vinet, J. H. Rose, J. Ferrante and J. R. Smith, J. Phys. Condens. Matter 1989, 1, 1941. S. K. Saxena, N. Chatterjee, Y. Fei and G. Shen, Thermodynamic Data on Oxides and Silicates. Berlin: SpringerVerlag, 1993.
2.3 Condensed phases
55
Further reading O. L. Anderson, Equations of State of Solids for Geophysics and Ceramic Science. Oxford: Oxford University Press, 1995. P. W. Atkins and J. de Paula, Physical Chemistry, 7th edn. Oxford: Oxford University Press, 2001. J. W. Gibbs, The Collected Work, Volume I Thermodynamics. Harvard: Yale University Press, 1948. L. D. Landau and E. M. Lifshitz, Statistical Physics. London: Pergamon Press, 1958. K. S. Pitzer, Thermodynamics. New York: McGrawHill, 1995. (Based on G. N. Lewis and M. Randall, Thermodynamics and the free energy of chemical substances. New York: McGrawHill, 1923. E. K. H. Salje Phase Transitions in Ferroelastic and Coelastic Crystals. Cambridge: Cambridge University Press, 1990.
3
Solution thermodynamics
So far we have discussed the thermodynamic properties of materials, which have been considered as pure and to consist of only a single component. We will now continue with systems containing two or more components and thereby solutions. Solutions are thermodynamic phases with variable composition, and are common in chemical processes, in materials and in daily life. Alloys – solutions of metallic elements – have played a key role in the development of human civilisation from the Bronze Age until today. Many new advanced materials are also solutions. Examples are tetragonal or cubic ZrO2, stabilized by CaO or Y2O3, with high toughness or high ionic conductivity, and piezoelectric and dielectric materials based on BaTiO3 or PbZrO3. In all these cases the mechanical or functional properties are tailored by controlling the chemical composition of the solid solution. The chemical and thermal stability of these complex materials can only be understood if we know their thermodynamic properties. The understanding of how the chemical potential of a component is changed by mixing with other components in a solution is an old and fascinating problem. The aim of this chapter is to introduce the formalism of solution thermodynamics. Models in which the solution is described in terms of the end members of the solution, solution models, are given special attention. While the properties of the end members must be described following the methods outlined in the previous chapter, the present chapter is devoted to the changes that occur on formation of the solutions. In principle one could describe the Gibbs energy of a mixture without knowing the properties of the end members, but since it is often of interest to apply a solution model in thermodynamic calculations involving other phases, the solution model often is combined with descriptions of the Gibbs energies of the end members to give a complete thermodynamic description of the system.
Chemical Thermodynamics of Materials by Svein Stølen and Tor Grande © 2004 John Wiley & Sons, Ltd ISBN 0 471 492320 2 57
58
3 Solution thermodynamics
3.1 Fundamental definitions Measures of composition The most important characteristic of a solution is its composition, i.e. the concentration of the different components of the phase. The composition of a solution is best expressed by the ratio of the number of moles of each component to the total number of moles. This measure of the composition is the mole fraction of a component. In the case of a binary solution consisting of the components A and B, the mole fractions of the two components are defined as xA =
nA nA + nB
and
xB =
nB nA + nB
(3.1)
and it is evident that x A + x B =1
(3.2)
For an infinitesimal change in composition of a binary solution the differentials of the two mole fractions are related as dx A = dx B
(3.3)
In dealing with dilute solutions it is convenient to speak of the component present in the largest amount as the solvent, while the diluted component is called the solute. While the mole fraction is a natural measure of composition for solutions of metallic elements or alloys, the mole fraction of each molecule is chosen as the measure of composition in the case of solid or liquid mixtures of molecules.1 In ionic solutions cations and anions are not randomly mixed but occupy different sublattices. The mole fractions of the atoms are thus an inconvenient measure of composition for ionic substances. Since cations are mixed with cations and anions are mixed with anions, it is convenient for such materials to define composition in terms of ionic fractions rather than mole fractions. In a mixture of the salts AB and AC, where A is a cation and B and C are anions, the ionic fractions of B and C are defined through XB =
nB =1  XC nB + nC
(3.4)
1 Note that volume fraction rather than mole fraction is recommended in mixtures of molecules with significant different molecular mass. This will be discussed in Chapter 9.
3.1 Fundamental definitions
59
In a binary solution AB–AC, the ionic fractions of B and C are identical to the mole fractions of AB and AC. It may therefore seem unnecessary to use the ionic fractions. However, in the case of multicomponent systems the advantage of ionic fractions is evident, as will be shown in Chapter 9. Mixtures of gases The simplest solution one can imagine is a mixture of ideal gases. Let us simplify the case by assuming only two types of ideal gas molecules, A and B, in the mixture. The total pressure in this case is the sum of the partial pressures of the two components (this is termed Dalton’s law). Thus, ptot = pA + pB
(3.5)
where pA and pB are the partial pressures of the two gases and ptot is the total pressure. By applying the ideal gas law (eq. 2.23), the volume of the gas mixture is V tot = n A V m,A + n BV m,B
(3.6)
where nA and nB are the number of moles of A and B in the mixture and Vm,A and Vm,B are the molar volumes of pure A(g) and B(g). In this case, where both A and B are ideal gases, Vm,A = Vm,B. It follows that, for a mixture of ideal gases pA = x A ptot
(3.7)
The chemical potential of an ideal gas A is given by eq. (2.26) as æp o + RT lnç A m A ( pA ) = m A ç po è A
ö ÷ = m o + RT ln p A A ÷ ø
(3.8)
o o where m A is the standard chemical potential of the pure ideal gas A at pA = 1 bar at a given temperature T. For a mixture of the ideal gases A and B at constant pressure o (ptot = pA =1 bar) the chemical potential of A for a given composition of the solution, xA, is, by using eq. (3.7)
æx p o + RT lnç A tot mA (xA ) = mA ç po A è
ö ÷ = m o + RT ln x A A ÷ ø
(3.9)
The difference between the chemical potential of a pure and diluted ideal gas is simply given in terms of the logarithm of the mole fraction of the gas component. As we will see in the following sections this relationship between the chemical potential and composition is also valid for ideal solid and liquid solutions.
60
3 Solution thermodynamics
In mixtures of real gases the ideal gas law does not hold. The chemical potential of A of a mixture of real gases is defined in terms of the fugacity of the gas, ƒA. The fugacity is, as discussed in Chapter 2, the thermodynamic term used to relate the chemical potential of the real gas to that of the (hypothetical) standard state of the gas at 1 bar where the gas is ideal: æ f o + RT lnç A mA (xA ) = mA ç po è A
ö ÷ = m o + RT ln( f ) A A ÷ ø
(3.10)
Solid and liquid solutions – the definition of activity In the solid or liquid state the activity, a, is introduced to express the chemical potential of the components of a solution. It is defined by m A = m *A + RT ln a A
(3.11)
o . where m *A is the chemical potential of A in the reference state. For p = 1 bar m *A = m A One of the most important tasks of solution thermodynamics is the choice of an appropriate reference state, and this is the topic of one of the following sections.
3.2 Thermodynamics of solutions Definition of mixing properties The volume of an ideal gas mixture is given by eq. (3.6). Let us now consider only solid or liquid mixtures. Our starting point is an arbitrary mixture of nA mole of pure A and nB mole of pure B. The mixing process is illustrated in Figure 3.1. We p, T constant nA Vm,A
nB Vm,B
mixing
nAVA + nBVB
Figure 3.1 Mixing of nA moles of A and nB moles of B at constant p and T. The molar volumes of pure A and B are VA and VB. The partial molar volumes of A and B in the solution are VA and VB, respectively.
3.2 Thermodynamics of solutions
61
will first derive the expressions for the volume of the system before and after the mixing. The volume before mixing is V ( before) = n A V m,A + n BV m,B
(3.12)
where V m,A and V m,B are the molar volumes of pure A and B. We now mix A and B at constant pressure p and temperature T and form the solution as illustrated in Figure 3.1. The expression for the volume of the solution is then V (after) = n A V A + n BV B
(3.13)
where V A and V B represent the partial molar volumes of A and B (defined by eq. 1.87) in the solution. These partial molar volumes may be seen as apparent volumes that when weighted with the number of A and B atoms give the observed total volume of the solution. The difference in the volume of the solution before and after mixing, the volume of mixing, is designated D mixV : D mixV = V (after)  V (before) = n A (V A  V A ) + n B (V B  V B )
(3.14)
The volume of mixing for one mole of solution is termed the molar volume of mixing, D mixV m , and is derived by dividing eq. (3.14) by the total number of moles (n A + n B ) in the system D mixV m =
D mixV = x A D mixV A + x B D mixV B (n A + n B )
(3.15)
The molar volume of mixing of two binary systems is shown in Figure 3.2. Pb–Sn shows positive deviation from the ideal behaviour at 1040 K [1] while the volume of mixing of Pb–Sb at 907 K is negative, with a minimum at xPb ¹ 0.5 and asymmetric with respect to the composition [2].
D mixVm / 106 m 3 mol 1
0.04 Pb–Sn
0.00 –0.04 –0.08 –0.12
Pb–Sb –0.16 0.0
0.2
0.4
0.6
0.8
1.0
xPb
Figure 3.2 Molar volume of mixing of molten Pb–Sn at 1040 K [1] and Pb–Sb at 907 K [2] as a function of composition.
62
3 Solution thermodynamics
The phenomenology described above can be applied to any thermodynamic extensive function, Y i , for a solution. The integral molar enthalpy, entropy and Gibbs energy of mixing are thus D mix H m = x A D mix H A + x B D mix H B
(3.16)
D mix S m = x A D mix S A + x B D mix S B
(3.17)
D mixG m = x A D mixG A + x B D mix G B
(3.18)
The three functions are interrelated by D mixG m = D mix H m  TD mix S m
(3.19)
o Since D mixG A = m A  m A , the integral molar Gibbs energy of mixing can alternatively be expressed in terms of the chemical potentials as o ) + x B ( m B  m Bo ) = RT ( x A ln a A + x B ln a B ) D mixG m = x A ( m A  m A
(3.20) o where m A and m Bo are the chemical potentials of pure A and B, whereas m A and m B are the chemical potentials of A and B in the given solution. Using G = H – TS, the partial molar Gibbs energy of mixing is given as o D mixG A = D mix H A  TD mix S A = m A  m A = RT ln a A
(3.21)
The partial molar entropy, enthalpy or volume of mixing can be derived from eq. (3.21) and are given by the relations æ ¶D G D mix S A =  çç mix A ¶T è
ö æ ¶ ln a A ö ÷÷ = R ln a A  RT ç ÷ è ¶T ø p øp
æ ¶ ln a A D mix H A = Rçç è ¶(1/ T )
ö ÷÷ øp
æ ¶D G D mixV A = çç mix A ¶p è
ö æ ¶ ln a A ÷÷ = RT çç è ¶p øT
(3.22)
(3.23)
ö ÷÷ øT
(3.24)
Corresponding equations can be derived for the partial molar properties of B.
3.2 Thermodynamics of solutions
63
Ideal solutions In Section 3.1 we showed that the chemical potential of an ideal gas in a mixture with other ideal gases is simply given in terms of a logarithmic function of the mole fraction. By comparing eqs. (3.9) and (3.10) we see that the fugacity/activity of the ideal gas is equal to the mole fraction. A solution (gas, liquid or solid) is in general called ideal if there are no extra interactions between the different species in addition to those present in the pure components. Thermodynamically this implies that the chemical activity is equal to the mole fraction, a i = x i , over the entire composition range. The molar Gibbs energy of mixing for an ideal solution then becomes D idmixG m = RT ( x A ln x A + x B ln x B )
(3.25)
The Gibbs energy of mixing of an ideal solution is negative due to the positive entropy of mixing obtained by differentiation of D idmixG m with respect to temperature: æ ¶D id G m D idmix S m =  ç mix ç ¶T è
ö ÷ = R( x ln x + x ln x ) A A B B ÷ øp
(3.26)
In the absence of additional chemical interactions between the different species that are mixed the solution is stabilized entropically; the solution is more disordered than a mechanical mixture of the components. The origin of the entropy contribution is most easily understood by considering the distribution of two species on a crystalline lattice where the number of lattice sites is equal to the sum of the number of the two species A and B. For an ideal solution, a specific number of A and B atoms can be distributed randomly at the available sites, i.e. in a large number of different ways. This gives rise to a large number of different structural configurations with the same enthalpy and thus to the configurational entropy given by eq. (3.26). This will be discussed further in Chapter 9. Two other characteristic properties of ideal solutions are D idmix H m = D idmixG m + TD idmix S m = 0 æ ¶D id G m D idmixV m = ç mix ç ¶p è
ö ÷ =0 ÷ øT
(3.27)
(3.28)
Or in words: in the absence of additional chemical interactions between the two types of atom, the enthalpy and volume of mixing are both zero. The partial molar properties of a component i of an ideal solution are readily obtained:
64
3 Solution thermodynamics
æ ¶D id G m D idmixG i = ç mix ç ¶n i è
ö ÷ = RT ln x i ÷ ø p ,T ,n j ¹ i
æ ¶D id S m D idmix S i = ç mix ç ¶n i è
ö æ ¶D id G i ÷ =  ç mix ÷ ç ¶T ø p ,T ,n j ¹ i è
(3.29)
ö ÷ = R ln x i ÷ ø p ,n j ¹ i
(3.30)
The thermodynamic properties of an ideal binary solution at 1000 K are shown in Figure 3.3. The integral enthalpy, entropy and Gibbs energy are given in Figure 3.3(a), while the integral entropy of mixing and the partial entropy of mixing of component A are given in Figure 3.3(b). Corresponding Gibbs energies are given in Figure 3.3(c). The largest entropic stabilization corresponds to the minimum Gibbs energy of mixing, which for an ideal solution is RT ln( 1 ) or –RT ln 2, or 2 about 0.7 times the thermal energy (RT) at 1000 K. Excess functions and deviation from ideality Most real solutions cannot be described in the ideal solution approximation and it is convenient to describe the behaviour of real systems in terms of deviations from the ideal behaviour. Molar excess functions are defined as D exc Y = D mix Y m  D idmixY m mix m
(3.31)
The excess molar Gibbs energy of mixing is thus D exc G = D mix G m  RT ( x A ln x A + x B ln x B ) mix m
(3.32)
= RT ( x A ln a A + x B ln a B )  RT ( x A ln x A + x B ln x B ) The activity coefficient of component i, g i , is now defined as a measure of the deviation from the ideal solution behaviour as the ratio between the chemical activity and the mole fraction of i in a solution. gi =
ai xi
or
ai = g i xi
(3.33)
For an ideal solution g i =1. The partial molar Gibbs energy of mixing of a component i in a nonideal mixture can in general be expressed in terms of activity coefficients as D mixG i = RT ln a i = RT ln x i + RT ln g i
(3.34)
3.2 Thermodynamics of solutions
65
SBo
Hm
o mA
H Bo m Bo
J K 1 mol 1
(a)
kJ mol 1
Sm o SA o HA
Gm 0.0
0.2
0.4
0.6
0.8
1.0
xB 20 –R ln xA
(b)
J K 1 mol 1
15 10 Dmix Sm 5 0 0.0
0.2
0.4
0.6
0.8
1.0
xB 0
(c)
kJ mol 1
–5 DmixGm –10 –15 –20 0.0
RT ln xA 0.2
0.4
xB
0.6
0.8
1.0
Figure 3.3 Thermodynamic properties of an arbitrary ideal solution A–B at 1000 K. (a) The Gibbs energy, enthalpy and entropy. (b) The entropy of mixing and the partial entropy of mixing of component A. (c) The Gibbs energy of mixing and the partial Gibbs energy of mixing of component A.
Using eq. (3.34) the excess Gibbs energy of mixing is given in terms of the mole fractions and the activity coefficients as G D mixG m = RT ( x A ln a A + x B ln a B ) = D idmixG m + D exc mix m = RT ( x A ln x A + x B ln x B ) + RT ( x A ln g A + x B ln g B )
(3.35)
66
3 Solution thermodynamics
Implicitly: D exc G = RT ( x A ln g A + x B ln g B ) mix m
(3.36)
Since D idmix H m = D idmixV m = 0 (eqs. 3.27 and 3.28), the excess molar enthalpy and volume of mixing are simply D exc V = D mix V m mix m
(3.37)
D exc H = D mix H m mix m
(3.38)
The excess molar entropy of mixing is the real entropy of mixing minus the ideal entropy of mixing. Using a binary A–B solution as an example, D exc S is mix m D exc S = D mix S m  R( x A ln x A + x B ln x B ) mix m
(3.39)
For a large number of the more commonly used microscopic solution models it is assumed, as we will see in Chapter 9, that the entropy of mixing is ideal. The different atoms are assumed to be randomly distributed in the solution. This means that the excess Gibbs energy is most often assumed to be purely enthalpic in nature. However, in systems with large interactions, the excess entropy may be large and negative. As shown above, the activity coefficients express the departure from ideality and thus define the excess Gibbs energy of the solution. Deviation from ideality is said to be positive when g >1(ln g is positive) and negative when g < 1(ln g is negative). A negative deviation implies a negative contribution to the Gibbs energy relatively to an ideal solution and hence a stabilization of the solution relative to ideal solution behaviour. Similar arguments imply that positive deviations from ideality result in destabilization relative to ideal solution behaviour. The activities of Fe and Ni in the binary system Fe–Ni [3] and the corresponding Gibbs energy and excess Gibbs energy of mixing are shown in Figures 3.4 and 3.5, respectively. The Fe–Ni system shows negative deviation from ideality and is thus stabilized relative to an ideal solution. This is reflected in the negative excess Gibbs energy of mixing. The activity coefficients g i , defined by eq. (3.33) as a i / x i , are readily determined from Figure 3.4. g Ni for the selected composition xNi = 0.4 is given by the ratio MQ/PQ. At the point of infinite dilution, xi = 0, the activity coefficient takes the value g i¥ . g i¥ is termed the activity coefficient at infinite dilution and is, as will be discussed in Chapter 4, an important thermodynamic characteristic of a solution. The activity coefficient of a given solute at infinite dilution will generally depend on the nature of the solvent, since the solute atoms at infinite dilution are surrounded on average by solvent atoms only. This determines the properties of the solute in the solution and thus g i¥ .
3.3 Standard states
67 1.0
a
aNi
aFe
0.8
• g Ni
0.6 • g Fe 0.4
P M
0.2 0.0 0.0
Q 0.4
0.2
xNi
0.6
0.8
1.0
Figure 3.4 The activity of Fe and Ni of molten Fe–Ni at 1850 K [3]. At xNi = 0.4 the activity coefficient of Ni is given by MQ/PQ.
D mixGm / kJ mol
1
0 –3
exc
D mixGm –6 –9 D mixGm
–12 –15 0.0
0.2
0.4
0.6
xNi
0.8
1.0
Figure 3.5 The molar Gibbs energy of mixing and the molar excess Gibbs energy of mixing of molten Fe–Ni at 1850 K. Data are taken from reference [3].
The formalism shown above is in general easily extended to multicomponent systems. All thermodynamic mixing properties may be derived from the integral Gibbs energy of mixing, which in general is expressed as G = RT å x i ln a i D mixG m = D idmixG m + D exc mix m i
= RT å x i ln x i + RT å x i ln g i i
(3.40)
i
3.3 Standard states In solution thermodynamics the standard or reference states of the components of the solution are important. Although the standard state in principle can be chosen freely, the standard state is in practice not taken by chance, but does in most cases reflect the type of model one wants to fit to experimental data. The choice of
68
3 Solution thermodynamics
standard state is naturally influenced by the data available. In some cases the vapour pressure of one of the components is known in the whole compositional interval. In other cases the activity of the solute is known for dilute solutions only. In the following, the Raoultian and Henrian standard states will be presented. These two are the far most frequent standard states applied in solution thermodynamics. Before discussing these standard states we need to consider Raoult’s and Henry’s laws, on which the Raoultian and Henrian standard states are based, in some detail. Henry’s and Raoult’s laws In the development of physical chemistry, investigations of dilute solutions have been very important. A dilute solution consists of the main constituent, the solvent, and one or more solutes, which are the diluted species. As early as in 1803 William Henry showed empirically that the vapour pressure of a solute i is proportional to the concentration of solute i: pi = x i k H,i
(3.41)
where xi is the mole fraction solute and k H,i is known as the Henry’s law constant. Here we have used mole fraction as the measure of the concentration (alternatively the mass fraction or other measures may be used). More than 80 years later François Raoult demonstrated that at low concentrations of a solute, the vapour pressure of the solvent is simply pi = x i p*i
(3.42)
where xi is the mole fraction solvent and p*i is the vapour pressure of the pure solvent. Raoult’s and Henry’s laws are often termed ‘limiting laws’. This use reflects that real solutions often follow these laws at infinite dilution only. The vapour pressure above molten Ge–Si at 1723 K [4] is shown in Figure 3.6 as an example. It is evident that at dilute solution of Ge or Si, the vapour pressure of the dominant component follows Raoult’s law. Raoult’s law is expressing that a real nonideal solution approaches an ideal solution when the concentration of the solvent approaches unity. In the corresponding concentration region Henry’s law is valid for the solute. The Ge–Si system shows positive deviation from ideality and the activity coefficients of the two components, given as a function of xi in Figure 3.6(b), are thus positive for all compositions (using Si and Ge as standard states). Raoult’s law is obeyed for a solvent at infinite dilution of a solute. Mathematically this implies ( da A /dx A ) xA ®1 = 1
(3.43)
3.3 Standard states
69
(a) 1.6
• g Ge
• g Si
Henry’s law
p /po
1.2 Ge
0.8
Si
0.4 Raoult’s law 0.0 0.0 (b)
1.6
0.2
0.4
xSi
0.6
0.8
1.0
• g Ge
• g Si
1.5 g
1.4
g Si
g Ge
1.3 1.2 1.1 1.0 0.0
0.2
0.4
0.6
0.8
1.0
xSi
Figure 3.6 (a) The vapour pressure above molten Si–Ge at 1723 K [4]. (b) The corresponding activity coefficients of the two components.
In terms of activity coefficients eq. (3.43) can be transformed to æ d( x A g A ) ö dg A æ çç ÷÷ = çç g A + x A dx A è dx A ø xA ®1 è
ö ÷÷ =1 ø xA ®1
(3.44)
Since g A ®1 when x A ®1 the expression for Raoult’s law becomes æ dg A çç è dx A
ö ÷÷ =0 ø xA ®1
(3.45)
This is a necessary and sufficient condition for Raoult’s law. A solute B obeys Henry’s law at infinite dilution if the slope of the activity curve a B versus x B has a nonzero finite value when x B ® 0: ( da B /dx B ) xB ®0 = g B¥
(3.46)
70
3 Solution thermodynamics
The finite value of the slope when x B ® 0, g B¥ , is the activity coefficient at infinite dilution defined earlier. In terms of activity coefficients eq. (3.46) becomes æ d( x B g B ) ö dg æ çç ÷÷ = çç g B + x B B dx B è dx B ø xB ®0 è
ö ÷÷ = g B¥ ø xB ®0
(3.47)
It follows that if Henry’s law behaviour is obeyed at infinite dilution: æ dg çç x B B dx B è
ö ÷÷ =0 ø xB ®0
(3.48)
Equation (3.48) is a necessary consequence of Henry’s law, but it is not a sufficient condition. It can be shown that Raoult’s law behaviour of the solvent follows as a consequence of Henry’s law behaviour for the solute, while the reverse does not follow. Raoultian and Henrian standard states The Raoultian standard state is the most frequently used standard state for a component in a solution. The Raoultian standard state implies that all thermodynamic properties are described relative to those of the pure component with the same structure as the solution. For liquids the specification of the structure seems artificial, but for solid solutions, which may have different crystal structures, this is of great importance. The activity of Ni in molten Fe–Ni at 1850 K using the Raoultian standard state is given in Figure 3.7 (ordinate given on the lefthand yaxis). The activity of pure Ni is set as standard state and is thus unity. While the Raoultian standard state represents a real physical reachable state, the Henrian standard state is a hypothetical one. The Henrian standard state for Ni in the Fe–Ni solution is found by extrapolation of the Henrian law behaviour at x Ni ®0 to x Ni =1; see Figure 1.0 0.8 1.0 0.6
H aNi
R a Ni
0.4
0.5
0.2 0.0 0.0
0.2
0.4
xNi
0.6
0.8
0.0 1.0
Figure 3.7 The activity of Ni of molten Fe–Ni at 1850 K using both a Raoultian and a Henrian standard state. Data are taken from reference [3].
3.3 Standard states
71
3.7. The activity of Ni in molten Fe–Ni at 1850 K using the Henrian standard state is also given in the figure (ordinate given on the righthand yaxis). If an arbitrary standard state is marked with *, a formal definition of a Raoultian standard state for component A of a solution is R m *A = m A
(3.49)
It follows that the activity coefficient with this standard state:
g
R A
=
R aA
xA
(3.50)
approaches 1 when the mole fraction x A approaches 1 or ( g RA ) xA ®1 = 1
(3.51)
Correspondingly, a formal definition of a Henrian standard state for component B of a solution is m *B = m BH
(3.52)
The activity coefficient with this standard state: g BH =
a BH xB
(3.53)
approaches 1 when x B approaches 0 or ( g BH ) xB ®0 = 1
(3.54)
The activities on the two standard states are related since m i = m iR + RT ln a iR = m iH + RT ln a iH
(3.55)
which gives a iR a iH
é (m R  m H ) ù i ú = expê i RT ê ú ë û
(3.56)
72
3 Solution thermodynamics
The ratio of two activities defined on the basis of two different standard states is constant and does not vary with the composition of the solution: a BR a BH
=
g BR x B g BR = g BH x B g BH
(3.57)
For the present case this constant can be deduced by using the conditions at infinite dilution as a constraint, thus: g BR g BH
ægR =ç B çgH è B
g BH =
ö g R ,¥ ÷ = B ÷ 1 ø xB ®0
(3.58)
g BR
(3.59)
g BR ,¥
Whereas the total Gibbs energy of the solution is independent of the choice of the standard state, the standard state must be explicitly given when it comes to the mixing properties of a solution. The molar Gibbs energy of mixing of the Fe–Ni system for which the activity of Ni is shown in Figure 3.7 is given in Figure 3.8. The solid and dashed lines represent Gibbs energies of mixing based on the Raoultian and Henrian standard states for Ni, respectively.
0
D mixGm / kJ mol 1
–4 R –mH m Ni Ni
–8 DmixG m
–12
H
D mixGm
–16 0.0
0.2
0.4
0.6
0.8
1.0
x Ni
Figure 3.8 The molar Gibbs energy of mixing of molten Fe–Ni at 1850 K using both the Raoultian (solid line) and Henrian (dashed line) standard states for Ni as defined in Figure 3.7. The Raoultian standard state is used for Fe. Data are taken from reference [3].
3.4 Analytical solution models
73
3.4 Analytical solution models Dilute solutions Binary solutions have been extensively studied in the last century and a whole range of different analytical models for the molar Gibbs energy of mixing have evolved in the literature. Some of these expressions are based on statistical mechanics, as we will show in Chapter 9. However, in situations where the intention is to find mathematical expressions that are easy to handle, that reproduce experimental data and that are easily incorporated in computations, polynomial expressions obviously have an advantage. Simple polynomial expressions constitute the most common analytical model for partial or integral thermodynamic properties of solutions: Y ( x B ) = Q 0 + Q1 x B + Q2 x 2B +… + Q n x Bn =
n
å Q i x Bi
(3.60)
i=0
or n
n
i=0
i=0
Y ( x B ) = x A x B å R i ( x A  x B ) i = x B (1  x B ) å R i (1  2 x B ) i
(3.61)
The variable x is usually the mole fraction of the components. The last expression was first introduced by Guggenheim [5]. Equation (3.60) is a particular case of the considerably more general Taylor series representation of Y as shown by Lupis [6]. Let us apply a Taylor series to the activity coefficient of a solute in a dilute binary solution: æ ¶ ln g B ln g B = ln g B¥ + çç è ¶x B 1 æ ¶ i ln g B + ç i ! ç ¶x i B è
ö 1 æ ¶ 2 ln g B xB + ç ÷÷ 2 ç ¶x 2 ø xB ®0 B è
ö ÷ x 2B +… ÷ ø xB ®0
(3.62)
ö ÷ x Bi ÷ ø xB ®0
The derivatives of the Taylor series are all finite. It is not necessary to expand the series at xB = 0, but it is most common and convenient for dilute solutions. The Taylor series expansion of ln g B may be expressed in a different notation as ln g B =
n
å J iB x Bi
i=0
(3.63)
74
3 Solution thermodynamics 0 2 J2Tlx Tl
lng Tl
–1 e1Tl x Tl
–2
• lng Tl
0.0
0.1
0.2 x Tl
0.3
0.4
Figure 3.9 An illustration of loworder terms in the Taylor series expansion of ln g i for dilute solutions using ln g Tl for the binary system Tl–Hg at 293 K as example. Here ¥ ln g Tl = 2.069, e1Tl = 10.683 and J2Tl = 14.4. Data are taken from reference [8].
where J iB =
1 æç ¶ i ln g B i ! ç ¶x i B è
ö ÷ ÷ ø xB ®0
(3.64)
The coefficients J iB are called interaction coefficients of order i. The coefficient of zeroth order is just the value of ln g B at infinite solution. The firstorder coefficient is the most used and is often designated by e 1B [7]. This coefficient is a measure of how an increase in the concentration of B changes ln g B , which explains why it is called the selfinteraction coefficient. The expression for ln g B with only three coefficients is ln g B = ln g B¥ + e 1B x B + J 2B x 2B
(3.65)
The orders of magnitude of the coefficients depend very much on the system studied. Generally stronger atomic interactions give larger interaction coefficients. An illustration of low order terms in the Taylor series expansion of ln g Tl in the binary system Tl–Hg is given in Figure 3.9 [8]. The same type of polynomial formalism may also be applied to the partial molar enthalpy and entropy of the solute and converted into integral thermodynamic properties through use of the Gibbs–Duhem equation; see Section 3.5. Solution models The simplest model beyond the ideal solution model is the regular solution model, first introduced by Hildebrant [9]. Here D mix S m is assumed to be ideal, while D mix H m is not. The molar excess Gibbs energy of mixing, which contains only a single free parameter, is then
3.4 Analytical solution models
D exc G = W xA xB mix m
75
(3.66)
where W is named the regular solution constant or the interaction coefficient. The molar Gibbs energy is in this approximation o G m = xA mA + x B m Bo + RT ( x A ln x A + x B ln x B ) + Wx A x B
(3.67)
The molar Gibbs energy of mixing D mixG m = RT ( x A ln x A + x B ln x B ) + Wx A x B
(3.68)
thus consists of one entropic and one enthalpic contribution: D mix S m = R( x A ln x A + x B ln x B )
(3.69)
D mix H m = Wx A x B
(3.70)
For ideal solutions W is zero and there are no extra interactions between the species that constitute the solution. In terms of nearest neighbour interactions only, the energy of an A–B interaction, uAB, equals the average of the A–A, uAA, and B–B, uBB, interactions or 1 é ù W = zL êu AB  (u AA + u BB ) ú 2 û ë
(3.71)
where z is the coordination number and L is Avogadro’s number. For the general case of a nonideal solution W < 0 gives an increased stability of the solution relative to an ideal solution, while W > 0 destabilizes the solution. It follows that W < 0 and W > 0 are usually interpreted as attraction and repulsion, respectively, between the A and B atoms. Repulsion between the different atoms of the solution will imply that the atoms do not mix at absolute zero, where the entropic contribution is zero. Complete solubility will be obtained when the temperature is raised sufficiently so that the entropy gain due to randomization of the atoms is larger than the positive enthalpic contribution to the Gibbs energy. The integral Gibbs energies of systems with W/RT larger and smaller than zero are shown in Figure 3.10. The regular solution model can be extended to multicomponent systems, in which case the excess Gibbs energy of mixing is expressed as D exc G = mix m
m 1 m
å å x i x j W ij
i =1 j >1
Thus for a ternary system
(3.72)
76
3 Solution thermodynamics W / RT =4
0.4 DmixGm / RT
3 0.0
2 1
–0.4
0 –0.8
–1 –2
–1.2 0.0
0.2
0.4
0.6
0.8
1.0
xB
Figure 3.10 The molar Gibbs energy of mixing of a regular solution A–B for different values of W/RT.
D exc G = x1 x2 W 12 + x1 x 3 W 13 + x2 x 3 W 23 mix m
(3.73)
An additional ternary interaction term, W123, may be incorporated. The regular solution model (eq. 3.68) is symmetrical about x A = x B = 0.5. In cases where the deviation from ideality is not symmetrical, the regular solution model is unable to reproduce the properties of the solutions and it is then necessary to introduce models with more than one free parameter. The most convenient polynomial expression with two parameters is termed the subregular solution model. D exc G = x A x B ( A21 x A + A12 x B ) mix m
(3.74)
If more than two parameters are necessary a general polynomial expression may be applied: m n
i j D exc G = å å xA x B A ij mix m
(3.75)
i =1 j =1
The Redlich–Kister expression G = x A x B [ W + A1 ( x A  x B ) + A2 ( x A  x B )2 D exc mix m
(3.76)
3
+ A3 ( x A  x B ) + … ] is a frequently used special case of this general polynomial approach. While the first term is symmetrical about x = 0.5, the second term changes sign for x = 0.5. The compositional variation of the third and fourth terms is given in Figure 3.11. In all these models the entropy of mixing is assumed to be ideal and the excess Gibbs energy is an analytical model for the enthalpy of mixing. The entropy of mixing of many real solutions will deviate considerably from the ideal entropy of mixing. However, accurate data are available only in a few cases. The simplest model to account for a nonideal entropy of mixing is the quasiregular model, where the excess Gibbs energy of mixing is expressed as
3.4 Analytical solution models
77
W xAx B
exc Gm Contribution to D mix
0.2
0.1
A3 xAxB (xA – x B )3
A1 xAxB (xA – x B )
0.0
A2 xAxB (xA – x B )2
–0.1 0.0
0.2
0.4
0.6
0.8
1.0
xB
Figure 3.11 Contributions to the molar excess Gibbs energy of mixing from the four first terms of the Redlich–Kister expression (eq. 3.76). For convenience W = A1 = A2 = A3 = 1.
T ö æ D exc G = x A x BW ç 1  ÷ mix m t ø è
(3.77)
Thus D exc S =mix m
G ) ¶( D exc mix m ¶T
æWö = x A x Bç ÷ èt ø
(3.78)
The sign of the excess entropy is given by the sign of t.
Derivation of partial molar properties The partial molar properties of binary solutions may be determined by both analytical and graphical methods. In cases where analytical expressions for integral extensive thermodynamic quantities are available, the partial molar quantities are obtained by differentiation, but graphical determination of partial molar properties also has a long history in thermodynamics. The molar Gibbs energy of mixing of molten Si–Ge at 1500 K is given as a function of the mole fraction of Ge in Figure 3.12. Pure solid Si and pure liquid Ge are chosen as standard states. If we draw a tangent to the curve at any composition, the intercept of this tangent upon the ordinate x Si =1 equals m Si and the intercept for x Ge =1 equals m Ge . In mathematical terms the partial molar properties of a binary system will in general be given through YA = Ym  x B and
dY m dx B
(3.79)
78
3 Solution thermodynamics
3 o m Ge
0
o
G m / kJ mol –1
6
–3
o m Si
–6
mSi
0.0
m Ge 0.2
0.4
0.6
0.8
1.0
xGe
Figure 3.12 The integral molar Gibbs energy of liquid Ge–Si at 1500 K with pure liquid Ge and solid Si as standard states. Data are taken from reference [4].
Y B = Y m + (1  x B )
dY m dx B
(3.80)
Application to the Gibbs energy of the two components of a binary solution therefore gives mA = G m  xB
dG m dx B
m B = G m + (1  x B )
dG m dx B
(3.81)
(3.82)
Taking the excess Gibbs energy of a regular solution as an example: G = W xA xB D exc mix m
(3.83)
the partial excess Gibbs energies of the two components are D exc G mix A RT D exc G mix B RT
= ln g A =
W 2 x RT B
(3.84)
= ln g B =
W 2 x RT A
(3.85)
In general, the chemical potential of species i for a multicomponent system is given as
3.5 Integration of the Gibbs–Duhem equation
mi = G m +
r
å (d ij  x j )
j =2
dG m dx j
79
(3.86)
where d ij = 0 for i ¹ j and d ij =1 for i = j.
3.5 Integration of the Gibbs–Duhem equation In experimental investigations of thermodynamic properties of solutions, it is common that one obtains the activity of only one of the components. This is in particular the case when one of the components constitutes nearly the complete vapour above a solid or liquid solution. A second example is when the activity of one of the components is measured by an electrochemical method. In these cases we can use the Gibbs–Duhem equation to find the activity of the second component. We have already derived the Gibbs–Duhem equation in Chapter 1.4. At constant p and T: n A dm A + n B dm B = 0
(3.87)
In terms of activity and mole fractions this yields x A d ln a A + x B d ln a B = 0
(3.88)
x A d ln x A + x A d ln g A + x B d ln x B + x B d ln g B = 0
(3.89)
or
Since x A d ln x A + x B d ln x B = x A
dx A dx + x B B = dx A + dx B = 0 xB xA
(3.90)
eq. (3.89) may be rewritten x A d ln g A + x B d ln g B = 0
(3.91)
or by integration ln g B  ln g B ( x B = 1) = 
xB
ò
x B =1
xA d ln g A xB
(3.92)
80
3 Solution thermodynamics 15
xNi / xFe
10
5
0 – 0.4
– 0.3
– 0.2
– 0.1
0.0
lngNi
Figure 3.13 x Ni / x Fe versus ln g Ni of molten Fe–Ni at 1850 K. Data are taken from reference [3].
If a Raoultian reference state is chosen for both A and B, ln g B = 0 when x B =1. Now by plotting x A / x B against ln g A , as done for the activity coefficient of Fe of molten Fe–Ni at 1850 K in Figure 3.13, the Gibbs–Duhem equation may be integrated graphically by determining the area between the limits. The challenge in our case is that when x Fe ® 0, x Ni / x Fe ® ¥ and ln g Ni ® 0. It may therefore be difficult to evaluate the integral accurately since this demands a large amount of experimental data for x Fe ® 0. We may also integrate the Gibbs–Duhem equation using an Henrian reference state for B: ln g B  ln g B ( x B = 0) = 
xB
ò
xB = 0
xA d ln g A xB
(3.93)
Henry’s law for B leads to ln g B = 0 when x B = 0. An alternative method of integrating the Gibbs–Duhem equation was developed by Darken and Gurry [10]. In order to calculate the integral more accurately, a new function, a, defined as ai =
ln g i (1  x i )2
(i = A or B)
(3.94)
was introduced for binary solutions, since this gave a convenient expression for the much used regular solution model. An expression for d ln g A is obtained by differentiation: d ln g A = d(a A x 2B ) = 2a A x B dx B + x 2B da A
(3.95)
3.5 Integration of the Gibbs–Duhem equation
81
By substituting eq. (3.95) into the Gibbs–Duhem equation (eq. 3.92) we obtain ln g B = 
xB
ò 2 a A x A dx B 
x B =1
xB
ò x A x Bda A
(3.96)
x B =1
Integrating by parts the second integral, we obtain xB
x A x B da A = [a A x A x B ]xx B =1 B x B =1
ò

xB
xB
x B =1
x B =1
ò a A x A dx B + ò a A x Bdx B
(3.97)
which gives the following expression for ln g B (eq. 3.96): ln g B = a A x A x B 
xB
ò a A ( x A + x B )dx B = a A x A x B 
x B =1
xB
ò a A dx B
(3.98)
x B =1
Integration of the Gibbs–Duhem equation applying the method by Darken and Gurry is illustrated by using the Fe–Ni system as an example: see Figure 3.14. aNi plotted against xFe gives a curve that is more easily integrated. A graphical integration of the Gibbs–Duhem equation is not necessary if an analytical expression for the partial properties of mixing is known. Let us assume that we have a dilute solution that can be described using the activity coefficient at infinite dilution and the selfinteraction coefficients introduced in eq. (3.64). ln g B = ln g B¥ + e 1B x B + J 2B x 2B
(3.99)
1.5
a Ni
1.0
0.5
0.0 0.0
0.2
0.4
0.6
0.8
1.0
xFe
Figure 3.14 aNi plotted versus xFe for molten Fe–Ni at 1850 K. Data are taken from reference [3]. The area under the curve represents integration from xFe = 1.0 to 0.1.
82
3 Solution thermodynamics
The Gibbs–Duhem equation can be modified to (1  x B )
¶ ln g B ¶ ln g A =0 + xB ¶x B ¶x B
(3.100)
and thus if the first and secondorder terms in the Taylor series for the solvent are termed J 1A and J 2A (i.e. ln g A = J 1A x B + J 2A x 2B ): (1  x B )(J 1A + 2 J 2A x B ) + x B (e 1B + 2 J 2B x B ) = 0
(3.101)
Hence this implies that J 1A = 0
(3.102)
1 J 2A =  e 1B 2
(3.103)
and
We are thus able to express the activity coefficient of the second component, A, in terms of e 2B : 1 ln g A =  e 1B x 2B 2
(3.104)
All other properties follow. For example, the excess Gibbs energy of mixing is 1 D exc G = RT ( x B ln g B¥ + e 1B x 2B + higher order terms) mix m 2
(3.105)
The relationship between the different selfinteraction coefficients of component A and B, J iA and J iB , may in general be obtained in a similar way. Although the Gibbs–Duhem equation due to the development of versatile and userfriendly thermodynamic software packages is less central than before, it is still of great value, for example for testing the consistency of experimental data and also for systematization of thermodynamic data. The order of magnitude of the major interaction coefficients discussed above may for alloy systems, for instance, be estimated with a fair degree of confidence by looking at trends and by comparison with data on similar systems.
3.5 Integration of the Gibbsâ€“Duhem equation
83
References [1]
H. R. Thresh, A. F. Crawley and D. W. G. White, Trans. Min. Soc. AIME, 1968, 242, 819. [2] O. Sato, Bull. Res. Inst. Mineral. Dress. Metall. 1955, 11, 183. [3] G. R. Zellars, S. L. Payne, J. P. Morris and R. L. Kipp, Trans. Met. Soc. AIME 1959, 215, 181. [4] C. Bergman, R. Chastel and R. Castanet, J. Phase Equil. 1992, 13, 113. [5] E. A. Guggenheim, Proc. Roy. Soc. London, Ser. A 1935, 148, 304. [6] C. H. P. Lupis, Acta Metall., 1968, 16, 1365. [7] C. Wagner, Thermodynamics of Alloys. Reading, MA, AddisonWesley, 1962. [8] T. W. Richards and F. Daniels, J. Am. Chem. Soc. 1919, 41, 1732. [9] J. H. Hildebrand, J. Am. Chem. Soc. 1929, 51, 66. [10] L. S. Darken and R. W. Gurry, Physical Chemistry of Metals. New York: McGrawHill, 1953, p. 264.
Further reading P. W. Atkins and J. de Paula, Physical Chemistry, 7th edn. Oxford: Oxford University Press, 2001. E. A. Guggenheim, Thermodynamics: An Advanced Treatment for Chemists and Physicists, 7th edn. Amsterdam: NorthHolland, 1985. C. H. P. Lupis, Chemical Thermodynamics of Materials. New York: NorthHolland, 1983. K. S. Pitzer, Thermodynamics. New York: McGrawHill, 1995. (Based on G. N. Lewis and M. Randall, Thermodynamics and the free energy of chemical substances. New York: McGrawHill, 1923.
4
Phase diagrams
Thermodynamics in materials science has often been used indirectly through phase diagrams. Knowledge of the equilibrium state of a chemical system for a given set of conditions is a very useful starting point for the synthesis of any material, for processing of materials and in general for considerations related to material stability. A phase diagram is a graphical representation of coexisting phases and thus of stability regions when equilibrium is established among the phases of a given system. A material scientist will typically associate a ‘phase diagram’ with a plot with temperature and composition as variables. Other variables, such as the partial pressure of a component in the system, may be given explicitly in the phase diagram; for example, as a line indicating a constant partial pressure of a volatile component. In other cases the partial pressure may be used as a variable. The stability fields of the condensed phases may then be represented in terms of the chemical potential of one or more of the components. The Gibbs phase rule introduced in Section 2.1 is an important guideline for the construction and understanding of phase diagrams, and the phase rule is therefore referred to frequently in the present chapter. The main objective of the chapter is to introduce the quantitative link between phase diagrams and chemical thermodynamics. With the use of computer programs the calculation of phase diagrams from thermodynamic data has become a relatively easy task. The present chapter focuses on the theoretical basis for the calculation of heterogeneous phase equilibria with particular emphasis on binary phase diagrams.
4.1 Binary phase diagrams from thermodynamics Gibbs phase rule In chemical thermodynamics the system is analyzed in terms of the potentials defining the system. In the present chapter the potentials of interest are T (thermal Chemical Thermodynamics of Materials by Svein Stølen and Tor Grande © 2004 John Wiley & Sons, Ltd ISBN 0 471 492320 2 85
86
4 Phase diagrams
potential), p (mechanical potential) and the chemical potential of the components m1 , m2 , … , m N . We do not consider other potentials, e.g. the electrical and magnetic potentials treated briefly in Section 2.1. In a system with C components there are therefore C + 2 potentials. The potentials of a system are related through the Gibbs–Duhem equation (eq. 1.93): SdT  Vdp + å n i dm i = 0
(4.1)
i
and also through the Gibbs phase rule (eq. 2.15): F + Ph = C + 2
(4.2)
The latter is used as a guideline to determine the relationship between the number of potentials that can be varied independently (the number of degrees of freedom, F) and the number of phases in equilibrium, Ph. Varied independently in this context means varied without changing the number of phases in equilibrium. For a singlecomponent system, the Gibbs phase rule reads F + Ph = C + 2 = 3, and we can easily construct a p,Tphase diagram in two dimensions (see Figure 2.7, for example). To apply the Gibbs phase rule to a system containing two or more components (C > 1) it is necessary to take into consideration the nature of the different variables (potentials), the number of components, chemical reactions and compositional constraints. Initially we will apply the Gibbs phase rule to a binary system (C = 2). The Gibbs phase rule is then F + Ph = C + 2 = 4, and since at least one phase must be present, F is at most 3. Three dimensions are needed to show the phase relations as a function of T, p and a compositional variable (or a chemical potential). Here, we will use the mole fraction as a measure of composition although in some cases the weight fraction and other compositional variables are more practical. When a single phase is present (F = 3), T, p and the composition may be varied independently. With two phases present (F = 2) a set of two intensive variables can be chosen as independent; for example temperature and a composition term, or pressure and a chemical potential. With three phases present only a single variable is independent (F = 1); the others are given implicitly. Finally, with four phases present at equilibrium none of the intensive variables can be changed. The observer cannot affect the chemical equilibrium between these four phases. It is sometimes convenient to fix the pressure and decrease the degrees of freedom by one in dealing with condensed phases such as substances with low vapour pressures. Gibbs phase rule then becomes F = C – Ph + 1
(4.3)
often called the reduced or condensed phase rule in metallurgical literature. For a binary system at constant pressure the phase rule gives F = 3 – Ph and we need only two independent variables to express the stability fields of the phases. It is most often convenient and common to choose the temperature and composition, given for
4.1 Binary phase diagrams from thermodynamics
87
example as the mole fraction. An example is the phase diagram of the system Ag–Cu shown in Figure 4.1 [1]. There are only three phases in the system: the solid solutions Cu(ss) and Ag(ss) and the Ag–Cu liquid solution. Cu(ss) and Ag(ss) denote solid solutions with Cu and Ag as solvents and Ag and Cu as solutes, respectively. When a single phase is present, for example the liquid, F = 2 and both composition and temperature may be varied independently. The stability fields for the liquid and the two solid solutions are therefore twodimensional regions in the phase diagram. With two phases in equilibrium, the temperature and composition are no longer independent of each other. It follows that the compositions of two phases in equilibrium at a given temperature are fixed. In the case of a solid–liquid equilibrium the composition of the coexisting phases are defined by the solidus and liquidus lines, respectively. This is illustrated in Figure 4.1 where the composition of Cu(ss) in equilibrium with the liquid (also having a distinct composition) for a given temperature, T2, is indicated by open circles. Since F = 1 this is called a univariant equilibrium. Finally, when three phases are present at equilibrium, F = 0 and the compositions of all three phases and the temperature are fixed. In this situation there are no degrees of freedom and the three phases are therefore present in an invariant equilibrium. In the present example, the system Ag–Cu, the two solid and the liquid phases coexist in an invariant eutectic equilibrium at 1040 K. The eutectic reaction taking place is defined in general for a twocomponent system as one in which a liquid on cooling solidifies under the formation of two solid phases. Hence for the present example the eutectic reaction is liquid ® Cu(ss) + Ag(ss)
(4.4)
The temperature of the eutectic equilibrium is called the eutectic temperature and is shown as a horizontal line in Figure 4.1. It should be noted that we have here considered the system at constant pressure. If we are not considering the system at isobaric conditions, the invariant equilibrium becomes univariant, and a univariant equilibrium becomes divariant, etc. A 1400 x
1300
T1
T/K
1200
T2 Cu(ss)
liq
1100 Ag(ss) + liq
Cu(ss) + liq
Ag(ss)
1000 900 0.0
Ag(ss) + Cu(ss)
T3 O 0.2
0.4
0.6
0.8
P Q 1.0
xCu
Figure 4.1 Phase diagram of the system Ag–Cu at 1 bar [1].
88
4 Phase diagrams
consequence is that the eutectic temperature in the Agâ€“Cu system will vary with pressure. However, as discussed in Section 2.3, small variations in pressure give only minor variations in the Gibbs energy of condensed phases. Therefore minor variations in pressure (of the order of 1â€“10 bar) are not expected to have a large influence on the eutectic temperature of a binary system. One of the useful aspects of phase diagrams is that they define the equilibrium behaviour of a sample on cooling from the liquid state. Assume that we start at high temperatures with a liquid with composition x in the diagram shown in Figure 4.1. On cooling, the liquidus line is reached at T1. At this temperature the first crystallites of the solid solution Cu(ss) are formed at equilibrium. The composition of both the liquid and Cu(ss) changes continuously with temperature. Further cooling produces more Cu(ss) at the expense of the liquid. If equilibrium is maintained the last liquid disappears at the eutectic temperature. The liquid with eutectic composition will at this particular temperature precipitate Cu(ss) and Ag(ss) simultaneously. The system is invariant until all the liquid has solidified. Below the eutectic temperature the two solid solutions Cu(ss) and Ag(ss) are in equilibrium, and for any temperature the composition of both solid solutions can be read from the phase diagram, as shown for the temperature T3. The relative amount of two phases present at equilibrium for a specific sample is given by the lever rule. Using our example in Figure 4.1, the relative amount of Cu(ss) and Ag(ss) at T3 when the overall composition is x Cu , is given by the ratio Ag( ss ) x Cu  x Cu OP = OQ x Cu ( ss )  x Ag( ss ) Cu Cu
(4.5)
Cu( ss ) Ag( ss ) where x Cu and x Cu denote the mole fractions of Cu in the two coexisting solid solutions. The lines OP and OQ are shown in the figure. An isothermal line in a twophase field, like the line OQ, is called a tieline or conode. As the overall composition is varied at constant temperature between the points O and Q, the compositions of the two solid phases remain fixed at O and Q; only the relative amount of the two phases changes.
Conditions for equilibrium Phase diagrams show coexistent phases in equilibrium. We have seen in Chapter 1 that the conditions for equilibrium in a heterogeneous closed system at constant pressure and temperature can be expressed in terms of the chemical potential of the components of the phases in equilibrium: m ai = m ib = m gi =â€Ś for i = 1, 2, ..., C
(4.6)
Here a, b and g denote the different phases, whereas i denotes the different components of the system and C the total number of components. The conditions for equilibrium
4.1 Binary phase diagrams from thermodynamics
89
between two phases a and b in a binary system A–B (at a given temperature and pressure) are thus b b m aA ( x aA ) = m A (xA )
(4.7)
b m aB ( x aA ) = m Bb ( x A )
(4.8)
and
b where x aA and x A are the mole fractions of A in the phases a and b at equilibrium i (remember that x A + x Bi =1). At a given temperature and pressure eqs. (4.7) and (4.8) must be solved simultaneously to determine the compositions of the two phases a and b that correspond to coexistence. At isobaric conditions, a plot of the composition of the two phases in equilibrium versus temperature yields a part of the equilibrium T, xphase diagram. Equations (4.7) and (4.8) may be solved numerically or graphically. The latter approach is illustrated in Figure 4.2 by using the Gibbs energy curves for the liquid and solid solutions of the binary system Si–Ge as an example. The chemical potentials of the two components of the solutions are given by eqs. (3.79) and (3.80) as
m Ge = G m + (1  x Ge )
m Si = G m  x Ge
dG m dx Ge
dG m dx Ge
(4.9)
(4.10)
Here G m is the Gibbs energy of the given solution at a particular composition xGe. The equilibrium conditions can now be derived graphically from Gibbs energy versus composition curves by finding the compositions on each curve linked by a common tangent (the common tangent construction). In the case shown in Figure 4.2(a) the solid and liquid solutions are in equilibrium; they are not in the case shown in Figure 4.2(b). The compositions of the coexisting solid and liquid solutions are marked by arrows in Figure 4.2(a). The relationship between the Gibbs energy of the phases present in a given system and the phase diagram may be further illustrated by considering the variation of the Gibbs energy of the phases in the system Si–Ge with temperature. Similar common tangent constructions can then be made at other temperatures as well using thermodynamic data by Bergman et al. [2]. The phase diagram of the system is given in Figure 4.3(a). A sequence of Gibbs energy–composition curves for the liquid and solid solutions are shown as a function of decreasing temperature in Figures 4.3(b)–(f). The two Gibbs energy curves are broad and have shallow minima and the excess Gibbs energies of mixing are small since Ge and Si are chemically closely
90
4 Phase diagrams 4
4
0 sol
–4
(b) liq
–8
liq ss mSi = mSi
–12 0.0
0.2
liq ss m Ge = m Ge
0.4 0.6 xGe
0.8
1.0
Gm / kJ mol 1
(a)
Gm / kJ mol 1
0
sol –4 liq –8
–12 0.0
0.2
0.4 0.6 xGe
0.8
1.0
Figure 4.2 Gibbs energy curves for the liquid and solid solution in the binary system Si–Ge at 1500 K. (a) A common tangent construction showing the compositions of the two phases in equilibrium. (b) Tangents at compositions that do not give two phases in equilibrium. Thermodynamic data are taken from reference [2].
related. This is often termed nearideal behaviour. At high temperatures, e.g. at T1, where the liquid solution is stable over the whole composition region, the Gibbs energy of the liquid is more negative than that of the solid solution for all compositions (Figure 4.3(b)). On cooling, the Gibbs energy of the solid solution, having lower entropy than the liquid solution, increases more slowly than that of the liquid solution. At T2, the Gibbs energies of pure liquid Si and pure solid Si are equal, and the melting temperature of pure Si is reached (Figure 4.3(c)). For xSi < 1 the liquid solution is more stable than the crystalline phase. Further cooling gives situations corresponding to T3 or T4, where the solid solution is stable for the Sirich compositions and the liquid solution for the Gerich compositions. The Gibbs energy curves at these two temperatures are shown in Figures 4.3(d) and (e). The compositions of the two phases in equilibrium at these temperatures are given by the common tangent construction, as illustrated in Figure 4.3(d). At T5 the liquid has been cooled down to the melting temperature of pure Ge (see Figure 4.3(f)). Below this temperature the solid solution is stable for all compositions. Since Ge and Si are chemically closely related, Si–Ge forms a complete solid solution at low temperatures. The resulting equilibrium phase diagram, shown in Figure 4.3(a), is a plot of the locus of the common tangent constructions and defines the compositions of the coexisting phases as a function of temperature. The solidus and liquidus curves here define the stability regions of the solid and liquid solutions, respectively. Ideal and nearly ideal binary systems Let us consider a binary system for which both the liquid and solid solutions are assumed to be ideal or near ideal in a more formal way. It follows from their near
4.1 Binary phase diagrams from thermodynamics T1 T2 idus
1600 soli du
s
T3
sol
T5
Gm / kJ mol –1
0.2
0.4
xGe
0.6
0.8
1.0
(d) sol
0.2
0.4
xGe
0.6
0.8
Gm / kJ mol –1
1.0
xGe
0.6
0.8
liq (f) sol
1.0
sol
0
liq ss x Ge
liq x Ge
liq ss mSi = mSi
0.2
liq ss m Ge = m Ge
0.4
xGe
0.6
0.8
10 5
1.0
T5 liq
0
–5
–10 0.0
0.4
T3
0.0
T4
0 –5
0.2
5
–10
10
(e)
liq
–5
liq
–10
5
sol
10
T2
0
0.0
0
0.0
5
–5
5
–10
Gm / kJ mol –1
0.0
T1
–5
T4
1200
(c)
(b)
ss+liq
1400
10
liq
Gm / kJ mol –1
T/K
(a)
10
liqu
Gm / kJ mol –1
1800
91
sol
–10 0.2
0.4
0.6 xGe
0.8
1.0
0.0
0.2
0.4
0.6
0.8
1.0
xGe
Figure 4.3 (a) Phase diagram for the system Si–Ge at 1 bar defining the five temperatures for the Gibbs energy curves shown in (b) T1; (c) T2; (d) T3; (e) T4; (f) T5 . Thermodynamic data are taken from reference [2].
ideal behaviour that the two components must have similar physical and chemical properties in both the solid and liquid states. Two systems which show this type of behaviour are the Si–Ge system discussed above and the binary system
92
4 Phase diagrams
FeO–MnO1,2. However, we will initially look at a general A–B system. The chemical potentials of component A in the liquid and solid states are given as ss s,o ss mA = mA + RT ln a A
(4.11)
liq l,o liq = mA + RT ln a A mA
(4.12)
Similar expressions are valid for the chemical potential of component B of the two phases. According to the equilibrium conditions given by eqs. (4.7) and (4.8), the ss liq solid and liquid solutions are in equilibrium when m A and m Bss = m Bliq , giving = mA the two expressions s,o ss l,o liq mA + RT ln a A = mA + RT ln a A
(4.13)
m Bs,o + RT ln a Bss = m Bl,o + RT ln a Bliq
(4.14)
which may be rearranged as æ a liq lnç A ç a ss è A
o( s ®l ) ö ÷ =  Dm A ÷ RT ø
(4.15)
æ a liq lnç B ç a ss è B
o( s ®l ) ö ÷ =  Dm B ÷ RT ø
(4.16)
and
Here Dm io( s ®l ) is the change in chemical potential or Gibbs energy on fusion of pure i. By using G = H – TS we have Dm io( s ®l ) = m il,o  m is,o = D fus G io = D fus H io  TD fus S io
(4.17)
At the melting temperature we have D fus G io = 0, which implies that D fus S io = D fus H io / T fus,i . If the heat capacity of the solid and the liquid are assumed to be equal, the enthalpy of fusion is independent of temperature and eq. (4.17) becomes 1 The FeO–MnO system is in principle a threecomponent system, but can be treated as a twocomponent system. This requires that the chemical potential of one of the three elements is constant. 2 The fact that FeO is nonstoichiometric is neglected.
4.1 Binary phase diagrams from thermodynamics
93
æ T Dm io( s ®l ) = D fus H io  TD fus S io = D fus H io ç 1 ç T fus,i è
ö ÷ ÷ ø
(4.18)
Substitution of eq. (4.18) into eqs. (4.15) and (4.16) gives æ a liq lnç A ç a ss è A
o( s ®l ) o ö D fus H A ÷ =  Dm A =÷ RT R ø
æ a liq lnç B ç a ss è B
o( s ®l ) ö D fus H Bo æ 1 ÷ =  Dm B ç  1 =ç T T fus,B ÷ RT R è ø
æ1 ç  1 ç T T fus,A è
ö ÷ ÷ ø
(4.19)
ö ÷ ÷ ø
(4.20)
and
If we furthermore assume that the solid and liquid solutions are ideal the activities can be replaced by mole fractions and eqs. (4.19) and (4.20) rearrange to æ1 ç  1 ç T T fus,A è
öù ÷ú ÷ú øû
(4.21)
é D fus H o æ 1 1 Bç x Bliq = x Bss expêç R ê è T T fus,B ë
öù ÷ú ÷ú øû
(4.22)
é D fus H o liq ss A xA = xA expêR ê ë and
Analytical equations for the solidus and liquidus lines can now be obtained from liq ss these equations by noting that x A + x Bliq =1 and x A + x Bss =1, giving é D fus H o ss A xA expêR ê ë
æ1 ç  1 ç T T fus,A è
é D Ho æ öù ÷ú + x ss expê fus B ç 1  1 B ÷ú ç T T fus,B R ê øû è ë
öù ÷ú = 1 ÷ú øû (4.23)
and liq xA
é D fus H o A expê ê R ë
æ1 ç  1 ç T T fus,A è
éD H o æ öù ÷ú + x liq expê fus B ç 1  1 B ÷ú ç T T fus,B ê R øû è ë
öù ÷ú = 1 ÷ú øû (4.24)
94
4 Phase diagrams 1700 1600
liq
T/K
1500 1400 1300 1200 0.0
ideal model liq + ss D Cp = 0 ideal model D Cp π 0 ss 0.2
0.4
0.6
0.8
1.0
xGe
Figure 4.4 Phase diagram for the system Si–Ge at 1 bar. The solid lines represent experimental observations [2] while the dotted and dashed lines represent calculations assuming that the solid and liquid solutions are ideal with DC p ¹ 0 and DC p = 0, respectively.
In this particular case of ideal solutions the phase diagram is defined solely by the temperature and enthalpy of fusion of the two components. Using the analytical equations derived above, we are now able to consider the phase diagrams of the two nearly ideal systems mentioned above more closely. In the calculations we will initially use only the melting temperature and enthalpy of fusion of the two components as input parameters; both the solid and liquid solutions are assumed to be ideal. The observed (solid lines) and calculated (dashed lines) phase diagrams for the systems Si–Ge [2] and FeO–MnO [3] are compared in Figure 4.4 and 4.5. Although the agreement is reasonable, the deviation between the calculated and observed solidus and liquidus lines is significant. 2200
ideal model
2000 T/K
liq liq + ss
1800 ss 1600 0.0
0.2
0.4
0.6
0.8
1.0
xMnO
Figure 4.5 Phase diagram of FeO–MnO at 1 bar. The solid lines represent experimental observations [3]. The activity of iron is kept constant and equal to 1 by equilibration with liquid Fe. Dashed lines represent calculations assuming that the solid and liquid solutions are ideal.
4.1 Binary phase diagrams from thermodynamics
95
15 DCp = 0 10
o
D fusGm / kJ mol
–1
DCp π 0 5 0
Si Ge
–5 DCp π 0
–10
DCp = 0
–15 1200
1300
1400 1500 T/K
1600
1700
Figure 4.6 Gibbs energy of fusion of Ge and Si. The solid lines represent experimental data [4] while the broken lines are calculated neglecting the heat capacity difference between liquid and solid.
Let us now consider the effect of a difference between the heat capacity of pure liquid i and pure solid i on the enthalpy and entropy of fusion and subsequently on the phase diagram. This effect is easily taken into consideration by using eqs. (1.24) and (1.54). Dm io( s ®l ) is now given as Dm io( s ®l )
= D fus H io
T
+
ò DC
Tfus, i
o dT p ,i
ö æ T DC o ÷ ç p ,i o  T ç D fus S i + ò dT ÷ T ÷ ç Tfus, i ø è
(4.25)
o( s ®l ) s,o where DC op = C l,o for p  C p . We will use the system Si–Ge as example. Dm i Si and Ge with (solid lines) and without (dashed lines) taking the heat capacity difference into consideration are shown in Figure 4.6 [4], while the effect of DC op on the calculated liquidus and solidus lines is shown in Figure 4.4 (dotted lines). In this particular case, the liquids and solidus lines are shifted some few degrees up and down in temperature, respectively, and the resulting twophase field is only slightly broader than that calculated without taking the heat capacity difference between the liquid and the solid into consideration. The lack of quantitative agreement between the experimentally observed phase diagram and the calculated ones shows that significant excess Gibbs energies of mixing are present for one or both of the solution phases in the Si–Ge system. This indicates what is in general true: nonideal contributions to the solution energetics in general have a much larger effect on the calculated phase diagrams than the heat capacity difference between the liquid and solid. This is reflected in the phase diagram for the binary system KCl–NaCl shown in Figure 4.7(a) [5]. This system is characterized by negative deviation from ideal behaviour in the liquid state and positive deviation from ideality in the solid state (see the corresponding G–x curves for the solid and liquid solutions in Figure 4.7(b)). In general a negative excess Gibbs energy of mixing
96
4 Phase diagrams 2
1050
0
1000
(b) liq + KCl(ss)
liquid
liq + NaCl(ss)
950
Gm / kJ mol
(a)
T/K
–1
1100
–2 solid solution
–4 liquid solid solution
900 0.0
0.2
0.4 0.6 xNaCl
0.8
1.0
–6 0.0
0.2
0.4 0.6 xNaCl
0.8
1.0
Figure 4.7 (a) Phase diagram of the system KCl–NaCl. (b) Gibbs energy curves for the solid and liquid solutions KCl–NaCl at 1002 K. Thermodynamic data are taken from reference [5].
corresponds to a stabilization of the solution and a deeper curvature of the G–x curve compared to ideal solution behaviour. Correspondingly, a positive deviation from ideal behaviour destabilizes the solution and the G–x curve becomes shallower. These features affect the resulting phase diagrams and the liquidus and solidus lines may show maxima or minima for intermediate compositions, as evident for the KCl–NaCl system in Figure 4.7(a). Simple eutectic systems Ag–Cu (Figure 4.1) and many other inorganic systems give rise to simple eutectic phase diagrams. In these systems the two solid phases have such different chemical and physical properties that the solid solubility is limited. The phases may have different structures and hence be represented by different Gibbs energy curves, or they may take the same structure but with a large positive enthalpic interaction giving rise to phase separation or immiscibility at low temperatures. The latter situation, where two solid solutions are miscible at high temperatures, is more usual for alloys and less usual in inorganic material systems. It is, however, a very useful situation for illustrating the link between thermodynamics and phase diagrams, as we will see in the next section on regular solution modelling. It is worth noting that two components that have different properties in the solid state still may form a nearideal liquid solution. The system MgO–Y2O3 [6] can be used to exemplify the link between Gibbs energy curves and the characteristic features of a simple eutectic phase diagram. The MgO–Y2O3 phase diagram is shown in Figure 4.8(a). MgO and Y2O3 have different crystal structures and the solid solubility of the two oxides is therefore limited. Furthermore, Y2O3 is found in both hexagonal and cubic polymorphs. Gibbs
4.1 Binary phase diagrams from thermodynamics
97
3200
10
T1
3000
liquid
T/K
2800
(a)
2600 2400
(b)
liq + hY2O3(ss)
T3
T4 T5
0.4
0.6 x YO1.5
0.8
liquid
0.2
0.4 0.6 x YO1.5
0.8
20
T2
1.0
T3
15 cY2O3(ss)
MgO(ss)
(d)
0 –5
Gm / kJ mol –1
Gm / kJ mol –1
(c)
–5
0.0
1.0
10 5
0
–15
hY2O3(ss) + MgO(ss) hY2O3(ss)
0.2
cY2O3 MgO
–10
MgO(ss)
2200 0.0
15
liq + cY2O3(ss)
T2 MgO(ss) + liq
Gm / kJ mol –1
5
cY2 O3 (ss)
T1
cY2O3(ss)
10 5
MgO(ss) hY2O3(ss)
0 liquid
–10 0.0
–5
liquid
0.2
0.4
0.6 x YO1.5
0.8
25
1.0
0.0
T4
(f)
hY2O3(ss)
5
1.0
T5
15 10
0 0.2
0.4
0.6 x YO1.5
hY2O3(ss)
5
liquid
MgO(ss)
Gm / kJ mol –1
Gm / kJ mol –1
cY2O3(ss)
10
0.0
0.8
20
15
0
0.4 0.6 x YO1.5
25
20
(e)
0.2
0.8
1.0
0.0
MgO(ss) liquid
0.2
0.4 0.6 x YO1.5
0.8
1.0
Figure 4.8 (a) Phase diagram of the binary system Y2O3–MgO at 1 bar defining the five temperatures for the Gibbs energy curves shown in (b) T1; (c) T2; (d) T3; (e) T4; (f) T5. Thermodynamic data are taken from reference [6].
energy representations for the selected temperatures given in the phase diagram are shown in Figures 4.8(b)–(f). At T1 the liquid is stable at all compositions (Figure 4.8(b)). At T2 solid MgO(ss) has become stable for MgOrich compositions (Figure 4.8(c)) and the twophase field between MgO(ss) and the liquid is
98
4 Phase diagrams
established by the common tangent construction. At T3 solid MgO(ss) is stable for MgOrich compositions, while the cubic polymorph of Y2O3(ss) is stable for Y2O3rich compositions. At intermediate compositions the liquid is stable. The compositions of the liquid coexisting with MgO(ss) and Y2O3(ss) are again defined by common tangent constructions. Cubic Y2O3(ss) transforms to the hexagonal polymorph at the phase transition temperature given by the horizontal line at T = 2540 K. This transition will be further considered below. At the eutectic temperature, T4, three phases are in equilibrium (see Figure 4.8(e)) according to liquid = hY2O3(ss) + MgO(ss)
(4.26)
At an even lower temperature, T5, a sample in equilibrium will consist of the crystalline phase hY2O3(ss), MgO(ss) or a twophase mixture of these (see Figure 4.8(f)). The compositions of the two phases in equilibrium are again given by the common tangent construction.
Regular solution modelling The examples focused on so far have demonstrated that phase diagrams contain valuable information about solution thermodynamics. We will illustrate this further by using the regular solution model, introduced in Section 3.4, to calculate a range of phase diagrams. Although the regular solution model may represent a very crude approximation for a large number of real solutions, it has proven to be very efficient in many respects. The equilibrium conditions given by eqs. (4.15) and (4.16) can in general be expressed through the activity coefficients. Using a solid–liquid phase equilibrium as an example we obtain æ a liq lnç A ç a ss è A
æ liq liq ö ÷ = lnç x A g A ç x ss g ss ÷ è A A ø
o( s ®l ) ö ÷ =  Dm A ÷ RT ø
(4.27)
æ a liq lnç B ç a ss è B
æ liq liq ö ÷ = lnç x B g B ç x ss g ss ÷ è B B ø
o( s ®l ) ö ÷ =  Dm B ÷ RT ø
(4.28)
and
These expressions can be simplified since the activity coefficient in the particular case of a regular solution can be expressed by the regular solution constant W through eqs. (3.84) and (3.85):
4.1 Binary phase diagrams from thermodynamics 1400
T1
T1 solid solution
T3 T4
T/K
1000
(b)
T5
800
T5
0
D mix Gm / kJ mol –1
T2
1200
(a)
99
T4 –1 T3 T2 –2
V2O3(ss) – Cr2O3(ss)
600
T1 –3 400 0.0
0.2
0.4 0.6 xAl2O3
0.8
1.0
0.0
0.2
0.4 0.6 xAl2O3
0.8
1.0
Figure 4.9 (a) Immiscibility gap of the binary solid solution V2O3–Cr2O3 as described by the regular solution model. (b) Gibbs energy of mixing curve of the solid solution at the temperatures marked in the phase diagram. Thermodynamic data are taken from reference [7].
ln(1  x Bliq ) +
ln x Bliq +
o( s ®l )
Dm A W liq liq 2 W ss ss 2 ( x B )  ln(1  x Bss ) (xB ) = RT RT RT
(4.29)
o( s ®l )
Dm B W liq W ss (1  x Bliq )2  ln x Bss (1  x Bss )2 = RT RT RT
(4.30)
These two simultaneous equations can then be solved numerically to calculate the solidus and liquidus lines. It should be remembered that if we assume that a solution phase in a hypothetical A–B system is regular, a positive interaction parameter implies that the different types of atom interact repulsively and that if the temperature is not large enough phase separation will occur. Let us first consider a solid solution only. The immiscibility gap of the solid solution in the binary system V2O3–Cr2O3 [7] given in Figure 4.9(a) can be described by a regular solution model and thus may be used as an example. The immiscibility gap is here derived by using the positive interaction parameter reported for the solid solution [7]. There is no solubility at absolute zero. As the temperature is raised, the solubility increases with the solubility limits given by the interaction coefficient, W , and by temperature. Figure 4.9(b) show the Gibbs energy curves for the solid solution and the common tangent constructions defining the compositions of the coexisting solid solutions at different selected temperatures. Let us now return to our hypothetical system A–B where we also consider the liquid and where the solid and liquid solutions are both regular (following Pelton and
100
4 Phase diagrams
Thompson [8]). Pure A and B are assumed to melt at 800 and 1000 K with the entropy of fusion of both compounds set to 10 J K–1 mol–1 (this is the typical entropy of fusion for metals, while semimetals like Ga, In and Sb may take quite different values – in these three specific cases 18.4, 7.6 and 21.9 J K–1 mol–1, respectively). The interaction coefficients of the two solutions have been varied systematically in order to generate the nine different phase diagrams given in Figure 4.10. In the diagram in the middle (Figure 4.10(e)), both the solid and liquid solutions are ideal. Changing the regular solution constant for the liquid to –15 or +15 kJ mol–1, while keeping the solid solution ideal evidently must affect the phase diagram. In the first case (Figure 4.10(d)), the liquid is stabilized relative to the solid solution. This is reflected in the phase diagram by a shift in the liquidus line to lower temperatures and in this particular case a minimum in the liquidus temperature is present for an intermediate composition. Correspondingly, the positive interaction energy for the liquid destabilizes the liquid relative to the solid solution and the liquidus is in this case shifted to higher temperatures: see Figure 4.10(f). For the composition corresponding to the maximum or minimum in the liquidus/ solidus line, the melt has the same composition as the solid. A solid that melts and forms a liquid phase with the same composition as the solid is said to melt congruently. Hence the particular composition that corresponds to the maximum or minimum is termed a congruently melting solid solution. Positive deviations from ideal behaviour for the solid solution give rise to a miscibility gap in the solid state at low temperatures, as evident in Figures 4.10(a)–(c). Combined with an ideal liquid or negative deviation from ideal behaviour in the liquid state, simple eutectic systems result, as exemplified in Figures 4.10(a) and (b). Positive deviation from ideal behaviour in both solutions may result in a phase diagram like that shown in Figure 4.10(c). Negative deviation from ideal behaviour in the solid state stabilizes the solid solution. Wsol = –10 kJ mol–1, combined with an ideal liquid or a liquid which shows positive deviation from ideality, gives rise to a maximum in the liquidus temperature for intermediate compositions: see Figures 4.10(h) and (i). Finally, negative and close to equal deviations from ideality in the liquid and solid states produces a phase diagram with a shallow minimum or maximum for the liquidus temperature, as shown in Figure 4.10(g). The mathematical treatment can be further simplified in one particular case, that corresponding to Figure 4.10(a). As we saw in the previous section, in some binary systems the two terminal solid solution phases have very different physical properties and the solid solubility may be neglected for simplicity. If we assume no solid ss solubility (i.e. a A = a Bss =1) and in addition neglect the effect of the heat capacity difference between the solid and liquid components, eqs. (4.29) and (4.30) can be transformed to two equations describing the two liquidus branches: liq ln x A +
o D fus H A W liq liq 2 (xB ) = RT R
æ1 ç  1 ç T T fus,A è
ö ÷ ÷ ø
(4.31)
4.1 Binary phase diagrams from thermodynamics
101
W liq / kJ mol 1
–15
15
0 (c)
(b)
1200
liq liq
15
liq
A(ss)
liq + A(ss) liq + B(ss) B(ss)
liq + A(ss) B(ss)
liq + B(ss)
liq + B(ss) A(ss)
liq + A(ss)
900
A(ss)
T/K
(a)
600
A(ss) + B(ss)
A(ss) + B(ss) B(ss)
300
A(ss) + B(ss)
Wsol / kJ mol 1 Æ
(d)
(e)
(f)
liq + ss
0
liq + ss
liq
liq
liq + ss liq +ss
liq
liq + ss ss
ss ss 0.0
0.2
0.4
0.6
xB
0.8
1.0
liq
liq
liq liq + ss
liq + ss liq liq + ss
ss
liq + ss
–10
liq + ss
liq + ss
ss
(g)
ss
(h)
(i)
Figure 4.10 (a)–(i) Phase diagrams of the hypothetical binary system A–B consisting of regular solid and liquid solution phases for selected combinations of Wliq and Wsol. The entropy of fusion of compounds A and B is 10 J K–1 mol–1 while the melting temperatures are 800 and 1000 K.
ln
x Bliq
D fus H Bo æ 1 W liq liq 2 ç  1 + (xA ) = ç T T fus,B RT R è
ö ÷ ÷ ø
(4.32)
102
4 Phase diagrams
The two branches intersect at the eutectic point and the phase diagram thus relies on a single interaction parameter, Wliq, only. In the present section we have focused on the calculation of phase diagrams from an existing Gibbs energy model. We can turn this around and derive thermodynamic information from a welldetermined phase diagram. Modern computational methods utilize such information to a large extent to derive consistent data sets for complex multicomponents systems using both experimental thermodynamic data and phase diagram information. Still, it should be remembered that the phase diagram data does not give absolute values for the Gibbs energy, but rather relative values. A few welldetermined experimental data points are, however, enough to ‘calibrate the scale’, and this allows us to deduce a large amount of thermodynamic data from a phase diagram. Invariant phase equilibria In the examples covered so far several invariant reactions defined by zero degrees of freedom have been introduced. For a twocomponent system at isobaric conditions, F = 0 corresponds to three phases in equilibrium. Eutectic equilibria have been present in several of the examples. Also, congruent melting for the solid solutions with composition corresponding to the maxima or minima in the liquidus lines present in Figures 4.10(f) and (d), for example, corresponds to invariant reactions. At the particular composition corresponding to the maximum or minimum, the system can be considered as a singlecomponent system, since the molar ratio n A /n B = x A / x B remains constant in both the solid and liquid solutions. The molar ratio between the two components is a stoichiometric restriction that reduces the number of components from two to one. A third invariant reaction is the hexagonal to cubic phase transition of pure Y2O3 represented in Figure 4.8(a). While pure Y2O3 is clearly a singlecomponent system, the solid solubility of the component MgO in hY2O3(ss) and cY2O3(ss) increases the number of components by one relative to pure Y2O3. Two coexisting condensed phases give one degree of freedom and the solid–solid transition is no longer an invariant reaction according to the phase rule, but occurs over a temperature interval. The twophase region is, however, narrow and not visible in Figure 4.8(a). Several other invariant equilibria may take place. A peritectic reaction is defined as a reaction between a liquid and a solid phase under the formation of a second solid phase during cooling. Such an invariant reaction is seen in Figure 4.10(c), where the reaction B(ss) + liquid ® A(ss)
(4.33)
takes place at T = 837 K. It is possible for a solid solution to play the role of the liquid in a similar reaction. Equilibria of this type between three crystalline phases are termed peritectoid. Similarly, eutectic reactions, where the liquid is replaced by a solid solution (hence involving only solid phases), are termed eutectoid.
4.1 Binary phase diagrams from thermodynamics 1600
103
liquid
1400 A(liq) + B(liq)
B(liq) + a (ss)
T/K
1200 A(liq) + a (ss)
1000
solid solution
800 600 0.0
a (ss)
a (ss) + a ' (ss)
a (ss)
0.2
0.4
0.6
0.8
1.0
xB
Figure 4.11 Phase diagram of the hypothetical binary system A–B consisting of regular solid and liquid solutions. Wliq = 20 kJ mol–1 and Wsol = 15 kJ mol–1. Thermodynamic data for components A and B as in Figure 4.10.
A miscibility gap in the liquid state in general results in another invariant reaction in which a liquid decomposes on cooling to yield a solid phase and a new liquid phase liq1 ® b(ss) + liq2
(4.34)
in a monotectic reaction. Finally, a phase diagram showing phase separation in both the liquid and solid states is depicted in Figure 4.11. Here a syntectic reaction (liq 1 + liq 2 ® a( ss)) takes place at 1115 K. Formation of intermediate phases The binary systems we have discussed so far have mainly included phases that are solid or liquid solutions of the two components or end members constituting the binary system. Intermediate phases, which generally have a chemical composition corresponding to stoichiometric combinations of the end members of the system, are evidently formed in a large number of real systems. Intermediate phases are in most cases formed due to an enthalpic stabilization with respect to the end members. Here the chemical and physical properties of the components are different, and the new intermediate phases are formed due to the more optimal conditions for bonding found for some specific ratios of the components. The stability of a ternary compound like BaCO3 from the binary ones (BaO and CO2(g)) may for example be interpreted in terms of factors related to electron transfer between the two binary oxides; see Chapter 7. Entropystabilized intermediate phases are also frequently reported, although they are far less common than enthalpystabilized phases. Entropystabilized phases are only stable above a certain temperature,
104
4 Phase diagrams 0 3200 liq
CSZ + liq cZrO 2 (ss)
2800
liq+ cCaZrO3
(b)
–10
liq+ CaO(ss)
cCaO(ss)
2400 T/K
Gm / kJ mol –1
(a)
CSZ
cCaZrO3 + CaO(ss)
CSZ + oCaZrO3
2000
–20 1600
CSZ + cCaZrO3
CaO(ss)
CaZr4O9 TSZ Ca 6 Zr19O44 +CSZ oCaZrO 3 + CaO(ss)
TSZ TSZ + oCaZrO 3
–30 0.0
1200
CaZrO 3
0.2
0.4
0.6 x CaO
0.8
1.0
0.0
MSZ
MSZ + oCaZrO 3
0.2
0.4
0.6 x CaO
0.8
1.0
Figure 4.12 (a) Gibbs energy representation of the phases in the system ZrO2–CaO at 1900 o o K. m CaO = m ZrO = 0. TSZ is not included for clarity. (b) Calculated phase diagram of the 2 system ZrO2–CaO. Thermodynamic data are taken from reference [9].
where the entropy contribution to the Gibbs energy exceeds the enthalpy difference between this phase and the phase or phase assemblage stable at lower temperatures. One example is wüstite, Fe1–yO, which forms eutectoidally from Fe and Fe3O4 at 850 K. The formation of intermediate phases will naturally significantly influence the phase diagram of a given system. Before we give some examples of phase diagrams involving intermediate phases, it is useful to discuss the compositional variation of the Gibbs energy of such phases. Some intermediate phases may be regarded as stoichiometric. Here the homogeneity range or the compositional width of the singlephase region is extremely narrow. This reflects the fact that the Gibbs energy curves rise extremely rapidly on each side of the minimum, which is located at exactly the stoichiometric composition of the phase. This is illustrated in Figure 4.12(a) for CaZrO3, which may be seen as an intermediate phase of the system CaO–ZrO2 [9].3 The sharpness of the G–x curve implies that CaZrO3 is represented by a vertical line in the CaO–ZrO2 phase diagram shown in Figure 4.12(b). The fact that the solid solubility or nonstoichiometry of CaZrO3 is negligible is understood by considering the crystal structures of the compounds involved; CaZrO3 takes a perovskiterelated crystal structure, while the two end members ZrO2 and CaO have the fluorite and rock salt structures, respectively. In the perovskite structure there are 3 The system Ca–Zr–O is principally a ternary system. However, as long as the oxidation state of Zr and Ca are the same in all phases, the system can be redefined as a twocomponent system consisting of CaO and ZrO2.
4.1 Binary phase diagrams from thermodynamics Ti5Si3
105
Ti5Si4
2000
liq.
T /K
bTi
1000 TiSi
Ti3Si
aTi 0 0.0
0.2
0.4
0.6
TiSi2
0.8
1.0
x Si
Figure 4.13 Phase diagram of the system Si–Ti [10].
unique lattice sites for both Ca and Zr, and neither interchange of Zr and Ca nor the generation of vacant sites are thermodynamically favourable for CaZrO3.4 In optimization of thermodynamic properties of stoichiometric compounds, the compositional variation is often neglected and the Gibbs energy is simply given as a function of temperature (and possibly pressure). CaZrO3 melts congruently, i.e. the coexisting liquid and solid phases have the exact same composition and CaZrO3 may hence be considered as a singlecomponent system. Here two phases present in equilibrium at constant pressure give zero degrees of freedom. The congruent melting of CaZrO3 is therefore an invariant equilibrium. Correspondingly, an incongruently melting compound melts under the formation of a new solid phase and a liquid with composition different from the original compound. The phase diagram of the binary system Si–Ti shown in Figure 4.13 [10] is even more complex. In this system several intermediate phases are formed. Solid solubility is present for the intermediate phase Ti5Si3, while the other intermediate phases Ti3Si, Ti5Si4, TiSi and TiSi2 all have very narrow homogeneity ranges. The G–x curve for ‘Ti5Si3’ should therefore display a shallow minimum at the Ti5Si3 composition, while the G–x curve for the other intermediate phases should possess sharp minima at the exact composition of the phases. In the thermodynamic description of the Gibbs energy of the nonstoichiometric phase Ti5Si3, the variation of the Gibbs energy with composition must be taken into account explicitly in order to calculate the homogeneity range. In this particular case, the Gibbs energy model may contain several different sublattices (see Chapter 9) so that the distribution of different species on the relevant sublattices is represented.
4 It should be mentioned that oxygen vacancies are often formed in the perovskitetype structure ABO3 in cases where the B atom is a transition metal that readily exists in more than one oxidation state.
106
4 Phase diagrams
The intermediate phases in the system Si–Ti display also a variety of other features. While TiSi2 and Ti5Si3 are congruently melting phases, Ti5Si4 and TiSi melt incongruently. Finally, Ti3Si decomposes to bTi and Ti5Si3 at T = 1170 K, in a peritectoid reaction while bTi decomposes eutectoidally on cooling forming aTi + Ti3Si at T = 862 K. Melting temperature: depression or elevation? While until now we have considered relatively simple phase diagrams and the fundamentals of the connection between phase diagrams and thermodynamics, we are here going to consider a somewhat more complex example, but only briefly. The calculation of phase diagrams is possible if the equilibrium between the different phases can be evaluated as a function of the variables of the system. A relatively simple case is obtained by considering the effect of impurities on the melting temperature of a ‘pure metal’ following Lupis’s treatment of the calculation of the phase boundaries in the vicinity of invariant points [11]. The impurity may be solved both in the solid and liquid phases and the presence of impurities in a ‘pure’ metal leads to interval freezing. The fusion interval is generally offset towards higher or lower temperatures depending on the nature of the impurity. These alternatives are discussed here with reference to binary phase diagrams exemplifying either a eutectictype or peritectictype behaviour in the composition range adjoining the pure metal. The term eutecticlike behaviour is used for all diagrams with the liquidus line sloping downwards, and peritecticlike is used for all those with the liquidus line sloping upwards. Monotectic diagrams, as well as those that include intermediate phases decomposing peritectically below the fusion temperature of the pure metal (e.g. SnSb in the phase diagram of the Sn–Sb system in Figure 4.14) are presently classed in the eutecticlike category. Nearly ideal 550 liq.
800
liq.
liq + Sb
450
400
liq. + Bi
Sn + liq.
T/K
T/K
500
600
Sn(ss) Bi(ss)
400
350 0.2
liq.+ Sn 3Sb2 SnSb
Sn + Bi
0.0
Sb(ss)
liq.+ SnSb
Sn(ss)
0.4
0.6 xBi
0.8
1.0
0.0
Sn + SnSb
0.2
0.4
SnSb + Sb
0.6 xSb
0.8
1.0
Figure 4.14 Phase diagrams of the systems (a) Sn–Bi [13] and (b) Sn–Sb [14]. Reprinted from [12]. Copyright (1999), with permission from Elsevier.
4.1 Binary phase diagrams from thermodynamics
107
systems, with complete solid and liquid solubility, are categorized as peritectic if the impurity fuses at a higher temperature than the pure metal. The equilibrium compositions of an impurity B, x aB and x Bb , in the two phases a and b at a given temperature are given by eqs. (4.27) and (4.28), which may be rewritten as æ 1  xa B lnç ç b 1 x B è æ xa lnç B ç b è xB
ö ÷ + ln g a  ln g A ÷ ø
b A
o( a ®b )

Dm A
RT
=0
(4.35)
o( a ®b ) ö ÷ + ln g a  ln g b  Dm B =0 B B ÷ RT ø
(4.36)
Here Raoultian standard states are used for both the pure metal and the impurity. The slope dx B / dT of the phase boundaries can now be derived by differentiation with respect to temperature. Let f(xB) denote the lefthand side of eq. (4.35) or (4.36); then (see Lupis, Further reading) æ ¶ f ( x ) ö æ dx a æ df ( x B ) ö B ÷ ç B ÷ =ç ç a ÷ ç dT ç d T ø eq è ¶x B ø è è T =0
ö æ ¶ f ( x ) ö æ dx b ÷+ç B ÷ ç B ÷ ç ¶ x b ÷ ç dT ø è B øT è
ö ¶f ( x ) ÷+æ B ö ÷ çè ¶T ÷ø a b x B ,x B ø (4.37)
where dx aB / dT and dx Bb / dT are the slopes of the two phase boundaries [11]. Equation 4.37 is identical to zero since f(xB) is zero along the boundaries. The slope of the phase boundaries can now be evaluated using eqs. (4.35) and (4.36). Further treatment [11] gives the following equations for the slopes of the phase boundaries – using a solid–liquid transition (melting) as an example: æ dx ss ç B ç dT è
o ö g 2¥ ,liq ( D fus S A / RT fus,A ) ÷ = ¥ ,liq ÷  g B¥ ,ss exp( D fus G Bo / RT fus,A ) ø xBss ®0 g B
(4.38)
and æ dx liq ç B ç dT è
o ö g ¥ ,ss ( D fus S A / RT fus,A ) exp(D fus G Bo / RT fus,A ) ÷ = B ÷ g B¥ ,liq  g B¥ ,ss exp( D fus G Bo / RT fus,A ) ø xBliq ®0
(4.39)
108
4 Phase diagrams
Here g B¥ ,liq and g B¥ ,ss are the activity coefficients of component B in the liquid and solid solutions at infinite dilution with pure solid and liquid taken as reference o is the standard molar entropy of fusion of component A at its fusion states. D fus S A temperature T fus,A and D fus G Bo is the standard molar Gibbs energy of fusion of component B with the same crystal structure as component A at the melting temperature of component A. The melting temperature depression or enhancement may now be expressed in terms of the melting temperature and the entropy of fusion of component A, the activity coefficients of impurity B in the liquid and solid solutions at infinite dilution, and the total concentration of the impurity B, xB [12]: DT = T  T fus,A = 
x B RT fus,A é 1 ù o êë F  K úû D fus S A
(4.40)
where F is the fraction of the sample melted at DT departure from T fus,A , and K is an interaction coefficient. If the liquid standard state is used for the activity coefficient of component B in both solid and liquid solutions: K=
g B¥ ,liq
(4.41)
g B¥ ,liq  g B¥ ,ss
In this case the equations are greatly simplified and the ratio of the slopes of the two phase boundaries at x A =1 is given by the activity coefficients of B at infinite dilution in the liquid and solid phases [11]: ( dT / dx Bss ) x ss ®0 B
( dT / dx Bliq ) x liq ®0 B
=
g B¥ ,ss g B¥ ,liq
(4.42)
Eutectic behaviour persists for 0 > K >  ¥, that is for g B¥ ,liq  g B¥ ,ss < 0. Peritectic behaviour is obtained for 1 < K < ¥, that is for g B¥ ,liq  g B¥ ,ss > 0. The phase diagrams of the Sn–Bi and Sn–Sb systems are shown in Figure 4.14, and they illustrate the effect of Bi and Sb on the melting temperature of pure Sn. ,ss Experimental thermodynamic data for the Sn–Bi system gives l ¥ = 7.5 and Bi ¥ ,liq l Bi =1.3 [13]; the slope of the Sn solidus is steeper than for the Sn liquidus, K = –0.2, and a eutectic type behaviour is expected. For the Sn–Sb system ,ss ,liq l¥ = 0 .12 and l ¥ = 0 .27 [14], the slope of the Sn liquidus is steeper than that Sb Sb for the Sn solidus, K = 1.8, and a peritectictype behaviour is suggested. Both results are in agreement with the experimental phase diagrams. Activity coefficients at infinite dilution are in general very important and frequently used in thermodynamic analyses. Examples are analyses of trace element
4.2 Multicomponent systems
109
partitioning between solids and melts in geological systems [15] and analyses of the distribution of longlived chemicals throughout the environment [16].
Minimization of Gibbs energy and heterogeneous phase equilibria The heterogeneous phase equilibria considered in the preceding sections have implicitly been derived by finding the phase or phase assemblage with the lowest Gibbs energy. Heterogeneous phase equilibria in general are calculated by minimizing the Gibbs energy, and computer software has been available for several decades to perform similar calculations in multicomponent systems consisting of any number of components and phases. Generally, the Gibbs energy in a system consisting of the components A, B, C, …, the stoichiometric phases a, b, g , ... and the solution phases 1, 2, 3, … can be expressed as G = na D f G ao + n b D f G bo + ng D f G go + … +
å
å
i =1,2 ,3 ,.. j = A,B,C,…
n j ( m oj + RT ln a j )
(4.43)
For a given set of constraints (for example temperature, pressure and overall composition), the algorithm identifies the phases present and the relative amounts of these phases, as well as the mole fraction of all the components in all phases. The global minimum evidently must obey the Gibbs phase rule, and not all phases need to be present at the global equilibrium. A thorough description of strategies and algorithms for minimization of Gibbs energy in multicomponent systems is outside the scope of the present text. The monograph by Smith and Missen (see Further reading) gives an excellent overview of the topic.
4.2 Multicomponent systems Ternary phase diagrams For threecomponent (C = 3) or ternary systems the Gibbs phase rule reads Ph + F = C + 2 = 5. In the simplest case the components of the system are three elements, but a ternary system may for example also have three oxides or fluorides as components. As a rule of thumb the number of independent components in a system can be determined by the number of elements in the system. If the oxidation state of all elements are equal in all phases, the number of components is reduced by 1. The Gibbs phase rule implies that five phases will coexist in invariant phase equilibria, four in univariant and three in divariant phase equilibria. With only a single phase present F = 4, and the equilibrium state of a ternary system can only be represented graphically by reducing the number of intensive variables.
110
4 Phase diagrams B 0.0
P
1.0 0.8
0.2
x
C
xB
0.6
0.4 0.6
0.4 X
0.2
0.8 1.0 0.0 C
0.2 Q
0.4
0.6 xA
0.8
0.0 1.0 A
Figure 4.15 Equilateral composition triangle for defining composition in a ternary system A–B–C.
It is sometimes convenient to fix the pressure and decrease the degrees of freedom by one in dealing with condensed phases such as substances with low vapour pressure. The Gibbs phase rule for a ternary system at isobaric conditions is Ph + F = C + 1 = 4, and there are four phases present in an invariant equilibrium, three in univariant equilibria and two in divariant phase fields. Finally, three dimensions are needed to describe the stability field for the single phases; e.g. temperature and two compositional terms. It is most convenient to measure composition in terms of mole fractions also for ternary systems. The sum of the mole fractions is unity; thus, in a ternary system A–B–C: x A + x B + x C =1
(4.44)
and there are two independent compositional variables. A representation of composition, symmetrical with respect to all three components, may be obtained from the equilateral composition triangle as shown for the system A–B–C in Figure 4.15. The three corners of the triangle correspond to the three pure components. Along the three edges are found the compositions corresponding to the three binary systems A–B, B–C and A–C. Lines of constant mole fraction of component A are parallel to the B–C edge (exemplified by the broken line for x A = 0 .2), while lines of constant mole fraction of B and C are parallel to the A–C and A–B binary edges respectively (exemplified by broken lines for x B = 0 .2 and x C = 0 .6). The three lines intersect at the point marked X, which thus have the composition x A = 0 .2, x B = 0 .2, x C = 0 .6. Note that the sum of the lengths of the perpendiculars from any composition point to the three edges is constant (using the point X as an example once more, the perpendiculars are given by bold lines in the figure). It is upon this property that the representation is based and the three perpendiculars are measures of the mole fractions of the three components.
4.2 Multicomponent systems
111
(a) (b)
Figure 4.16 (a) Triangular prism phase diagram for a ternary system A–B–C with the equilateral triangular base giving composition. Temperature is given along the vertical axis [17]. (b) Projection of the liquidus surface onto the ternary composition triangle. The bold line is the intersection between the primary crystallization fields of C and the solid solution a. The dashed line represents the extension of the solid solution a. Reprinted with permission of The American Ceramic Society, www.ceramics.org. Copyright [1984]. All rights reserved.
To represent a ternary system at constant pressure completely, the effect of temperature must be incorporated in the phase diagram. Such a ternary temperature–composition phase diagram at constant pressure may be plotted as a threedimensional space model using a triangular prism. The ternary composition triangle would then form the base while temperature is given along the vertical axes as shown in Figure 4.16(a) for a hypothetical ternary system A–B–C [17]. On the three faces of the prism we find the phase diagrams of the three binary systems A–B, B–C and A–C. In the hypothetical system illustrated in Figure 4.16(a) complete solid solubility is present in the close to ideal binary system A–B (the solid solution phase is denoted a), while the two other binary systems B–C and A–C are eutectic systems with a limited solubility of C in the solid solution phase a. Recall that the Gibbs phase rule gives F + Ph = C + 1 = 4 for a ternary system at constant pressure. Within the prism two liquidus surfaces are shown: one descending from the melting temperature of pure C and the other from the liquidus of a in the binary A–B system. Compositions on the two surfaces corresponds to compositions of the liquid in equilibrium with one of the two solid phases, C or a. For an equilibrium between a solid and the liquid, Ph = 2 and thus F = 2; the two surfaces are divariant. The two liquidus surfaces intersect along the univariant line (F = 1) starting from one of the binary eutectics (E1) and ending in the other (E2). The intersection of adjoining liquidus surfaces in a ternary phase diagram is generally termed
112
4 Phase diagrams
a common boundary line. Along the univariant common boundary line three phases (liq, C and a) are in equilibrium. In the present case there are no ternary invariant equilibria in the system, partly due to the complete solid solubility of the A–B system. In a ternary system composed from three binary eutectic subsystems, three univariant lines would meet in a ternary eutectic equilibrium: liq. « A(ss) + B(ss) + C(ss)
(4.45)
which is an invariant equilibrium at isobaric conditions. Phase diagrams based on the triangular prism give an illustrative representation of isobaric ternary systems, but the construction of the diagram is very timeconsuming and of less convenience. A more convenient twodimensional representation of the ternary liquidus surface may be obtained by an orthogonal projection upon the base composition triangle. This is shown for the system A–B–C in Figure 4.16(b) [17]. The lines of constant temperature are called liquidus isotherms. In Figure 4.16(b) the bold line shows the common boundary line of the two liquidus surfaces descending from the melting temperature of pure C and from the liquidus of a in the binary A–B system discussed above. Often an arrow is used to indicate the direction of decreasing temperature along univariant lines. We will now apply Figure 4.16 to find the equilibrium behaviour of a sample with overall composition marked P in the diagrams, when it is cooled from above the liquidus surface to below the solidus temperature for the given overall composition. The point marked P lies within the primary crystallization field of a. That is, it lies within the composition region in which a will be the first solid to precipitate during cooling. When cooling the liquid, a will start to precipitate when the liquidus temperature is reached just below 700 °C; see Figure 4.16(b). During further cooling the amount of solid a will increase at the expense of the amount of liquid. It is important to note that the composition of a is not constant during the crystallization. Two selected isothermal sections of the phase diagram that show relevant twophase equilibria are given in Figure 4.17 [17]. The thin lines illustrate the tielines between the compositions of two phases in equilibrium (a + liq.) or (C + liq). The tieline going through the overall composition point P in Figure 4.17(a) defines the composition of the two conjugate phases, a and liquid, at that particular temperature. During cooling the composition of a is enriched on A and also the composition of the liquid changes. The two phases remain in equilibrium until the liquid reaches the intersection of the primary crystallization fields of a and phase C. At this temperature, the second solid phase, denoted phase C, will start to precipitate in addition to a. On further cooling, the composition of the liquid is defined by the common boundary line from E1 to E2 in Figure 4.16, where the liquid is in equilibrium with a and C. The compositions of the three phases in equilibrium are given by a triangle in an isothermal section. This is illustrated for the temperature corresponding to that where the liquid phase disappears, i.e. when P reaches the edge of
4.2 Multicomponent systems
(a)
113
(b)
Figure 4.17 Isothermal sections of the ternary phase diagram A–B–C shown in Figure 4.16 at (a) 650 °C and (b) 450 °C [17]. Here L denotes liq. Reprinted with permission of The American Ceramic Society, www.ceramics.org. Copyright [1984]. All rights reserved.
the threephase triangle in Figure 4.17(b). On further cooling the two solid phases remain in equilibrium. Since the solubility limit of a decreases with decreasing temperature, the relative amounts of the two phases in equilibrium also change. A sample in the primary crystallization field of phase C will behave differently during crystallization. Here phase C precipitates with composition identical to C (no solid solubility) during cooling keeping the A:B ratio in the melt constant until the melt hits the intersection of the two primary crystallization fields. At this temperature a will start to precipitate together with further C and from this point on the cooling process corresponds to that observed for the sample with overall composition P after this sample reaches the same stage of the crystallization path. The relative amount of the different phases present at a given equilibrium is given by the lever rule. When the equilibrium involves only two phases, the calculation is the same as for a binary system, as considered earlier. Let us apply the lever rule to a situation where we have started out with a liquid with composition P and the crystallization has taken place until the liquid has reached the composition 2 in Figure 4.17(a). The liquid with composition 2 is here in equilibrium with a with composition 2 ¢. The relative amount of liquid is then given by y liq =
2¢P 2¢2
(4.46)
where 2 ¢P denotes the distance between 2 ¢ and P and 2 ¢2 that from 2 ¢ to 2. The amount of solid (a) ya is given by 1  y liq . With three phases in equilibrium, the relative amounts of the three phases are also given by the lever rule, but its use is slightly more complex. In this case the relative amounts of the three phases are determined in terms of a triangle defined by the composition of the three phases in equilibrium. A line from each of the three corners is drawn through the point representing the overall composition of the sample to the opposite edge. The relative
114
4 Phase diagrams
Figure 4.18 Phase diagram for the ternary system NaF–MgF2–CaF2 [18]. Reprinted with permission © 2001 by ASM International and TMS (The Minerals, Metals and Materials Society).
amount of a given phase (represented as a corner in the diagram) is defined as the length of the line from the overall composition to the opposite edge divided by the total length from the corner to the edge. This is illustrated in Figure 4.15. Here the relative amount of phase B for a sample with overall composition X is equal to QX/QP. Similar procedures for the two other components give the relative amount of all three phases in equilibrium. Let us now consider two real ternary systems to illustrate the complexity of ternary phase diagrams in some detail. While the first is a system in which the solid state situation is rather simple and attention is primarily given to the liquidus surfaces, the solid state is the focus of the second example. The phase diagram of the ternary system NaF–MgF2–CaF2 is shown in Figure 4.18 [18]. Of the three binary subsystems NaF–CaF2 and MgF2–CaF2 are simple eutectic systems, while an intermediate phase, NaMgF3, is formed in the third system, NaF–MgF2. The latter can however be divided into two simple eutectic subsystems: NaF–NaMgF3 and NaMgF3–MgF2. The overall system consists of the four solid phases described above, all with their own primary crystallization field and all four phases melt congruently. The borderline between the primary crystallization fields of the phases are shown as bold lines. Two ternary eutectics are shown with the eutectic compositions within the two ternary subsystems NaF–CaF2–NaMgF3 and CaF2–MgF2–NaMgF3. The binary join between CaF2 and NaMgF3 is termed a true Alkemade line defined as a join connecting the compositions of two primary phases having a common boundary line. This Alkemade line intersects the boundary curve separating the primary phases CaF2 and NaMgF3. The point of intersection represents the temperature maximum on the
4.2 Multicomponent systems
(a)
115
(b)
Figure 4.19 Isothermal sections of the ternary system C–Si–Ti at (a) 1400 °C and (b) 1800°C [10]. Reprinted with permission of The American Ceramic Society, www.ceramics.org. Copyright [2000]. All rights reserved.
boundary curve, while the liquidus along the Alkemade line has a minimum at the same composition; hence the intersection represents a saddle point. If the Alkemade line does not intersect the boundary curve, then the maximum on the boundary curve is represented by that end which if prolonged would intersect the Alkemade line. The binary join NaF–MgF2 is not an Alkemade line since these two solid phases are not coexistent. Finally, the a–b CaF2 phase transition at 1151 °C is shown as a bold line in the figure. For ternary systems with complex phase behaviour in the solid state it is more convenient to use only isothermal sections. This is shown for two temperatures for the ternary system Ti–Si–C in Figure 4.19 [10]. In this system several binary and ternary intermediate phases are stable, and the system is divided into several ternary subsystems. Tielines for twophase equilibria are also shown in the two isothermal sections. Quaternary systems In a quaternary system, three dimensions are required to represent composition and a fourth dimension is needed for the temperature if the temperature dependence is to be displayed. Since we live in a threedimensional world this is awkward. The dilemma is partly overcome by constructing a diagram, which is analogous to the plane projection made for ternary systems. This is shown for the system A–B–C–D in Figure 4.20. The phase diagram is a tetrahedron, and the four corners of the tetrahedron correspond to the four components. The four faces of the tetrahedron correspond to the plane projections of the four limiting ternary systems. The Gibbs phase rule for the quaternary system at isobaric conditions is Ph + F = C + 1 = 5. With only a single phase present and for a given temperature, three composition variables may be varied (i.e. F = 3), and the stability field for each phase is thus a
116
4 Phase diagrams
Figure 4.20 Tetrahedron space model for the phase diagram of the quaternary system A–B–C–D. The isotherms T1, T2, T3 are shown for the primary phase volume of component A [17]. Reprinted with permission of The American Ceramic Society, www.ceramics.org. Copyright [1984]. All rights reserved.
volume in the tetrahedron. Two phases are in equilibrium along surfaces, three phases are present in univariant equilibria and finally there are four phases in invariant equilibria. The addition of further components makes the presentation of the phase diagrams increasingly complex. The principles are general, however, and calculation of a vertical section in a quinternary system like Fe–Cr–Mo–W–C [19], for example, is fairly easily done by the use of large computer programs for calculation of phase diagrams based on thermodynamics. Ternary reciprocal systems A ternary reciprocal system is a system containing four components, but where these components are related through a reciprocal reaction. One example is the system LiCl–LiF–KCl–KF. Solid LiCl, LiF, KCl and KF are highly ionic materials and take the rock salt crystal structure, in which the cations and anions are located on separate sublattices. It is therefore convenient to introduce ionic fractions (Xi) for each sublattice as discussed briefly in Section 3.1. The ionic fractions of the anions and cations are not independent since electron neutrality must be fulfilled: X F  + X Cl  = X Li + + X K+ =1
(4.47)
For this reason, the system is defined by the four neutral components LiCl, LiF, KCl and KF, which in addition can be related by the reciprocal reaction
4.3 Predominance diagrams
117
Figure 4.21 Calculated phase diagram of the ternary reciprocal system LiCl–LiF–KCl–KF [20]. Reprinted with permission © 2001 by ASM International and TMS (The Minerals, Metals and Materials Society).
LiCl + KF = LiF + KCl
(4.48)
The sign of the Gibbs energy of this reciprocal reaction determines which of the two pairs of compounds are coexistent at a given temperature (and pressure). In our specific case, the Gibbs energy of the reciprocal reaction is negative and the products are coexistent phases, while the reactants are not. A reciprocal ternary phase diagram is in general constructed by the combination of two ternary systems that both contain the two coexistent phases. Thus in the present case the ternary phase diagrams of the systems LiF–KCl–LiCl and LiF–KCl–KF are combined. The calculated phase diagram of the ternary reciprocal system considered is shown in Figure 4.21 [20]. Here the sign of the reciprocal reaction is reflected in that the stable diagonal in the system is LiF–KCl and not LiCl–KF. Both the ternary systems are simple eutectic ones and the composition of the system is represented by the ionic fraction of one of the cations and one of the anions. In Figure 4.21 the ionic fraction of Li+ is varied along the Xaxis, while the ionic fraction of F– is varied along the Yaxis.
4.3 Predominance diagrams In the preceding sections the phase diagrams have been represented in terms of composition. Alternatively, the chemical potential of one or more of the components may be used as variables. This gives rise to a range of similar diagrams that
118
4 Phase diagrams 0
log ( pO2 / bar)
–5
Fe2O3
–10 Fe 3O4
FeO
–15
–20
bFe
aFe 600
800
1000
1200
T / °C
Figure 4.22 log pO 2 versus T predominance phase diagram for the binary system Fe–O. Thermodynamic data are taken from reference [21].
have many applications in materials science. These will here be termed predominance diagrams. They are of great importance for understanding materials’ stability under hostile conditions (for example hot corrosion) and in planning the synthesis of materials; for example for chemical vapour deposition. In addition to being of great practical value, they also further illustrate the principles of Gibbs energy minimization and the Gibbs phase rule. In predominance diagrams one or more base elements are defined which must be present in all the condensed phases. A predominance diagram for the binary system Fe–O is shown in Figure 4.22. The diagram is divided into areas or domains of stability of the various solid phases of the Fe–O system. In this simple binary case the base element is iron, which is present in all five condensed phases in the system: three oxides and two solid modifications of Fe. The Gibbs phase rule reads Ph + F = C + 2 = 4 if the pressure of oxygen is considered as the mechanical potential p. Alternatively, ptot may be considered to be constant e.g. 1 bar. In the latter case, a third component, an inert gas, must be added to the system to maintain the isobaric condition. Thus Ph + F = C + 1, which for C = 3 again gives Ph + F = 4. In conclusion, we may have a maximum of four phases in equilibrium: three condensed phases and a gas phase. A univariant line (F = 1) is for this two component system a phase boundary separating the domains of two condensed phases, for instance Fe3O4 and Fe2O3. These univariant lines are defined by heterogeneous phase equilibria like 4/3 Fe3O4(s) + 1/3 O2(g) = 2 Fe2O3(s)
(4.49)
The stability fields for the condensed phases correspond to F = 2, which means that both temperature and the partial pressure of O2 can be varied independently. In order to derive the phase boundaries in Figure 4.22 we need the Gibbs energy of formation of the oxides. This type of data is conveniently given in an Ellingham
4.3 Predominance diagrams
119
0P
0
2 CuO
–200
–5
2 CoO
2 PbO
2 H2O 2/3 Fe 2O3
O3 2 /3 Mn2
–15
SiO2
(
o
2 ZnO
2
–600
–10
)
CO2
log pO / bar
DG / kJ mol –1
MoO 2
–400
–20
–800 TiO 2
–25
–1000
Z rO2 l O 3 2 MgO 2 CaO 2/3 A 2
–30 –1200 0
500
1000
1500
2000
T /K
Figure 4.23 Ellingham diagram for various metal oxides. Thermodynamic data are taken from reference [21].
diagram [22,23] where the Gibbs energy ‘of formation’ of various oxides is plotted versus the temperature, as shown in Figure 4.23. Note that the Gibbs energy of formation is given per mole O2, which is not in accordance with the definition of the energies of formation given in Chapter 1 and used frequently thereafter. For a binary oxide like Fe2O3 the reaction in question is 4/3 Fe(s) + O2(g) = 2/3 Fe2O3(s)
(4.50)
Assuming that the metal and oxygen are in their standard states, the equilibrium constant corresponding to reaction (4.50) is given as K = 1/ pO2 = exp( D r G o / RT )
(4.51)
If the oxygen partial pressure is lower than pO2 = 1/K the reactant (in our case Fe) is stable. If it is higher, the product (in our case Fe2O3) is formed. The slopes of the lines in the Ellingham diagram are given by the entropy change of the formation reaction: D r S o . The entropy changes are in general negative due to the consumption of gas molecules with higher entropy and the slopes are thus positive. In the large scale of the plot the lines appear to be linear, suggesting
120
4 Phase diagrams
constant entropies of the reactions (or in other words that the difference in heat capacity between the reactants and products is zero). On a different scale the curvature of the Gibbs energy curves is visible. Furthermore, it should be noted that the breaks in the slopes of the curves are due to firstorder phase transitions of the metal or the oxide. The Ellingham diagram contains a lot of useful information. By drawing a line from the point P that intersects the Gibbs energy curve of a particular compound at a temperature of interest, the partial pressure that corresponds to decomposition/ formation of the oxide from pure metal and gas at that particular temperature can be derived. The partial pressure of oxygen is obtained by extrapolation to the log pO2 scale on the righthand side of the diagram. For example, at 1000 K the partial pressure of oxygen corresponding to equilibrium between Zn and its monoxide, ZnO, is 10–26 bar. From the diagram in Figure 4.23 it is evident that the oxides with the more negative Gibbs energies of formation have the highest stability and are harder to reduce to the elemental state. In materials science, the controlled partial pressure of oxygen is often obtained by using gas mixtures. Here the ratio of the partial pressures of e.g. H2(g) and H2O(g) or CO(g) and CO2(g) are varied to give the desired pO2 at a given temperature. The ratios pH 2 / pH 2O and pCO / pCO2 are related to the partial pressure of O2 by the reactions 2H2O(g) = 2H2(g) + O2(g)
(4.52)
2CO2(g) = 2CO(g) + O2(g)
(4.53)
Calculated ratios pCO / pCO2 and pH 2 / pH 2O for selected partial pressures of oxygen at a total pressure of 1 bar are given in Figure 4.24. The equilibrium between a metal and an oxide in a CO–CO2 atmosphere can then be obtained by combining the formation reaction of the oxide with reaction (4.53). As an example the equilibrium between Co, O2 and CoO combined with reaction (4.53) gives Co(s) + CO2(g) = CO(g) + CoO(s)
(4.54)
After finding the partial pressure of oxygen at a given temperature through Figure 4.23, the composition of the gas mixture is obtained from Figure 4.24(a). Let us now include an additional component to the Fe–O system considered above, for instance S, which is of relevance for oxidation of FeS and for hot corrosion of Fe. In the Fe–S–O system iron sulfides and sulfates must be taken into consideration in addition to the iron oxides and ‘pure’ iron. The number of components C is now 3 and the Gibbs phase rule reads Ph + F = C + 2 = 5, and we may have a maximum of four condensed phases in equilibrium with the gas phase. A twodimensional illustration of the heterogeneous phase equilibria between the pure condensed phases and the gas phase thus requires that we remove one degree of
4.3 Predominance diagrams
121 –30
log ( p CO / p CO2 )
0
(b) 10 –25 –20 –15 –10 –5
0 log pO2 =
–10
–20
–30
–30
0 log ( p H2 / p H2O )
(a) 10
–25 –20 –15 –10 –5
0 log pO2=
–10
–20
500
1000
1500
–30
2000
500
1000
T/K
1500
2000
T/K
Figure 4.24 Relationship between the partial pressure of oxygen and the composition of CO–CO2 and H2–H2O gas mixtures at 1 bar. (a) pCO / pCO 2 versus temperature and (b) pH 2 / pH 2 O versus temperature at selected partial pressures of oxygen. Thermodynamic data are taken from reference [21].
freedom. This can be done by keeping either the temperature or a chemical potential constant. To exemplify the former choice, the isothermal predominance diagram for the Fe–S–O system at 800 K is shown in Figure 4.25. Here the partial pressures of SO2 and O2 are used as variables. An univariant line (F = 1) or phase boundary separates domains of two different condensed phases. For Fe2O3 and FeSO4 this line is defined by the heterogeneous phase equilibrium
log ( pSO2 / bar)
2
FeS2
FeSO4 Fe2(SO4)3
0
–2 Fe 3O4
Fe 2O3
–4 –20
–15
–10
–5
0
log (pO2 / bar)
Figure 4.25 log pSO 2 versus log pO 2 predominance diagram for the system Fe–S–O at 527 °C. Thermodynamic data are taken from reference [21].
122
4 Phase diagrams 1 Fe O (s) + SO (g) + 1 O (g) = FeSO (s) 2 4 2 2 3 4 2
(4.55)
æ ç 1 D r G o = RT ln K = RT lnç 1/ 4 ç pSO2 pO 2 è
(4.56)
Since ö ÷ ÷ ÷ ø
the phase boundary is given by the line log K =  log pSO2  1 log pO2 , where K is 4 the equilibrium constant for reaction (4.55). The domain of stability for each of the condensed phases corresponds to two degrees of freedom (F = 2), while three condensed phases are in equilibrium with the gas phase at an invariant point (F = 0). Three lines corresponding to three different univariant phase equilibria meet at an invariant point. As indicated above, rather than keeping the temperature constant, we can replace the partial pressure of one of the gas components with the temperature as a variable. Figure 4.26 is a diagram of the Fe–S–O system in which ln pO2 is plotted versus temperature. Here pSO2 is fixed in order to allow a twodimensional representation. There are in principle no restrictions on the number of components in a predominance diagram and examples of four and fivecomponent systems are shown in Figure 4.27. In Figure 4.27(a) the predominance diagram of the system Si–C–O–N at 1500 K is given as a function of log pO2 and log pN 2 . The system has four components, and Si and C are the two base elements. The amount of Si is assumed to be in excess relative to SiC. At constant temperature, the Gibbs phase rule gives Ph + F = C + 1 = 5. Thus at an invariant point four condensed phases are in equilibrium with the gas phase. Two such invariant points are evident in Figure 4.27(a). Three condensed phases are in equilibrium along the lines in the diagram (F = 1), whereas 1200 1100
FeS(l)
FeS2
Fe 3O4
T / °C
1000 FeS
900 800
Fe 2O3
700 Fe 2(SO4) 3
600 –20
–15
–10
–5
0
log (pO2 / bar)
Figure 4.26 T versus log pO 2 predominance diagram for the Fe–S–O system at pSO 2 = 01 . bar. Thermodynamic data are taken from reference [21].
4.3 Predominance diagrams
123 –4
–18 (a)
(b)
SiC + 3Al 2O3·2SiO2
SiO2 + C
SiO2 + SiC
–22 –24
Si + SiC
Si3N4 + SiC
Si3N4 +C
–26
log ( pCO2 / bar)
log ( pO 2 / bar)
–20
SiO2 + 3Al2O3 ·2SiO2
–6
Si3N4 + 3Al2O3·2SiO2
Si3N4 + Al2O3
unstable gas mixture
–8 Si3N4 +
–28 –8
SiC + Al 2O3
SiC + AlN
AlN
–6 –4 –2 log (pN2 / bar)
0
–4
–3 –2 –1 log (pCO / bar)
0
Figure 4.27 (a) Predominance diagram for the system Si–C–O–N at 1500 K, N Si > N C. (b) Predominance diagram for the system Al–Si–C–O–N at 1700 K and pN 2 = 0.5 bar, N Si > 0.25 N Al . Thermodynamic data are taken from reference [21].
two condensed phases are coexistent in the twodimensional phase fields. Si 3N4 and SiC, which are often present in ceramic composites, are only thermodynamically coexistent in a narrow log pN 2 range at low partial pressures of O2. Thermodynamic data for the oxynitride phase Si 2ON2 are not available, but at 1500 K it has a narrow stability region between SiO2 and Si3N4. In Figure 4.27(b) the predominance diagram of the fivecomponent system Si–Al–C–O–N is shown as a function of log pCO2 and log pCO at a constant partial pressure of N2 equal to 0.5 bar at 1700 K. The two base elements of the plot are Si and Al (n Si > 025 . n Al ). The Gibbs phase rule reads Ph + F = C + 2 = 7, which at constant temperature and constant partial pressure of N2 gives Ph + F = 5. The predominance diagram shown in Figure 4.27(b) is therefore analogous to the one shown in Figure 4.27(a), in that the same number of phases is present for a certain degree of freedom. Aluminium nitride is only stable at low partial pressures of CO and CO2. Note that the gas mixture in the lower right corner in Figure 4.27(b) is unstable due to the Boudouard reaction C(s) + CO2(g) = 2 CO(g)
(4.57)
At 1700 K the equilibrium constant for this reaction is K = 6946 = p2CO / pCO2
(4.58)
The CO–CO2 gas mixture is therefore unstable at conditions below the line defined by eq. (4.57) and will here lead to formation of graphite. It may be useful to note
124
4 Phase diagrams (a)
–40
0
m (O) RT
m(Co) RT
0
–170
0
m (Ti) / RT
–120
(b)
Figure 4.28 (a) Threedimensional chemical potential diagram for the system Co–Ti–O at 1000 K. (b) Twodimensional chemical potential diagram at the same conditions [24]. Reprinted with permission of The American Ceramic Society, www.ceramics.org. Copyright [1989]. All rights reserved.
that in many commercial thermodynamic software packages it is not prohibited to calculate phase equilibria for unstable gas compositions, and care should be taken. In cases where ternary compounds, e.g. oxides, are being investigated, other related types of diagrams may be more efficient. The thermodynamic stability of ternary oxides at constant pressure, for example, is visually well represented in threedimensional chemical potential diagrams [24]. In Figure 4.28(a) the phase relations in the system Co–Ti–O are plotted as a function of the chemical potential of the three elements. At constant temperature, the Gibbs phase rule gives Ph + F = 3 + 1 = 4, and an invariant point corresponds to three condensed phases in equilibrium with the gas phase. The stability field of each single phase is given as a plane, while two phases are in equilibrium along univariant lines. The same phase equilibria may also be represented in two dimensions, as exemplified by Figure 4.28(b). Here the stability of the metallic elements and their binary oxides and double
4.3 Predominance diagrams
125
oxides are presented as areas in a log( a A / a B ) versus log pO2 plot (at constant temperature). Complex phase relations for double oxides are in this way visualized in a clear and compact manner.
References [1]
[2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21]
[22] [23] [24]
P. R. Subramanian and J. H. Perepezko, Ag–Cu (silver–copper) system, in Phase Diagrams of Binary Copper Alloys (P. R. Subramanian, D. J. Chakrabarti and D. E. Laughlin, eds.). Materials Park, OH: ASM International, 1994. C. Bergman, R. Chastel and R. Castanet, J. Phase Equilibria 1992, 13, 113. P. Wu, G. Eriksson and A. D. Pelton, J. Am. Ceram. Soc. 1993, 76, 2065. NISTJANAF Thermochemical Tables, 4th edn (M. W. Chase Jr, ed.). J. Phys. Chem. Ref. Data Monograph No. 9, 1998. A. D. Pelton, A. Gabriel and J. Sangster, J. Chem. Soc. Faraday Trans. 1, 1985, 81, 1167. Y. Du and Z. P. Jin, J. Alloys and Comp. 1991, 176, L1. S. S. Kim and T. H. Sanders Jr, J. Am. Ceram. Soc. 2001, 84, 1881. A. D. Pelton and W. T. Thompson, Progr. Solid State Chem. 1975, 10, 119. Y. Du, Z. P. Jin and P. Y. Huang, J. Am. Ceram. Soc. 1992, 75, 3040. Y. Du, J. C. Schuster, H. J. Seifert and F. Aldinger, J. Am. Ceram. Soc., 2000, 83, 197. C. H. P. Lupis, Chemical Thermodynamics of Materials, New York: NorthHolland, 1983, p. 221. S. Stølen and F. Grønvold, J. Chem. Thermodyn. 1999, 31, 379. H. Ohtani and K. Ishida, J. Electron. Mater. 1994, 23, 747. B. Jönsson and J. Ågren, Mater. Sci. Techn. 1986, 2, 913. N. L. Allan, J. D. Blundy, J. A. Purton, M. Yu. Laurentiev and B. J. Wood, EMU Notes in Mineralogy, 2001, 3(11), 251. S. I. Sandler, Pure Appl. Chem. 1999, 71, 1167. C. G. Bergeron and S. H. Risbud, Introduction to Phase Equilibria in Ceramics, The American Ceramic Society, Westerville, Ohio, 1984. P. Chartrand and A. D. Pelton, Metal. Mater. Trans. 2001, 32A, 1385. B. Jönsson and B. Sundman, High Temp. Sci. 1990, 26, 263. P. Chartrand and A. D. Pelton, Metal. Mater. Trans. 2001, 32A, 1417. C. W. Bale, A. D. Pelton and W. T. Thompson, F*A*C*T (Facility for the Analysis of Chemical Thermodynamic), Ecole Polytechnique, Montreal, 1999, http:// www.crct.polymtl.ca/. H. T. T. Ellingham, J. Soc. Chem. Ind. 1944, 63, 125. F. D. Richardson and J. H. E. Jeffes, J. Iron Steel Inst. 1948, 160, 261. H. Yokokawa, T. Kawada and M. Dokiya, J. Am. Ceram. Soc. 1989, 72, 2104.
Further reading J. W. Gibbs, The Collected Works, Volume I Thermodynamics. Harvard: Yale University Press, 1948. M. Hillert, Phase Equilibria, Phase Diagrams and Phase Transformations. Cambridge: Cambridge University Press, 1998. L. Kaufman and H. Bernstein, Computer Calculation of Phase Diagrams. New York: Academic Press, 1970.
126
4 Phase diagrams
C. H. P. Lupis, Chemical Thermodynamics of Materials, New York: NorthHolland, 1983. A. Prince, Alloy Phase Equilibria. Amsterdam: Elsevier Science, 1966. A. D. Pelton, Phase diagrams, in Physical Metallurgy, 4th edn (R. W. Cahn and P. Haasen, eds.). Amsterdam: Elsevier Science BV. Volume 1, Chapter 6, 1996. N. Saunders, and A. P. Miodownik, CALPHAD: Calculation of Phase Diagrams. Oxford: Pergamon, Elsevier Science, 1998. W. R. Smith and R. W. Missen, Chemical Reaction Equilibrium Analysis: Theory and Algorithms. New York: Wiley, 1982.
5
Phase stability
When referring to a phase as stable in thermodynamics we usually mean the phase that has the lowest Gibbs or Helmholtz energy at the given conditions. In Section 1.1 the concept of metastability was introduced. Both stable and metastable phases are in local equilibrium, but only the thermodynamically stable phase is in global equilibrium; a metastable state has higher Gibbs energy than the true equilibrium state. We may also have unstable phases, and here, as will be described further below, the nature of the instability is reflected in the second derivative of the Gibbs energy with regard to the thermodynamic potentials defining the system. Both stable and metastable states are in internal equilibrium since they can explore their complete phase space, and the thermodynamic properties are equally well defined for metastable states as for stable states. However, there is a limit to how far we can extend the metastable region with regard to temperature, pressure and composition. If we use temperature as a variable, there is a limit to superheating a crystal above its melting temperature or cooling a liquid below its freezing temperature. A supercooled liquid will either crystallize or transform to a glass. Glasses are materials out of equilibrium or in other words nonergodic states; glasses cannot explore their complete phase space and some degrees of freedom are frozen in. An analogous situation is obtained if we consider pressure as variable instead of temperature. Some crystals may exist, as metastable phases, far above the pressure where thermodynamically they should transform to a denser highpressure polymorph. However, there is a limit for ‘superpressurizing’ a crystal above its transformation pressure. The phase will either recrystallize (in a nonequilibrium transition) to the more stable phase, or transform to an amorphous state with higher density. To make the analogy with superheating and supercooling complete, highpressure phases may remain as metastable states when the pressure is released. Chemical Thermodynamics of Materials by Svein Stølen and Tor Grande © 2004 John Wiley & Sons, Ltd ISBN 0 471 492320 2 127
128
5 Phase stability
However, at some specific pressure the highdensity polymorph becomes mechanically unstable. This lowpressure limit is seldom observed, since it often corresponds to negative pressures. When the mechanical stability limit is reached the phase becomes unstable with regard to density fluctuations, and it will either crystallize to the lowpressure polymorph or transform to an amorphous phase with lower density. Phases may also become unstable with regard to compositional fluctuations, and the effect of compositional fluctuations on the stability of a solution is considered in Section 5.2. This is a theme of considerable practical interest that is closely connected to spinodal decomposition, a diffusionfree decomposition not hindered by activation energy. Since the formation of a stable phase may be kinetically hindered, it is of interest to calculate phase diagrams without the presence of a particular phase. This is an exercise easily done using thermodynamic software for phase diagram analysis, but the general effects can be understood based on Gibbs energy rationalizations. Closely related to this topic is the thermal evolution of metastable states with time. The reactivity of a metastable phase is governed by both thermodynamic and kinetic factors. Although the transformation toward equilibrium is irreversible, the direction is given, and the rate of transformation influenced, by the Gibbs energy associated with the transformation. Finally, kinetic factors are also of great importance in many other applications of materials and kinetic demixing, and decomposition of materials in potential gradients are briefly described in the last section of the chapter.
5.1 Supercooling of liquids â€“ superheating of crystals It is well known that a liquid can be cooled below its equilibrium freezing temperature. The crystallization of the stable crystalline phase is hindered due to an activation barrier caused by the surface energy of the crystal nuclei. In some cases, such as B2O3, stable crystals barely form, and the supercooled liquid turns into a glass even at very slow cooling rates. In other cases high cooling rates are needed to produce glasses, notably metallic glasses where cooling rates of the order of 10 6 K sâ€“1 might be needed. The supercooled liquid passes through a transition to a glass at the glass transition temperature, Tg, which is typically 2 of the melting tempera3 ture, Tfus. At this transition some degrees of freedom are frozen in and the sample becomes nonergodic. Since, the transition is an outofequilibrium transition, the properties of the resulting glass depend on its thermal history (see Section 8.5). The entropy difference between the supercooled liquid and the crystal is given by o o D fus S m (T ) = D fus S m (T fus ) +
T
Ă˛
Tfus
DC po T
dT
(5.1)
5.1 Supercooling of liquids – superheating of crystals
129
o where D fus S m (T fus ) is the standard entropy of fusion at the melting temperature o and DC p is the difference between the standard heat capacity of the supercooled liquid and the stable crystalline phase. Many supercooled liquids possess heat capacities that substantially exceed those of the corresponding crystals, as in the case of selenium shown in Figure 5.1(a) [1–3]. The entropy difference between a crystal and the corresponding liquid, which is positive at the fusion temperature, is reduced with decreasing temperature and become zero at some temperature below the equilibrium freezing temperature. Although helium3 melts exothermally [4], a negative entropy of fusion is in general considered to be a paradox since the entropy of the disordered phase then becomes lower than the entropy of the ordered phase. This argument was first put forward by Kauzman [5] and is often referred to as the Kauzmann paradox. By extrapolation of the heat capacity of the supercooled liquid below its Tg, the temperature at which the entropy of fusion becomes zero can be calculated. This temperature is called the Kauzmann temperature, TK, or the ideal glass transition temperature. The entropy of crystalline and liquid selenium is shown as an example in Figure 5.1(b). Here the entropy of the supercooled liquid crosses the entropy of crystalline Se at around T = 180 K. Kauzmann proposed that this paradox is avoided through a nonequilibrium transition above the ideal glass transition temperature where a glass is formed. Experiments have confirmed this prediction and all known glassforming liquids display a glass transition at temperatures above TK. For our example, Se, the glass transition temperature is approximately 120 K above the Kauzmann temperature. Unlike supercooling of liquids, superheating of crystalline solids is difficult due to nucleation of the liquid at surfaces. However, by suppressing surface melting, superheating to temperatures well above the equilibrium melting temperature has
(a)
(b) Se
40
90
Tfus
Se
o Cp,m / J K–1 mol –1
Smo / J K–1 mol –1
liquid Tg
liquid
35
30
supercooled 60 liquid Tg
30 25 200
solid TK
Tfus solid 400
600
800
1000
0
0
200
400 600 T/K
800 1000
Figure 5.1 (a) Heat capacity of crystalline, liquid and supercooled liquid Se as a function of temperature [1–3]. (b) Entropy of crystalline, liquid and supercooled liquid Se as a function of temperature.
130
5 Phase stability
been achieved. As for many other phenomena in physical sciences, superheating is discussed using both kinetic and thermodynamic arguments. Of the early models, those by Lindemann [6] and Born [7] are the most important. Lindemann [6] proposed that bulk melting is caused by a vibrational instability in the crystal lattice when the root mean displacement of the atoms reaches a critical fraction of the distance between them. Somewhat later, Born [7] proposed that a ‘rigidity catastrophe’ caused by a vanishing elastic modulus determines the melting temperature of the bulk crystal in the absence of surfaces. The conditions for mechanical instability can be derived from a set of criteria for the stability of equilibrium systems put forward by Gibbs [8]. Considering instability with regard to temperature and pressure, the criteria for stability are æ ¶2 G ç ç ¶ p2 è
ö ÷ = æç ¶V ç ÷ ø T è ¶p
æ ¶2 G ç ç ¶T 2 è
ö ÷ =  æç ¶S ö÷ < 0 ÷ è ¶T ø p øp
ö ÷÷ < 0 øT
(5.2)
(5.3)
Equation (5.2) requires that the bulk modulus is positive. KT =
1 V =>0 kT (¶V / ¶p) T
(5.4)
When this criterion is fulfilled the compound is stable with respect to the spontaneous development of inhomogeneities in the average atomic density. The phase is in other words stable with regard to infinitesimal density fluctuations. Equation (5.3) requires that the heat capacity is positive. Equation (5.2) also implies that a crystalline solid becomes mechanically unstable when an elastic constant vanishes. Explicitly, for a threedimensional cubic solid the stability conditions can be expressed in terms of the elastic stiffness coefficients of the substance [9] as C11 + 2C12 > 0
(5.5)
C 44 > 0
(5.6)
C11  C12 > 0
(5.7)
The complexity of the stability conditions increases the lower the symmetry of the crystal. For an isotropic condensed phase, such as a liquid or fluid the criteria can be simplified. Here, C11  C12 = 2C 44 and the stability conditions reduce to
5.1 Supercooling of liquids – superheating of crystals
131
3K T = 2C 44 + 3C12 > 0
(5.8)
C 44 > 0
(5.9)
where KT is the bulk modulus and C44 is the shear modulus. The temperature dependences of the isothermal elastic moduli of aluminium are given in Figure 5.2 [10]. Here the dashed lines represent extrapolations for T > Tfus. Tallon and Wolfenden found that the shear modulus of Al would vanish at T = 1.67Tfus and interpreted this as the upper limit for the onset of instability of metastable superheated aluminium [10]. Experimental observations of the extent of superheating typically give 1.1Tfus as the maximum temperature where a crystalline metallic element can be retained as a metastable state [11]. This is considerably lower than the instability limits predicted from the thermodynamic arguments above. In recent years other types of thermodynamic arguments for the upper limit for superheating a crystal have also been proposed. One argument is based on the fact that the heat capacity of the solid increases rapidly with temperature above the melting temperature due to vacancy formation. Inspired by the Kauzmann paradox, Fecht and Johnson [12] argued that the upper limit for superheating is defined by the isoentropic temperature, at which the entropies for a superheated crystal and the corresponding liquid become equal. The argument is thus the superheating equivalent of the Kauzmann paradox. The temperature corresponding to this ‘entropy catastrophe’ is again calculated using eq. (5.1) except that we now have to extrapolate the heat capacity of the solid above the melting temperature. The resulting entropies for liquid and solid aluminium [12] are shown in Figure 5.3. Here, the temperature at which the entropy of supercooled liquid aluminium reaches that of crystalline aluminium, the ideal glass transition temperature, is 0.24Tfus. Correspondingly, the temperature at which the entropy of the crystal on
Elastic moduli / 1010 Pa
5 Al
C11–C12
4 3 2
Instability
C44
1 0
500
1000
1500
2000
T/K
Figure 5.2 Temperature dependence of the isothermal elastic stiffness constants of aluminium [10].
132
5 Phase stability
Sm / J K –1 mol–1
80
liquid
Al
Tfus
60
supercooled liquid
40
crystal
20
Tlim. cryst.
TK 500
1000
1500
T/K
Figure 5.3 Entropy of liquid and crystalline aluminium in stable, metastable and unstable temperature regions [12]. The temperatures where the entropy of liquid and crystalline aluminium are equal are denoted TK and Tlim cryst, respectively.
heating again becomes as large as that of the liquid is 1.38Tfus. The latter is far lower than 1.67Tfus, obtained from the Born stability criteria [10]. The vacancy concentration at the stability limit is approximately 10% and the volume effect of this amount of vacancies corresponds to the volume change of melting at Tfus. It has therefore been argued that the isentropic temperature in general may coincide with the temperature at which the volume of the superheated crystal becomes equal to the volume of the liquid. Finally, Tallon [13] has suggested another instability point where the entropy of the superheated crystal becomes equal to that for a superheated diffusionless liquid (a glass) rather than that of the liquid. Since the glass has lower entropy than the liquid, this instability temperature is lower than that predicted by Fetch and Johnson [12].
5.2 Fluctuations and instability The driving force for chemical reactions: definition of affinity The equilibrium composition of a reaction mixture is the composition that corresponds to a minimum in the Gibbs energy. Let us consider the simple chemical equilibrium A « B, where A and B could for example be two different modifications of a molecule. The changes in the mole numbers dnA and dnB are related by the stoichiometry of the reaction. We can express this relation as –dnA = dnB = dx where the parameter dx represents an infinitesimal change in the extent of the reaction and expresses the changes in mole numbers due to the chemical reaction. The rate of reaction is the rate at which the extent of the reaction changes with time. The driving force for a chemical reaction is called affinity and is defined as the slope of the Gibbs energy versus the extent of reaction, x. The differential of the Gibbs
G / arbitrary units
5.2 Fluctuations and instability
133
drG < 0 drG > 0
drG = 0
Extent of reaction, x
Figure 5.4 Gibbs energy as a function of the extent of reaction.
energy at constant T and p is (taking into consideration the Gibbs–Duhem equation, eq. (1.93)) d r G = m A dn A + m B dn B = m A dx + m B dx = (m B  m A ) dx
(5.10)
The affinity of the reaction, Ak, is defined as the difference between the chemical potential of the reactant and the product at a particular composition of the reaction mixture: Ak = m A  m B
(5.11)
Since the chemical potential varies with the fraction of the two molecules, the slope of the Gibbs energy against extent of reaction changes as the reaction proceeds. The reaction A ® B is spontaneous when m A > m B , whereas the reverse reaction, B ® A, is spontaneous when m B > m A . The different situations are illustrated in Figure 5.4. The slope of the Gibbs energy versus the extent of the reaction is zero when the reaction has reached equilibrium. At this point we have mA = mB
(5.12)
and the equilibrium criteria for a system at constant temperature and pressure given by eq. (1.84) are thus fulfilled. Stability with regard to infinitesimal fluctuations In general, the first derivative of the Gibbs energy is sufficient to determine the conditions of equilibrium. To examine the stability of a chemical equilibrium, such as the one described above, higher order derivatives of G are needed. We will see in the following that the Gibbs energy versus the potential variable must be upwards convex for a stable equilibrium. Unstable equilibria, on the other hand, are
134
5 Phase stability (a)
(c)
(b)
(d)
Figure 5.5 Ball in a gravitational field; illustration of (a) stable, (b) unstable, (c) spinodal and (d) metastable equilibria.
characterized by a downward convex Gibbs energy versus the potential variable. This is illustrated in Figure 5.5 where we have used a ball in a gravitational field as an example. In example (a) the ball is in a stable equilibrium and is stable against fluctuations in both directions. In (b) the ball is unstable towards fluctuations in both directions and it follows that this is an unstable equilibrium. In (c) the ball is stable for fluctuations to the left but unstable for fluctuations to the right. This is defined as a spinodal equilibrium. Finally, in (d) the ball is located in a locally stable but globally metastable equilibrium. Let us assume the existence of a Taylor series for the Gibbs energy at the equilibrium point. This implies that the Gibbs energy and all its derivatives vary continuously at this point. The Taylor series is given as æ ¶G ö 1 æ ¶2 G (  A k )z ®0 = çç ÷÷ z + ç 2 ! çè ¶z 2 è ¶z øz = 0
ö æ n ÷ z 2 +… + 1 ç ¶ G ÷ n ! çè ¶z n øz = 0
ö ÷ zn ÷ øz = 0
(5.13)
where z is an infinitesimal fluctuation. In principle, the fluctuation could be a fluctuation in concentration, temperature or pressure. Equilibrium is identified when the affinity is zero, which means that the first derivative (¶G / ¶z )z = 0 = 0. If (¶ 2 G / ¶z 2 )z = 0 ¹ 0 the sign of (  A k )z ®0 is the sign of (¶ 2 G / ¶z 2 )z = 0 z 2 . Since z2 is always positive, the equilibrium is stable if æ ¶2 G ç ç ¶z 2 è
ö ÷ >0 ÷ øz = 0
(5.14)
The equilibrium is unstable if this second derivative is negative. If æ ¶2 G ç ç ¶z 2 è
ö ÷ =0 ÷ øz = 0
(5.15)
5.2 Fluctuations and instability
135
Table 5.1 The criteria for stability of solutions with regard to infinitesimal fluctuations. Criteria
Equilibrium state
æ ¶2 G ö ç ÷ >0 ç ¶z 2 ÷ è øz = 0
Stable or metastable
æ ¶2 G ö ç ÷ <0 ç ¶z 2 ÷ è øz = 0
Unstable
æ ¶2 G ö ç ÷ =0 ç ¶z 2 ÷ è øz = 0
Spinodal point
Comment
Separates a stable region from an unstable region.
we have to examine higher order derivatives. The affinity is then given as (  A k )z ®0 =
1 æç ¶ 3G 3! çè ¶z 3
ö æ 4 ÷ z3 + 1 ç¶ G ÷ 4! çè ¶z 4 øz = 0
ö ÷ z4 +… ÷ øz = 0
(5.16)
If (¶ 3G / ¶x 3 )x = 0 ¹ 0, it is possible to choose the sign of z so that (  A k )z ®0 is negative. Hence the equilibrium is unstable since small compositional fluctuations can have any sign. The stability criteria are summarized in Table 5.1. The correspondence with a ball in a gravitational field illustrated in Figure 5.5 is evident. The stable and unstable regions are defined as the regions where the second derivative of the Gibbs energy with regard to z are positive and negative, respectively, and correspond to upward and downward convexity of the Gibbs energy with respect to z. When the second derivative is zero we have a situation corresponding to the inflection point which separates the regions of instability and stability with regard to small fluctuations. This inflection point represents a spinodal equilibrium and is called a spinodal point. Compositional fluctuations and instability The criterion given in Table 5.1 may be used to consider the stability of different compositions of a liquid or solid solution by looking at the variation of the Gibbs energy with composition. As discussed in Section 4.1, the miscibility gap of a solution is usually due to a positive enthalpy of mixing balanced by the entropy increment obtained when a disordered solution is formed. The enthalpy is here a segregation force, whereas the entropy is an opposing mixing force. At low temperatures the TDS term of the Gibbs energy is less important than DmixH, and segregation occurs. At high temperatures, the entropy gained by distributing different species on a given lattice is large and complete solubility is obtained. If we start from the absolute zero, the miscibility gap decreases with increasing temperature until a certain temperature, called the critical temperature, Tc. Above the critical temperature complete solubility in the liquid or solid state is obtained.
136
5 Phase stability
Let us initially consider the Gibbs energy of the solid solution Al2O3–Cr2O3 at 1200 K [14] given in Figure 5.6. The solution is partly miscible and the composition of the two coexisting solutions a and b is given by the equilibrium condition m aAl
b
= m Al
2O3
and
2O3
b
m aCr O = m Cr O 2 3
(5.17)
2 3
The phase boundaries at this specific temperature are given by the points x1 and x2 in Figure 5.6(a), defined by the common tangent (the dotted line). Three different situations for the variation of the Gibbs energy of the solution with composition are marked by the points A, B and C/C ¢. A solution with composition A is stable with regard to fluctuations in composition, while one with composition B is unstable. At the two spinodal points (C and C ¢) the second derivative of the Gibbs energy with regard to composition changes sign (see Figure 5.6(b)) and in general æ ¶2 G ç m ç ¶x 2 B è
ö ÷ =0 ÷ s ø xB = xB
(5.18)
where x Bs is the composition at the spinodal point. The samples with composition C and C ¢ are stable with regard to fluctuations in composition in one direction, but not with regard to fluctuations in composition in the other direction. The compositions of the two spinodal points vary with temperature and approach each other as the temperature is raised, and the two points finally merge at the critical temperature, where (a)
0
(b) 40 B
–1
d2D mixGm / dx 2 / kJ mol–1
Dmix Gm / kJ mol –1
x1 C'
C
–2
x2
–3
A
20
0
C'
C
–20 0.0
0.2
0.4 0.6 x Cr2O3
0.8
1.0
0.0
0.2
0.4 0.6 x Cr2O3
0.8
1.0
Figure 5.6 (a) Gibbs energy of mixing of the system Al2O3–Cr2O3 at 1200 K [14]. A, B and C/C¢ correspond to stable, unstable and spinodal points. The points x1 and x2 give the compositions of the two coexisting solutions. (b) The compositional dependence of (d 2 D mixG m / d 2 x).
5.2 Fluctuations and instability
æ ¶ 3G ç m ç ¶x 3 B è
137
ö ÷ =0 ÷ c ø xB = xB
(5.19)
Here x Bc is the composition at the critical point. Let us now calculate the immiscibility gap and the spinodal line for a regular solution A–B: o G m = xA mA + x B m Bo + RT ( x A ln x A + x B ln x B ) + Wx A x B
(5.20)
o Let us for simplicity assume that m Bo = m A = 0, for which case the immiscibility gap is given by
¶G m = RT (ln x B  ln x A ) + W(1  2 x B ) = 0 ¶x B
(5.21)
An analytical expression that defines the compositions of the two coexisting solutions is easily derived: ln
xB W =(1  2 x B ) xA RT
(5.22)
The spinodal line is correspondingly given using eq. (5.18) as ¶2 G m ¶x 2B
æ 1 1 = RT çç + è xA xB
ö ÷÷  2 W = 0 ø
(5.23)
and it follows that the spinodal line for a regular solution is a parabola: x A x B = (1  x B ) x B =
RT 2W
(5.24)
At the critical point xA = xB = 0.5 and the critical temperature and the interaction coefficient are related through T c = W / 2R
(5.25)
Both the binodal line, defining the immiscibility gap, and the spinodal line are for a regular solution symmetrical about xA = xB = 0.5. This is shown in Figure 5.7(a), where theoretical predictions of the miscibility gaps in selected semiconductor systems are given [15].
138
5 Phase stability (a)
(b)
0.2 InN–GaN
AlN–InN 0.0
InN–GaN
binodal
T/K
2000
Dmix Gm / kJ mol–1
3000
spinodal
1000
–0.2 –0.4
spinodal points
C'
–0.6 binodal
–0.8
0.2
0.4
0.6
x2
x1
AlN–GaN 0 0.0
C
0.8
1.0
–1.0 0.0
0.2
x
0.4 0.6 xGaN
0.8
1.0
Figure 5.7 (a) Theoretical predictions of the unstable regions (miscibility gap) of the solid solutions in the systems AlN–GaN, InN–GaN and AlN–InN [15]. For the system InN–GaN both the phase boundary (binodal) and spinodal lines are shown. (b) Gibbs energy of mixing for the solid solution InN–GaN at 1400 K.
Physically, the spinodal lines separate two distinct regions in a phase diagram. Between the binodal and the spinodal lines (i.e. the compositional regions between x1 and C ¢ and between C and x2 in Figure 5.7(b)) the solution is in a metastable state. Between the spinodal points or in the spinodal region (i.e. the compositional regions between C ¢ and C in Figure 5.7(b)), the solution is unstable. Samples with overall composition within the metastable regions and within spinodal regions are expected to behave differently on cooling from high temperatures where complete solid solubility prevails. Let us consider a portion of the Gibbs energy curve for a composition within and outside the spinodal region in some detail. In Figure 5.8(a), we consider the Gibbs (a)
(b)
1 2 G
3
G
x
extent of reaction, x
Figure 5.8 (a) Gibbs energy curve for an unstable system. (b) Gibbs energy of the unstable system as a function of the extent of reaction during spinodal decomposition of a sample with composition indicated by the arrow in figure (a).
5.2 Fluctuations and instability
139
energy in the vicinity of a composition that is well within the spinodal region. Assume that a sample with the overall composition marked with an arrow is cooled to below the critical temperature. Below the critical temperature, small fluctuations in composition lead to a continuous decrease in the Gibbs energy, as illustrated in Figure 5.8(b), and the separation of the original homogeneous solution occurs without nucleation of a new phase. Instead, two different regions with different composition emerge. As the system approaches equilibrium the difference in the composition increases and approaches the difference between the two equilibrium compositions. The decomposition occurs without any thermal activation and with continuous changes in composition. The decomposition of a homogeneous solution resulting from infinitesimal concentration fluctuations is called spinodal decomposition. The decomposition of a solution with composition outside the spinodal region but within the metastable region can be analyzed in a similar way. Let us assume that a sample with composition in this region is cooled to low temperatures. Small fluctuations in composition now initially lead to an increase in the Gibbs energy and the separation of the original homogeneous solution must occur by nucleation of a new phase. The formation of this phase is thermally activated. Two solutions with different composition appear, but in this case the composition of the nucleated phase is well defined at all times and only the relative amount of the two phases varies with time. Both decomposition mechanisms are used actively in the design of materials. The two important commercial glasses in the system Na2B8O13–SiO2, Pyrex and Vycor, represent striking examples. Figure 5.9 shows the relevant phase diagram for the system Na2B8O13–SiO2 [16]. Here the liquid shows immiscibility below the liquidus temperature of the system. On supercooling liquids with compositions given by the arrows the immiscibility dome at some point is reached. The supercooled liquids are here still in internal equilibrium since the glass transition
1800 liq. T/K
1500 1200
Na2B8O13 + liq.
900 Na2B8O13 + SiO2 Na2B8O13
SiO 2 + liq.
phase separation weight %
SiO2 Vycor
Pyrex
Figure 5.9 Phase diagram showing liquid immiscibility in the Na2B8O13–SiO2 system below the liquidus [16].
140
5 Phase stability
temperatures are even lower. On cooling the liquid further partial immiscibility is obtained and the composition of the two liquids in metastable equilibrium at different temperatures are given by the dotted line in the figure.1 While Vycor has a composition within the spinodal region of the system, Pyrex lies outside the spinodal region but within the binodal region. In Vycor, the spinodal mechanism secures a complete connectivity of the two metastable liquid/ glass phases throughout the matrix. The Na2B8O13rich phase can be etched out with acid and a ‘close to pure’ silica glass is produced. Since the original Na2B8O13–rich melt can be homogenized at relatively low temperatures compared with pure SiO2 this secures a rather low production cost. For Pyrex the composition of the melt is outside the spinodal region and the Na2B8O13 phase is formed by nucleation and growth. Complete connectivity is not obtained and spherical particles of an Na2B8O13rich melt forms a minority phase within the SiO2rich matrix. A glass with low softening and melting temperatures is thus produced. The van der Waals theory of liquid–gas transitions In Section 2.2 we introduced the van der Waals equation of state for a gas. This model, which provides one of the earliest explanations of critical phenomena, is also very suited for a qualitative explanation of the limits of mechanical stability of a homogeneous liquid. Following Stanley [17], we will apply the van der Waals equation of state to illustrate the limits of the stability of a liquid and a gas below the critical point. The van der Waals equation of state for one mole of gas is expressed in terms of the critical pressure, temperature and volume by eq. (2.40) as æ 3 çç p + V2 è
ö ÷÷ (3V  1) = 8T ø
(5.26)
where p = p/ pc , T = T / T c and V = V / V c . For a simple gas comprised of spherical molecules, eq. (5.26) is fairly well obeyed at low density or high temperature. At higher density the equation of state become less accurate in describing real systems. Some p–V isotherms of the van der Waals equation of state for H2O are shown in Figure 5.10(a). At high temperatures the volume of the gas falls near asymptotically with increasing pressure, as expected from the ideal gas law. At a particular temperature, corresponding to the temperature at the critical point, the first derivative (¶p / ¶V ) T = 0 becomes zero for a given value of V . This is an inflection point where not only (¶ 2 G / ¶p2 ) T = 0 ,
1 In practice the glasses are made by first quenching the liquid. The phase separation takes place by reheating and annealing the glass between the glass transition and the critical temperature.
5.2 Fluctuations and instability
141
but also (¶ 3G / ¶p 3 ) T = 0. This critical point is analogous to the critical point for the miscibility gap of solutions that phase separate into two phases of different composition. In the present case, the supercritical fluid separates into a liquid and a gas with different density. For subcritical isotherms (T < T c ), the parts of the isotherm where (¶p/ ¶V ) T < 0 become unphysical, since this implies that the thermodynamic system has negative compressibility. At the particular reduced volumes where (¶p/ ¶V ) T = 0, (¶ 2 G / ¶p2 ) T = 0 and we have spinodal points that correspond to those discussed for solutions in the previous section. This breakdown of the van der Waals equation of state can be bypassed by allowing the system to become heterogeneous at equilibrium. The two phases formed at T < T c , liquid and gaseous H2O, must have the same temperature and pressure in order to obey the equilibrium criteria. The variation of the Helmholtz energy of the van der Waals equation of state for H2O with volume can be calculated by æ ¶A ö ÷ = p ç è ¶V ø T
(5.27)
Integration gives Vf
A(V ) =  ò pdV
(5.28)
Vi
The Helmholtz energy curves for three different isotherms are given in Figure 5.10(b). The volume of the two phases in equilibrium at a given temperature can be derived in at least two different ways. In the first approach, we can apply a common tangent construction to the Helmholtz energy curve as shown for T = 0.8 in Figure 5.10(b). The dashed line is tangent to the Helmholtz energy curve at the ‘highdensity’ point A and at the ‘lowdensity’ point B. These volumes define the volumes of the two phases (liquid and gas) in equilibrium. At a specific temperature, the pressure is implicitly defined by these two volumes. Alternatively, the equilibrium pressure for the coexistence of liquid and gas can be determined using what is called the Maxwell equalarea construction. In practice, this is done by adjusting the horizontal line in Figure 5.10(a), so that the areas marked C and D become equal. The equilibrium pressure for which liquid and gas are in equilibrium is given as a function of temperature for the van der Waals equation of state for H2O in Figure 5.11(a). The corresponding equilibrium densities of the coexisting liquid and gas are given in Figure 5.11(b). In these two figures the spinodal lines defining the mechanical stability limits of the liquid and gas phases are shown as dotted curves. The stable regions of the potential space for the liquid and gas phases are separated by the equilibrium line for the heterogeneous phase equilibrium, while the
142
5 Phase stability (a) 2.0
(b) 0 A T/Tc = 0.8
T/Tc = 1.1 A / arbitrary units
1.5 p / pc
1.0 1.0
0.9 A
D
–20 1.0 B – 40 1.2
B
C
0.5 0
1
2 3 V / Vc
4
–60
5
0
1
2
3 4 V / Vc
5
6
Figure 5.10 (a) pV isotherms of the van der Waals equation of state for H2O at T/Tc = 1.1, 1.0 and 0.9. (b) The Helmholz energy A(T,V) for the van der Waals equation of state of H2O as a function of V/Vc at T/Tc = 1.2, 1.0 and 0.8.
spinodal lines define the maximum extension of the metastable regions for the liquid and gas phase, respectively. For example, the liquid can be extended to negative pressure (liquid under tension) if nucleation of gas can be avoided. However, below the spinodal line the liquid becomes mechanically unstable. The T–r plot shown in Figure 5.11(b) resembles the T–x plot of a binary solution. The equilibrium between the two phases is, as we have seen above, given by a similar set of equilibrium conditions in both cases. Within the spinodal regions of the (a) 30
(b) Tc pc
20
H 2O(l)
H2O(g) 600
H 2O(l)
gas spinodal
0 H2O(g)
T/K
p / MPa
10
H2O(g) + H 2O(l)
500
–10 spinodal –20 liquid spinodal –30 400 450 500 550 600 650 T/K
400
spinodal 0.0
0.4
0.8 1.2 r / g cm –3
1.6
Figure 5.11 The pT (a) and the Tr (b) phase diagrams of H2O calculated using the van der Waals equation of state.
5.2 Fluctuations and instability
143
potential space, phase separation in the binary solution system is driven by concentration fluctuations, while the formation of the stable state in the singlecomponent system is driven by density fluctuations.
Pressureinduced amorphization and mechanical instability Pressureinduced amorphization of solids has received considerable attention recently in physical and material sciences, although the first reports of the phenomenon appeared in 1963 in the geophysical literature (actually amorphization on reducing the pressure [18]). During isothermal or near isothermal compression, some solids, instead of undergoing an equilibrium transition to a more stable highpressure polymorph, become amorphous. This is known as pressureinduced amorphization. In some systems the transition is sharp and mimics a firstorder phase transition, and a discontinuous drop in the volume of the substance is observed. Occasionally it is strictly not an amorphous phase that is formed, but rather a highly disordered denser nanocrystalline solid. Here we are concerned with the situation where a true amorphous solid is formed. The report of the pressureinduced amorphization and amorphous–amorphous transition of porous Si captures most of the current understanding of this phenomenon [19]. In Figure 5.12(a) the p,T phase diagram of Si is shown. Three phases are present: the fourcoordinated lowpressure modification (diamondtype) and the sixcoordinated highpressure modification (b–Sntype) of crystalline Si, as well as liquid Si. The behaviour of crystalline Si under compression is most easily understood by considering the melting line, which is extended into the metastable pressure region in Figure 5.12(a). This melting line has been extrapolated by using a simple twospecies lattice model for the liquid, first introduced by Rapoport [20, 21]. In this model the liquid is seen to consist of atoms that are all in one of two different possible states. These two states are described as two different species A and B that, for the given liquid, are assumed to be in chemical equilibrium at any given temperature and pressure. Thus, Si A Si B
(5.29)
The Gibbs energy of reaction (5.29) is D r G = G Si,B  G Si,A = D r H  TD r S + pD r V
(5.30)
Here G Si,A and G Si,B are the Gibbs energy of the ‘pure’ species A and B. D r H = H Si,B  H Si,A , D r S = S Si,B  S Si,A and D r V = V Si,B  V Si,A are the corresponding enthalpy, entropy and volume changes of reaction (5.29). The integral Gibbs energy of the liquid is determined by the relative population of the two states or in other words by the equilibrium constant for the reaction. We will deduce an expression for this below.
144
5 Phase stability (a) Si(liq.)
T/K
1600
Tc , pc
1200 Si(s) diamondtype
Si(s) b Sntype
800 spinodal
400 –5
(b)
0
spinodal 5
10 p / GPa
1800
(c)
0.9
0.8
xB
T/K
1.0 Ts
0.6
Tc
0.2 1200 0.1
0.4
Ts
0.2
1000 –1
20
0.8
1600 1400
15
0
1 2 p / GPa
3
4
0.0 600
800 1000 1200 1400 1600 T/K
Figure 5.12 (a) The pT phase diagram of Si. The melting lines for the lowpressure polymorph of Si and the liquid–liquid phase transition are calculated by using the twostate model and the parameters given in Table 5.2. (b) Isoconcentration lines for species B in the pT plane. (c)) The fraction of species B as a function of temperature at constant pressure p = 2 GPa.
In the twostate model [20, 21] the two different species interact and the interaction can be expressed using the regular solution model. Thus the Gibbs energy of the liquid is G liq = x Si,A G Si,A + x Si,BG Si,B + RT [ x Si,A ln x Si,A + x Si,B ln x Si,B ] (5.31) + Wx Si,A x Si,B Table 5.2 Model parameters used in the thermodynamic description of liquid Si. D r V = VSi,B  VSi,A = 2.6 cm3 mol–1 D r H = HSi,B  HSi,A = 30 kJ mol–1 D r S = SSi,B  SSi,A = 21 J K–1 mol–1 W = 24 kJ mol–1 D fus HSi,A = HSi,A  H sol = 26.4 kJ mol–1 D fus SSi,A = SSi,A  S sol = 9 J K–1 mol–1 D fusVSi,A = VSi,A  V sol = 0.95 cm3 mol–1
5.2 Fluctuations and instability
145
Here W is the regular solution constant and x Si,B the fraction of Si atoms in silicon state B. By noting that x Si,A = 1  x Si,B , equation (5.31) becomes G liq = G Si,A + x Si,B (G Si,B  G Si,A ) + RT [(1  x Si,B ) ln(1  x Si,B )
(5.32)
+ x Si,B ln x Si,B ] + W(1  x Si,B ) x Si,B Equation (5.32) looks like the Gibbs energy for a regular binary solution. However, it is important to note that x Si,B for the twostate model has a slightly different interpretation than xB for a binary regular solution. In the latter case, xB is an external parameter that describes the composition of the solution. For the twostate model, on the other hand, x Si,B is an internal parameter describing the relative population of the two states present in the singlecomponent system. The equilibrium value of x Si,B is determined by minimizing G liq with respect to x Si,B : x Si,B ¶G liq = G Si,B  G Si,A + W(1  2 x Si,B ) + RT ln 1  x Si,B ¶x Si,B = D r G + W(1  2 x Si,B ) + RT ln
x Si,B 1  x Si,B
(5.33)
=0
Equation (5.33) can alternatively be written in terms of the equilibrium constant for reaction (5.29) as x Si,B æ D Gö éW ù K 5.29 = exp ç  r ÷ = exp ê (1  2 x Si,B ) ú ë RT û è RT ø 1  x Si,B
(5.34)
The relative populations of the two states vary with temperature and pressure. The species A which dominates at low temperature and low pressure has the larger molar volume, while the denser species B becomes increasingly more favoured at high pressures. We are now able to use this model for the Gibbs energy of the liquid to calculate the melting line for fourcoordinated Si by using the Clapeyron equation (eq. 2.10): dT D fus V = dp D fus S
(5.35)
When W is assumed to be independent of temperature and pressure the entropy and volume of the liquid is given as
146
5 Phase stability
æ ¶G liq S liq =  ç ç ¶T è
ö ÷ = x Si,A S Si,A + x Si,B S Si,B ÷ øp
(5.36)
 R[(1  x Si,B ) ln(1  x Si,B ) + x Si,B ln x Si,B ] and æ ¶G liq V liq = ç ç ¶p è
ö ÷ = x Si,A V Si,A + x Si,BV Si,B ÷ øT
(5.37)
The slope of the melting curve follows: dT V liq  V sol = dp S liq  S sol = =
x Si,A V Si,A + x Si,BV Si,B  V sol x Si,A S Si,A + x Si,B S Si,B  R[(1  x Si,B ) ln(1  x Si,B ) + x Si,B ln x Si,B ]  S sol D fus V Si,A + x Si,B D r V D fus S Si,A + x Si,B D r S  R[(1  x Si,B ) ln(1  x Si,B ) + x Si,B ln x Si,B ] (5.38)
The parameters of the model, given in Table 5.2, are obtained by fitting expression (5.38) to the experimental melting line. The extensions of the melting line to negative pressures and beyond the triple point between the liquid and the two solid polymorphs are given by dotted lines in Figure 5.12(a). Note that the model is predicting a melting temperature maximum for Si at negative pressure (–3 GPa). We are now in a position to analyze the behaviour of Si under compression. Compression of crystalline Si at temperatures above that of the triple point will lead to conventional melting of fourcoordinated Si. Compression at temperatures between that of the triple point and the glass transition temperature will also cause melting of fourcoordinated Si, but this melting is not an equilibrium reaction. The reason is that the transformation of fourcoordinated Si to the sixcoordinated polymorph (denoted bSn type in the figure) is kinetically hindered. Following this argument, fourcoordinated Si melts at the pressure corresponding to the extrapolated melting line for the melting of fourcoordinated Si, but with subsequent crystallization of the stable sixcoordinated highpressure polymorph. Under compression at temperatures below the glass transition, an ergodic liquid can no longer be produced, since the thermal energy is too low for the needed structural rearrangements. Still, at some given pressure fourcoordinated crystalline Si becomes unstable towards density fluctuations and an amorphous, nonergodic solid is formed. It follows that the pressureinduced amorphization at ambient
5.2 Fluctuations and instability
147
temperature occurs at pressures exceeding those of the extension of the melting line for fourcoordinated crystalline Si. The amorphization is therefore not a twophase melting process, but occurs at the mechanical stability limit for the lowpressure modification of crystalline Si. On decompression, amorphous Si formed by mechanical amorphization undergoes an amorphous–amorphous transition. The volume change associated with the transition is large, reflecting a change in coordination of Si from six to four. Transitions of this type between two different amorphous states have been reported in other cases as well. One of the more studied transitions is that between low and highpressure amorphous ice [22]. The existence of more than one amorphous modification for a given substance has been given the name polyamorphism [23], by analogy with polymorphism used for crystalline compounds. A closely related topic is that of liquid–liquid transitions. The possible coexistence of two modifications of a given liquid with the same chemical composition but with different densities has been much discussed. While two coexisting chemically identical liquids with different densities have been reported in quenched Y2O3–Al2O3 melts [24], a firstorderlike liquid–liquid transition has been reported in an in situ hightemperature–highpressure study of liquid phosphorous [25]. At ambient pressure molten phosphorus is a molecular liquid consisting of P4 molecules, while at high pressures molecular units with low density become unstable and a denser liquid is formed [25]. The regular solutiontype twostate model for the liquid induces two coexisting liquids under certain p,T conditions when the interaction parameter, W, is positive. Transitions between two amorphous states have for that reason been rationalized in terms of the model. One example is the analysis of the transition between low and highdensity amorphous ice by Ponyatovsky et al. [26]. We will now consider the transition between low and highdensity amorphous Si in a similar analysis. In the following discussion we disregard the fact that the liquid becomes a glass below the glass transition and thereby transforms to a nonergodic state. Below the critical temperature, G liq ( x Si,B ) has two minima that are interpreted as representing two different liquids. The deeper minimum in Gibbs energy corresponds to the equilibrium phase at a given temperature and pressure. Hence the two different phases are stable in different parts of the p,T potential space. At the particular conditions where the Gibbs energies of the two minima are equal, the two liquids coexist. Using the twostate model based on the regular solution expression, the relative populations of state B in the two coexisting phases are related by liq.1 liq.2 x Si,B + x Si,B =1 since the regular solution expression is symmetrical about x = 0.5. Let us now return to the relative population of the two states of the liquid given by eq. (5.34). Isoconcentration lines (x Si,B = constant) in the pT potential space are shown in Figure 5.12(b) (data are taken from Table 5.2). At low temperature and pressure (or even negative pressure) species A with high molar volume and low entropy relatively to the denser polymorph is favoured and x Si,B is low. At increasing pressure species B become increasingly more favoured and x Si,B is high at high pressures irrespective of the temperature.
148
5 Phase stability
Furthermore, Figure 5.12(b) illustrates the temperature–pressure conditions where two liquids coexist in equilibrium. The temperature and pressure of both phases must be equal at the transition point. In addition, the relative population of state B of the two liq.1 liq.2 liquids in equilibrium must be related through x Si,B + x Si,B =1since we use a regular solutiontype twostate model. This implies (using a specific example) that two liquids coexist at the intersection point of the isoconcentration lines for xSi,B = 0.2 and 0.8. On heating the liquid at the pressure corresponding to this intersection point (along the dotted line in the figure), the population of state B, xSi,B, increases continuously until reaching the temperature where the two liquids coexist in equilibrium. Here, x Si,B jumps discontinuously from the value in the low temperature phase, xSi,B = 0.2, to that of the high temperature phase, xSi,B = 0.8. Further heating results in a slow increase in x Si,B . The variation of the population of state B with temperature for p = 2 GPa is given in Figure 5.12(c). The dashed lines in the figure give the concentration of B for the two liquids in the metastable regions limited by the spinodals (see below). The equilibrium line for the liquid–liquid transition given in Figure 5.12(a) is also given in Figure 5.12(b). This line goes through the intersections of all pairs of liq.1 liq.2 lines that satisfy x Si,B + x Si,B =1, e.g. the intersection of the lines for xSi,B = 0.1 and 0.9 and that for xSi,B = 0.2 and 0.8. These two specific examples represent two discrete points on the equilibrium curve. It can be shown that the equilibrium temperature for the liquid–liquid transition is given as T trs =
W(1  2 x B,Si )/R ln( x B,Si /(1  x B,Si ))
(5.39)
This equilibrium line terminates at the critical point where the critical temperature is given by the twostate regular model as T c = W /2 R. The pressure corresponding to a given equilibrium temperature is given by p=
T trs D r S  D r H D rV
(5.40)
We have now derived the phase boundary between the two liquids. By analogy with our earlier examples, the two phases may exist as metastable states in a certain part of the p,T potential space. However, at some specific conditions the phases become mechanically unstable. These conditions correspond to the spinodal lines for the system. An analytical expression for the spinodals of the regular solutiontype twostate model can be obtained by using the fact that the second derivative of the Gibbs energy with regards to xSi,B is zero at spinodal points. Hence, æ 2 liq. ç¶ G ç ç ¶x 2Si,B è
ö RT ÷ =0 ÷ = 2 W + x ÷ Si,B (1  x Si,B ) øT
(5.41)
5.3 Metastable phase equilibria and kinetics
149
The calculated spinodal lines are given together with the equilibrium phase boundary in Figure 5.12(a). All three lines terminate at the critical point. The amorphous–amorphous transition observed during decompression of amorphous Si can now be understood in terms of crossing the spinodal line for the highpressure amorphous phase on reducing pressure. Finally, it should be noted that a transition similar to that shown in Figure 5.12(c) may illustrate what is observed during flash heating of amorphous Si at ambient pressure [27]. Amorphous Si shows a ‘firstorderlike’ transition to supercooled liquid Si when crystallization of amorphous Si is suppressed by a high heating rate. In spite of the apparent success of the two state model, the model used gives a very simplistic description of a liquid and further experimental and theoretical evidence is needed to confirm the very existence of liquid–liquid transitions.
5.3 Metastable phase equilibria and kinetics Metastable materials are becoming increasingly important as the use of extreme farfromequilibrium conditions during preparation is expanding. The formation of a large fraction of these phases cannot be rationalized using thermodynamic arguments. Most zeolites for example are kinetically stabilized through the use of templates during synthesis. Another and more specific example is YMnO3, which takes the perovskite structure under equilibrium conditions, but crystallizes in a different structure as a thin film or powder prepared from precursors [28, 29]. While thermodynamic arguments may fail in cases like this, thermodynamic analyses can in other cases be used to predict synthesis routes to new compounds, and there are numerous examples of metastable alloys formed when the nucleation of the stable phases is suppressed. In these cases the metastable phase equilibria can be analysed thermodynamically, and may even be represented in phase diagrams. Phase diagrams reflecting metastability One of the classical examples of metastable heterogeneous phase equilibria occurs in the system Fe–C. The eutectic between gFe and graphite shown in Figure 5.13(a) is important for many cast irons. If the Clevel is low, as in steels, solidification directly to d  or g Fe may occur. On cooling, these steels become unstable with regard to the formation of graphite. Although there is a driving force for precipitation of graphite, the volume change for this precipitation reaction in the solid state is high and nucleation becomes difficult. For many conditions the metastable phase Fe3C, cementite, is formed instead. Hence for practical purposes the metastable Fe–Fe3C phase diagram is more important than the equilibrium Fe–C phase diagram. In the section of the binary phase diagram Fe–C shown in Figure 5.13(a), both the stable phase boundaries and phase boundaries corresponding to metastable phase equilibria involving cementite, Fe3C, are given. The stability field of gFe when gFe is in metastable equilibrium with cementite is slightly larger than when gFe is in the stable equilibrium with graphite [30]. This can be
150
5 Phase stability (b) 1800
liq.
1600 T/K
liq. + C 1400 gFe(ss)
1200
liq. + Fe3C Fe 3C
phase border metastable equil. g Fe
phase border stable equil.
1000 aFe 0.0
metastable phase
dFe
G / arbitrary units
(a)
0.1 0.2 x in Fe1–xC x
stable phase
mole fraction
Figure 5.13 (a) Phase diagram of the Fe–C system. Solid lines represent the stable phase diagram where gFe is in equilibrium with graphite. Dotted lines represent the metastable phase diagram where gFe is in equilibrium with cementite, Fe3C. (b) Schematic Gibbs energy rationalization of the effect of a metastable equilibrium on solid solubility.
rationalized for a general situation through the schematic Gibbs energy diagram given in Figure 5.13(b). The Gibbs energy of a metastable phase is higher than that of the mixture of gFe and the stable phase. The result is that the common tangent construction that determines the extension of the phase field of gFe touches the Gibbs energy curve of gFe at a higher mole fraction of carbon for the metastable case than is the case for the stable phase equilibrium. Cementite is marginally metastable, and it follows that the effect on the phase boundaries is small. Thermodynamic representations of phase diagrams may reveal such and more complex metastable situations. The phase relations in the Sn–Sb system are shown in Figure 5.14 [31]. The diagram on the righthand side represent a metastable situation where the nonstoichiometric phase SnSb is considered as kinetically hindered from formation. The terminal solid solubility of Sn in Sb and of Sb in Sn increases; furthermore, Sn3Sb2 will in this case be apparently stable even at low temperatures. Diagrams of this type may correspond to situations high in Gibbs energy that are of little practical importance. In other situations they correspond to phase equilibria close in Gibbs energy to the stable situation. Such situations may be observed as metastable equilibria under certain conditions. Thermal evolution of metastable phases Although the formation of a large number of metastable materials that are far from equilibrium cannot be explained thermodynamically, thermodynamics predicts that they will with time transform to the stable phase or phase mixture, often via intermediate phases. More than one hundred years ago, Ostwald pointed out that
5.3 Metastable phase equilibria and kinetics
(a)
(b) liq.
800
T/K
151
liq + Sb Sn(ss)
600
400 0.0
liq.+ SnSb
Sn(ss)
600
Sn3Sb2 + Sb
SnSb + Sb
0.4
0.6
xSb
0.8
Sb(ss) liq. + Sn 3Sb 2
SnSb
Sn + SnSb
0.2
liq + Sb
Sb(ss)
liq.+ Sn 3Sb 2
liq.
800
400 1.0
Sn + Sn3Sb2
1.0
0.8
0.6
0.4
xSn
0.2
0.0
Figure 5.14 Calculated (a) stable and (b) metastable phase diagrams for the Sn–Sb system.
nonequilibrium thermodynamic systems appear to evolve through a sequence of states of progressively lower Gibbs energy [32]. In this rationalization scheme, it is not the most stable form of the material with the lowest Gibbs energy that is obtained as the initial product, but the least stable that is nearest to the original in Gibbs energy. If several metastable phases, or mixtures of phases, are possible, they will follow one another in the order of a stepwise decrease in Gibbs energy. Ostwald’s step rule has considerable value in materials science. This will be illustrated here by considering crystallization of metallic glasses in the system Fe–B [33] and diffusional amorphization in the system Ni–Zr [34]. The glass formation ability in the system Fe–B is largest for alloys close to the eutectic where a melt with xB = 0.20 on cooling solidifies under the formation of Fe and Fe2B. The crystallization sequence observed depends on the composition of the glass and often involves the metastable compound Fe 3B [33]. A large portion of the experimental observations can be rationalized using the schematic Gibbs energy representation given in Figure 5.15. For an alloy with composition given by the point A, primary crystallization of Fe(ss) is observed. The glass/supercooled liquid near Tg is simultaneously enriched in B. On further thermal evolution, the metastable phase equilibrium between Fe(ss) and Fe3B is reached. Only in a third and final stage is the stable phase equilibrium between Fe(ss) and Fe2B obtained. The three stages of the crystallization are marked in Figure 5.15 by arrows. In this simple rationalization of the experimental observations, the fact that Fe can crystallize in different structures which are close in Gibbs energy is not taken into consideration. It has for example been shown that molten droplets of certain Fe–Ni alloys crystallize in a bcctype structure before transforming to the more stable fcc structure [35]. Although the Gibbs energy rationalization can often predict the
152
5 Phase stability
G / arbitrary units
glass Fe3 B
Fe2 B
A o aFe(ss)
glass formation xB
Figure 5.15 Schematic Gibbs energy rationalization of the crystallization of metallic glasses in the system Fe–B.
phase sequence formed, some phases may be kinetically hindered from formation, as in the case of graphite in the system Fe–C described above. Thermodynamic rationalization of diffusional amorphization similarly relies on Ostwald’s step rule. One example is the formation of amorphous Ni–Zr alloys on interdiffusion in stacks of thin –Ni–Zr–Ni–Zr– foils [34]. Since, the kinetics is slow, the formation of intermetallic phases is prevented. The thermodynamic stability of the liquid determines whether or not a glass is formed. The Gibbs energy of formation of the liquid must be intermediate in Gibbs energy between the Gibbs energy of the mixture of the elements and the mixture of different intermetallic compounds. Glass formation and growth in diffusion couples like this was first observed for Ni–Zr in 1983, but has subsequently also been seen in a large number of other intermetallic systems [36]. Materials in thermodynamic potential gradients A last example of kinetic effects is given by the behaviour of materials in thermodynamic potential gradients [37]. Materials are often applied in situations where they are not in equilibrium with their immediate surroundings. Gradients in temperature, chemical or electrical potential act as driving forces on atoms in a crystalline material, and fluxes of atoms across an initially homogeneous solid solution result. This effect tends to separate the components if they have different mobilities and is a phenomenon of practical significance. Materials subject to thermodynamic potential gradients in general may demix or even decompose. One example is engineering components subject to large temperature gradients like turbine blades (Ludvig–Soret effect). Let us initially look at a semiconducting binary oxide A1–d O in a chemical gradient; an oxygen potential gradient. Reduction takes place on the low oxygen
5.3 Metastable phase equilibria and kinetics pO2 high
153 pO2low
A1窶電 O xvac
jA jvac distance / position
t=0 t = t'
Figure 5.16 Schematic illustration of demixing in a binary oxide A1窶電O in a gradient in the chemical potential of O2.
activity side with the result that the oxide loses oxygen at the surface. Oxygen molecules leave the oxide while the cations left behind move toward the higher oxygen potential side; see Figure 5.16. Oxidation takes place at the high oxygen activity side were cations are recombined with oxygen atoms from the gas and the oxide grows. Both the oxide/gas surfaces move in the direction of the high oxygen activity side (indicated by arrows in Figure 5.16) relative to the immobile oxygen lattice. The composition, the vacancy concentration, of the binary oxide will vary across the oxide due to the oxygen potential gradient. For ternary mixed cation oxides like (A,B)1窶電 O more pronounced effects may be encountered in addition to growth at the high pO2 surface at the expense of the low pO2 surface [37, 38]. Demixing of the different cations will occur in an applied oxygen potential gradient in cases where the two cations have different mobility. The result of these transport processes is concentration gradients and a material is usually enriched in the more mobile cation species at the high oxygen potential side. The degree of demixing increases with increasing difference in mobility between the cations and with decreasing thickness of the material. The segregation or demixing is a purely kinetic effect and the magnitude depends on the cation mobility and sample thickness, and is not directly related to the thermodynamics of the system. In some specific cases, a material like a spinel may even decompose when placed in a potential gradient, although both potentials are chosen to fall inside the stability field of the spinel phase. This was first observed for Co2SiO4 [39]. Formal treatments can be found in references [37] and [38].
References [1] [2]
F. Grﾃｸnvold, J. Chem. Thermodyn. 1973, 5, 525. S. S. Chang and A. B. Bestul, J. Chem. Thermodyn. 1974, 6, 325.
154
[3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30]
[31] [32] [33] [34] [35] [36] [37] [38]
5 Phase stability
S. Stølen, H. B. Johnsen, C. S. Bøe, T. Grande and O. B. Karlsen, J. Phase Equil. 1999, 20, 17. J. C. Wheatley, Rev. Mod. Phys. 1975, 47, 415. W. Kauzmann, Chem. Rev. 1948, 43, 219. F. A. Lindemann, Z. Phys. 1910, 11, 609. M. Born, J. Chem. Phys. 1931, 7, 591. J. W. Gibbs, The Collected Work, Volume I Thermodynamics. Harvard: Yale University Press, 1948. M. Born and K. Huang, Dynamic Theory of Crystal Lattices. Oxford: Oxford University Press, 1954. J. L. Tallon and A. Wolfenden, J. Phys. Chem. Solids 1979, 40, 831. K. Lu and Y. Li, Phys. Rev. Lett. 1998, 80, 4474. H. J. Fecht and W. L. Johnson, Nature 1988, 334, 50. J. L. Tallon, Nature, 1989, 342, 658. S. S. Kim and T. H. Sanders Jr, J. Am. Ceram. Soc. 2001, 84, 1881. T. Takayama, M. Yuri, K. Itoh, and J. S. Harris, Jr, J. Appl. Phys. 2001, 90, 2358. T. J. Rockett and W. R. Foster, J. Am. Ceram. Soc. 1966, 49, 30. H. E. Stanley, Introduction to Phase Transitions and Critical Phenomena. Oxford: Oxford University Press, 1971. B. J. Skinner and J. J. Fahey, J. Geophys. Res. 1963, 68, 5595. S. K. Deb, M. Wilding, M. Somayazulu and P. F. McMillan, Nature, 2001, 414, 528. E. Rapoport, J. Chem. Phys. 1967, 46, 2891. E. Rapoport, J. Chem. Phys. 1968, 48, 1433. O. Mishima, L. D. Calvert and E.Whelley, Nature 1985, 314, 76. P. H. Poole, T. Grande, C. A. Angell and P. F. McMillan, Science, 1996, 275, 322. S. Aasland and P. F. McMillan, Nature 1994, 369, 633. Y. Katayama, T. Mizutani, W. Utsumi, O. Shimomura, M. Yamakata and K. Funakoshi, Nature 2000, 403, 170. E. G. Ponyatovsky, V.V. Sinitsyn and T. A. Pozdnyakova, J. Chem. Phys. 1998, 109, 2413. M. O. Thompson, G. J. Galvin, J. W. Mayer, P. S. Peercy, J. M. Poate, D. C. Jacobson, A. G. Cullis and N. G. Chew, Phys. Rev. Lett. 1984, 52, 2360. H. W. Brinks, H. Fjellvåg and A. Kjekshus, J. Solid State Chem. 1997, 129, 334. P. A. Salvador, T. D. Doan, B. Mercey and B. Raveau, Chem. Mater. 1998, 10, 2592. R. Hultgren, P. D. Desai, D. T. Hawkins, M. Gleiser and K. K. Kelley, Selected Values of the Thermodynamic Properties of Binary Alloys. Metals Park, OH: Am. Soc. Metals, 1973. B. Jönsson and J. Ågren, Mater. Sci. Techn. 1986, 2, 913. W. Ostwald, Z. Phys. Chem. 1897, 22, 289. K. Köster and K. Herold, Topics in Applied Physics, Vol. 46. Berlin: SpringerVerlag, 1981. M. Atzmon, J. R. Verhoeven, E. D. Gibson and W. L. Johnson, Appl. Phys. Lett. 1984, 45, 1052. R. E. Cech, Trans. Met. Soc. AIME 1956, 206, 585. W. L. Johnson, Progr. Mater. Sci. 1986, 30, 81. H. Schmalzried, in Chemical Kinetics of Solids. Weinheim: VCH, 1995, Chapter 8. M. Martin, Mater. Sci. Rep. 1991, 7, 1.
5.3 Metastable phase equilibria and kinetics
155
[39] H. Schmalzried, W. Laqua and P. L. Lin, Z. Naturforsch. 1979, A34, 192.
Further reading J. W. Gibbs, The Collected Work, Volume I Thermodynamics. Harvard: Yale University Press, 1948. D. Kondepudi and I. Prigogine, Modern Thermodynamics: from Heat Engines to Dissipative Structures. New York: John Wiley & Sons, 1998. H. Schmalzried, Chemical Kinetics of Solids. Weinheim: VCH, 1995. H. E. Stanley, Introduction to Phase Transitions and Critical Phenomena. Oxford: Oxford University Press, 1971.
6
Surfaces, interfaces and adsorption
In Chapter 1, heterogeneous systems were described as a set of homogeneous regions separated by surfaces or interfaces. The surface or interface is chemically different from the bulk material and the surface or interface energy represents an excess energy of the system relative to the bulk. When considering the macroscopic thermodynamic properties of a system the surface/interface contribution can be neglected as long as the homogeneous regions are large. ‘Large’ in this context can be identified from Figure 6.1. Here the enthalpy of formation of NaCl is shown as a function of the size of single crystals formed as cubes where a is the
Df H m / kJ mol–1
–300
–330
–360
–390
–420 0.01
0.1
1
10
100
1000
a / mm
Figure 6.1 The molar enthalpy of formation of NaCl as a function of the cube edge a of the NaCl crystal cubes. Chemical Thermodynamics of Materials by Svein Stølen and Tor Grande © 2004 John Wiley & Sons, Ltd ISBN 0 471 492320 2 157
158
6 Surfaces, interfaces and adsorption
length of a cube edge. The enthalpy of formation of NaCl becomes less negative as the cube size decreases because the surface energy is positive (energy is required to form surfaces), and the relative contribution from the surface increases with decreasing size of the cubes. However, the number of surface atoms is significant only for very small cubes and the contribution from the surface energy becomes measurable only when the cubes are smaller than ~1 mm. A thermodynamic system can therefore be analyzed in terms of the bulk properties of the system when the homogeneous regions are larger than roughly 1 mm. Although the surface energy may be neglected in considering macroscopic systems, it is still very important for the kinetics of atomic mobility and for kinetics in heterogeneous systems. Nucleation and crystal growth in solid or liquid phases and sintering or densification in granular solids are largely influenced by the surface or interface thermodynamics. In these cases the complexity of the situation further increases since the curvature of the surfaces or interfaces is a key parameter in addition to surface energy. Moreover, materials science is driven towards smaller and smaller dimensions, and the thermodynamics of surfaces and interfaces are becoming a key issue for materials synthesis and for understanding the properties of nanoscale materials. For a cube containing only 1000 atoms, as many as 50% of the atoms are at the surface and the surface energy is of great importance. The purpose of this chapter is to introduce the effect of surfaces and interfaces on the thermodynamics of materials. While interface is a general term used for solid–solid, solid–liquid, liquid–liquid, solid–gas and liquid–gas boundaries, surface is the term normally used for the two latter types of phase boundary. The thermodynamic theory of interfaces between isotropic phases were first formulated by Gibbs [1]. The treatment of such systems is based on the definition of an isotropic surface tension, s, which is an excess surface stress per unit surface area. The Gibbs surface model for fluid surfaces is presented in Section 6.1 along with the derivation of the equilibrium conditions for curved interfaces, the Laplace equation. Surfaces of crystals, which are inherently anisotropic in nature, are also briefly treated. Gibbs’ treatment of interfaces was primarily related to fluid surfaces, and the thermodynamic treatment of solid surfaces was not fully developed before the second half of the 20th century [2]. While the thermodynamics of surfaces and interfaces in the case of isotropic systems are defined in terms of the surface tension, surface energy is the term used for nonisotropic systems. The surface energy, g, is defined as the energy of formation of a new equilibrium surface of unit area by cutting a crystal into two separate parts. The surface energy according to this definition cannot be isotropic since the chemical bonds broken due to the cleavage depend on the orientation of the crystal. The consequences of surface energy anisotropy for the crystal morphology are discussed. Trends in surface tension and average surface energy of the elements and some salt systems are reviewed and finally the consequences of differences in surface energy/tension between different phases in equilibrium on the morphology of the interface are considered generally.
6.1 Thermodynamics of interfaces
159
In the last two sections the formal theory of surface thermodynamics is used to describe material characteristics. The effect of interfaces on some important heterogeneous phase equilibria is summarized in Section 6.2. Here the focus is on the effect of the curvature of the interface. In Section 6.3 adsorption is covered. Physical and chemical adsorption and the effect of interface or surface energies on the segregation of chemical species in the interfacial region are covered. Of special importance again are solidâ€“gas or liquidâ€“gas interfaces and adsorption isotherms, and the thermodynamics of physically adsorbed species is here the main focus.
6.1 Thermodynamics of interfaces Gibbs surface model and definition of surface tension A real interface region between two homogeneous phases a and b is schematically illustrated in Figure 6.2(a). A hypothetical geometric surface termed the Gibbs dividing surface, S, is constructed lying in the region of heterogeneity between the two phases a and b, as shown in Figure 6.2(b). In the Gibbs surface model [1], S has no thickness and only provides a geometrical separation of the two homogeneous phases. At first sight this simple description may seem to be inadequate for a real interface, but in the following we will show the usefulness of the model. The energetic contribution of the interface is obtained by assigning to the bulk phases the values of these properties that would pertain if the bulk phases continued uniformly up to the dividing surface. The value of any thermodynamic property for the system as a whole will then differ from the sum of the values of the thermodynamic properties for the two bulk phases involved. These excess thermodynamic properties, which may be positive or negative, are assigned to the interface. Let us now consider an interface between two isotropic multicomponent phases. The number of moles of a component i in the two phases adjacent to the interface are given as n ai and n ib . Since the mass balance of the overall system must be obeyed, it is necessary to assume that the dividing surface contains a certain
a
b
b
a
(a)
(b)
Gibbs dividing surface S
Figure 6.2 (a) Illustration of a real physical interface between two homogeneous phases a and b. (b) The hypothetical Gibbs dividing surface S.
160
6 Surfaces, interfaces and adsorption
number of moles of species i, n si , such that the total number of moles of i in the real system, n i , is equal to n i = n ai + n ib + n si
(6.1)
The surface excess moles or the number of moles of species i adsorbed or present at the surface is then defined as n si = n i  n ai  n ib
(6.2)
n si divided by the area As of S yields the adsorption of i: Gi = n si / A s
(6.3)
Gi may become positive or negative, depending on the particular interface in question. Other surface excess properties, such as the surface internal energy and surface entropy, are defined similarly: U s =U U a U b
(6.4)
Ss = S  Sa  S b
(6.5)
Recall that the Gibbs dividing surface is only a geometrical surface with no thickness and thus has no volume: Vs =V Va V b =0
(6.6)
It follows that the surface excess properties are macroscopic parameters only. In order to define the surface tension we will consider the change in internal energy connected with a reversible change in the system. For an open system dU is given by eq. (1.79) as dU = TdS  pdV + 책 m i dn i
(6.7)
i
For a reversible process, where the interfaces remain fixed, the volumes of the two phases remain constant and eq. (6.7) becomes dU = TdS + 책 m i dn i
(6.8)
i
An infinitesimal change in the surface internal energy dU s = dU  dU a  dU b
(6.9)
6.1 Thermodynamics of interfaces
161
can be expressed in terms of the changes in internal energy of the two homogeneous phases separated by the fixed boundary C
dU a = TdS a + 책 m i dn ai
(6.10)
i =1
C
dU b = TdS b + 책 m i dn ib
(6.11)
i =1
Here C is the number of components in the system. Combination of eqs. (6.9), (6.10) and (6.11) yields C
dU s = T ( dS  dS a  dS b ) + 책 m i ( dn i  dn ai  dn ib )
(6.12)
i =1
The expressions in the two parentheses can be identified as the surface excess moles and surface excess entropy defined by eqs. (6.2) and (6.5). Equation (6.12) thus reduces to C
dU s = TdS s + 책 m i dn si
(6.13)
i =1
The exact position of the geometrical surface can be changed. When the location of the geometrical surface S is changed while the form or topography is left unaltered, the internal energy, entropy and excess moles of the interface vary. The thermodynamics of the interface thus depend on the location of the geometrical surface S. Still, eq. (6.13) will always be fulfilled. The effect of variations in the form of the geometrical interface on the energy can be deconvoluted into two contributions: changes in energy related to changes in the area of the interface and changes in energy related to changes in the curvatures of the interface [3]. The two principal curvatures c1 and c2 at a point Q on a arbitrary surface are indirectly illustrated in Figure 6.3. Two planes normal to the surface at Q are defined by the normal at point Q and the unit vectors in the two principal directions, u and v. A circle can be constructed in each of the two planes which just touches the surface at point Q. The radii r1 and r2 of the two circles are the two principal radii at point Q and the two principle curvatures are defined as the reciprocal radii c1 = 1/ r1 and c2 = 1/ r2 . For systems where the thickness of the real physical interface is much smaller than the curvature of the interface, Gibbs [1] showed that the dividing surface could be positioned such that the contribution from the curvature of the interface is negligible. Assuming the surface to have such a position, only the term related to a change in the interfacial area needs to be considered. An infinitesimal change in the surface internal energy is
162
6 Surfaces, interfaces and adsorption u
N Q
v
Figure 6.3 Illustration of the curvature of a geometrical surface.
dU s = TdS s + å m i dn si + s dA s
(6.14)
i
where s is the partial derivative of U with respect to the area As. We are now going to investigate the significance of the variable s. For a reversible process dU is dU = dU s + dU a + dU b
(6.15)
The change in internal energy for the two phases adjacent to the interface is now C
dU a = TdS a + å m i dn ai  pa dV a
(6.16)
i =1
C
dU b = TdS b + å m i dn ib  p b dV b
(6.17)
i =1
Incorporating these two equations in eq. (6.15) yields the following expression for the change in internal energy for the system: dU = T ( dS s + dS a + dS b ) C
+ å m i ( dn si + dn ai + dn i )  pa dV a  p b dV b + s dA s b
(6.18)
i =1
or C
dU = TdS + å m i dn i  pa dV a  p b dV b + s dA s i =1
(6.19)
6.1 Thermodynamics of interfaces
163
where the surface tension, s, is æ ¶U s = çç è ¶A s
ö ÷÷ ø S ,V a ,V b ,n i
(6.20)
This is the definition of the surface tension according to the Gibbs surface model [1]. According to this definition, the surface tension is related to an interface, which behaves mechanically as a membrane stretched uniformly and isotropically by a force which is the same at all points and in all directions. The surface tension is given in J m–2. It should be noted that the volumes of both phases involved are defined by the Gibbs dividing surface S that is located at the position which makes the contribution from the curvatures negligible. Equilibrium conditions for curved interfaces The equilibrium conditions for systems with curved interfaces [3] are in part identical to those defined earlier for heterogeneous phase equilibria where surface effects where negligible: T a =T
b
=T s
(6.21)
m ai = m ib = m si
(6.22)
and
Note that the chemical potential of a given component at the interface is equal to that in the two adjacent phases. This is important since this implies that adsorption can be treated as a chemical equilibrium, as we will discuss in Section 6.3. To establish the equilibrium conditions for pressure we will consider a movement of the dividing surface between the two phases a and b. The dividing surface moves a distance dl along its normal while the entropy, the total volume and the number of moles n i are kept constant. An infinitesimal change in the internal energy is now given by dU =  pa dV a  p b dV b + s dA s
(6.23)
The changes in the volume of the two phases are related by dV a = A s dl = dV b
(6.24)
and also the change in area of the surface is related to dl. dAs can be expressed in terms of the two principal curvatures c1 and c2 of the interface [3]:
164
6 Surfaces, interfaces and adsorption
dA s = (c1 + c2 ) A s dl
(6.25)
Substitution of eqs. (6.24) and (6.25) into eq. (6.23) yields dU = ( p b  pa ) A s dl + s (c1 + c2 ) A s dl = [( p b  pa ) + s (c1 + c2 )]A s dl (6.26) At equilibrium ( dU ) S ,V ,n i = 0, which leads to the equilibrium condition for pressure expressed in terms of the two principal curvatures or alternatively in terms of the two principal radii of curvature: æ1 1 ö p b  pa = s (c1 + c2 ) = s çç + ÷÷ è r1 r2 ø
(6.27)
Equation (6.27) is the Laplace equation, or Young–Laplace equation, which defines the equilibrium condition for the pressure difference over a curved surface. In Section 6.2 we will examine the consequences of surface or interface curvature for some important heterogeneous phase equilibria. For planar surfaces the pressure difference over the interface becomes zero and the equilibrium condition for pressure, eq. (6.27) reduces to p b = pa
(6.28)
The surface tension for a planar surface thus is æ ¶U s = çç è ¶A s
ö ÷÷ ø S ,V ,n i
(6.29)
and here only the total volume needs to be kept constant. The position of the geometrical surface S no longer affects the definition of s, as for curved surfaces. The surface energy of solids The surface tension defined above was related to an interface that behaved mechanically as a membrane stretched uniformly and isotropically by a force which is the same at all points on the surface. A surface property defined this way is not always applicable to the surfaces of solids and the surface energy of planar surfaces is defined to take anisotropy into account. The surface energy is often in the literature interchanged with surface tension without further notice. Although this may be useful in practice, it is strictly not correct. The surface energy can be derived by an alternative treatment. Let us initially consider a large homogeneous crystal that contains N atoms and that has a planar
6.1 Thermodynamics of interfaces
165
surface. The change in energy on forming solid surfaces is often deconvoluted into two contributions. The first contribution is due to a change in the surface area that does not disturb the structural arrangement of the atoms and which thus leaves the surface structure identical to that of the bulk. The second contribution is elastic in nature, and relates to the deformation of the surface when relaxed or reconstructed. To create a new surface we have to break bonds and remove the superfluous atoms. At equilibrium at constant pressure and temperature the work demanded to increase the surface area of a onecomponent system by an amount dAs is given as dW T , p = g dA s
(6.30)
where g is the surface energy (J m–2). This energy is the excess energy relative to the bulk and depends on the number of bonds per unit area and the strength of these bonds. The reversible work is equal to the change in Gibbs energy due to the formation of a surface, and the change in the Gibbs energy of a onecomponent system can now be written as dG =  SdT + Vdp + g dA s
(6.31)
æ ¶G g = çç è ¶A s
(6.32)
where ö ÷÷ øT , p
For an isotropic phase there are no differences between surface energy and surface tension. However, for crystals, which are anisotropic in nature, the relationship between these two quantities is significant and also theoretically challenging, see e.g. the recent review by Rusanov [2]. It is important to note that the formation of a surface always leads to a positive Gibbs energy contribution. This implies that smaller particles are unstable relative to larger particles and that the equilibrium shape of crystals is determined by the tendency for surfaces of higher energy to be sacrificed while those of lower Gibbs energy grow. This is the topic of the next section. Anisotropy and crystal morphology Basically, the surface energy is given by the number of bonds per unit surface area and by the bond strength. Different crystal surfaces have different numbers of bonds per unit surface area and the measured surface energies for crystals are often an average value over many different crystal surfaces. Using a facecentred cubic structure as an example, the density of atoms in specific planes generally decreases with increasing Miller indices [hkl]. The exception is the closepacked [111] plane. For a [111] plane there are six nearest neighbours in the plane, three above and
166
6 Surfaces, interfaces and adsorption
three below the plane. Hence three bonds are broken for each surface atom when the crystal is cut in two along [111]. For the [100] and [110] planes there are four and six broken bonds respectively, and thus taking only nearest neighbours into consideration the surface energies for these planes are larger. The different surface energies for different types of crystal surfaces control the equilibrium shape of a crystal, as first discussed by Wolf [11]. This important phenomenon occurs not only for solidâ€“gas interfaces but also for all other interfaces. For liquidâ€“gas interfaces the surface tension is independent of orientation and the equilibrium shape is a sphere. This represents the smallest surface area for a body of a given size. Experimental studies indicate that spheres become energetically favourable also for solids at high temperatures. Hence the difference in surface energy between different surfaces is less important at high temperatures. The equilibrium shape of a crystal can be constructed using the Wulff construction [4]. Consider a onecomponent system in which only the solid and gas phases are present. Assume that the phases have their equilibrium volumes and can only change their shape. Hence we need to be able to describe the volume of the crystal. Let us start looking at a single crystal in the form of a polyhedron of some kind. This is shown for a twodimensional case in Figure 6.4. From some point O in the interior of a crystal, normals to all crystal faces are drawn. The distance between O and the face v is h v . If a straight line is drawn from O to each corner of the body, the crystal will be divided into N pyramids of height h v , base A v and volume 1/ 2 A v h v . Using a similar analysis, the volume of a threedimensional crystal can be expressed as V=
1 N ĂĽ Av h v 3 v =1
(6.33)
For a reversible change at constant temperature and volume of both phases and for a constant number of moles of the components, the equilibrium shape can be Ai hi
hi+1
O
Figure 6.4 Geometric parameters describing a twodimensional crystal.
6.1 Thermodynamics of interfaces
167
found by minimization of the Helmholtz energy of the system. It can be shown that the equilibrium morphology of a single crystal is given by [3] g1 g2 g = =… = N h1 h2 hN
(6.34)
Here g i is the surface energy of the crystal surface i. The equilibrium shape of a crystal is thus a polyhedron where the area of the crystal facets is inversely proportional to their surface energy. Hence the largest facets are those with the lowest surface energy. Equation (6.34), defining the equilibrium shape of crystals, is only relevant for crystals of a certain size. For large crystals changes in shape involve diffusion of large numbers of atoms and the driving force may not be sufficient, since the surface contribution is small compared with the bulk. Hence metastable crystal shapes are more likely to be reached. But even for small crystals the Wulff relationship may break down. Here twinning may lead to configurations which lower the Gibbs energy of the crystal, and this results in a different crystal morphology. Herring [5, 6] and Mullins [7] give extended discussions of the topic. The Laplace equation (eq. 6.27) was derived for the interface between two isotropic phases. A corresponding Laplace equation for a solid–liquid or solid–gas interface can also be derived [3]. Here the pressure difference over the interface is given in terms of the factor that determines the equilibrium shape of the crystal: pa  p b = 2
g1 g g = 2 v =… = 2 N h1 hv hN
(6.35)
Comparing this expression with eq. (6.27), we see that g v / h v for each crystal face represents s divided by the radius of curvature for an isotropic spherical phase. As a first approximation we may replace g v / h v with g /r for nearspherical crystals. In this case g represents an average surface energy of all possible crystal faces. In the remaining part of the chapter we will use the term g for interfaces that involve solids. It should then implicitly be understood that we are here considering bulk solids that are treated as isotropic systems and that the surface energy thus defined is the average value of the surface energies for different crystal surfaces. Furthermore, we will consistently use superscripts to denote the phases adjacent to the interface in the rest of Section 6.1 and in Section 6.2. Trends in surface tension and surface energy Periodic variations in the surface tension of liquid metals, s lg, are shown in Figure 6.5. The much higher surface tension of dblock metals compared to the s and pblock metals suggests that the surface tension relates to the strength of interatomic bonding. Similar periodic trends can be found also for the melting temperature and the enthalpy of vaporization, and the surface tension of liquid metals is strongly
168
6 Surfaces, interfaces and adsorption 3.0 6
s lg / J m–2
2.5 5
2.0 Period 2
1.5 1.0
4 3
0.5 0.0
Period 3
1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 Group of periodic table
Figure 6.5 Periodic trends in the surface tension of selected liquid elements in periods 2–6 at their melting temperature [8]. 4 g sg and s lg / kJ m –2
g
sg
= 0.067 + 0.015D vap Hm /Vm2/3
3 Re Mo V Rh Fe Co Pt Cr Ni Pd Be Cu TiZr
2
1
0
Nb
Ru, Ir Ta
Os Tc
Ag Au Mn Zn Al Si Sc CdMg lg 2/3 LaGaGe In Sn Tl,Pb,Bi,Li s = 0.063 + 0.021D vapHm /Vm Hg Ca Sb Sr Ba Cs,Rb,K Na
0
50
100 150 Dvap HmVm–2/3/ kJ cm –2
200
Figure 6.6 Surface tension of the liquid elements at Tfus, s lg (open squares), and surface energy of the solid elements at 0 K, g sg (filled circles), versus D fus H m Vm2 / 3 [8].
correlated with these and other physical properties that depend on the strength of the interatomic bond. The correlation between the surface tension of the liquid o metals and their enthalpy of vaporization, in the form of D vap H m × V m2 / 3 , first discussed by Shapski [9] and Grosse [10], is shown in Figure 6.6. Data for the average surface energy of solid metals, g sg, are also included in this figure. It can be noted that the average surface energy of solids has also been shown to correlate with other cohesionrelated properties like Young’s modulus and the Debye temperature [11]. Surface tension and average surface energies for selected inorganic compounds are given in Table 6.1. In Figure 6.7, different interfacial tensions or energies of metals are correlated with the fusion temperature in the form T fus × V m2 / 3 . In general the ratio of the average surface energy of the solid to the surface tension of the liquid is around 1.2
6.1 Thermodynamics of interfaces
169
Table 6.1 Surface tension or average surface energy of some solid and liquid substances [12, 13]. Substance
slg /J m–2
NaCl(l) (1000 °C) Al2O3(l) (2050 °C) SiO2(l) (1800 °C) P2O5(l) (100 °C) Cu2S(l) (1200 °C) NiS(l) (1200 °C) PbS(l)(1200 °C) Sb2S3(l) (1200 °C) H2O(l) (25 °C)
0.098 0.69 0.307 0.06 0.4 0.577 0.2 0.094 0.072 g sg/J m–2
LiF(s) (25 °C) CaF2(s) (25 °C) NaCl(s) (25 °C) MgO(s) (25 °C)
0.34 0.45 0.227 1.2
Pt Ni
s or g / J m –2
2.5
g sg
Cu
2.0
s lg
Au
1.5
Ag Al
1.0
g gb
0.5 150 200 250 300 350 400 450 500 550 TfusVm–2/3 / K cm –2
Figure 6.7 Average grain boundary energy, g gb, surface energy of crystals at 0 K, g sg, and surface tension s lg of liquid Al, Ag, Au, Ni and Pt as a function of melting temperature TfusVm2 / 3 [8, 11].
at a given temperature. g sg for Al and Pt at 0 K are 1.2 and 2.55 J m–2 respectively, while s lg at the melting temperature of the metals are 0.865 and 1.86 J m–2 [8]. Although less pronounced, similar trends can be found also for molten salts, as shown in Figure 6.8 [14, 15]. g sl is as a first estimate proportional to the enthalpy of fusion and separate proportionality coefficients are reported for metallic and semimetallic elements [16].
170
6 Surfaces, interfaces and adsorption 0.4 fluorides chlorides bromides iodides carbonates nitrides sulphates
s lg / J m –2
0.3
0.2
0.1
0.0
0
50
100 TvapVm–2/3 /
150 K cm
200
–2
Figure 6.8 Surface tension of fused salts as a function of melting temperature normalized with the molar volume TvapVm2 / 3 [14, 15].
The average interfacial energy between the solid and liquid forms of a given element is generally lower than g sg and s lg, e.g. 0.093 and 0.24 J m–2 for Al and Pt. For materials which change coordination number upon melting g sl is larger. Solid–solid interface energies are normally termed grain boundary energies, g ss = g gb, and they are comparable to solid–liquid interfacial energies. Average grain boundary energies for some f.c.c. metals are given in Figure 6.7. Again a correlation with T fus × V m2 / 3 is observed. We have now treated surface and interfacial energies without considering the effect of temperature. The excess Gibbs energy of a surface is expected to decrease with temperature since the excess entropy of the surface compared to the bulk is expected to be positive. Intuitively, the surface atoms have more degrees of freedom than atoms in the bulk and thus higher vibrational entropy. In addition, the formation of vacancies and disorder in general at the surface gives a positive configurational contribution to the entropy. Typically (dg sg /dT ) is –45 mJ m–2 K–1 for pure solid elements and slightly less for liquid elements. A semiempirical equation for predicting the temperature variation of the surface energy of liquids was proposed by van der Waals [17] and Guggenheim [18]. The surface tension is here given as
s
lg
æ = s olg çç 1 è
T Tc
ö ÷÷ ø
n
(6.36)
The equation implies that the surface tension becomes zero at the critical temperature, Tc, where the two phases become indistinguishable. The exponent n has been determined to be around 1.2 for metals [11].
6.1 Thermodynamics of interfaces
171 b
s abt ab qb
s
bc bc
t
q
c
q
a
a
c s actac
Figure 6.9 Twodimensional projection of equilibrium at a plane of contact between three phases a, b and c where the angles between the three twophase boundaries meeting in a line of contact are denoted q a , q b and q c .
Morphology of interfaces The equilibrium shape of a crystal is, as described above, a polyhedron where the size of the crystal facets is inversely proportional to their surface energy, g sg . In the present section we will consider other types of interfaces as well and we will show that the interface energies determine the equilibrium morphology of interfaces in general. A twodimensional illustration of three phases a, b and c in equilibrium is shown in Figure 6.9. Two phases coexist in equilibrium in planes perpendicular to the lines indicated in the twodimensional figure and all three phases coexist along a common line also perpendicular to the plane of the drawing. Each of the three twophase boundaries, which meet at the point of contact, has a characteristic interfacial tension, e.g. s ab for the a–b interface, which tends to reduce the area of the boundary. Here we assume the interfacial tensions to be independent of the orientation and that the surface forces are the only ones present. The three forces for the three boundaries are in mechanical equilibrium if s ab t ab + s bc t bc + s ac t ac = 0
(6.37)
where t ij is a unit vector tangent to the i–j boundary at the point of contact. Using the three angles defined in Figure 6.9, the equilibrium condition becomes s ab sin q c
=
s bc sin q a
=
s ac sin q b
=0
(6.38)
If the three interfacial tensions are equal, the three angles are also equal: q i = 120°. The conditions for mechanical equilibrium can now be applied to a simple case of great practical importance. Let us consider the interfaces that occur when a liquid phase is brought into equilibrium with a solid surface in a gaseous
172
6 Surfaces, interfaces and adsorption gas s lg
liquid g sl
q
g sg
solid
Figure 6.10 Contact angle q of a liquid drop resting on a solid surface. The definition of the forces used in the figure eliminates the contribution from gravity.
atmosphere. The wetting of a solid by a liquid drop is characterized by the contact angle, q, defined in Figure 6.10. The condition for mechanical equilibrium can be rearranged to give the surface energy balance: g
sg
=g
sl
+ s lg cos q = 0
(6.39)
Equation (6.39) was first derived by Young, and is often referred to as the Young–Dupré equation. We usually distinguish between full (q < 90°) and partial wetting (q > 90°) and an alternative measure of the same property is given by the wetting coefficient: k=
g
sg
g
s lg
sl
= cos q
(6.40)
A solid is not wetted if k £ 1, partly wetted for 1< k < 1 and fully wetted for k >1. Wetting is favoured when the difference (g sg – g sl) approaches and becomes larger than s lg. In this case the interaction between the droplet and the substrate increases and the contact angle decreases. It follows that materials with high surface energy are better substrates for deposition of another phase than substrates with low surface energy. One consequence is that metal surfaces are often readily wetted while polymeric surfaces often are not. The sessile drop technique for determination of interfacial energies is based on the configuration shown in Figure 6.10. If the surface tension of the liquid is known, the difference between the interfacial energies of the solid–gas and solid–liquid interfaces can be determined directly by measurement of the contact angle. Experimentally it is difficult to obtain reproducible data on wetting because of two factors: the influence of the surface roughness and the sensitivity of the interfacial energies to the presence of surfaceactive species. These species may be introduced through contaminations from the surrounding atmosphere or they may be present in the materials used.
6.1 Thermodynamics of interfaces
173
Interfacial tensions also play an important role in the distribution of phases in polycrystalline solids. The presence of secondary phases is quite typical, since as grain growth proceeds nonsoluble impurities accumulate, usually at the grain boundaries. In other cases the secondary phases may become embedded in the majority phase if the grain boundaries are not pinned at the inclusions. In powder metallurgy and ceramic technology secondary phases are often introduced on purpose in order to enhance sintering or inhibit grain growth. Generally, an equilibrium situation is difficult to obtain due to slow kinetics when governed by solid (bulk or grain boundary) diffusion. When a secondary liquid phase is present the kinetics is governed by liquid diffusion and equilibrium situations are more likely to be reached. The distribution of the liquid is determined by the interfacial energy between the liquid and the solid matrix relatively to the grain boundary energy. An example is shown in Figure 6.11(a), where an important characteristic of grain boundaries, the
(b) a b
a
180째
a
(a) a
a
O
f
a
b
a
b
a a
135째
a b
a
a
0째
Figure 6.11 (a) Definition of the dihedral angle, f, at a junction of three grain boundaries in a polycrystalline solid. (b) Schematic illustration of the shape of an inclusion phase for different dihedral angles.
174
6 Surfaces, interfaces and adsorption
dihedral angle f, is defined. The dihedral angle at the point O is at equilibrium defined through æf g aa  2 g ab cosç è2
ö ÷=0 ø
(6.41)
Depending on the value of the two interfacial energies the dihedral angle can take any value from 0 to 180°. The shapes taken by the secondary phase for different dihedral angles are illustrated in Figure 6.11(b). Since the dihedral angle governs the distribution of secondary phases, the mechanical properties of polycrystalline solids are to a great extent determined by the interfacial energies, although it is also evident that the amount of the secondary phase is important. In composites the strength of the material can be modified by changing the interfacial tension and thereby the distribution of phases. The fracture toughness of the material is here to a large degree determined by the mechanical strength of the interface between the two phases. Our final example of the effect of interfacial energies relates to microscopic studies of grain sizes and grain distributions in sintered materials. The materials are typically polished and then thermally etched (annealing in air or an inert atmosphere at temperatures significantly below the sintering temperature). After polishing, the grain boundaries are not easily seen by electron microscopy. On thermal annealing the surface relaxes and the surface microstructure become modified. A schematic illustration of the effect of thermal etching on a grain boundary is given in Figure 6.12. The dihedral angle defines the microstructure after etching and the relaxed surface microstructure is much more visible; the grain boundaries are easily seen. The surface of the ceramic material La0.5Sr0.5Fe0.5Co0.5O3 shown in Figure 6.13 constitutes an excellent example. In cases where the interfacial energy is dependent on orientation, the equilibrium condition (6.41) does not hold [19]. Some grain boundaries will then represent higher Gibbs energies than others, and if kinetics allow for reorientation, certain grain boundaries will become dominant. However, in most cases the kinetics of
f
solid grain A solid grain B
solid grain A
solid grain B
Figure 6.12 Grain boundary after polishing (a) and after the subsequent thermal etching (b).
6.2 Surface effects on heterogeneous phase equilibria
175
Figure 6.13 Surface of thermally etched La0.5Sr0.5Fe0.5Co0.5O3, a polycrystalline ceramic material .
reorientation of the crystal lattice in order to reduce the interfacial energy is slow and the distribution of grain boundaries is thus not determined by thermodynamics.
6.2 Surface effects on heterogeneous phase equilibria For small particles with large curvature the surface has, as previously stated, a significant effect on the thermodynamics, and the concepts developed apply to all types of interfaces between solid, liquid and gas. The fact that the curvature of the surface affects a heterogeneous phase equilibrium can be seen by analyzing the number of degrees of freedom of a system. If two phases a and b are separated by a planar interface, the conditions for equilibrium do not involve the interface and the Gibbs phase rule as described in Chapter 4 applies. On the other hand, if the two coexisting phases a and b are separated by a curved interface, the pressures of the two phases are no longer equal and the Laplace equation (6.27) (eq. 6.35 for solids), expressed in terms of the two principal curvatures of the interface, defines the equilibrium conditions for pressure: pa  p b = s ab (c1 + c2 )
(6.42)
Equation (6.42) introduces a new independent variable of the system: the mean curvature c = 1 (c1 + c2 ). This variable must be taken into account in the Gibbs 2 phase rule, which now reads F + Ph = C + 2 + 1. The number of degrees of freedom (F) of a twophase system (Ph = 2) with a curved interface is given by F = C +1
(6.43)
176
6 Surfaces, interfaces and adsorption
Effect of particle size on vapour pressure In this first example, a singlecomponent system consisting of a liquid and a gas phase is considered. If the surface between the two phases is curved, the equilibrium conditions will depart from the situation for a flat surface used in most equilibrium calculations. At equilibrium the chemical potentials in both phases are equal: ml = mg
(6.44)
For any reversible change dm l = dm g
(6.45)
At constant temperature dm = Vdp and eq. (6.45) becomes V g dp g = V l dp l
(6.46)
Here V g and V l are the molar volume of the two phases, but the subscript m is not used for simplicity. The pressure of the two phases is related by the Laplace equation (6.27), which for a spherical liquid droplet surrounded by its own vapour becomes, in differential form, æ 2s lg d( p g  p l ) = dç ç r è
ö ÷ ÷ ø
(6.47)
Here 2/ r = [(1/ r1 ) + (1/ r2 )] since r1 = r2 . Combining eqs. (6.46) and (6.47) yields V g V l Vl
æ 2s lg dp g = d ç ç r è
ö ÷ ÷ ø
(6.48)
Assuming the gas to be ideal (V g = RT / p g ) and noting that V g  V l » V g we obtain RT dp g V l pg
æ 2s lg = dç ç r è
ö ÷ ÷ ø
(6.49)
If the pressure dependence of the molar volume of the liquid is neglected, integration from a flat interface (r = ¥) yields
6.2 Surface effects on heterogeneous phase equilibria
177
1.5
pZn / poZn
1.4 1.3 1.2 1.1 1.0 0.01
0.1 r / mm
1
10
Figure 6.14 The vapour pressure of Zn over a spherical droplet of molten Zn at the melting o = 2◊10–4 bar, slg = 0.78 J m–2 and r = temperature as a function of the droplet radius. pZn –3 6.58 g cm [8].
ln
pg prg=¥
=
V l 2s lg RT r
(6.50)
Equation (6.50) is often referred to as the Thomson’s (or Kelvin’s) equation. As an example of the effect of this equation, the vapour pressure of a spherical droplet of molten Zn at the melting temperature is shown as a function of the droplet radius in Figure 6.14. A consequence of the decreasing vapour pressure with increasing size of the droplet is that in a distribution of droplets the larger droplets will grow at the expense of the smaller ones; a fact that will be discussed more thoroughly below. Effect of bubble size on the boiling temperature of pure substances We now return to the equilibrium condition (eq. 6.44), and assume that the liquid is subjected to a constant pressure, p l . For reversible changes eq. (6.44) becomes  S g dT + V g dp g =  S l dT
(6.51)
which may be rearranged to V g dp g = ( S g  S l ) dT = (H g  H l )
dT T
(6.52)
Let us consider a spherical bubble of vapour inside its coexisting liquid. Again the gas phase is assumed to be ideal, and eq. (6.52) becomes
178
6 Surfaces, interfaces and adsorption
dT T2
=
dp g R D vap H m p g
(6.53)
The pressure can be substituted by the mean curvature through the Laplace equation, for which dT T2
=
d(2s lg / r ) R D vap H m ( p l + [2s lg / r ])
(6.54)
If the enthalpy of vaporization is assumed to be independent of the curvature, integration of eq. (6.54) from a flat surface (r = ¥) yields (T constant) æ 2s lg / r R æ1ö æ1ö ç ÷ = lnç 1 + ç ÷ è T ør =¥ è T ør D vap H m çè pl
ö ÷ ÷ ø
(6.55)
The boiling temperature of molten Na is plotted versus the radius of the vapour bubble in Figure 6.15. The boiling temperature is increased by several hundred degrees for a gas bubble with radius 1 mm relative to a flat gas–liquid interface. If the liquid is free of impurities and heterogeneous interfaces, substantial superheating of the liquid above its bulk boiling temperature is possible, as also discussed in Chapter 5. The effect of curvature is much more pronounced for the thermodynamics of a gas bubble than for the liquid droplet. The curvature is a pressure effect, which is much larger for gases than for condensed phases, reflecting the much larger molar volume of the gas.
1700
Tvap / K
1600 1500 1400 1300 1200 1100
Tvap , bulk 0.1
1
10
100
r / mm
Figure 6.15 The boiling temperature of Na as a function of the radius of a vapour bubble surrounded by molten Na. DvapHm = 101.3 kJ mol–1 and slg = 0.19 J m–2 [8].
6.2 Surface effects on heterogeneous phase equilibria
179
Solubility and nucleation We will now consider a case where a spherical crystal with radius r of a single component solid phase is surrounded by a liquid with more than one component. The differential of the Laplace equation (6.27) is æ 2g sl d( p s  p l ) = dç ç r è
ö ÷ ÷ ø
(6.56)
We will consider a reversible change in the system at constant temperature and pressure of the liquid phase p l . Furthermore, we will assume that the equilibrium concentration of all components in the liquid, except for the single component, i, of the solid phase, is fixed. The equilibrium condition yields æ 2 g sl dm il = dm is = V is dp s = V is dç ç r è
ö ÷ ÷ ø
(6.57)
Assuming that V is is independent of pressure we obtain ( m il )r  (m il )r =¥ = V is
2 g sl r
(6.58)
where ( m il )r is the chemical potential of i in the liquid in equilibrium with a solid phase of radius r. By expressing the chemical potential in terms of activity (eq. 3.11), eq. (6.58) can be rewritten as
ln
( a il )r ( a il )r =¥
=
V is 2g sl RT r
(6.59)
Furthermore, if the liquid is assumed to be ideal the activity of a component is equal to the mole fraction of the component. Now the mole fraction of i in the liquid phase can be derived as a function of the radius of the solid phase:
ln
( x il )r ( x il )r =¥
=
V is 2g sl RT r
(6.60)
The important consequence of eq. (6.60) is that the solubility of the solid increases with decreasing radius of crystal. Although the effect is small this illustrates the need for supersaturation on homogeneous nucleation in a liquid. Supersaturation is necessary in order to obtain nucleation since the solubility of the nuclei is higher
180
6 Surfaces, interfaces and adsorption
than for the bulk. In addition, the interface energy is also important for the kinetics of nucleation, as illustrated below by classical nucleation theory. In classical nucleation theory the Gibbs energy of a nucleus is considered as the sum of contributions from the bulk and the surface. Let us consider nucleation of a spherical crystal from its liquid below its melting temperature at 1 bar. The difference in Gibbs energy between a nucleus with radius r and its liquid is 4 æ r D l  s G =  pr 3 ç 3 èM
ö 2 ÷D fus G m + 4pr g ø
sl
(6.61)
where D fus G m is the molar Gibbs energy of melting, ( M/ r) is molar volume (M is molar mass and r is density), 4 pr 3 is the volume of the spherical nuclei and g sl is 3 the surface energy of the solid–liquid interface. Here the effect of curvature has been neglected and the surface of the nucleus is assumed to be planar. Since the two terms in eq. (6.61) have opposite sign, the Gibbs energy goes through a maximum as a function of r, the surface term dominating for small r and the bulk term at large r. This maximum corresponds to the thermodynamic barrier to nucleation. The critical radius corresponding to a maximum in Gibbs energy is determined by differentiating eq. (6.61) with respect to r: dD l  s G æ r ö = 4pr 2 ç ÷D fus G m + 8prg dr èMø
sl
(6.62)
At the maximum dD l  s G / dr = 0 and the critical radius is r * = [2( M/ r)g sl ] / D fus G m . Finally, by substituting r = r * into eq. (6.61) the thermodynamic barrier for nucleation is obtained: D l  sG * =
16p ( g sl ) 3 M 2 3r 2 D fus G 2m
(6.63)
Since D fus G m increases with decreasing temperature, the critical radius and the thermodynamic barrier decrease with decreasing temperature. At the same time the thermodynamic driving force for nucleation is increasing. This is illustrated for crystallization of aluminium in Figure 6.16(a). The Gibbs energy of a nucleus of aluminium is given as a function of the radius of the nucleus in Figure 6.16(b) (at For small nuclei the surface term dominates. Above the critical T / T fus = 095). . radius the bulk contribution will stabilize the nuclei. Ostwald ripening During sintering of granular solids (for example ceramics or hard metals) grain growth may occur by a dissolution–precipitation mechanism if a secondary liquid phase is present. The chemical driving force for grain growth by this mechanism is
6.2 Surface effects on heterogeneous phase equilibria 1
(a) 1000
(b) 1.0
181 T/Tfus = 0.95
100
0.1
1 0.1 r*
DG*
1017DG / D fusGm
r* / mm
DG* / DfusGm1015
0.5 10
0.0
–0.5
0.01 0.01 1E–3 0.90 0.92 0.94 0.96 0.98 1.00 T / Tfus
–1.0 0.00
0.02
0.04 r / mm
0.06
0.08
Figure 6.16 (a) The critical radius (r*) and thermodynamic barrier for nucleation of Al (DG*) versus degree of supercooling T/Tfus. (b) The Gibbs energy of a spherical Al crystal relative to the supercooled Al(l) as a function of its radius. DfusHm = 10.794 kJ mol–1, Tfus = 933.47 K and r = 2.55 g cm–3 [8].
derived by looking at the system we considered for our analysis of solubility and nucleation. A spherical crystal with radius r of the singlecomponent solid is surrounded by a multicomponent liquid phase. Equation (6.58) can be used to find an expression for the difference in chemical potential between to particles of different radii: æ1 1 ö ( m is )r ¢  ( m is )r ¢ = 2V is g sl ç  ÷ è r ¢ r ¢¢ ø
(6.64)
Equation (6.64) shows that the chemical potential of i in the smaller grain (r ¢) is higher than in the larger (r ¢¢) and consequently larger grains will grow at the expense of the smaller ones. This phenomenon is known as Ostwald ripening. Ostwald ripening plays an important role in materials science, for example in relation to grain growth and elimination of pores (pore ripening) during the final stage of sintering of refractory metals or ceramics. The difference in the chemical potential between a spherical Au particle with radius 10 mm and a smaller spherical Au particle of radius r is shown in Figure 6.17. The Gibbs energy difference becomes significant below 0.1 mm, i.e. when the ratio between the radius of the two particles is larger than 100. Effect of particle size on melting temperature It is becoming increasingly more popular to prepare submicrometre sized artificially engineered structures with new properties. In particular, the tailoring of
182
6 Surfaces, interfaces and adsorption
Dm / kJ mol –1
0
–10
–20
–30 10 –3
10 –2
10 –1
10 0
10 1
r / mm
Figure 6.17 The difference in the chemical potential of Au(s) between a spherical particle with radius 10 mm and a smaller particle with radius r. r = 18.4 g cm–3 and g sl = 1.38 J m–2 [21].
electronic properties of semiconductors by reducing the particle size is important. The thermodynamics is also affected. It has been known for a relatively long time that particle size affects the melting temperature of pure substances. Two simple expressions for freezing temperature depression with origin in size have been derived by Hansen [20] and Buffat and Borel [21]. In the first approach, the equilibrium between a solid and a liquid droplet with the same mass is considered. The pressure and temperature contribution to the chemical potential can be expressed as a power series: æ ¶m ö æ ¶m ö * m(T , p) = m * + ç ÷÷ ( p  p* ) +… ÷ (T  T ) + çç T p ¶ ¶ øp è øT è
(6.65)
where m * is the chemical potential at a chosen reference state at T * and p* . The partial derivatives of the chemical potential with respect to temperature and pressure are –S and V respectively, and the following expression for the chemical potential is obtained: m(T , p) = m * (T * , p* )  S (T  T * ) +
M ( p  p* ) +… r
(6.66)
Here M/r is the molar volume of the substance. At equilibrium, the chemical potential of the liquid and solid droplet are equal: m s (T , p s ) = m l (T , p l )
(6.67)
6.2 Surface effects on heterogeneous phase equilibria
183
The equilibrium conditions require equal temperatures but different pressures due to the curvature. Using eq. (6.66) for both phases, the equilibrium condition, eq. (6.67), yields m *l (T * , p* )  m *s (T * , p* ) + ( S l  S s )(T  T * )
(6.68)
M l M s ( p  p* ) ( p  p* ) = 0 rl rs
+
Here r s and r l are the density of the solid and liquid and p s and p l the pressures inside the solid and liquid droplets, respectively. Rearrangement of eq. (6.68) yields 
D fus H m T
(T  T * ) +
*
M l M s ( p  p* ) ( p  p* ) = 0 rl rs
(6.69)
where D fus H m is the enthalpy of fusion of the substance. The pressures inside the particles are given by the Laplace equation as 2g
ps = pg +
sg
(6.70)
rs 2s lg
pl = pg +
(6.71)
rl
where p g , the external pressure in the surrounding vapour, is set to p* . Substituting eqs. (6.70) and (6.71) into (6.69) gives 
D fus H m
(T  T * ) +
T*
M 2s lg M 2 g sg =0 rl r l rs r s
(6.72)
The difference in curvature between the liquid (r l ) and the solid (r s ) particles can be found since they are related by r l V l = r s V s and V i = 4 p(r i ) 3 which gives 3
1/ 3
ær ö r l = çç s ÷÷ è rl ø
rs
(6.73)
Here, we have used the fact that the masses of the liquid and solid droplet are equal. Substituting eq. (6.73) in eq. (6.72) gives the following equation for the melting temperature as a function of the radius r of the solid phase:
184
6 Surfaces, interfaces and adsorption 1300
Tfus , bulk
Tfus / K
1200 1100 1000 900 1E3
0.01
0.1
1
10
r / mm
Figure 6.18 The suppression of the melting temperature of a spherical gold particle as a function of its radius. DfusHm = 12.35 kJ mol–1, Tfus = 1336 K, rl = 17.28 g cm–3, rs = 18.4 g cm–3, s lg = 1.135 J m–2, g sg = 1.38 J m–2 [21].
(T fus )r 2M 1= s (T fus )r =¥ r r s D fus H m
é êg ê ë
sg
lg æ
r  s çç s è rl
2 /3 ù
ö ÷÷ ø
ú ú û
(6.74)
where (T fus )r =¥ = T * and (T fus )r are the melting temperature of a bulk material and a particle with radius rs, respectively. An alternative expression can be derived by an approach in which the solid particle is considered to be embedded in a thin liquid overlayer [20, 21]. Both models give the same qualitative relationship between r and T fus , but the physical interpretation is somewhat different. The calculated melting point of gold versus the radius of the gold particle is shown in Figure 6.18. The estimated temperature of fusion versus particle size is in relatively good agreement with experimental data [21]. The considerations presented above could in principle be extended to binary systems and phase diagrams. In this case one might imagine that the solid particle is embedded in the coexisting liquid, and that the pressure gradient across the solid–liquid interface is determined by the solid–liquid interfacial energy. Like the bulk thermodynamics, the interfacial thermodynamics also depend on composition [22]. An approach to estimating the effect of particle size on phase diagrams has recently been reported [23, 24]. The estimates consider a hypothetical equilibrium between spherical solid and liquid particles at constant pressure. The difference in the Gibbs energy of the liquid and solid spheres is described by one bulk and one surface term. Since the surface tension of liquids is usually lower than the surface energy of solids, the liquidus and solidus lines are suppressed to lower temperatures as the radius is reduced [23, 24].
6.2 Surface effects on heterogeneous phase equilibria
185
Particle sizeinduced phase transitions It has been shown for several materials that synthesis of finegrained powders has resulted in the formation of a polymorph other than the stable bulk polymorph. A typical example is that nanocrystalline alumina is usually found as g Al2O3, while the stable polymorph for bulk alumina is aAl2O3. It is commonly assumed that these metastable (relative to the bulk) structures are adopted in order to lower the total Gibbs energy of the material through a decrease in surface energy. The enthalpy difference between g Al2O3 and aAl2O3 is shown as a function of the surface area in Figure 6.19. The average surface energy of g Al2O3 is lower than for aAl2O3, and g Al2O3 becomes energetically more stable than aAl2O3 when the surface area exceeds ~135 m2 g–1 (smaller than 12 nm grain size) [25]. A difference in surface energy will also affect the equilibrium transition temperature between two polymorphs when measured as a function of the particle size. An expression for the variation of the phase transition temperature between a highsurface energy, lowtemperature polymorph a and a lowsurface energy, hightemperature polymorph b can be described using the phenomenology of the solid–liquid phase transition described above. The transition temperature versus the size of a grain is now expressed as é (T trs )r 2M êg ag  g 1= (T trs )r =¥ rr a D trs H m ê êë
bg æç
ra ç rb è
2 /3 ù
ö ÷ ÷ ø
ú ú úû
(6.75)
where (T trs )r =¥ and (T trs )r are the bulk transition temperature and the transition temperature for a particle with radius r respectively. Equation (6.75) establishes that depression of the phase transition temperature is only possible when g ag > g bg ( r a / r b )2 / 3 . In Figure 6.20 the monoclinic to tetragonal phase transition 15
D trs Hm / kJ mol –1
10 5 0 –5 –10 0
50
100
150
Surface area /
200
250
m 2 g–1
Figure 6.19 The enthalpy of transition of gAl2O3 to aAl2O3 as a function of the surface area of the nanocrystalline particles [25].
186
6 Surfaces, interfaces and adsorption 1400
Ttrs bulk
Ttrs / K
1200 1000 800 600 400 0.01
0.1 r / mm
1
10
Figure 6.20 The transition temperature between monoclinic and tetragonal zirconia versus eq = 1447 K, rm = 5.45 g cm–3, rt = 5.77 g cm–3, g mg grain size. DtrsHm = 5.94 kJ mol–1, Ttrs tg = 1.46 J m–2, g = 1.1 J m–2 [26].
of ZrO2 is shown as a function of the grain size. Monoclinic zirconia becomes stable below 20 nm grain size at room temperature, in reasonable agreement with experimental observations [26]. Due to recent developments in synthesis, the preparation of nanocrystalline polymorphs, which are usually unstable as bulk phases, has been achieved for several materials such as ZrO2, TiO2 and various perovskites. The appearance of these exotic materials does not necessarily mean that they are thermodynamically stable, since the kinetics (templates and surfactants) are probably more important for the processes than the thermodynamics. Adsorption of water may also play an important role as in the case of alumina, but in the data given in Figure 6.19 the effect of water has been accounted for [25].
6.3 Adsorption and segregation The adsorption of gases on solids can be classified into physical and chemical adsorption. Physical adsorption is accompanied by a low enthalpy of adsorption, and the adsorption is reversible. The adsorption/desorption characteristics are in these cases often described by adsorption isotherms. On the other hand, chemical adsorption or segregation involves significantly larger enthalpies and is generally irreversible at low temperatures. It is also often accompanied by reconstruction of the surface due to the formation of strong ionic or covalent bonds. Gibbs adsorption equation The adsorption of an adsorbent of a solution b on an adsorbate a is formally described below. The adsorbent is atoms or molecules and the solution a liquid or a
6.3 Adsorption and segregation
187
gas, while the adsorbate is a solid or liquid phase. Both the solution b and the phase a are in general multicomponent systems. The concentration of the adsorbent at the interface between the two phases is described in terms of the adsorption, G, defined by equation (6.3). The following section will relate adsorption to surface tension and in this section we will not use superscripts on s. The internal energy of the system described in Figure 6.2 is C
U = TS  pa V a  p b V b + å n i m i + sA s
(6.76)
i =1
By subtracting the internal energy of the two homogeneous phases adjacent to the dividing surface from equation (6.76) the internal energy of the dividing surface is obtained: C
U s = TS s + å n si m i + sA s
(6.77)
i =1
Differentiation of eq. (6.77), when combined with eq. (6.14), gives the Gibbs–Duhem equation in internal energy for a system where the surface energy is not negligible: C
S s dT + å n si dm i + A s ds = 0
(6.78)
i =1
Reorganization of eq. (6.78) and using eq. (6.3) leads to the Gibbs adsorption equation: ds = 
C Ss dT  å Gi dm i As i =1
(6.79)
For solid–gas and liquid–gas interfaces, where b is a gas phase (eq. 6.79) can be further simplified if the adsorbate contains only two components, A and B, since changes in the chemical potential of the two components of the adsorbate due to a change in mole fraction are related by eq. (1.92) as dm A = 
xB dm B xA
By substituting eq. (6.80) into eq. (6.79) we obtain at constant temperature
(6.80)
188
6 Surfaces, interfaces and adsorption
æ ds  çç è dm B
é ö æx ÷÷ = êGB  çç A øT ë è xB
ö ù ÷÷ GA ú ø û
(6.81)
where x A and x B are the mole fraction of A and B in the adsorbate a. This equation can be further developed. The adsorption G depends on the position of the Gibbs dividing surface and it is therefore convenient to define a new function, the relative adsorption, that is not dependent on the dividing surface. The absorption of component i at the interface is defined by eq. (6.3) as Gi =
n si As
=
1 1 ( n i  n ai  n ib ) = ( n i  c ai V a  c ib V b ) As As
(6.82)
where c ai = n ai / V a and c ib = n ib / V b are the concentrations of i in the two phases adjacent to the interface and V a and V b are the volumes of these phases. Since eq. (6.82) can be rewritten in terms of the total volume as Gi =
1 [ n i  c ai V  (c ib  c ai )V b ] As
(6.83)
the adsorption of component A can be expressed as GA =
1 b [ n A  c aA V  (c A  c aA )V b ] As
(6.84)
V b can be eliminated by combining eqs. (6.83) and (6.84). We thus obtain the following important expression: æ ca  c b i Gi  GA ç i ç a b è cA  cA
æ ca  c b ö 1 é ÷= i ê(n i  c a V )  ( n A  c a V )ç i A ç a i ÷ A ê b s è cA  cA ø ë
öù ÷ú ÷ú øû
(6.85)
The advantage of this expression is that although the adsorption of each component depends on the Gibbs dividing surface, the righthand side is independent of its position. We can thus define the relative adsorption of component B with respect to component A: æ ca  c b B GB( A ) = GB  GA ç B ç a b è cA  cA
ö ÷ ÷ ø
(6.86)
6.3 Adsorption and segregation
189 S
b
cAÆ
a
xÆ
Figure 6.21 Schematic illustration of the concentration of component A across an interface. The Gibbs dividing surface is positioned such that it gives zero adsorption of component A since the algebraic sum of the two shaded areas with opposite sign is zero.
Since GB( A ) is independent of the position of S, we can choose the position of S to correspond to GA = 0, as illustrated for a schematic twodimensional interface in Figure 6.21. The two shaded areas, above and below the interface, are equal and give zero adsorption of A. Recall that it is only for planar surfaces that the position of the Gibbs dividing surface is arbitrary, and in the following we will restrict our treatment to planar surfaces only. Relative adsorption and surface segregation We can now use the relative adsorption to describe a twocomponent system at constant temperature. The relative adsorption of B with respect to A for GA = 0 is given by eq. (6.81) as æ ¶s GB = GB(A) =  çç è ¶m B
ö ÷÷ øT
(6.87)
Thus the adsorption of B at the interface is given by the variation of the surface tension with chemical potential. Equation (6.87) is the basis for most adsorption measurements associated with liquid solutions. When (¶s / ¶m B ) T is negative, GB is positive and there is an excess of the solute at the interface. For (¶s / ¶m B ) T > 0, GB is negative and there is a deficiency of the solute at the interface. In other words, solutes that reduce the surface tension are enriched at the surface. The relative adsorption of component B is clearly affected by its partial pressure. Let us consider a binary system A–B where GA = 0 and B is an ideal gas with partial pressure pB . The chemical potential of B can be expressed in terms of the partial pressure of B and this is then also the case for the relative adsorption of B
190
6 Surfaces, interfaces and adsorption
GB = GB(A) = 
1 RT
æ ¶s çç è ¶ ln pB
ö ÷÷ øT
(6.88)
The effect of an impurity on the surface energy is often discussed in terms of the surface activity of the impurity B, jB, defined as the slope of the surface tension or energy versus composition at infinite dilution: æ ¶s j B =  çç è ¶x B
ö ÷÷ ø xA ®1
(6.89)
Using the Gibbs absorption equation and assuming Henry’s law (eq. 3.42) jB = 
1 RT
æ ¶s çç è ¶x B
ö ÷÷ ø xA ®1
=
1 RT
æ ¶s çç è ¶m B
æ ¶m B ö çç ÷÷ ø xA ®1 è ¶x B
=+
1 ( A ) æ ¶m B G ç RT B çè ¶x B
æ ¶ ln a B = GB( A ) çç è ¶x B
ö ÷÷ ø xA ®1
(6.90)
ö ÷÷ ø xA ®1
ö ÷÷ ø xA ®1
Experimentally jB is found to be finite. The slope of the relative adsorption versus composition, which is also finite, is referred to as Henry’s law for surfaces. For electronegative elements on metallic surfaces the surface activity becomes very high, often of the order of 103. This means that very small amounts of these elements have a large effect on the surface energy, and that the experimental determination of reliable surface energies needs systems of extreme purity. The effect of composition on s with a focus on the dilute limit, is shown for selected systems in Figure 6.22. A considerable degree of segregation must be expected for these example systems. Physically this situation corresponds to solute atoms that have large positive size misfits, and/or large positive enthalpies of mixing and these solutes are thus expected to segregate readily to the surface. Substances that have a large effect on the interfacial energy even at small concentrations are called surfaceactive species. For most metals, oxygen, sulfur and other elements of group 16 are generally strong surfaceactive species. Similarly, the surface tension of liquid oxides or halides is strongly influenced by the addition of small amounts of other components that have the opposite acid–base properties. For example the surface tension of silicates is easily modified by addition of basic oxides such as alkali or alkali earth metal oxides.
6.3 Adsorption and segregation
191 P–Fe(s)
1.6 1.2
lg
s or g
O–Fe(liq)
Bi–Cu(s)
sg
/Jm
–2
2.0
S–Fe(liq)
0.8
O–Ag(s)
0.4 1E–5
1E–4
1E–3 x
0.01
0.1
1
Figure 6.22 Surface tension as a function of the concentration for some surfaceactive species in solid Fe, Cu and Ag near their melting temperatures [27] and liquid Fe at 1550–1600 °C [28].
In most systems the variation of the surface tension with composition is much lower. Data for some binary liquids are shown in Figure 6.23. A limited degree of segregation is expected in these systems. Adsorption isotherms Here we are considering the dynamic equilibrium between molecular species in the gas phase and the adsorbed gas species on a surface. Let us consider the following quasichemical equilibrium between the species B in the gas, Bg, and the available sites at the surface of the adsorbate: ka ¾¾ ® B g + V MON ¬ ¾ ¾ B MON
(6.91)
kd
Fe–Ni, 1550 °C
1.5 s lg / J m –2
Fe–Sn, 1550 °C
1.0
Ag–Au, 1108 °C
0.5 SiO2 –PbO, 1100 °C KNO3–NaNO3, 397 °C
0.0 0.0
MgCl 2 –NaCl, 827 °C
0.2
0.4
0.6
0.8
1.0
x
Figure 6.23 Isothermal surface tension versus composition of some binary metals [28], oxide [29] and salt systems [14, 15].
192
6 Surfaces, interfaces and adsorption
Here V MON and B MON represent the available vacant sites and surface sites occupied by B, respectively, of the first monolayer on a solid absorbate. The equilibrium constant KL for the reaction is given by the ratio of the rate constant for ka for adsorption and kd for desorption KL =
ka GB = g sat k d a (G  GB ) B B
(6.92)
where GB is the adsorption of B at the surface, GBsat  GB the concentration of vacant sites in the monolayer and a Bg the activity of B in the gas phase. By introducing the fractional coverage of the adsorbate surface q, eq. (6.92) can be transformed into the Langmuir adsorption isotherm [30] given as GB / GBmax 1  GB / GBmax
=
q = K LaB 1q
(6.93)
where GBmax is the maximum adsorption. In this simplest physically realistic adsorption isotherm it is assumed that adsorption cannot precede beyond a monolayer coverage, all sites are equivalent and the ability of a molecule to adsorb is independent of the occupation of the neighbouring sites, i.e. there are no mutual interactions. Typical adsorption isotherms are shown in Figure 6.24 for different values of KL. The Langmuir model was extended to include interaction between the adsorbed atoms/molecules by Fowler and Guggenheim [31]. The model now becomes K L a Bb =
é æ zw q expê2çç 1q ë è k BT
ö ù ÷÷q ú ø û
(6.94)
1.0 KL = 100
0.8 KL = 10
q
0.6
1.0
0.4
KL = 1
0.2
0.8 0.6 G 0.4 0.2 0.0 0
0.0 0.01
G Bsat
0.1
1
2 p / bar
4
10
p / bar
Figure 6.24 Adsorption isotherms following Langmuir adsorption isotherm.
6.3 Adsorption and segregation
193
where z is the number of nearest neighbours within the surface layer, w is the regular solution parameter and a Bb is the activity of B in b. For w = 0, the Fowler–Guggenheim adsorption reduces to the Langmuir isotherm. A major advance in adsorption theory generalized the treatment of monolayer adsorption and incorporated the concept of multilayer adsorption. This is known as the BET theory after Brunauer, Emmett and Teller [32]. The adsorption of a gas on a solid surface can be described by p 1 C 1 = + m A ( p0  p) m MON C m MON C
æ p ö çç ÷÷ è p0 ø
where mA is the total amount of gas adsorbed and mMON is the quantity of gas adsorbed corresponding to a monolayer. p and p0 are the pressure and saturation pressure of the absorbent and C is a constant. A plot of p/[ m A ( p0  p)] versus p/ p0 gives a straight line with intercept1/ m MON C and slope (C 1)/ m MON C . The values of C and mMON may then be obtained from a linear regression of experimental points of mA versus p/ p0 . By using the mean area per molecule adsorbent the surface area of the solid can be calculated from mMON. This method is frequently used to determine specific surface area of porous materials. Experimentally the enthalpy of adsorption is observed to be a function of the fractional surface coverage q since it depends on interactions between the adsorbent molecules/atoms and rearrangements of the surface due to the formation of new chemical bonds. In some cases, for example for CO adsorption on single crystal surfaces of metals, the enthalpy of adsorption can change abruptly when the structure of the absorbed layer changes [33]. Although the determination of accurate enthalpies of adsorption is difficult and values reported often vary from one laboratory to another, clear trends in the enthalpy of adsorption are often observed. It is clear that the enthalpy of adsorption of gases like, CO, H2, N2 and NH3 on transition metals decreases when going from left to right along a period [33]. For adsorption of metals on metal oxides, as exemplified by Cu on the (100) surface of MgO, the lowcoverage heats of adsorption when the metals are mainly in twodimensional islands correlate with the bulk sublimation enthalpy of the adsorbent. This suggests that covalent metal–Mg bonding dominates the interaction at low coverage [34]. On adsorption beyond the first monolayer the enthalpy of adsorption approaches the enthalpy of sublimation of Cu. Accurate data on the enthalpy of adsorption are known in only a few systems, and a recent report [35], which shows that the particle size has a much larger effect on the energetics than predicted by equations of the type considered in Section 6.2, suggests that our knowledge on this complex topic is still limited.
References [1]
J. W. Gibbs, The Collected Works, Volume I Thermodynamics. Harvard: Yale University Press, 1948.
194
[2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34] [35]
6 Surfaces, interfaces and adsorption
A. I. Rusanov, Surf. Sci. Reports 1996, 23, 247. C. H. P. Lupis, Chemical Thermodynamics of Materials. Amsterdam: Elsevier Science, 1983. G. Wulff, Z. Krist. 1901, 23, 449. C. Herring, in Structure and Properties of Solid Surfaces (R. Gomer and C. S. Smith, eds.). Chicago: University of Chicago Press, 1953. C. Herring, Phys. Rev. 1951, 82, 87. W. W. Mullins, Metal Surfaces: Structure, Energetics and Kinetics. Metals Park, OH: Am. Soc. Metals, 1963, Ch. 2. J. H. Alonso and N. H. March, Electrons in Metals and Alloys. London: Academic Press, 1989. A. S. Shapski, J. Chem. Phys. 1948, 16, 386. A. A. V. Grosse, J. Inorg. Nucl. Chem. 1964, 6, 1349. J. M. Howe, Interfaces in Materials. New York: John Wiley & Sons, 1997. G. A. Somorjai, Principles of Surface Chemistry. Englewood Cliffs, NJ: Prentice Hall, 1972. F. D. Richardson, Physical Chemistry of Melts in Metallurgy. London: Academic Press, 1974. G. J. Jans, U. Krebs, H. F. Siegenthaler and R. P. T. Tomkins, J. Phys. Chem. Ref. Data, 1972, 1, 680. G. J. Jans, R. P. T. Tomkins , C. B. Allen, J. R. Downey Jr, G. L. Gardner and U. Krebs, J. Phys. Chem. Ref. Data, 1975, 4, 1117. D. Turnbull, J. Appl. Phys. 1950, 21, 1022. J. D. van der Waals, Z. Chem. Phys. 1894, 13, 657. E. A. Guggenheim, J. Chem. Phys. 1945, 13, 253. C. Herring, in Physics of Powder Metallurgy (W. E. Kingston ed.). New York: McGrawHill, 1951. K.J. Hansen, Z. Phys. 1960, 157, 523. Ph. Buffat and J.P. Borel, Phys. Rev. A 1976, 13, 2287. R. T. DeHoff, Thermodynamics in Materials Science. New York: McGrawHill, 1993. T. Tanaka and S. Hara, Z. Metallkd. 2001, 92, 467. T. Tanaka and S. Hara, Z. Metallkd. 2001, 92, 1236. J. M. McHale, A. Auroux, A. Perrotta and A. Navrotsky, Science 1997, 277, 788. R. C. Garvie, J. Phys. Chem. 1978, 82, 218. E. D. Hondros, in Precipitation in Solids (K.C. Russel and H. I. Aaronson eds.). Warrendale, PA: The Metallurgical Society of AIME, 1978. L. E. Murr, Interfacial Phenomena in Metals and Alloys. Reading, MA: AddisonWesley, 1975. L. Shartsis, S. Spinner and A. W. Smack, J. Am. Ceram. Soc. 1948, 31, 23. I. Langmuir, J. Am. Chem. Soc. 1918, 40, 1361. R. Fowler and E. A. Guggenheim, Statistical Thermodynamics. Cambridge: Cambridge University Press, 1939, p. 430. S. Brunauer, P. H. Emmett and E. Teller, J. Am. Chem. Soc. 1938, 60, 309. G. A. Somorjai, Chemistry in Two Dimensions: Surfaces. Ithaca, NY: Cornell University Press, 1981. C. T. Campbell and D. E. Starr, J. Am. Chem. Soc. 2002, 124, 9212. C. T. Campbell, S. C. Parker and D. E. Starr, Science 2002, 298, 811.
6.3 Adsorption and segregation
195
Further reading J. M. Howe, Interfaces in Materials. New York: John Wiley & Sons, 1997. M. J. Jaycock and G. D. Parfitt, Chemistry of Interfaces. John Wiley & Sons, New York, 1981. J. Lyklema, Fundamentals of Interface and Colloid Science, Vol. 1: Fundamentals. London: Academic Press, 1991. L. E. Murr, Interfacial Phenomena in Metals and Alloys. Reading, MA: AddisonWesley, 1975. G. A. Somorjai, Chemistry in Two Dimensions: Surfaces. Ithaca, NY: Cornell University Press, 1981. G. A. Somorjai, Introduction to Surface Chemistry and Catalysis. New York: John Wiley & Sons, 1994.
7
Trends in enthalpy of formation
o The standard enthalpy of formation, D f H m , of a compound at 0 K reflects the strength of the chemical bonds in the compound relative to those in the constituent elements in their standard state. The standard enthalpy of formation of a binary oxide such as CaO is thus the enthalpy change of the reaction
Ca(s) + 1 O2 (g) = CaO(s)
(7.1)
2
at p = 1 bar. A number of theoretical approaches can account for the fact that an enthalpy of formation of such a binary oxide or a ternary oxide is large and negative. The stability of a ternary oxide relative to the binary constituent oxides is, however, often small, as demonstrated in Table 7.1 using Mg2SiO4 as an example [1]. The enthalpy differences between the three different polymorphs of Mg2SiO4 – olivine, bphase and spinel – are less than 2% of the enthalpy of formation of the polymorphs. These enthalpy differences are comparable in magnitude to the enthalpy Table 7.1 Magnitudes of enthalpies of various reactions of a ternary oxide using Mg2SiO4 as an example (after Navrotsky [1]). 2Mg(s) + Si(s) + 2O2(g) = Mg2SiO4 (olivine) 2MgO + SiO2(s) = Mg2SiO4 (olivine) Mg2SiO4 (olivine) = Mg2SiO4 (liq.) Mg2SiO4 (olivine) = Mg2SiO4 (b) Mg2SiO4 (b) = Mg2SiO4 (spinel)
–2170.41 kJ mol–1 –56.61 kJ mol–1 114 kJ mol–1 29.9 kJ mol–1 9.1 kJ mol–1
Chemical Thermodynamics of Materials by Svein Stølen and Tor Grande © 2004 John Wiley & Sons, Ltd ISBN 0 471 492320 2 197
198
7 Trends in enthalpy of formation –236.0 solid solution
–236.2 TinO2n–1
–236.4
o
D f Gm / kJ mol –1
Ti3O5
–236.6
solid Ti4O7 solution Ti8O15 Ti5O9 Ti O Ti9O17 6 11 Ti7O13
–236.8 0.63
0.64
0.65
0.66
xO
Figure 7.1 The Gibbs energies of formation of stoichiometric and nonstoichiometric compounds in the system Ti3O5–TiO2 [4]. Composition given as mole fraction O.
of formation of olivine from the binary oxides, and to the enthalpy of fusion of olivine. The fact that different structural modifications of a given ternary oxide may be close in enthalpy and thereby in Gibbs energy at low temperatures makes predictions of phase diagrams far from trivial. Still, quantum mechanical approaches have in recent years been increasingly able to derive the relative enthalpies of different structural modifications of ordered compounds with a given composition, see e.g. [2, 3] and also Chapter 11. Although the existence of polymorphism is challenging to theory, the prediction of the compositions of the phases that exist in a given binary or ternary system is in general even more challenging. The Gibbs energy of formation of stoichiometric and nonstoichiometric compounds in the system Ti3O5–TiO2, presented graphically in Figure 7.1 [4], constitutes an excellent example. A large number of phases of the homologous series TinO2n–1 are close in Gibbs energy and the Gibbs energy differences between different phases or phase mixtures are tiny. In general, a phase with a given stoichiometry must be stable relative to other phases of the same composition, but also relative to the neighbouring phases. A large number of marginally stable and marginally metastable phases exist in many material systems. It is in general much more difficult to predict the compositions of the compounds that exist in a given binary or multicomponent system than the relative stability of different polymorphs of a given composition. The composition and crystal structure of the materials that are formed are complex functions of a large number of factors. Solid compounds may be qualitatively assigned to have ionic, covalent or metallic bonds, and although a number of compounds exist in which one of these bonding schemes dominates, most compounds do not belong to clearcut categories and even for largely ionic compounds covalent contributions must be taken into consideration. While the valence electrons are localized in ionic and covalent compounds, they are highly delocalized in metals. Schematically the character of bonding in any compound may be indicated
7.1 Compound energetics: trends
199 ionic CsF
electronegativity difference increases
Al2O3 NiS
CuAl 2
ZnS BN
metallic
covalent electron negativity increases
Figure 7.2 Schematic categorization of bonding in solids.
in a triangular diagram, such as Figure 7.2, whose corners are the three extremes of pure covalent, ionic and metallic bonding [5]. The electronegativity difference between the components is a major factor and a number of rationalization schemes have been proposed in which the energetics are characterized in terms of two factors, one related to size and one related to electronegativity. Most energetic contributions are, as we have discussed, difficult to predict and large experimental efforts have for that reason been devoted to derive systematic trends in the energetics of classes of materials. In this chapter we will try to convey an overview of periodic trends in the thermodynamic properties of inorganic compounds and we will also present selected examples illustrating some of the more usual rationalization schemes. Finally, trends in enthalpy of mixing are treated. Also here we aim to look at trends and rationalization schemes. The chapter is by no means exhaustive â€“ only selected classes of compounds and selected rationalization schemes are discussed.
7.1 Compound energetics: trends Prelude on the energetics of compound formation Let us consider the enthalpy of formation of an ionic compound like NaCl, or in general terms MX: M(s) + 1 X2(g) = MX(s) 2
(7.2)
This reaction may be analyzed through the thermodynamic cycle given in Figure 7.3 where the following five reactions and associated enthalpy changes are involved:
200
7 Trends in enthalpy of formation MX(s)
–D latt Hm
+
M (g)
+
D egHm
D ion Hm D f Hm
M(g)
+
D atom Hm M(s)
–
X (g)
+
X(g)
D diss Hm 1/2X2(g)
Figure 7.3 Thermodynamic cycle for the formation of MX(s).
M+(g) + X–(g) = MX(s)
–DlattHm
(7.3)
M(s) = M(g)
DatomHm
(7.4)
M(g) = M+(g) + e–(g)
DionHm
(7.5)
1 X (g) 2 2
DdissHm
(7.6)
DegHm
(7.7)
= X(g)
X(g) + e– = X–(g)
The lattice enthalpy, DlattHm, is the molar enthalpy change accompanying the formation of a gas of ions from the solid. Since the reaction involves lattice disruption the lattice enthalpy is always large and positive. DatomHm and DdissHm are the enthalpies of atomization (or sublimation) of the solid, M(s), and the enthalpy of dissociation (or atomization) of the gaseous element, X2(g). The enthalpy of ionization is termed electron gain enthalpy, DegHm, for the anion and ionization enthalpy, DionHm, for the cation. The enthalpy of formation of the compound MX is now the sum of these five contributions: DfHm(MX) = –DlattHm + DatomHm + DionHm + DdissHm + DegHm
(7.8)
While the enthalpy of formation is the property of interest in chemical thermodynamics of materials, many books focus on the lattice enthalpy when considering trends in stability. The static nonvibrational part of the lattice enthalpy can be deconvoluted into contributions of electrostatic nature, due to electron–electron repulsion, dispersion or van der Waals attraction, polarization and crystal field effects. The lattice enthalpy is in the 0 K approximation given as a sum of the potential energies of the different contributions:
7.1 Compound energetics: trends
DlattHm = Felectrostatic + Frepulsion + Fdispersion + Fpolarization + Fcrystal field
201
(7.9)
and trends in this property become evident only when the relative importance of these different contributions are considered. The largest contribution, the electrostatic interaction, is due to attraction between ions with opposite charge and repulsion between ions of the same charge. Using the NaCltype crystal structure as an example, the electrostatic potential energy is evaluated taking one particular M+ at the body centre of the unit cell as a starting point and calculating the interaction between this particular ion and its neighbours. The central M+ is surrounded by an octahedron of six X– ions with each X– ion at distance rMX. The attractive energy ignoring X––X– interactions is then 6
e2 q M q X rMX
(7.10)
The next nearest neighbours to the central M+ are 12 M+ at distance 2r. The repulsive cation–cation interaction term is given as 12
e2 q M q X
(7.11)
2rMX
Correspondingly, the contribution from the third nearest neighbours, 8 X– at 3r is 8
e2 q M q X
(7.12)
3rMX and so on. The net attractive energy between the central M+ and all other ions in the crystals is thus given by the infinite series F=
e2 q M q X rMX
ö æ 12 8 6 + + × × × ÷÷ çç 6 2 3 4 è ø
(7.13)
The crystal arrangement is hence important for the lattice enthalpy and Velectrostatic can be extracted for a specific crystal structure as Felectrostatic =
NMe 2 q M q X rMX
(7.14)
202
7 Trends in enthalpy of formation
where M is the Madelung constant for a given structure and rMX is the shortest MX distance. The Madelung constant depends only on the geometrical arrangement of the point charges defined by the crystal structure. A second and repulsive energy term must be introduced to take account of the electron–electron repulsion that arises at very short interatomic distances. Several models are used to describe this repulsive term. Often used is the Buckingham potential, which, however, includes both attractive and repulsive components: æ rij V vdw (rij ) = A expç ç r è
ö C ÷÷ 6 ø rij
(7.15)
Here the first term reproduces the effective twobody repulsion and the second the effective twobody van der Waals attraction. rij is the interatomic distance, whereas A, r and C are constants that are usually determined empirically. The repulsive term is steeply increasing at low interatomic distances but quickly becomes negligible beyond the nearest neighbour distance. In general, the electrostatic terms contribute 75 to 90% to the total lattice enthalpy, while the repulsive contribution is about 10 to 20%. It follows that the lattice enthalpy depends largely on the charge and on the relative size of the cation and anion, since these factors dominate the electrostatic term in eq. (7.14). This is reflected in the lattice enthalpies presented in Figures 7.4(a) and (b). The lattice enthalpy of the Na halides becomes less positive from NaF to NaI. Similarly, the lattice enthalpy of the alkali iodides becomes less positive from LiI to CsI. While this effect is clearly important when considering enthalpies of formation, this is not the only factor to be taken into account [6, 7]. As indicated by the thermodynamic cycle in Figure 7.3, the variation in the atomization and ionization enthalpies of the metal atom and in the dissociation and electron gain enthalpies of the nonmetal atom must also be considered. The relevant data are given in Figures 7.4(c) and (d). Periodic trends in the enthalpy of formation of binary compounds Let us now consider trends in enthalpy of formation and first trends for the alkali halides with a given halide ion, i.e. the alkali fluorides and the alkali iodides. The ease with which a free gaseous ion is formed from the solid metal increases down group 1 of the periodic system. Similarly, the ionization enthalpy becomes less positive as seen in Figure 7.4(d). The enthalpy of formation analyzed in terms of eq. (7.8) involves the formation of the compound from the gaseous ions and thus involves –DlattHm. The effect of the lattice enthalpy is thus opposite to the trend in the atomization and ionization enthalpies and as a result of the balance of these two opposing trends there is often little change in the enthalpy of formation down these groups, as is evident in Figure 7.5(a). For the alkali fluorides the size of the anion implies that the most negative enthalpy of formation is that of LiF. The less endothermic enthalpy of atomization and ionization of Cs gives CsI the higher stability among the alkali iodides.
7.1 Compound energetics: trends
203 (b) 800
(a)
LiI
NaCl
800
NaBr NaI 700
Dlatt Hm / kJ mol–1
Dlatt Hm / kJ mol–1
900
NaF
750 NaI
700
KI
650
RbI
CsI
600 550
(d)
100 Dissociation
0
D r Hm / kJ mol–1
D r Hm / kJ mol–1
(c)
–100 –200 –300 –400
Electron gain F
Ionization 400 300 200 Atomization
100
I
Br
Cl
500
Li
Na
K
Cs
Rb
Figure 7.4 Thermodynamic data needed in evaluation of the enthalpy of formation of MX(s). (a) Lattice enthalpy of sodium halides; (b) lattice enthalpy of alkali iodides; (c) electron gain and dissociation enthalpies of halides; (d) ionization and atomization enthalpies of alkali metals.
Larger differences are observed when comparing the enthalpy of formation of the different halides of a given alkali metal. The enthalpy of formation of gaseous halide ions is exothermic since the exothermic electron gain enthalpy in absolute value is larger than the endothermic dissociation enthalpy. Furthermore, the enthalpy of formation of gaseous halide ions becomes less favourable with (a)
0
(b) NaI
–100
LiH
NaH
KH
RbH
CsH
–300
Na 2Se Na 2S
D f Hmo / kJ mol–1
–200 LiI –300 –400
NaI KI
LiCl
NaCl
–600
NaF
RbI
Na 2O
CsI
KCl
RbCl CsCl
KF
RbF
–500 LiF
NaBr
–400
Na 2Te
NaCl
–500
CsF –600 NaF
–700
Figure 7.5 Enthalpy of formation of binary compounds of the alkali metals.
204
7 Trends in enthalpy of formation 0
Df Hmo / kJ mol–1
HgCl2 –300 BeCl2 –600
ZnCl2 MgCl2
ZnF 2
–900 –1200
12
BeF2
MgF2
CdCl2 HgF 2
CdF 2
BaCl2
CaCl2
SrCl2
CaF2
SrF2
2 BaF2
Figure 7.6 Enthalpy of formation of group 2 and 12 dichlorides and difluorides.
increasing size of the halogen atom. The trend in the lattice enthalpy amplifies this effect and the enthalpy of formation of the Na halides varies much more with the halide ion than the alkali iodides did with the alkali metal; see Figure 7.5(b). The enthalpies of formation of the group 2 halides given in Figure 7.6 show many of the same effects. The fluorides are more stable than the chlorides and the stability increases with increasing size of the cation. The ease of atomization of the metal here increases more on a relative scale than it did for the alkali metals. The group 12 halides are also included in Figure 7.6. Their enthalpies of formation are distinctly less exothermic than those of group 2. The reason for this is the increase by +10 in nuclear charge between Ca and Zn and between Sr and Cd, and of +24 between Ba and Hg. These extra electrons are not screening the nuclear charge effectively, resulting in a much higher ionization enthalpy for the group 12 elements and a less negative enthalpy of formation for the group 12 compounds compared with the group 2 compounds. This destabilization effect is visible also in the enthalpy of formation of the metal oxides of groups 2 and 12, 3 and 13, 4 and 14 and 5 and 15; see Figure 7.7. Here, the enthalpies of formation of the metal oxides of group 13 and periods 4, 5 and 6 are much less exothermic than the for corresponding metal oxides of group 3. The same argument is valid for metal oxides of group 4 versus 14 and for group 5 versus 15. While we have interpreted the trends observed using a simple thermodynamic cycle where the electrostatic enthalpy is given in terms of formal charges of the ions and their interatomic distance (eq. 7.14), most solid compounds cannot be described properly without taking polarization into consideration. The larger the electronegativity difference between the two elements of a compound, the more polar the compound is. Polarization is more extensive for the lower coordination numbers and depends on the polarizing power and the polarizability of the ions involved in the bonding. The polarizing power increases the smaller the ion is and the higher charge it has, while polarizability is usually larger for large ions – anions with loosely bond electrons. Polarization always leads to a decrease in interatomic distance and thus to an increase in the lattice enthalpy. The difference between
(a)
205
Df Hmo / kJ mol –1
0
HgO 12
–200 ZnO
CdO
–400 –600
BaO
BeO MgO
CaO
SrO
(b)
0
Df Hmo / kJ mol –1
7.1 Compound energetics: trends
–400
2
Tl 2O3 13
–800 –1200
Ga2O3
3
–1600 Al2O3
–800 0 –300
(d) PbO2 CO2(g)
14 GeO2
–600 –900
SnO2
SiO2 4
–1200
TiO 2
ZrO2
HfO2
Df Hmo / kJ mol –1
Df Hmo / kJ mol –1
(c)
In2O3
B2O3
0
Sc 2O3
15 As 2O3
–500 P2O 3
Sb2O3
As 2O5 V2O3
–1500 P2O5
–2000
La 2O3
N2O3(g) N2O5(g)
–1000
Y2O3
V2O5 5
Bi2O3
Sb 2O5 Nb 2O5 Ta O 2 5
Figure 7.7 Enthalpy of formation of binary oxides of (a) group 2 and 12, (b) 3 and 13, (c) 4 and 14 and (d) 5 and 15 metals.
lattice enthalpies derived using experimental data and the thermodynamic cycle given in Figure 7.3 and calculated lattice enthalpies is often ascribed to polarization effects. However, the use of both pairwise potentials and models that neglect anion–anion shortrange interactions is in general questionable for compounds where there is a covalent contribution and directionality of the bonds starts to play a role. In general, overlap of incompletely filled p orbitals results in large deviations from pure ionic bonding, and covalent interactions result. Incompletely filled f orbitals are usually well shielded from the crystal field and behave as essentially spherical orbitals. Incompletely filled d orbitals, on the other hand, have a large effect on the energetics of transition metal compounds and here the socalled crystal field effects become important. All the d orbitals are equal in energy for an isolated atom. In an electric field of lower than spherical symmetry caused by the surrounding ligands, ligand field or crystal field splitting is observed. In an octahedral environment the five d orbitals of a transition metal are no longer degenerate but split into two groups; the lower energy t2g and the higher energy eg groups. This splitting is, according to the crystal field theory, due to the interaction between the negative charges on the ligands and the electrons in the d orbitals. Electrons in the two d orbitals that are pointing directly along the Cartesian axes, d x 2  y 2 and d z 2 are repelled more strongly by the negative charges on the ligands (which in the octahedral case are placed along the Cartesian axes) than the electrons in the three d orbitals that are pointing between the ligands: dxy, dxz, dyz. For a tetrahedral local environment (ligands placed between the Cartesian axes) similar arguments give stabilization of the
206
7 Trends in enthalpy of formation dz2 dxy
dxz
dx2 –y 2 eg
d yz
t2g 0.6D oct
0.4D tetr all
–0.4D oct
–0.6D tetr dxy
eg dz2
dxz
dyz
t 2g
dx2 –y 2
tetrahedral field
free ion
octahedral field
Figure 7.8 d level splitting for octahedral and tetrahedral crystal fields.
eg orbitals and destabilization of the t2g orbitals. The splitting is schematically shown in Figure 7.8 for octahedral and tetrahedral symmetry. The extent of the splitting is often called crystal field (ionic picture) or ligand field (covalent picture) splitting, and the accompanying energy is often given the symbol D. This splitting energy measures the interaction between the cation and the surrounding anions, and depends strongly on the interatomic distance that again depends on the nature of the ligand. It is also affected by temperature, pressure, crystal structure and composition of the compound. For an octahedral cation the crystal field stabilization energy for one electron in the dxy, dxz or dyz orbital is –0.4Doct while an electron in a d z 2 or d x 2  y 2 are destabilized by 0.6Doct; see Figure 7.8. The energy effect of the crystal field is, although considerable, not necessarily directly reflected in the enthalpy of formation of transition metal compounds; other effects may dominate. Even so, the relative stability of the binary compounds of the d elements varies in a characteristic way. The enthalpy of formation of transition metal dichlorides, difluorides and monoxides for the first series transition metals are shown in Figure 7.9(a). The stabilization of the manganese (II) compounds relative to their nearest neighbours in terms of d electrons, Cr and Fe, is mainly due to a low atomization enthalpy for Mn (Figure 7.9(b)). The sum of the first and second ionization enthalpies varies more regularly with the number of d electrons (Figure 7.9(c)). By using the experimental enthalpies of formation, the lattice enthalpies of the compounds can be derived. The data for the dichlorides given in Figure 7.9(d) show a characteristic variation with the number of d electrons that reflects crystal field stabilization. Ions that do not show crystal field stabilization are the d0(Ca), d5(Mn) and d10(Zn) ions. For these three ions, the distribution of d electrons around the core is spherically symmetric since the d orbitals are either empty (Ca), singly (Mn) or doubly (Zn) occupied, and their lattice enthalpies thus fall on the lower, dotted curve. Although the crystal field effect is clearly present in the lattice enthalpies derived by the thermodynamic cycle
7.1 Compound energetics: trends (a)
207
0
(b)
TmCl2
–500 –750 –1000
TmF 2
400 300 200 100
Ti
V
Cr
Mn
Fe
Co
Ni
Cu
(c) 2800
Sc Ti
V
Cr Mn Fe Co Ni Cu Zn
–1
(d) D lattice Hm / kJ mol
–1
D ion Hm / kJ mol
500
–1
–250
D atom Hm / kJ mol
D f Hm / kJ mol
–1
TmO
2400
2000
Sc Ti
V
Cr Mn Fe Co Ni Cu Zn
2800 TmCl 2 2600
2400
2200
Ca Sc Ti V Cr Mn Fe Co Ni Cu Zn
Figure 7.9 Thermodynamic data (b)–(d) needed in analysis of the enthalpy of formation of the binary transition metal compounds given in (a). (b) Atomization enthalpy of first series transition metals; (c) sum of first and second ionization enthalpies of first series transition metals; (d) derived lattice enthalpy of transition metal dihalides.
using experimental enthalpies of formation, the effect is seen even more clearly in the calculated lattice enthalpies given by filled symbols and a dashed line in Figure 7.9(d). The stabilization due to the crystal field is considerable and for the halides the stabilization increases in size from F to I in accordance with the spectrochemical series. Water, oxide ions, hydroxide ions and fluoride ions have comparable crystal field strengths and thus comparable stabilization energies. For typical oxides and hydrates of divalent first row transition elements Doct is of the order 8–15 kJ mol–1 and typically twice as large for the corresponding trivalent ions. Values for second and third row transition elements are substantially higher than for the first row elements. Regularities corresponding to those observed for the transition metal compounds are seen for the oxides, nitrates and chlorides of the lanthanide metals in Figure 7.10(a). While the variation in the enthalpies of formation for the different types of lanthanide compounds shows a large degree of similarity, small deviations from a close to linear variation with the number of f electrons are observed for the europium and ytterbium compounds in Figure 7.10(a). These ‘anomalous’ effects are largely due to high ionization enthalpies for Eu and Yb (Figure 7.10(b)). The relatively low atomization enthalpies (Figure 7.10(c)) of Eu and Yb counteract the large ionization energies to a limited degree only. The calculated lattice enthalpies for the lanthanide trichlorides are given in Figure 7.10(d).
208 (b) –1
–900 –1200
LnCl3
–1500
Ln(NO3)3
D ion Hm / kJ mol
D f Hm / kJ mol
–1
(a)
7 Trends in enthalpy of formation
–1800
4200 3900 3600
Ln2O3 –2100
La
Pr
Pm
Eu
Tb
Ho
Tm
3300
Lu
(c)
La
Pr
Pm
Eu
Tb
Ho
Tm
Lu
Eu
Tb
Ho
Tm
Lu
(d) –1
D lattice Hm / kJ mol
D atom Hm / kJ mol
–1
4600 400
300
200 La
Pr
Pm
Eu
Tb
Ho
Tm
Lu
4500 LnCl3
4400 4300 4200
La
Pr
Pm
Figure 7.10 Thermodynamic data (b)–(d) needed in analysis of the enthalpy of formation of the binary lanthanide metal compounds given in (a). (b) Sum of first, second and third ionization enthalpies of lanthanide metals; (c) atomization enthalpy of lanthanide metals; (d) derived lattice enthalpy of lanthanide trichlorides.
Transition metals are characterized by their ability to form compounds in several oxidation states. We will here use the 3d transition metal oxides to illustrate trends in stability with oxidation state. In general, there is a gradual decrease in stability of the oxides in any given oxidation state relative to the metal across the transition metal series, as shown in Figure 7.11(a). The decrease in stability of oxides of a given oxidation state within a period is most marked in the higher oxidation states. It follows that the ease of oxidation of metals, or of metals in a lower oxidation state oxide to a higher oxidation state one, decreases going to the right within a period. An analogous behaviour is observed for the metals in acidic aqueous solutions where the complexes of the later transition metals are powerful oxidizing agents. While the stability of an oxide is given in terms the Gibbs energies of formation, the stability of the different species of an element M in aqueous solutions can be represented in what is termed Frost diagrams. Here the Gibbs energy is given in terms of the standard potential E o as –NFE o , where N is the oxidation number of the metal. In the Frost diagram NE o for the reaction M(N) + Ne– ® M(0) is plotted versus the oxidation number N.
(7.16)
7.1 Compound energetics: trends (a)
209 (b)
0
2
CuO
o
MnO2
–600
CrO3
H2Cr2O7
3+
Ni 3+ Co MnO 2 3+ Fe
VO
2+
–2 2+
TiO
–4
V2O5
–900 0
DfHmo / kJ mol metal–1
NE / eV
Fe 2O3
Sc 2O3
(c)
0
Ni2O3 Co3O4
–300
1
–6
TiO2
2 3 4 oxidation number
5
6 (d)
0
–300
TmO
Tm2O3
–600
–900
TmO2
Ti
V
Mn
Fe
Co
Ni
1
2 3 4 oxidation number
5
6
0 –200 –400
CrO2 MoO2
–600 –800
Cr
3+
Sc
0
DfHmo / kJ mol –1
DfHmo / kJ mol metal–1
2+
Cu
CrO3
WO2 Cr2O3
MoO3 WO3
Cu
Figure 7.11 Enthalpy of formation of binary oxides of the 3d transition metals (a) and (c), Frost diagram for the same 3d metals (b) Enthalpy of formation of binary oxides of the group 6 transition metals.
The Frost diagrams for the first series of the d block elements in acidic solution, pH = 0, given in Figure 7.11(b) show many similarities with the variation of the enthalpy of formation of the oxides. Only the oxidation states observed for solid oxides are included. The relative stabilities of the dioxides, sesquioxides and monoxides for first period transition metals are given in Figure 7.11(c). The stability of the higher oxidation state oxides decreases across the period. As we will discuss later, higher oxidation states can be stabilized in a ternary oxide if the second metal is a basic oxide like an alkaline earth metal. The lines in Figure 7.11(c) can in such cases be used to estimate enthalpies of formation for unstable oxidation states in order to determine the enthalpy stabilization in the acid–base reactions; see below. Finally, it should be noted that the relative stability of the oxides in the higher oxidation states increases from the 3d via 4d to the 5d elements, as illustrated for the Cr, Mo and W oxides in Figure 7.11(d). We have in the preceding treatment largely confined our discussions to oxides and halides. Similar arguments could also be used on sulfides or nitrides, for example. The variation of the enthalpy of formation of selected binary compounds of group 15 and 16 anions with a common cation are shown in Figure 7.12. The enthalpy of formation becomes more negative the larger the electronegative difference, and thus with increasing group number and decreasing period number for the anion.
210
7 Trends in enthalpy of formation
0
0 FeN
Mg3Sb2 Mg3P2
–300 CaTe
CaSe
CaS CaI2
CaO CaBr2 CaCl2
–900
–1200
DfHm / kJ mol –1
DfHm / kJ mol –1
Mg3N2
–600
FeP
Mg3As2
–300
FeSb
FeAs FeS FeSe
FeTe FeI2
FeBr2
FeO FeCl2
–600 FeF2
–900
–1200
CaF2
Figure 7.12 Enthalpy of formation of selected binary compounds of group 15, 16 and 17 anions.
Intermetallic compounds and alloys In metals the electrons lose their association with individual atoms and the number of valence electrons is often used in rationalization schemes. Estimated enthalpies of formation for equiatomic alloys, MM ¢, of two elements of the first transition metal series are given as a function of the difference in number of valence electrons in Figure 7.13 [8]. Compounds of a given common metal are given a specific symbol. For example, the scandium compounds ScM ¢ where M ¢ = Ti, V, Cr, Mn, Fe, Co, Ni and Zn, are given by open circles. The metal M ¢ of the compound MM ¢ is
Df Hmo / kJ mol–1
20
0
–20
20 0
–40
Sc Ti V Cr Mn Fe Co Ni Mo W
–20 –40
–60 –8
–60
–6 –4 –2 0 2 4 6 difference in number of valence electrons
8
Figure 7.13 Estimated enthalpies of formation of equiatomic compounds MM¢ of the first transition metal series. Data for MoM¢ and WM¢ are also given [8]. The insert shows agreement between experimental and calculated values for cases where experimental values are available.
7.2 Compound energetics: rationalization schemes
211
given by the difference in number of valence electrons between the specific metal M (in our case Sc) and the other element M ¢. This difference in number of valence electrons between M and M ¢ is given as the ordinate in Figure 7.13. The data used in the figure is, as mentioned above, estimated since this enables better visualization of the trends in enthalpy of formation. Values are taken from the semiempirical twoparameter model by Miedema et al. [8] that have proven to give good estimates of the enthalpy of formation of a large number of intermetallic compounds and alloys. The insert to the figure shows the agreement between the estimated and experimental values for selected intermetallic compounds as a function of the enthalpy of formation of the compound. The enthalpy of formation of MM ¢ varies in a systematic way for all the elements of the first transition metal series. Small differences in the number of valence electrons correspond to small differences in electronegativity and thereby a low degree of stabilization due to a small degree of electron transfer between the two elements. The size mismatch between the two elements is in this case the more important enthalpy contribution, giving a destabilization effect. The strain energy due to size mismatch is further discussed in Section 7.3. Larger differences in the number of valence electrons and thus in electronegativity give more negative enthalpies of formation. Data for Mo and W compounds (MoM ¢ and WM ¢) are included in Figure 7.13 to show the effect of going from one period to the next. The variation in enthalpy of formation with the difference in number of valence electrons is similar; however, the enthalpies of formation are more exothermic for the Mo M ¢ and WM ¢ compounds compared with the corresponding first transition metal series element compounds CrM ¢. Finally, it should be added that the enthalpies of formation of equiatomic alloys of elements of the same group are close to zero.
7.2 Compound energetics: rationalization schemes Acid–base rationalization Although periodic trends in enthalpies of formation are often striking, these trends can in general not be used to estimate accurate data for compounds where experimental data are not available. Other schemes are frequently used and these estimates are often based on atomic size and electronegativityrelated arguments. As an example, the enthalpy of formation of a ternary oxide from the binary constituent oxides, i.e. the enthalpy of a reaction like AO + BxOy = ABxO1+y
(7.17)
is often interpreted in terms of factors related to electron transfer between the two oxides. The electron donor/acceptor quality of an oxide is considered in terms of acidity/basicity. A basic oxide, e.g. Na2O, is one that easily transfers its oxygens to the coordination sphere of an acid oxide like SiO2 forming a complex, welldefined
212
7 Trends in enthalpy of formation 0
Df,oxHmo / kJ mol–1
AAl2O4 –200 ACO3
–400 ASO4 Mg
Ca
Sr
Ba
Figure 7.14 Enthalpy of formation of selected ternary oxides from their binary constituents.
covalently bonded anion SiO24 . The larger the difference in acidity of AO and BxOy, the more exothermic is the enthalpy of reaction (7.17). This concept, developed by Flood and Førland [9, 10], following the initial idea of Lux [11], is frequently used in modified form, not only for oxides (see e.g. Navrotsky [1]), but even for alloys [8, 12]. In many ways this approach is analogous to what we observe in aqueous solutions. Still, in oxides the complex ions formed are often not easily defined and the oxygen atoms are bonded to several types of cations. Although the arguments are mostly used qualitatively, a quantitative optical basicity scale has been developed based on UV–visible spectroscopy and redox properties in general [13]. While the s block oxides are usually basic, the p block oxides are acidic. The basicity increases when going down a specific group e.g. MgO < CaO < SrO < BaO. The same trend is observed for the p block oxides and the oxides in general become more acidic across a specific period, e.g. Al < Si < P < S. The acidity/basicity of transition metal oxides depends on several factors. The acidity increases with increasing number of d electrons and with the oxidation state. It follows that oxides of the early transition elements in their lower oxidation states are the more basic ones. Using these simple rules the relative stability of the ternary ‘oxides’ presented in Fig. 7.14 is rationalized. BaO is the most basic oxide among those considered and the ternary Ba oxides have the most negative enthalpy of formation in the three cases considered. Similarly, the sulfates are more stable than the carbonates and aluminates relative to the binary constituent oxides, since the acidity of SO3 is larger than for CO2 and Al2O3. For compounds consisting of binary oxides of similar basicity, the enthalpy of formation is much smaller in magnitude. Here the enthalpy difference between the ternary oxide and its binary constituent oxides is small and the entropy of formation may become decisive for the stability. A ternary oxide like mullite 3Al2O3◊2SiO2, where the enthalpy of formation from the oxides is positive, is stabilized by entropy [14].
7.2 Compound energetics: rationalization schemes 20
(a)
oxides nitrides
(b)
Mg AO + 1/2S2(g) = AS + 1/2O2 (g)
100
–20
D r Gmo / kJ mol–1
or D f H nitrides / kJ mol N3 
D f Hoxides / kJ mol O2 
0
213
–40 –60 –80
Ca
Li Sr
Ba
0 Na
–100 K
–100
–120 0
5 10 15 ( zA / rA ) /( zB / rB )
1.0 1.2 Optical basicity
1.4
Figure 7.15 (a) Enthalpy of formation of ternary oxides and nitrides from their binary constituent compounds as a function of the ratio of ionic potential [16]. Reprinted with permission from [16] Copyright (1997) American Chemical Society. (b) Gibbs energy of the oxide–sulfide equilibrium for group 1 and 2 metals at 1773 K as a function of the optical basicity of the metal.
Two other examples of acid–base rationalizations are given in Figure 7.15. Figure 7.15(a) shows a large amount of data on the enthalpy of formation of ternary oxides and nitrides from the binary constituents. For both types of materials the enthalpy of formation scales with the acid–base ratio. The difference in acidity is here represented in terms of ionic potentials. The ionic potential is defined as the formal charge divided by the ionic radius. A rough grouping relating acidity and ionic potential can be made as follows: q/r < 2, strongly basic; 2 < q/r < 4, basic; 4 < q/r < 7, amphoteric; q/r > 7, acidic (here r is given in Å) [15]. The stabilization observed for a given ratio of ionic potential appears to be larger for nitrides than for oxides. The slope obtained using data for over 80 ternary oxides is smaller in magnitude than the slope observed for the ternary nitrides considered; see Figure 7.15(a) [16]. The difference may result from the greater polarizability of the N3– anion and the related higher degree of covalency in the bonding in the ternary nitrides. Figure 7.15(b) show the Gibbs energy of the oxide–sulfide equilibrium AyO (s) + 1 S2(g) = AyS(s) + 1 O2(g) 2
2
(7.18)
for group 1 and 2 metals at 1773 K as a function of the optical basicity of the metal. The linear relation observed shows the applicability of these concepts for such reactions and acid–base arguments are often successfully used in considerations of metal–slag systems [17].
214
7 Trends in enthalpy of formation
Figure 7.16 The perovskitetype structure. Small black circles represent the B atom, large grey circles represent O atoms and open circles represent the A atom.
Atomic size considerations Systematization of thermodynamic data in terms of the relative atomic size of the different ions in a compound or in terms of the ionic radius of a given cation of an isostructural series of compounds are frequently seen. The perovskitetype structure ABO3 named after the mineral with ideal composition CaTiO3 is a wellknown example. The crystal structure of the perovskite is shown in Figure 7.16. A is in the perovskitetype structure 12coordinated, while B is octahedrally surrounded by oxygen atoms. The BO6 octahedra are linked via corners and form a network. The bond lengths and angles of the BO6 octahedra can be distorted to allow a wide range of cation sizes to be accommodated into the structure compared to what would have been possible for a purely cubic arrangement. For a cubic perovskite, the tolerance factor, t, introduced already in 1926 by Goldschmidt [18], is defined as t=
rAO 2rBO
=
rA + rO 2(rB + rO )
(7.19)
where ri is the ionic radius of species i. Although t = 1 correspond to the optimum cationâ€“anion bond length, values in the range 0.8 < t < 1.1 are common. The enthalpies of formation of selected perovskitetype oxides are given as a function of the tolerance factor in Figure 7.17. Perovskites where the A atom is a Group 2 element and B is a d or f element that readily takes a tetravalent state [19, 20] show a regular variation with the tolerance factor. Empirically, it is suggested that the cations that give t close to 1 have the most exothermic enthalpies of formation. When t is reduced, the crystal structure becomes distorted from cubic symmetry and this also appears to reduce the thermodynamic stability of the
7.2 Compound energetics: rationalization schemes 0
0
SrCeO3
Df,ox Hmo / kJ mol–1
CaHfO3
–50
215
–50
CaZrO3
NdGaO3 SmAlO 3 NdAlO3 LaMnO3 LaGaO3 LaAlO3 CaMnO 3 SrMnO3
–100
SrUO 3 SrHfO3
BaCeO3
–150
SrZrO3
0.90
0.95
1.00
1.05
CaTiO 3
–100 BaHfO3
BaZrO3
SrTiO 3
–150
BaTiO 3
0.90
0.95 1.00 Tolerance factor, t
1.05
Figure 7.17 Enthalpy of formation of selected perovskitetype oxides as a function of the tolerance factor. Main figure show data for perovskites where the A atom is a Group 2 element and B is a d or f element that readily takes a tetravalent state [19, 20]. The insert shows enthalpies of formation of perovskitetype oxides where the A atom is a trivalent lanthanide metal [21] or a divalent alkaline earth metal [22] whereas the B atom is a late transition metal atom or Ga/Al.
compound. Although this rationalization may be useful for chemically related compounds, compounds that are significantly different in chemical nature should not be expected to follow the same correlation. This is evident from the insert, which shows enthalpies of formation of selected perovskitetype oxides that are chemically different from those considered in the main graph. Here, the A atom is a trivalent lanthanide metal [21] or a divalent alkaline earth metal [22], whereas the B atom is a late transition metal atom or Ga/Al. However, even here we could draw a curve roughly parallel to the one for the oxides in the main figure. Hence this rationalization scheme works well for chemically related compounds, but should in general be used with care. Similar thermodynamic regularities have been reported for the structurally closely related K2NiF4type oxides [23]. This and related schemes require that we have welldefined ionic radii for the different elements. There have been many reports on approaches for deriving internally consistent radii from bond lengths and atomic, ionic, covalent and metallic radii are found in literature. The radii reported by Shannon and Prewitt [24] are commonly used for oxides and fluorides. Cation radii vary much more than anion radii and increase markedly when we move down a group in the periodic table. It decreases with increasing cation charge for a given element and the radii of ions of the same charge decreases across a period. Finally, the cation radius increases with increasing coordination number. Electron count rationalization Experimental studies have shown that in many alloy systems the number of valence electrons is the dominant factor. Electron density is usually taken to denote the
216
7 Trends in enthalpy of formation
D f Hmo / kJ mol–1
0
–40
carbides borides
–80
–120
3
4
5 ne
6
7
Figure 7.18 Enthalpy of formation of binary carbides and diborides [25, 26] as a function of the average number of valence electrons per atom.
number of valence electrons per unit cell (provided all atomic sites are occupied), or alternatively it may be taken as the ratio of all valence electrons to the number of atoms. The trends in the enthalpy of formation of intermetallic compounds clearly relates to this factor. Importantly, the same type of arguments may also be used for less metallic compounds. The enthalpy of formation of complex binary carbides and diborides [25, 26] are shown in Figure 7.18. A good correlation with the average number of valence electrons per atom, ne, is observed. A similar variation with the average number of valence electrons is also observed for nitrides. Zhukov et al. [27] showed that an observed linear decrease in the enthalpy of formation of selected NiAstype oxides and carbides for 4 < ne < 5.5 could be understood from simple electron band structure considerations. TiC with ne = 4 has a high enthalpy of formation since the Fermi level falls in a pronounced gap in density of electronic states separating bonding and antibonding electron bands. Further increase in the number of valence electrons reduces the enthalpy of formation since antibonding states are filled. Correspondingly, the decrease in enthalpy of formation at lower electron concentrations shown by FernandezGuillermet and Grimvall [28] is due to a reduced number of electrons in the bonding states. This general approach can be used also for more complex structures. Volume effects in microporous materials Microporous materials is an important class of compounds with many applications and also interesting since the energetic factors affecting the enthalpy of formation must be expected to be different from those considered in the previous sections. Although most zeolites are kinetically stabilized through the use of templates during synthesis, there are several aspects of the energetics that are worth noting. Pure silica zeolites or molecular sieves are metastable with regards to the thermodynamic stable polymorph at ambient conditions, aquartz. However, they are
7.2 Compound energetics: rationalization schemes
217
D trsHmo / kJ mol–1
15
10
5 AlPO4 polymorphs SiO2 polymorphs 0 0
10
20 30 D trsVm / cm3 mol–1
40
Figure 7.19 Enthalpy of transition from the stable polymorph versus volume correlations for micro and mesoporous SiO2 and AlPO4 materials [29, 34].
only 7–14 kJ mol–1 less stable than aquartz and only 0.5–7 kJ mol–1 less stable than dense SiO2 glass [29]. The low barrier between different local energy minima explains the number of structural polymorphs. There exist around 30 different pure SiO2 structures. The enthalpy of formation correlates well with framework density and with molar volume [29]; see Figure 7.19. The packing of the tetrahedra is thus the main factor for structural stability and this relates directly to the internal surface area of the zeolites. It has been shown that the enthalpy differences between the stable modification, aquartz and the metastable silica zeolites can be described based on an average internal surface enthalpy of 0.093 ± 0.0009 J m–2 [30]. This surface energy is similar to that reported for various amorphous silicas. The correlation between framework density and enthalpy of formation is reproduced in lattice enthalpy calculations on 26 structures with widely different framework densities [31]. While the enthalpy is largely dependent on the framework density, the standard entropies of the zeolites at 298 K are not. They are only slightly higher (3–4 J K–1 mol–1) than for aquartz despite the much larger molar volume [32] since the local structural elements are the same as in the denser compounds; the structures are built as rigid frameworks of SiO4 tetrahedra that is expected to have similar vibrational characteristics that does not vary largely with connectivity. From the magnitudes of the enthalpy and entropy contributions it can be concluded that the Gibbs energies of the zeolites relative to aquartz are in total within twice the thermal energy at 298 K. The importance of framework density and molar volume is evident also for large pore, mesoporous silica [33] and for AlPO4 polymorphs [34]. Data for the latter are included in Figure 7.19. For mesoporous silica a transition from a regime where cages and pores affects the energetics to one in which the large pores act as inert diluent is reported. A further increase in pore diameter does not appear to increase the enthalpy of the compound [33]. The similarity in enthalpy of many different structures shows that the synthesis of metastable microporous framework
218
7 Trends in enthalpy of formation
structures is not limited by energetic constraints. Similar effects have been shown, e.g. for layered manganese dioxides [35] and iron oxides [36].
7.3 Solution energetics: trends and rationalization schemes Solid solutions: strain versus electron transfer The factors that affect the energetics of solid solutions and indirectly solid solubility are to a large extent the same as those that control the enthalpy of formation of compounds. Most often the differences between the atomic radii of the participating elements, in electronegativity and in valence electron density are considered for solutions of elements. For solid solutions of binary compounds, similar factors are used, but some measure of the volume of the compounds is often used instead of atomic radii. Two elements or compounds that do not adopt the same crystal structure cannot exhibit complete solid solubility except when one of the space groups is a subgroup of the other. The energetics of solid solutions of compounds with different structures are obviously difficult to treat systematically and trends may be impossible to obtain, since the energetics is largely related to structural shortrange order. We will thus confine our discussion of solid solutions to systems where the two endmembers take the same crystal structure. Let us first consider metallic alloys. The enthalpies of formation of intermetallic compounds, and also the enthalpy of mixing of solid intermetallic solutions, can largely be interpreted in terms of the relative atomic size of the elements being mixed and the difference in electronegativity. The difference in size generates a local misfit or distortion and thus results in a strain energy that increases with the size difference. The empirically derived rule of HumeRothery states that restricted solid solubility is expected if the difference between the atomic sizes of the component elements forming the alloy exceeds 15% [37]. A second and negative term is related to the electronegativity of the elements. The more electronegative elements tend to attract the electrons from the less electronegative elements on compound or solution formation and the excess enthalpy of mixing varies from large negative values in systems with large electron transfer between the two elements, e.g. Pdâ€“Zr, to about zero for elements of similar size and similar electronegativity, e.g. Tiâ€“Zr. A large negative enthalpy of formation implies that different atoms attract each other, and a consequence of this is that compound formation becomes more likely. Generally, the number of intermetallic phases found in a binary system correlates with the enthalpy of mixing. An empirically relationship is shown in Figure 7.20 [8]. For ionic solutions the strain energy seem to be relatively more important than for the metallic alloy systems [38â€“40] and the size difference between the two components being mixed dominates the energetics, although other factors are also of importance. In cases where the the covalency or ionicity of the components being mixed are largely different a limited solid solubility also must be expected, even
number of intermediate phases
7.3 Solution energetics: trends and rationalization schemes
219
5 4 3 2 1 0 –100
–80
–60 –40 D f Hmo (AB)
–20
0
Figure 7.20 Empirical relationship between the number of intermetallic phases in binary systems and the enthalpy of formation of AB [8].
when the ions being mixed are of similar size. It follows that both the NaCl–AgCl and NaBr–AgBr systems show large positive enthalpies of mixing, although atomic size considerations would indicate the opposite. The oxidation state of the components of the ionic solution is also important, higher valence difference leading to lower solubility. Finally, the electron configuration is of particular importance for transition metal systems, where a similar electron configuration is necessary for a large degree of solid solubility. Still, the strain enthalpy is of particular importance. An elastic continuum model for this size mismatch enthalpy shows that, within the limitations of the model, this enthalpy contribution correlates with the square of the volume difference [41, 42]. The model furthermore predicts what is often observed experimentally: for a given size difference it is easier to put a smaller atom in a larger host than vice versa. Both the excess enthalpy of mixing and the solubility limits are often asymmetric with regard to composition. This elastic contribution to the enthalpy of mixing scales with the twoparameter subregular solution model described in Chapter 3 (see eq. 3.74): D mix H m = x A x 2Bc A
DV 2 DV 2 + x B x 2A c B 3V A 3V B
(7.20)
where VA and VB are the molar volumes of A and B and DV is volume change on solution formation.The proportionality constants cA and cB are related to the shear and bulk moduli of the two components [42]. The suggested proportionality between the enthalpy of mixing and the square of the volume mismatch is also supported by computer simulations [43]. An analysis of a large amount of experimental data by Davies and Navrotsky has also shown that the enthalpy of mixing of ionic solid solutions correlates with the volume mismatch [39]. The volume mismatch was in the simplest case assumed to
220
7 Trends in enthalpy of formation
60 MgO–CaO
W / kJ mol –1
CaO–NiO
40 CaO–FeO CaO–CoO CaO–SrO MgO–MnO
20
CaO–MnO
MgO–FeO MgO–CoO
0 0.0
CaO–CdO
0.1
0.2
0.3
0.4
0.5
2(VA– VB )/(VA+ VB )
Figure 7.21 Enthalpies of mixing of selected NaCltype systems involving the alkali earth oxides. The solid and dashed lines show scaling with the volume mismatch and with the square of the volume mismatch, respectively.
correlate with the interaction coefficient W of the regular solution model. Within the experimental accuracy of the data, a close to linear relationship was observed for rock salt oxides and chalcogenide solid solutions, and also for alkali halide solutions. The deduced experimental enthalpies of mixing of selected NaCltype systems involving the alkali earth oxides are compared with theoretical expectations in Figure 7.21. The experimental data do not allow discrimination between variation with volume mismatch or with the square of the volume mismatch. In addition, other contributions to the enthalpy of mixing than the strain enthalpy will affect the experimental data. The importance of the size of the solute relative to that of the solvent mentioned above is evident also from experimental determinations of the extent of solid solubility in complex oxides and from theoretical evaluations of the enthalpy of solution of large ranges of solutes in a given solvent (e.g. a mineral). The enthalpy of solution for mono, di and trivalent trace elements in pyrope and similar systems shows an approximately parabolic variation with ionic radius [44]. For the pure mineral, the calculated solution energies always show a minimum at a radius close to that of the host cation. Solubility of gases in metals For interstitial solid solutions, too, the criteria used historically for the degree of solid solubility relates to elastic and electronic interactions. Experimentally observed maximum interstitial solubilities of H, B, C and N in Pd are inversely proportional to the sum of the s and p electrons, and hence are controlled by the valence electron concentration. Thus the electronic interactions dominate the
7.3 Solution energetics: trends and rationalization schemes
221
energetics; the electronic interaction between solute and matrix is more important than the elastic contribution [45]. The solubility of gases in metals is of particular importance. In these systems, the concentration of a solute like hydrogen can be varied by controlling the temperature and partial pressure of the solute in the gas phase. Hydrogen dissolves interstitially in many metals, and at low concentrations the solubility of a diatomic gas is proportional to the square root of its partial pressure. At higher concentrations of hydrogen, large repulsive interactions between the hydrogen atoms give rise to immiscibility at low temperatures. The resulting twophase regions are reflected in the corresponding partial pressure–composition isotherms. Focusing on the low concentrations situation, all isotherms are characterized by xµ p
(7.21)
The slope is, for a specific system, given by the enthalpy and entropy of solution of hydrogen in the metal; in other words by the energetics of the following reaction M + x H2(g) = MHx 2
(7.22)
The relationship between the concentration of hydrogen in the metal and the partial pressure of hydrogen is now xµ
S ö æD Hö p æD expç 7.22 ÷ expç 7.22 ÷ p0 è R ø è RT ø
(7.23)
This relation is termed Sievert’s law. Values for the enthalpy of solution of hydrogen in transition metals at infinite dilution shown in Figure 7.22 are more negative for the early transition metals. It should be noted that the enthalpies of solution in general are functions of the concentration of the solute. Still, the values at infinite dilution are useful when looking for systematic variations, particularly since changes with composition are often limited. Nonstoichiometry and redox energetics Hydrides of variable composition are not only formed with pure metals as solvents. A large number of the binary metal hydrides are nonstoichiometric compounds. Nonstoichiometric compounds are in general common for d, f and some p block metals in combination with soft anions such as sulfur, selenium and hydrogen, and also for somewhat harder anions like oxygen. Hard anions such as the halides, sulfates and nitrides form few nonstoichiometric compounds. Two factors are important: the crystal structures must allow changes in composition, and the transition metal must have accessible oxidation states. These factors are partly related. FeO,
222
7 Trends in enthalpy of formation
inf.dil D sol Hm / eV atom 1
1.0
3d 4d 5d
0.5 0.0 –0.5 –1.0
Sc Y La
Ti Zr Hf
V Nb Ta
Cr Mo W
Mn Te Re
Fe Ru Os
Co Rh Ir
Ni Pd Pt
Cu Ag Au
Figure 7.22 Enthalpy of solution of hydrogen in transition metals at infinite dilution [45].
CoO and NiO all take the NaCltype structure and the difference in nonstoichiometry relates to the relative stability of the formal di and trivalent oxidation states. The stability of the trivalent state and the degree of nonstoichiometry decreases from Fe3+ to Ni2+. Hence the nonstoichiometric nature of Fe1–yO is made possible by the relatively high stability of Fe3+ that is reflected in the fact that Fe2O3 is a stable compound in the Fe–O system, whereas Ni 2O3 is not in the Ni–O system. This relative stability of the different oxidation states is also reflected in Figure 7.11(c). As indicated above, the crystal structure is also important and the difference between hexagonal and cubic SrMnO3–d may serve as example. Acid–base factors affect the relative stability of the different oxidation states of a given metal, and in general the redox energetics of ternary oxides must be expected to be quite different from that of the binary ones. As an example Fe(IV) is stabilized in SrFeO3, and while iron dioxide is a nonexisting binary compound, the enthalpy of oxidation of Fe(III) to Fe(IV) in SrFeO3–d is large and negative, –120 kJ per mol O2 at 800 K [46]. Similarly, the enthalpy of oxidation of Mn(III)2O3 to Mn(IV)O2 is –158 kJ per mol O2 , while the corresponding enthalpies of oxidation for CaMnO3d and SrMnO3d are –356 and –293 kJ per mol O2 [47]. Hence Mn(IV) is stabilized by the basic alkaline earth oxide relative to Mn(III). Even though the difference in enthalpy of formation between the cubic and hexagonal modification of SrMnO3 is only about 6 kJ mol–1, the temperature of initial reduction of the hexagonal modification in air takes place 600 K above the temperature where the initial reduction appears for cubic SrMnO3. This difference is due to a large difference in the relative Gibbs energy of the oxidized and reduced limiting compounds of the two solid solutions. While cubic SrMnO2.50 is relatively stable (can be prepared in the laboratory), hexagonal SrMnO2.50 is unstable. The Gibbs energy difference between the oxidized and reduced compounds is hence much larger for the hexagonal case than for the cubic case. The reason for this can
7.3 Solution energetics: trends and rationalization schemes
(a)
223
(b)
Figure 7.23 Connectivity of transition metal BO6 octahedra in (a) cubic and (b) hexagonal perovskite SrMnO3.
be understood by taking the structure of hexagonal SrMnO3 into consideration. While the Mn–O6 octahedra share corners in the usual cubic perovskitetype structure, they share faces in the hexagonal structure: see Figure 7.23. Reduction of the cubic structure gives rise to square pyramidal coordinated manganese while reduction of the hexagonal structure in the end would lead to faceshared octahedra with high vacancy concentrations in localized areas of the crystal structure. The latter structure must be expected to be energetically unfavourable. In conclusion, the redox energetics of a phase depends strongly on the crystal structure, a fact that should be taken into account when looking for trends in redox properties. In terms of defect chemistry the defect–defect interaction energy is much larger for hexagonal SrMnO3 than for cubic SrMnO3. The enthalpy of oxidation of Mn(III) to Mn(IV) for hexagonal SrMnO3–d is estimated to be –590 kJ per mol O2 , i.e. twice the value for the cubic structure [47]. Liquid solutions In the crystalline state the solution is restricted by the crystal structures taken by the solid solution. The coordination numbers of the atoms or ions are not allowed to change unless the solid solution involve occupation of interstitial lattice sites. Liquid solutions, on the other hand, have in principle no such structural restrictions and an endothermic enthalpy of mixing is overcome by the entropy of mixing, provided the temperature is high enough. However, in cases where the positive enthalpy of mixing is large, the solubility of one liquid in the other is limited. Liquid immiscibility occurs typically when the two liquids have significantly different chemical and physical properties. One type of system that shows limited solubility is mixtures of liquid metals and molten salts. Another classical example of demixing in the liquid state occurs in the system CaO–SiO2 and other binary silicate systems where SiO2 is mixed with basic oxides. While the solubility of SiO2(l) in the basic oxide is high, there is a
224
7 Trends in enthalpy of formation (a)
0
(b)
0
SiO2 –PbO
–20 D mix Hmo / kJ mol 1
D mix Hmo / kJ mol 1
–20
–40 SiO 2–CaO
–60
–80
SiO 2–1/2Na2O
ZrF4–LiF
ZrF4–NaF
– 40 ZrF4–KF
–60 SiO 2 –1/2K2O
–100 0.0
0.2
0.4
ZrF4–RbF
0.6
1–xSiO2
0.8
1.0
0.0
0.2
0.4 0.6 1–x ZrF4
0.8
1.0
Figure 7.24 Enthalpy of mixing of (a) binary silicate [48] (reprinted by permission of A. Navrotsky) and (b) fluoride systems [49].
immiscibility gap at high SiO2 concentrations. In some of these systems the immiscibility occurs in the metastable supercooled region, as discussed for the system Na2B8O13–SiO2 in Chapter 5. The solubility of CaO(l) in SiO2(l) is strongly limited, since Si4+ in SiO2 is 4coordinated, while Ca2+ would prefer a near 6coordinated environment, as in CaO(l). Thus, Ca2+ is energetically not favoured to replace Si4+ in the covalently bonded liquid SiO2, where a high degree of shortrange order is present. On the other hand, the solubility of SiO2(l) in CaO(l) or other basic oxides is energetically strongly favourable. This reflects the different acid–base properties of CaO and SiO2 [9–11]. The enthalpy of mixing of several binary silicate systems is shown in Figure 7.24(a) [48]. The enthalpies of mixing of SiO2 with alkali and alkali earth oxides are exothermic and become increasingly more exothermic with increasing basicity of the alkali and alkali earth oxide. The shape of the curves reflects the local structure of the liquid. A relatively sharp minimum is evident near the orthosilicate composition, for example Ca2SiO4. Here a high degree of local order exists in the liquid that consists of Ca2+ cations and SiO 4anions. At higher concentration of 4 42– the basic oxide, SiO 4 is mixed with O on an anion quasilattice, and the enthalpy of mixing becomes less exothermic. Moreover, the SiO 4complex anions 4 start to polymerize to form, for example, dimer Si2 O 6or linear chains of 7 (SiO23 ) n . Even though the enthalpy of mixing increases with increasing concentration of SiO2, melts with compositions corresponding to metasilicates, e.g. CaSiO3, also show large negative enthalpies of mixing; see Figure 7.24(a). At even higher concentrations of SiO2 the enthalpy of mixing increases rapidly and the immiscibility at high SiO2 concentration is reflected by a change in sign of the second derivative (inflection point) of the enthalpy of mixing that is not, however, that easily seen at the resolution of the figure. The strong local order found in
7.3 Solution energetics: trends and rationalization schemes
225
silicate systems due to the energetically preferred structural SiO4 entity is also a characteristic of other types of system, such as phosphates and borates where PO 34 and BO 5are the energetically preferred entities. In borate melts, local order due to 4 formation of planar trigonal BO3 entities is also known. A crude analysis of the enthalpy of mixing based on the acidity/basicity of the end members involved in the solution can also be applied for fluoride melts. One example is the alkali fluoride–zirconium fluoride mixtures in Figure 7.24(b). Here the enthalpies of mixing of several systems are displayed [49]. ZrF 4 can be regarded as a strong Lewis acid, while the basicity of the alkali fluoride increases with increasing size of the alkali metal. The enthalpy of mixing becomes increasingly more exothermic with increasing basicity of the alkali metal, and for all the systems a minimum is evident near the composition corresponding to the complex anion ZrF 62  . The minima become increasingly more pronounced with increasing basicity of the alkali metal. Other complexes may also be present in the liquid [49]. The similarity to the binary oxide mixtures shown in Figure 7.24(a) is evident. The enthalpies of mixing of other binary halide or oxide systems that have an asymmetrical charge distribution display similar behaviour. The enthalpy of mixing becomes more exothermic with increasing difference in acidity, and a sharp minimum in the enthalpy of mixing for a given composition points to a high degree of local order corresponding to a particular complex anion. Most halide systems are ionic in nature. Still, halides like AlCl3 and BeF2 are characterized by formation of liquids with a high degree of local order due to a preference for fourfold coordination. While, BeF2 has a similar local structure to SiO2, AlCl3, is a molecular liquid consisting of Al2Cl6 molecules. AlCl3–XCl melts, where X is an alkali metal, are dominated by the formation of AlCl 4 complex anions. Large sets of experimental data exist also for simpler ionic solutions such as mixtures of simple molten salt of alkali or alkali earth cations and halogen anions or complex anions like NO 3 , CO23 and SO24 . Enthalpies of mixing of such systems are reviewed by Kleppa [50]. Generally, the enthalpy of mixing is small in the range of a few kJ mol–1 at x = 0.5. For charge symmetrical systems, where the cations and anions have equal charge, the enthalpy of mixing can be understood in terms of Coulombic interactions and polarization of the ions. These interactions are described using the size parameter d = ( d A  d B ) / ( d A + d B ), where d A and d B are the sums of the cation and anion radii of the two salts A and B [50]. For most systems with a common anion, the enthalpy of mixing is exothermic, while with common cations, anion–anion repulsion may dominate, leading to a positive enthalpy of mixing. The energetics of liquid metal alloys mimics the energetics of the solid state, and the semiempirical approach by Miedema and coworkers seems to be in reasonable agreement with experimental observations [8]. However, for mixtures containing d block metals, a third interaction due to p–d hybridization must be added [51]. Generally, the enthalpy of mixing is strongly exothermic in systems, in which intermediate compounds are stable, while the lack of intermediate phases reflects a less exothermic enthalpy of mixing in accordance with Figure 7.20. One example of a system where no intermetallic phases are formed is the binary system Au–Ag,
226
7 Trends in enthalpy of formation
where the enthalpy of mixing at xAg = 0.50 is about 4.0 kJ mol–1 [51]. The formation of intermediate compounds also implies that the liquid phase will be energetically stabilized relative to the end members.
References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31]
A. Navrotsky, Am. Mineral. 1994, 79, 589. D. G. Pettifor, Bonding and Structure of Molecules and Solids. Oxford: Clarendon Press, 1995. T. B. Massalski, Met. Trans. 1989, 20A, 1295. R. R. Merritt and B. G. Hyde, Phil. Trans. Roy. Soc. 1973, 274A, 627. W. B. Jensen, J. Chem. Educ. 1998, 8, 817. C. S. G. Phillips and R. J. P. Williams, Inorganic Chemistry. Oxford: Clarendon Press, 1965. D. A. Johnson, Some Thermodynamic Aspects of Inorganic Chemistry. Cambridge: Cambridge University Press, 1982. F. R. de Boer, R. Boom, W. C. M. Mattens, A. R. Miedema and A. K. Niessen, Cohesion in Metals. Amsterdam: Elsevier Science Publishers, 1988. H. Flood and T. Førland, Acta Chem. Scand. 1947, 1, 592. H. Flood, T. Førland and B. Roald, Acta Chem. Scand. 1947, 1, 790. H. Lux, Z. Electrochem. 1939, 45, 303. H.F. Wu and L. Brewer, J. Alloys Comp. 1997, 247, 1. J. A. Duffy, J. NonCryst. Solids. 1989, 109, 35. O. J. Kleppa and J. L. Holm, Amer. Mineral. 1966, 51, 1608. A. Navrotsky, Physics and Chemistry of Earth Materials. Cambridge: Cambridge University Press, 1994. J. M. McHale, A. Navrotsky, G. R. Kowach, V. E. Balbarin and F. J. DiSalvo, Chem. Mater. 1997, 9, 1538. C. Wagner, Metal. Trans. 1975, 6B, 405. V. M. Goldschmidt, Skr. Nors. Vidensk.Akad. Oslo 1926, 1, 1. J. Goudiakas, R. G. Haire and J. Fuger, J. Chem. Thermodyn. 1990, 22, 577. L. R. Morss, J. LessCommon Metals. 1983, 93, 301. Y. Kanke and A. Navrotsky, J. Solid State Chem. 1998, 141, 424. L. Rørmark, S. Stølen, K. Wiik and T. Grande, J. Solid State Chem. 2002, 163, 186. H. Yokokawa, T. Kawada and M. Dokiya, J. Am. Ceram. Soc. 1989, 72, 152. R. D. Shannon, Acta Cryst. 1976, A32, 751. A. Fernandez Guillermet and G. Grimvall, Phys. Rev. B 1989, 40, 10582. P. Vajeeston, P. Ravindran, C. Ravi and R. Asokamani, Phys. Rev. B 2001, 63, 045115. P. Zhukov, V. A. Gubanov, O. Jepsen, N. E. Christensen and O. K. Andersen, J. Phys. Chem. Solids. 1988, 49, 841. A. Fernandez Guillermet and G. Grimvall, J. Phys. Chem. Solids. 1992, 53, 105. P. M. Piccione, C. Laberty, S. Yang, M. A. Camblor, A. Navrotsky and M. E. Davis, J. Phys. Chem. B. 2000, 104, 10001. E. C. Moloy, L. P. Davila, J. F. Shackelford and A. Navrotsky, Micropor. Mesopor. Mater. 2002, 54, 1. N. J. Henson, A. K. Cheetham and J. D. Gale, Chem. Mater. 1994, 6, 1647.
7.3 Solution energetics: trends and rationalization schemes
227
[32] P. M. Piccione, B. F. Woodfield, J. BoerioGoates, A. Navrotsky and M. E. Davis, J. Phys. Chem. B 2001, 105, 6025. [33] Y. Hu, A. Navrotsky, C.Y. Chen and M. E. Davis, Chem. Mater. 1995, 7, 1816. [34] A. Navrotsky, I. Petrovic, Y. Hu, C.Y. Chen and M. E. Davis, Microporous Mater. 1995, 4, 95. [35] S. Fritsch, J. E. Post and A. Navrotsky, Geochim. Cosmochim. Acta. 1997, 61, 2613. [36] C. Laberty and A. Navrotsky, Geochim. Cosmochim. Acta. 1998, 62, 2905. [37] W. HumeRothery, Electrons, Atoms, Metals and Alloys. New York: Dover Publications, 1963. [38] D. M. Kerrick and L. S. Darken, Geochim. Cosmochim. Acta. 1975, 39, 1431. [39] P. K. Davies and A. Navrotsky, J. Solid State Chem. 1983, 46, 1. [40] C. A. Geiger, Amer. Mineral. 2000, 85, 893. [41] T. B. Massalski and H. W. King, Progr. Mater. Sci. 1961, 10, 1. [42] H. J. Greenwood, Geochim. Cosmochim. Acta. 1979, 43, 1873. [43] A. Bosenick, M. T. Dove, V. Heine and C. A. Geiger, Phys. Chem. Minerals. 2001, 28, 177. [44] W. van Westrenen, N. L. Allan, J. D. Blundy, J. A. Purton and B. J. Wood, Geochim. Cosmochim. Acta. 2000, 64, 1629. [45] Y. Fukai, The Metal–Hydrogen System. Berlin: SpringerVerlag, 1993. [46] C. Haavik, T. Atake and S. Stølen, Phys. Chem. Chem. Phys. 2002, 4, 1082. [47] L. Rørmark, A. B. Mørch, K. Wiik, T. Grande and S. Stølen, Chem. Mater. 2001, 13, 4005. [48] A. Navrotsky in Silicate Melts, Short Course Handbook (C. M. Scarfe ed.). Toronto: Mineralogical Association of Canada, 1986, vol. 12, p. 130. [49] T. Grande, S. Aasland and S. Julsrud, J. Am. Ceram. Soc. 1997, 80 1405. [50] O. J. Kleppa in Molten Salt Chemistry – An Introduction and Selected Applications (G. Mamantov and R. Marassi eds.). NATO ASI Series C: Mathematical and Physical Sciences vol. 202, Holland: Reidel Publishing Company, 1986. [51] O. J. Kleppa, J. NonCryst. Solids. 1984, 61&62, 101.
Further reading A. Navrotsky, Physics and Chemistry of Earth Materials. Cambridge: Cambridge University Press, 1994. C. S. G. Phillips and R. J. P. Williams, Inorganic Chemistry. Oxford: Clarendon Press, 1965. D. A. Johnson, Some Thermodynamic Aspects of Inorganic Chemistry. Cambridge: Cambridge University Press, 1982.
8
Heat capacity and entropy
The Gibbs energy of formation of a compound can be expressed as o o o = DfHm  TD f S m + pD f V mo D fG m
(8.1)
At low temperatures the enthalpy of formation usually constitutes the largest energetic contribution. And while high pressures favour the formation of dense compounds, the entropy become increasingly more important at high temperatures. We saw in the previous chapter that the enthalpy of formation of a ternary oxide from the binary constituent oxides is small compared to the enthalpy of formation from the elements and comparable to the enthalpy of melting and to the enthalpy difference between different modifications of the compound. Similarly, small differences in the enthalpy of formation are observed between different structure types of metallic compounds. These small differences in enthalpy of formation explain the occurrence of several polymorphs of many substances, which again points to the importance of entropy and volume contributions to the total Gibbs energy. Even for simple elements complex phase relations are observed. Using bismuth as an example, five different polymorphs are known, as shown in the p,T phase diagram in Figure 8.1. The absolute value of the entropy of a compound is obtained directly by integration of the heat capacity from 0 K. The main contributions to the heat capacity and thus to the entropy are discussed in this chapter. Microscopic descriptions of the heat capacity of solids, liquids and gases range from simple classical approaches to complex lattice dynamical treatments. The relatively simple models that have been around for some time will be described in some detail. These models are, because of their simplicity, very useful for estimating heat capacities and for relating the heat capacity to the physical and chemical Chemical Thermodynamics of Materials by Svein StĂ¸len and Tor Grande ÂŠ 2004 John Wiley & Sons, Ltd ISBN 0 471 492320 2 229
230
8 Heat capacity and entropy 700 Bi liq.
T /K
600
V IV
500 II I
400
0
III 3
6
9
p / GPa
Figure 8.1 pâ€“T phase diagram of Bi.
characteristics of the phases. Gases are briefly treated, followed by a more thorough discussion of the heat capacity of solids. Here we focus on physically based models, some of which may be used to deduce trends in the vibrational contribution to the entropy. Finally, heat capacity contributions of electronic origin and treatments of disordered systems are considered.
8.1 Simple models for molecules and crystals Let us first look at a monoatomic perfect gas consisting of N atoms. The internal energy of the gas is N 1 U = ĂĽ m i c 2i + F( r1 , r2 , r3 , ..., rN ) i =1 2
(8.2)
where c(cx,cy,cz) and r(rx,ry,rz) are the velocity and position of atom i. For a perfect monoatomic gas there are no atomic interactions and the potential energy, Fp ( r1 , r2 , r3 , ..., rN ), is negligible. The thermal energy of the system is thereby the mean of the kinetic energy of the atoms, and is given by the first term in eq. (8.2). A monoatomic gas has three translational degrees of freedom represented by three independent quadratic variables in the internal energy. Each of these contributes 1 k T to the total internal energy, and the mean internal energy per atom follows: B 2
3k T 1 m < c2 > = B 2 2
(8.3)
The molar internal energy of a monoatomic ideal gas is therefore Um = L
3 3 k BT = RT 2 2
(8.4)
8.1 Simple models for molecules and crystals
231
and the heat capacity at constant volume, obtained by differentiation with respect to temperature, is 3 æ ¶U m ö C V ,m = ç ÷ = R è ¶T øV 2
(8.5)
The internal energy is, as indicated above, connected to the number of degrees of freedom of the molecule: that is the number of squared terms in the Hamiltonian function or the number of independent coordinates needed to describe the motion of the system. Each degree of freedom contributes 1 RT to the molar internal 2 energy in the classical limit, e.g. at sufficiently high temperatures. A monoatomic gas has three translational degrees of freedom and hence, as shown above, U m = 3/ 2 RT and C V ,m = 3/ 2 R. A linear gas molecule can in addition rotate about any pair of directions perpendicular to each other and perpendicular to the axis of the linear molecule. A diatomic molecule therefore has two additional rotational degrees of freedom. Nonlinear polyatomic molecules, which can rotate about the three principal axes, have three rotational degrees of freedom and a total of six degrees of freedom of translational and rotational nature. In addition, the molecular vibrations must be taken into account. The energy of each mode of vibration has associated with it two terms: one kinetic and one potential energy term. Each mode therefore contributes R to the molar heat capacity. In general, a polyatomic molecule has (3n – 6) vibrational modes, where n is equal to the number of atoms in the molecule. If the molecule is linear the number of modes is (3n – 5). The number of translational, rotational and vibrational modes and the resulting limiting molar heat capacities of gases at constant volume and at constant pressure are given in Table 8.1. The difference between the heat capacity at constant pressure and constant volume, the dilational heat capacity, is, for an ideal gas: C p ,m  C V ,m =
a 2 TV =R kT
(8.6)
where a and k T are the isobaric expansivity and isothermal compressibility respectively. The molar heat capacities at constant pressure of H(g), H2(g) and H2O(g) are given in Figure 8.2. The classical heat capacity is in each case marked with open symbols at T = 5000 K. Monoatomic H(g) with only translational degrees of freedom is already fully excited at low temperatures. The vibrational frequencies (n) of H2(g) and H2O(g) are much higher, in the range of 100 THz, and the associated energy levels are significantly excited only at temperatures above 1000 K. At room temperature only a few molecules will have enough energy to excite the vibrational modes, and the heat capacity is much lower than the classical value. The rotational frequencies are of the order 100 times smaller, so they are fully excited above ~10 K.
232
8 Heat capacity and entropy
Table 8.1 Number of modes and heat capacity of gases in the classical limit. Number of modes Translational A(g) AB(g) AB2(g) nonlinear AB2(g) linear ABn–1(g) nonlinear ABn–1(g) linear
Classical
Rotational
Vibrational
CV,m/R
Cp,m/R 5/2 9/2 7
3 3 3
2 3
1 3
3/2 7/2 6
3
2
4
13/2
15/2
3
3
(3n – 6)
3 + (3n – 6)
4 + (3n – 6)
3
2
(3n – 5)
7/2 + (3n – 6) 9/2 + (3n – 6)
H2O(g)
C p,m / J K 1 mol 1
60 50
H2(g)
40 30
H(g) 20 0
1000
2000
3000
4000
5000
6000
T /K
Figure 8.2 Molar heat capacity at constant pressure of H(g), H2(g) and H2O(g). The open symbols at 5000 K represent the limiting classical heat capacity.
The statistical treatment of the vibrational degrees of freedom of crystals is far more difficult compared to gases. Let us initially consider a monoatomic crystal. An atom in a crystal vibrates about its equilibrium lattice position. In the simplest approach, three noninteracting superimposed linear harmonic oscillators represent the vibrations of each atom. The total energy, given by the sum of the kinetic and potential energies for the harmonic oscillators, is U = 1 mc 2 + 1 Kx 2 = 1 mA 2 w 2 cos 2 w t + 1 KA 2 sin 2 w t 2
2
2
2
(8.7)
where m is the mass of the atom, w is the angular frequency of the harmonic oscillator, A is the amplitude and x = A sin w t is the timedependent displacement of the atom from its equilibrium lattice position. The angular frequency of the harmonic oscillator is given by the force constant K and the mass m of the atom:
8.2 Lattice heat capacity
w = 2pn =
K m
233
(8.8)
Since w 2 = K / m, the mean potential and kinetic energy terms are equal and the total energy of the linear oscillator is twice its mean kinetic energy. Since there are three oscillators per atom, for a monoatomic crystal U m = 3RT and C V ,m = 3R = 2494 . J K–1 mol–1. This first useful model for the heat capacity of crystals (solids), proposed by Dulong and Petit in 1819, states that the molar heat capacity has a universal value for all chemical elements independent of the atomic mass and crystal structure and furthermore independent of temperature. Dulong–Petit’s law works well at high temperatures, but fails at lower temperatures where the heat capacity decreases and approaches zero at 0 K. More thorough models are thus needed for the lattice heat capacity of crystals.
8.2 Lattice heat capacity The Einstein model The decrease in the heat capacity at low temperatures was not explained until 1907, when Einstein demonstrated that the temperature dependence of the heat capacity arose from quantum mechanical effects [1]. Einstein also assumed that all atoms in a solid vibrate independently of each other and that they behave like harmonic oscillators. The motion of a single atom is again seen as the sum of three linear oscillators along three perpendicular axes, and one mole of atoms is treated by looking at 3L identical linear harmonic oscillators. Whereas the harmonic oscillator can take any energy in the classical limit, quantum theory allows the energy of the harmonic oscillator (e n ) to have only certain discrete values (n): e n = ( n + 1 ) w 2
(8.9)
The probability that an oscillator at a given temperature occupies a given energy state, e n , is given by Bose–Einstein statistics (see e.g. C. Kittel and H. Kroemer, Further reading) and the mean value of n at a given temperature is given by n=
1 exp( w / k BT )  1
(8.10)
In the Einstein model, all the independent oscillators have the same angular frequency, wE, and the average total internal energy is w E æ w E ö ÷ U = 3N ( 1 + n ) w E = 3N çç + 2 exp( w E / k BT )  1 ÷ø è 2
(8.11)
234
8 Heat capacity and entropy
The heat capacity is derived by differentiation with respect to temperature: 2
exp( Q E / T ) æ dU ö æQ ö C V ,m = ç ÷ = 3Rç E ÷ è T ø [exp( Q E / T )  1]2 è dT øV
(8.12)
where Q E , the Einstein temperature, is defined by QE =
w E kB
(8.13)
This model, the Einstein model for heat capacity, predicts that the heat capacity is reduced on cooling and that the heat capacity becomes zero at 0 K. At high temperatures the constantvolume heat capacity approaches the classical value 3R. The Einstein model represented a substantial improvement compared with the classical models. The experimental heat capacity of copper at constant pressure is compared in Figure 8.3 to C V ,m calculated using the Einstein model with QE = 244 K. The insert to the figure shows the Einstein frequency of Cu. All 3L vibrational modes have the same frequency, n = 32 THz. However, whereas CV,m is observed experimentally to vary proportionally with T3 at low temperatures, the Einstein heat capacity decreases more rapidly; it is proportional to exp( Q E / T ) at low temperatures. In order to reproduce the observed low temperature behaviour qualitatively, one more essential factor must be taken into account; the lattice vibrations of each individual atom are not independent of each other – collective lattice vibrations must be considered.
20 vibrational density of states
Cm / J K 1 mol 1
3R
10
3L
nE 0
0
0
200
10
20 n / THz
30
40
400
T /K
Figure 8.3 Experimental heat capacity of Cu at constant pressure compared with C V ,m calculated by the Einstein model using QE = 244 K. The vibrational frequency used in the Einstein model is shown in the insert.
8.2 Lattice heat capacity
235 un–2
un–1 K
un
un+1
a
Figure 8.4 Onedimensional chain of atoms with interatomic distance a and force constant K.
Collective modes of vibration A first impression of collective lattice vibrations in a crystal is obtained by considering onedimensional chains of atoms. Let us first consider a chain with only one type of atom. The interaction between the atoms is represented by a harmonic force with force constant K. A schematic representation is displayed in Figure 8.4. The average interatomic distance at equilibrium is a, and the equilibrium rest position of atom n is thus u n = na. The motion of the chain of atoms is described by the timedependent displacement of the atoms, u n ( t), relative to their rest positions. We assume that each atom only feels the force from its two neighbours. The resultant restoring force (F) acting on the nth atom of the one dimensional chain is now in the harmonic approximation F = K (u n  u n + 1 + u n  u n 1 )
(8.14)
The equation of motion of this nth atom is given by m
¶2 un ¶t
2
=
¶U = F = K (2u n  u n + 1  u n 1 ) ¶u n
(8.15)
Let us describe the displacement of the nth atom from its equilibrium rest position by a cosinewave with amplitude u 0 , angular frequency w and wave vector q = 2p/l:1 u n = u 0 cos(w t  qna)
(8.16)
Substituting this expression into the equation of motion (eq. 8.15) we obtain the expression for the angular frequency of the vibrational modes as a function of the wave vector: w( q) =
4K æ qa ö sinç ÷ m è 2 ø
(8.17)
The frequency versus wave vector graph, shown in Figure 8.5, is known as a dispersion curve. We only need to consider waves with wave vectors lying between 1 In two and three dimensions q is a vector. Usually q is also referred to as a vector even in one dimension.
236
8 Heat capacity and entropy 1.2
w /(4 K / m)1 / 2
1.0
wªa
K q m
0.8 0.6 0.4 0.2 0.0 –p/a
0 first Brillouin zone q
p/a
Figure 8.5 The dispersion curve for a onedimensional monoatomic chain of atoms.
–p/a < q < p/a. This range of wave vectors is within what is termed the first Brillouin zone of the onedimensional lattice. At longer wave vectors or shorter wavelengths,  q  > p / a, the periodicity of the wave is shorter than the interatomic distance. This has no physical meaning. For short wave vectors (or long wavelengths) corresponding to waves in the acoustic or ultrasonic range, eq. (8.17) reduces to w »a
K q m
(8.18)
The group velocity, dw /dq, is constant and independent of the wavelength, as shown in Figure 8.5. The discontinuous nature of matter can be neglected, and for these wavelengths the vibrational characteristics of the material can be described by its macroscopic properties (density and elastic constants). The group velocity is here equal to the speed of sound in the solid. At short wavelengths the frequency is no longer proportional to q and the velocity of propagation decreases as q increases. This is called dispersion and is reflected in Figure 8.5. The wavelength becomes comparable to the interatomic distance and the discrete nature of the atoms becomes important. The vibration frequency has its maximum value at the Brillouin zone boundary where q = p/a and the group velocity, dw /dq, is equal to zero. Thus here the wave vector corresponds to a standing wave. Successive atoms have displacements of alternating sign. The linear model can be extended to include more distant neighbours and to three dimensions. Let us consider an elastic lattice wave with wave vector q. The collective vibrational modes of the lattice are illustrated in Figure 8.6. The formation of small local deformations (strain) in the direction of the incoming wave gives rise to stresses in the same direction (upper part of Figure 8.6) but also perpendicular (lower part of Figure 8.6) to the incoming wave because of the elasticity of the material. The cohesive forces between the atoms then transport the deformation of the lattice to the
8.2 Lattice heat capacity
237 longitudinal q
u n–1
u n+1
un
u n+2
transverse un
u n+1
u n+2
u n+3
u n+4 q
Figure 8.6 Schematic representation of transverse and longitudinal collective vibrational waves.
neighbourhood. It is clear that the waves are vibrating not independently but collectively. When a wave propagates along q, entire planes of atoms move in phase with displacements either parallel or perpendicular to the direction of the wave vector. For each wave vector there are three modes: one of longitudinal polarization (longitudinal mode) and two of transverse polarization (transverse modes). For an isotropic solid the two transverse waves are degenerate. Also, in crystals of high symmetry, there are three, four or sixfold rotation axes along the direction of the wave vector, where the two transverse modes will be degenerate. When the symmetry of the crystal or a specific symmetry operator is lower, the complexity of the vibrational modes will increase. The dispersion relations in the [100], [110] and [111] directions for Pb (fcc structure) at 100 K [2] are given in Figure 8.7. The two transverse modes are degenerate for [100] and [111], which are four and threefold rotation axes, but not for [110], which is a twofold rotation axis. The method delineated in the preceding sections can readily be extended to the case of two atoms in the chain. An illustration of the diatomic chain model is given in Figure 8.8. The two atoms are characterized by having different masses m1 and m2. The two equations of motion obtained (one for each type of atom) must be solved simultaneously, giving two solutions for the angular frequency known as the acoustic and optic branches é æ m + m2 w 2a = K êçç 1 êè m1m2 ë
( m1  m2 )2 + 4m1 m2 cos 2 qa ù ö ú ÷÷ m m ú 1 2 ø û
(8.19)
é æ m + m2 w 2o = K êçç 1 êè m1m2 ë
( m1  m2 )2 + 4m1 m2 cos 2 qa ù ö ú ÷÷ + m1 m2 ú ø û
(8.20)
238
8 Heat capacity and entropy
Pb [z , 0, 0]
2
[z , z , 0]
[z , z , z ]
L
L
L
w / THz
T2
1 T
0
T1
T
0
1
0.5
Figure 8.7 Experimental dispersion relations for acoustic modes for lead at 100 K [2]. Reproduced by permission of B. N. Brockhouse and the American Physical Society. u1, nâ€“1 m1
K
u2, n
u1, n
u2, n+1
m2
m1
m2
2a
Figure 8.8 Onedimensional diatomic chain with lattice parameter 2a and force constant K.
The dispersion curve for a diatomic chain is given in Figure 8.9. The curve consists of two distinct branches: the acoustic and the optic. In the first of these the frequency varies from zero to a maximum w 1. The second one has a maximum value of w 0 at q = 0 and decreases to w 2 at q = q max . There are no allowed frequencies in the gap between w 1 and w 2 . The solution for the acoustic branch approaches zero as q goes to zero, and for small q: wa Âť a
2K q m1 + m2
(8.21)
For m1 = m2, the expression reduces to that obtained for a monoatomic chain (eq. 8.18). When q approaches zero, the amplitudes of the two types of atom become equal and the two types of atom vibrate in phase, as depicted in the upper part of Figure 8.10. Two neighbouring atoms vibrate together without an appreciable variation in their interatomic distance. The waves are termed acoustic vibrations, acoustic vibrational modes or acoustic phonons. When q is increased, the unit cell, which consists of one atom of each type, becomes increasingly deformed. At qmax the heavier atoms vibrate in phase while the lighter atoms are stationary.
8.2 Lattice heat capacity
239
2 K (m1 + m2 ) m1m2
2K = w2 m2
optic branch
w
2K = w1 m1
acoustic branch
0
p 2a
q
Figure 8.9 The dispersion curve for a onedimensional diatomic chain of atoms. m 2 < m1. transverse acoustic mode q
q transverse optic mode
Figure 8.10 Transverse acoustic and optic modes of motion in a onedimensional diatomic chain at the same wavelength.
The optical branch takes a nonzero limiting value at q = 0: w o ( q = 0) =
2 K ( m1 + m2 ) m1 m2
(8.22)
Close to this limit the displacements of the two types of atom have opposite sign and the two types of atom vibrate out of phase, as illustrated in the lower part of Figure 8.10. Thus close to q = 0, the two atoms in the unit cell vibrate around their centre of mass which remains stationary. Each set of atoms vibrates in phase and the two sets with opposite phases. There is no propagation and no overall displacement of the unit cell, but a periodic deformation. These modes have frequencies corresponding to the optical region in the electromagnetic spectrum and since the atomic motions associated with these modes are similar to those formed as response to an electromagnetic field, they are termed optical modes. The optical branch has frequency maximum at q = 0. As q increases w slowly decreases and
240
8 Heat capacity and entropy (a)
(b) LO TO
LO
DoS / arbitrary units
n / THz
CuCl
TA
6
4 LA 2
LO
LA
LA
LO TO
LA
TA 0
0
1 (e, e, 0)
0
2
4
6
n / THz
Figure 8.11 (a) Dispersion curve for CuCl(s) along [110] of the cubic unit cell. (b) Density of vibrational modes [3]. Here L, T, A and O denote longitudinal, transverse, acoustic and optic. Reproduced by permission of B. Hennion and The Institute of Physics.
approaches a minimum at qmax. As q increases the vibration becomes a mixture of displacement and deformation of the unit cell. For q = qmax the heavier atoms are stationary, whereas the lighter atoms vibrate in phase. Although acoustic and optic mode behaviour can be distinguished at the zone centre, this is not generally so at other values of q. Nevertheless, the convention is to refer to the whole branch as being optic or acoustic. In three dimensions, transverse and longitudinal optic and acoustic modes result. The dispersion curve for CuCl along [100] of the cubic unit cell [3] is shown in Figure 8.11(a) as an example. The number of discrete modes with frequencies in a defined interval can be displayed as a function of the frequency. This gives what is termed the density of vibrational modes or the vibrational density of states (DoS). The vibrational DoS of CuCl is given in Figure 8.11(b). In general a crystal that contains n atoms per unit cell have a total of 3L◊n vibrational modes. Of these there are 3L acoustic modes in which the unit cell vibrates as an entity. The remaining 3L(n – 1) modes are optic and correspond to different deformations of the unit cell. At high temperatures where classical theory is valid each mode has an energy kBT and the total heat capacity is 3R, in line with the Dulong–Petit law. The collective modes of vibration of the crystal introduced in the previous paragraph involve all the atoms, and there is no longer a single vibrational frequency, as was the case in the Einstein model. Different modes of vibration have different frequencies, and in general the number of vibrational modes with frequency between n and n + dn are given by
8.2 Lattice heat capacity
241 ¥
3N A g(n ) dn
ò g(n )dn = 1
where
(8.23)
0
and g(n ) is the density of vibrational modes at a particular frequency. When the density of vibrational modes is known as a function of n, the total internal energy can be calculated and the heat capacity obtained through differentiation with respect to temperature.
The Debye model The quantization of vibrational energy implies that at low temperatures only the lowfrequency modes of lattice vibrations will be appreciably excited. The usual very lowfrequency vibrations of a solid are the acoustic modes with wavelengths much longer than the atomic dimensions. Debye calculated the distribution of frequencies that result from the propagation of acoustic waves of permitted wavelengths in a continuous isotropic solid and assumed the same distribution to hold in a crystal [4]. The distribution of frequencies is then given by (see e.g. Grimvall, Further reading) g(w ) =
3w 2 3 wD
for w D ³ w
(8.24)
g(w ) = 0 for w > w D
(8.25)
The limiting angular vibrational frequency, w D , that exists defines the Debye temperature, Q D , as QD =
w D hn D = 2p kB kB
(8.26)
and it can be shown that the heat capacity corresponding to the Debye model is given by
C V ,m
æ T = 9R çç è QD
ö ÷÷ ø
3 QD /T
ò
0
ex (e x  1)2
x 4 dx
(8.27)
where x = w / k BT . Whereas the Debye heat capacity is equal to 3R at high temperatures, it reduces to
8 Heat capacity and entropy
20
3L
nD g(n)
Cm / J K 1 mol 1
242
10
3L 0
0
0
10
200
20
30 n / THz
40
50
400
T /K
Figure 8.12 Experimental heat capacity of Cu at constant pressure compared with the Debye and Einstein C V ,m calculated by using QE = 244 K and QD = 314 K. The vibrational density of states according to the two models is shown in the insert.
CV =
12p 4 æ T R çç 5 è QD
ö ÷÷ ø
3
(8.28)
at low temperatures. When the temperature approaches 0 K, the heat capacity tends to zero as T3, in agreement with experiment. The experimental constantpressure heat capacity of copper is given together with the Einstein and Debye constant volume heat capacities in Figure 8.12 (recall that the difference between the heat capacity at constant pressure and constant volume is small at low temperatures). The Einstein and Debye temperatures that give the best representation of the experimental heat capacity are QE = 244 K and QD = 315 K and schematic representations of the resulting density of vibrational modes in the Einstein and Debye approximations are given in the insert to Figure 8.12. The Debye model clearly represents the lowtemperature behaviour better than the Einstein model. Both the Einstein and the Debye temperatures reflect the bonding strength in a particular compound. A higher characteristic temperature represents stronger bonding between the atoms and the classical limit will be reached at higher temperatures. The lattice heat capacity of different polymorphs of carbon is displayed in Figure 8.13. The soft molecule C60 with weak intermolecular bonds has a low Debye temperature (QD = 46 K) [5]. Graphite with weak van der Waals bonds between the graphite layers has considerably higher QD = 760 K, while diamond with only strong covalent bonds between all the C atoms displays a very high Debye temperature (2050 K). Hence, while C60 approaches the classical value 3R (per carbon atom) far below 100 K, the heat capacity of diamond is only 20% of this value at 300 K.
8.2 Lattice heat capacity
243
30
CV ,m / J K 1 mol 1
25
C60
20
QD = 46 K
15 graphite
10 5 0
diamond
QD = 760 K
0
QD = 2050 K
100
200
300
T /K
Figure 8.13 Lattice heat capacity of three different polymorphs of carbon; C60 [5], graphite and diamond.
Since the vibrational contribution is generally the largest contribution to the heat capacity, trends in the Debye temperature largely defines trends in entropy. Periodic variations of the Debye temperature of the elements, and for Li, Na, K and Rb halides, are given in Table 8.2 and Figure 8.14, respectively. The Debye temperature for the halides decreases with the mass of both the cation and anion. The charge of the ions is constant and the variation in QD reflects the interatomic distance and the bonding strength. The fluorides, which in Chapter 7 were shown to have the more negative enthalpy of formation among the halides, have the highest Debye temperatures and thus the lowest entropies. Although the Debye model reproduces the essential features of the low and hightemperature behaviour of crystals, the model has its limitations. A temperaturedependent Debye temperature, QD(T), can be calculated by reproducing the heat capacity at each single temperature using the equation CV,Debye(T, QD) = CV,exper(T)
(8.29)
A dip in QD versus temperature is typically observed for QD/50 < T/K < QD/2. It follows that a constant Debye temperature is not able to reproduce the experimental observations over large temperature ranges. More importantly, the Debye model and also the Einstein model work best for materials that take crystal structures of high symmetry, for pure elements as well as for binary compounds where the two elements have similar masses and bonding. The approach is less applicable to complex materials that contain elements that differ largely in chemical bonding, coordination and/or mass. Furthermore, groups like carbonate anions and the SiO4 tetrahedra in silicates will retain their intrinsic properties to a large degree even in complex compounds. An alternative is to represent the massive vibrational modes of the unit cell as a whole by a Debye function and the internal vibrational modes of covalent groups by one or more Einstein functions. This approach will be further discussed below.
244
8 Heat capacity and entropy
Table 8.2. Debye temperature (QD in K) and electronic heat capacity coefficient (see Section 8.4) (g in mJ K–1 mol–1) of the elements. A QD g
B
N C 2050 0
O
F
Ne 75
Al 428 14
Si 645
P
S
Cl
Ar 92
Zn 327 6
Ga 320 6
Ge 374
As 282
Se 90
Br
Kr 72
Ag 225 6
Cd 209 7
In 108 18
Sn 200 18
Sb 211
Te 153
I
Xe 64
Au 165 7
Hg 72 19
Tl 79 15
Pb 105 34
Bi 119
Po
At
Rn
Li 344 18
Be 1440 2
Na 158 14
Mg 400 14
K 91 21
Ca 230 77
Sc 360
Ti 420 36
V 380 92
Cr 630 16
Mn 410 180
Fe 470 50
Co 445 48
Ni 450 73
Cu 315 7
Rb 56 24
Sr 147 37
Y 280
Zr 291 30
Nb 275 88
Mo 450 21
Tc
Ru 600 34
Rh 480 49
Pd 274 100
Cs 33 32
Ba 110 27
La 142
Hf 252 26
Ta 240 59
W 400 12
Re 430 25
Os 500 24
Ir 420 31
Pt 240 66
800 Li
QD / K
600 Na 400 K Rb
200 AF
ACl
ABr
AI
Figure 8.14 Debye temperature of the alkali halides.
The relationship between elastic properties and heat capacity Both the Einstein and Debye theories show a clear relationship between apparently unrelated properties: heat capacity and elastic properties. The Einstein temperature for copper is 244 K and corresponds to a vibrational frequency of 32 THz. Assuming that the elastic properties are due to the sum of the forces acting between two atoms this frequency can be calculated from the Young’s modulus of copper, E = 13 × 1010 N m–2. The force constant K is obtained by dividing E by the number of atoms in a plane per m2 and by the distance between two neighbouring planes of atoms. K thus obtained is 14.4 N m–1 and the Einstein frequency, obtained using the mass of a copper atom into account, 18 THz, is in reasonable agreement with that deduced from the calorimetric Einstein temperature.
8.2 Lattice heat capacity
245
Table 8.3 Comparison of Debye temperatures derived from heat capacity data and from elastic properties.
QD(Elastic) QD(CV)
Ag
Cu
Al
NaCl
KBr
LiF
226.4 226.2
344.4 345.1
428.2 426
321.9 320
182.8 184
834.1 838
Even better agreement is observed between calorimetric and elastic Debye temperatures. The Debye temperature is based on a continuum model for long wavelengths, and hence the discrete nature of the atoms is neglected. The wave velocity is constant and the Debye temperature can be expressed through the average speed of sound in longitudinal and transverse directions (parallel and normal to the wave vector). Calorimetric and elastic Debye temperatures are compared in Table 8.3 for some selected elements and compounds.
Dilational contributions to the heat capacity In general, C V is obtained from C p by taking the isobaric expansivity and isothermal compressibility of the crystal into consideration: C p ,m  C V ,m =
a 2 VT kT
(8.30)
The thermal expansivity of a solid is in general low at low temperatures and the anharmonic contribution to the heat capacity is therefore small in this temperature region and C V ,m Âť C p ,m. At high temperatures the difference between the heat capacity at constant pressure and at constant volume must be taken into consideration. The heat capacity models described so far were all based on a harmonic oscillator approximation. This implies that the volume of the simple crystals considered does not vary with temperature and C V ,m is derived as a function of temperature for a crystal having a fixed volume. Anharmonic lattice vibrations give rise to a finite isobaric thermal expansivity. These vibrations contribute both directly and indirectly to the total heat capacity; directly since the anharmonic vibrations themselves contribute, and indirectly since the volume of a real crystal increases with increasing temperature, changing all frequencies. The constant volume heat capacity derived from experimental heat capacity data is different from that for a fixed volume. The difference in heat capacity at constant volume for a crystal that is allowed to relax at each temperature and the heat capacity at constant volume for a crystal where the volume is fixed to correspond to that at the Debye temperature represents a considerable part of C p ,m  C V ,m . This is shown for Mo and W [6] in Figure 8.15.
246
8 Heat capacity and entropy
C / J K –1 mol –1
8 W:
(Cp – CV) (CV – CV, fix)
Mo:
(Cp – CV) (CV – CV, fix)
6
4
2
0.0
0.2
0.4
0.6
0.8
1.0
T / Tfus
Figure 8.15 C p , m  C V , m and C V , m  C V , m , fix for Mo and W [6].
In order to calculate the dilational contribution exactly a considerable quantity of data is needed. The temperature dependence of the volume, the isobaric expansivity and the isothermal compressibility is seldom available from 0 K to elevated temperatures and approximate equations are needed. The Nernst–Lindeman relationship [7] is one alternative. In this approximation C p ,m  C V ,m is given by C p ,m  C V ,m =
Va 2 k T C 2p ,m
C 2p ,m T = AC 2p ,m T
(8.31)
The parameter A is nearly constant over a wide range of temperatures and A can be calculated at any temperature if the data needed to derive its value are available at one temperature. The equation can be used over a wide temperature range without introducing large errors. In an alternative approach [7], applicable if the isobaric thermal expansivity is known as a function of temperature, C p ,m  C V ,m is given by Cp ,m  C V ,m = g G aC V ,m T
(8.32)
where g G is the Grüneisen parameter, defined as é ¶p ù aV gG =ê ú =k C ( / ) ¶ U V ë ûV T V ,m g G is largely independent of temperature at high temperatures.
(8.33)
8.2 Lattice heat capacity
247
Estimates of heat capacity from crystallographic, elastic and vibrational characteristics Most thermodynamic data are limited to a certain range in temperature and pressure and cannot be extrapolated to other p,T conditions. The data tabulated in major data compilations and thermodynamic tables are often obtained by fitting nonphysical models to experimental data and the fits are only valid over the temperature and pressure ranges where measurements have been carried out. Extrapolations to other T and p conditions are frequently done using simplified models of the vibrational density of states. These estimation schemes have been shown often to be accurate at temperatures above about 200 K. A model is typically developed by taking available crystallographic, vibrational and thermoelastic data into consideration and can be used over larger pressure and temperature ranges. Kieffer has estimated the heat capacity of a large number of minerals from readily available data [8]. The model, which may be used for many kinds of materials, consists of three parts. There are three acoustic branches whose maximum cutoff frequencies are determined from speed of sound data or from elastic constants. The corresponding heat capacity contributions are calculated using a modified Debye model where dispersion is taken into account. Highfrequency optic modes are determined from specific localized internal vibrations (Si–O, C–O and O–H stretches in different groups of atoms) as observed by IR and Raman spectroscopy. The heat capacity contributions are here calculated using the Einstein model. The remaining modes are ascribed to an optic continuum, where the density of states is constant in an interval from nL to nH and where the frequency limits nL and nH are estimated from Raman and IR spectra. This approach can be briefly illustrated through an analysis of the heat capacity of calcite. The primitive unit cell contains two CaCO3 formula units (10 atoms) and calcite thus has 30 degrees of freedom. Among these modes, 3 are acoustic and 12 are internal modes related to the vibrations of the two CO23 groups (with 3n – 6 vibrational modes), whereas the remaining 15 are optic modes that will be taken into account by the optic continuum. Directly measured acoustic velocities are available. The frequency of the internal optic modes represented by Einstein oscillators and the limits of the optic continuum are derived from the IR and Raman spectra given in Figures 8.16(a) and (b). The resulting approximate phonon density of states is shown in Figure 8.16(c), while the heat capacity and the relative contribution from the acoustic and internal optic modes and the modes of the optic continuum are given in Figure 8.16(d). The Kieffer approach uses a harmonic description of the lattice dynamics in which the phonon frequencies are independent of temperature and pressure. A further improvement of the accuracy of the model is achieved by taking the effect of temperature and pressure on the vibrational frequencies explicitly into account. This gives better agreement with experimental heat capacity data that usually are collected at constant pressure [9].
248
8 Heat capacity and entropy
(b) 100
IO3
Intensity
% Transmittance
(a)
nH IO1
IO1
IO4
IO2
0
4
11 1
(c) 0.3
Vibrational DOS
1000 1500 n / cm–1
IO1 IO2
Acoustic modes
0.2
0.1
2
2
2000 4
IO3
900 –1 1200 n / cm
1500
degeneracy
IO4
Internal optic modes
Optic continuum
600
(d) 100
Cm / J K 1 mol 1
500
Experiments Total calc. Optic continuum
50
Internal optic Acoustic
0.0
0
400
800 n / cm–1
1200
1600
0
0
200
400
600 T/ K
800
1000
Figure 8.16 (a) IR and (b) Raman spectra for the mineral calcite, CaCO3. The estimated density of vibrational states is given in (c) while the deconvolution of the total heat capacity into contributions from the acoustic and internal optic modes as well as from the optic continuum is given in (d).
8.3 Vibrational entropy The Einstein and Debye models revisited The vibrational heat capacity is the largest contribution to the total heat capacity and determines to a large extent the entropy. Analytical expressions for the entropy of the models described in the previous section can be derived. The entropy corresponding to the Einstein heat capacity is Q E /T é ù S E = 3R ê  ln[1  exp( Q E / T )]ú ë[exp( Q E / T )  1] û
(8.34)
where q E = w E / k B . Similarly, the expression for the entropy of the Debye model is é 4T 3 S D = 3R ê ê Q3 ë D
QD /T
ò
0
ù x 3 dx  ln[1  exp( Q D / T )]ú [exp( x)  1] ú û
(8.35)
8.3 Vibrational entropy
249
S / J K –1 mol–1
30
QD = 300 K QD = 400 K QD = 500 K
20
10
0
0
100
200
300
T /K
Figure 8.17 Entropy of a monoatomic solid for different values of the Debye temperature, QD.
and here q D = w D / k B and x = w /k BT . Whereas the latter expression must be solved numerically for low temperatures, the entropy at high temperatures can be derived by a series expansion [4]. For the Debye or Einstein models the entropy is essentially given in terms of a single parameter at high temperature: é4 æT S = 3R ê + lnçç êë3 è qi
2 4 ù ö 1 æ qi ö 1 æ qi ö ÷÷ + ç ÷ ç ÷ + …ú 2240 è T ø úû ø 40 è T ø
(8.36)
The entropy of a monoatomic solid is given as a function of the Debye temperature and the thermodynamic temperature in Figure 8.17. An alternative to deriving the Debye temperature from experimental heat capacities is to derive an entropybased Debye temperature by calculation of the QS that reproduces the observed entropy for each single temperature using SDebye(T, QS) = Sexper(T)
(8.37)
This relation yields QS(T), in an analogous manner to the heat capacitybased Debye temperature (eq. 8.29). While the derivation of Debye temperatures from heat capacities is done using lowtemperature data, the entropybased Debye temperature can be derived from hightemperature data since the vibrational part of the standard entropy usually dominates at high temperatures. As evident from eq. (8.36), at high temperatures the entropy depends on the logarithmic average of the phonon frequency. These phonon frequencies, as we have seen, depend on the interatomic forces and the atomic masses. The logarithmic average can be deconvoluted so that the effect of atomic mass is separated from the effect of the interatomic force constant. The entropy contribution related to the force constant
250
8 Heat capacity and entropy (a) 700
(b) MF 2 MCl2 MBr2 MI 2
600
600 QS / K
QS / K
500
700
400
M3C2 M2C M7 C3 M5C2 M3 C M23C6
500
300 400 200 100 Be
Mg
Ca
Sr
Ba
300 Sc Ti V Cr Mn Fe Co Ni
Figure 8.18 Entropy Debye temperature, QS, for (a) alkali earth dihalides [10] and (b) first series transition metal carbides [11].
depends on the electronic structure of the compounds and strong regularities are observed when chemically related materials are compared. The method was developed for estimation of the entropy of materials (stable and metastable) for which experimental entropy data are not available. A large number of compounds have been analyzed. Trends observed in the entropy Debye temperature are given for the alkaline earth dihalides [10] and transition metal carbides [11] in Figure 8.18. A close resemblance is observed between the trends for the normal Debye temperature of the alkali halides in Figure 8.14 and the entropy Debye temperatures for the alkaline earth dihalides in Figure 8.18(a). Effect of volume and coordination Firstorder estimates of entropy are often based on the observation that heat capacities and thereby entropies of complex compounds often are well represented by summing in stoichiometric proportions the heat capacities or entropies of simpler chemical entities. Latimer [12] used entropies of elements and molecular groups to estimate the entropy of more complex compounds: see Spencer for revised tabulated values [13]. Fyfe et al. [14] pointed out a correlation between entropy and molar volume and introduced a simple volume correction factor in their scheme for estimation of the entropy of complex oxides based on the entropy of binary oxides. The latter approach was further developed by Holland [15], who looked into the effect of volume on the vibrational entropy derived from the Einstein and Debye models. Even though the Einstein and Debye models are not exact, these simple oneparameter models illustrate the properties of crystals and should give reliable estimates of the volume dependence of the vibrational entropy [15]. The entropy is given by the characteristic vibrational frequency and is thus related to some kind of mean interatomic distance or simpler, the volume of a compound. If the unit cell volume is expanded, the average interatomic distance becomes larger and the
8.3 Vibrational entropy
251
bonding strength is usually reduced. Weaker bonding strength obviously results in a reduced vibrational frequency for the longitudinal phonons. The effect of a change in volume on the entropy is given by the ratio of the isobaric expansivity and isothermal compressibility of a compound: a æ ¶S ö ÷ = ç è ¶V ø T k T
(8.38)
The volume dependence of the entropy can alternatively be expressed as a function of the Einstein or Debye temperature as æ ¶Q ö æ ¶S ö æ ¶S ö ÷ ÷ ç ÷ =ç ç è ¶V ø T è ¶V ø T è ¶Q ø T
(8.39)
(¶S / ¶Q) T is given by differentiation of eqs. (8.34) or (8.35), while the variation of the characteristic temperature with volume is given by [15] 1/ 3
æV ö Q = Qoç o ÷ è V ø
(8.40)
Here Q o is the characteristic temperature at volume Vo. An average value for the volume dependence of the standard entropy at 298 K for around 60 oxides based on the Einstein model is 1.1 ± 0.1 J K–1 cm–3 [15]. A corresponding analysis using the Debye model gives approximately the same numeric value. In the preceding treatment we have assumed a volume change without taking the structure of the material into consideration; for a phase transition where the cation coordination is preserved DtrsS generally has the same sign as DtrsV and the transition temperature increases with pressure since dp/dT = DtrsS/DtrsV . A different conclusion can be derived for phase transitions which involves a change in the nearest coordination number. The vibrational properties of an atom will to a large degree depend on the local environment and a change in coordination necessarily implies a change in the vibrational density of states. For a transition that increases the coordination, the interatomic distances in the first coordination sphere become longer. Although the number of bonds increases, the vibrational density of states is generally shifted to lower frequencies. The denser compound thus has higher entropy than otherwise expected and may even in some cases have a higher entropy than the less dense modification, i.e. the Clapeyron slope becomes negative since DtrsS > 0 for DtrsV < 0. The effect of coordination may be illustrated by the vibrational properties of the four modifications of MgSiO3 [16]. Above 1000 K, the entropy of these modifications of MgSiO3 decreases in the order pyroxene > perovskite > garnet > ilmenite
252
8 Heat capacity and entropy
The density increases in the order pyroxene < garnet < ilmenite < perovskite Thus garnet, ileminite and perovskite are modifications stabilized by pressure and they are all stable at some specific pressure–temperature conditions. Using the volume argument, pyroxene is the highentropy modification, in line with experiments. On the other hand, the perovskite should have the lowest entropy. This is not observed and this reflects the opposing effect of a coordination change. All the Si atoms are tetrahedrally coordinated in pyroxene, while 50% are tetrahedrally coordinated and 50% octahedrally coordinated in garnet. In the ilmenite and perovskite modifications all Si atoms are octahedrally coordinated. When Si transforms from a tetrahedral to an octahedral coordination, the frequency of the Si–O stretching modes decreases from typically 900–1100 cm–1 (SiO4 tetrahedra) to 600–800 cm–1 (SiO6 octahedra). The bonds are stronger in the tetrahedra than in the octahedra [16]. A lower bond strength gives larger vibrational amplitudes, lower frequencies and thereby a larger entropy for the 6coordinated compounds. These factors explain why the perovskite has higher entropy than the garnet at high temperatures and that the slope of the p–T phase boundary between the two phases is negative.
8.4 Heat capacity contributions of electronic origin Electronic and magnetic heat capacity Quantization is important also for understanding the electronic contribution to the heat capacity. In classical theory the electrons were considered as small particles moving freely through the crystal, and the three translational degrees of freedom were expected in total to contribute 3/2R to the total heat capacity. The heat capacity of a monovalent metal, like copper, was by these considerations expected to be 3R + 3/2R. The experimental heat capacity is, however, as we have seen, close to 3R. The small electronic contribution to the heat capacity is due to quantization. Electrons follow Fermi–Dirac statistics (see e.g. C. Kittel and H. Kroemer, Further reading) and only electrons near the Fermi level can be excited at a given temperature. When the temperature rises from 0 K to T the total increase in internal energy is roughly DU = N 1 k BT
(8.41)
where N1 is the number of electrons that are excited by the thermal energy kBT. These electrons occupy electron states in a band of thickness kBT about the Fermi level, e F , as visualized in Figure 8.19, where the energy distribution for a free electron gas is given. It follows that the number of excited electrons, N1, at a given temperature is given by
8.4 Heat capacity contributions of electronic origin
253
density of electronic states
k BT
ef energy
Figure 8.19 Energy distribution for a free electron gas at 0 K (shaded) and an elevated temperature (dashed line), T.
N 1 = n(e F ) k BT
(8.42)
where n(eF) is the density of electronic states at the Fermi level. The internal energy of the electrons follows DU = n(e F ) k 2BT 2
(8.43)
Using this simple argument, the electronic heat capacity, C E , of a free electron gas is CE =
ÂśD U = 2 n(e F )k 2BT ÂśT
(8.44)
An exact derivation that takes into account the variation of the Fermi level with temperature gives basically the same result: CE =
p2 2 n(e F ) k B T 3
(8.45)
The electronic heat capacity thus varies linearly with temperature and is often represented as CE =gT
(8.46)
254
8 Heat capacity and entropy 1.5
TF
1.0
1.0
Ce / R
0.8 f(e)
0.6
0.5
0.4 0.2 0.0 0
0.0 0.0
0.5
1
2
3
1.0 T / TF
4 T/ K
5
6
1.5
7
8
2.0
Figure 8.20 Heat capacity of a free electron gas. The population of the electronic states at different temperatures is shown in the insert. TF is typically of the order of 105 K.
where g is termed the electronic heat capacity coefficient. The variation of g across the periodic table is given in Table 8.2. The electronic heat capacity for the free electron model is a linear function of temperature only for T<< TF = eF / kB. Nevertheless, the Fermi temperature TF is of the order of 105 K and eq. (8.46) holds for most practical purposes. The population of the electronic states at different temperatures as well as the variation of the electronic heat capacity with temperature for a free electron gas is shown in Figure 8.20. Complete excitation is only expected at very high temperatures, T > TF. Here the limiting value for a gas of structureless mass points 3/2R is approached. Since the lattice contribution to the heat capacity varies with T3, the total heat capacity at low temperatures (typically T < 10 K or lower) to a first approximation is given by C V = bT
3
+gT
(8.47)
A plot of C V / T against T2 should therefore give a straight line as illustrated for Cu in Figure 8.21. From this plot the electronic density of states at the Fermi level can be calculated, and calorimetry has frequently been used for this purpose. A striking example is the electronic heat capacity coefficients observed for Rh–Pd–Ag alloys given in Figure 8.22 [17]. In the rigid band approach the addition of Ag to Pd gives an extra electron per atom of silver and these electrons fill the band to a higher energy level. Correspondingly, alloying with Rh gives an electron hole per Rh atom and the Fermi level is moved to a lower energy. The variation of the electronic heat capacity coefficient with composition of the alloy maps approximately the shape of such an electron band. The electronic density of states for Rh–Pd–Ag alloys can be
8.4 Heat capacity contributions of electronic origin
255
C p,mT 1 / J K 2 mol 1
15 12
Cu Cp, m /T = g + bT 2
9 6 3
g = 7 mJ K–2 mol–1 0
0
100
200 2
300
2
T /K
Figure 8.21 Heat capacity of Cu plotted as Cp,m◊T–1 versus T2.
10 g / mJ K –2 mol –1
Rh–Pd
Pd–Ag
8 6 4 2 0 Rh
xPd
Pd
xAg
Ag
Figure 8.22 Variation of the electronic heat capacity coefficient with composition for the alloys Rh–Pd and Pd–Ag [17]. Solid and dotted lines represent the electronic DoS for the 5s and 4d bands, respectively.
understood by the superposition of a narrow 4d band on a flat 5s band. This is also indicated in Figure 8.22; the solid line represents the 5s band and the dotted line the 4d band. Whereas the vibrational and electronic contributions to the heat capacity are readily treated in terms of simple models, the treatment of the heat capacity due to excitation of collective magnetic excitation modes of ordered magnetic structures, often termed spin waves or magnons, is more complex. The ideally ordered magnetic states exist only in the absence of thermal agitation. At finite temperatures the spins at some sites are excited. By analogy with collective vibrational modes, spin waves are formed. If the magnon frequency for a particular wave vector is n(q) and g magn(n) is the density of states of magnon frequencies, the
256
8 Heat capacity and entropy
magnetic heat capacity can be expressed by analogy with that for the lattice heat capacity as (see e.g. Grimvall, Further reading) C magn = R ò
x2 e x (e x  1)2
g magn (w ) dw
(8.48)
where x = w / k BT . The magnon density of states is in general not easily calculated and the functional variation depends on the type of magnetic order. It can be shown that the magnetic frequencies for a ferromagnetic insulator scale with the square of the wave vector. The magnetic heat capacity resulting from this characteristic is proportional to T3/2 at low temperature. The heat capacity of an antiferromagnet shows a T3 variation at low temperatures. At higher temperatures, interactions between the magnons give rise to other terms. Electronic and magnetic transitions Electronic transitions like insulator–metal transitions, magnetic order–disorder transitions, spin transitions and Schottkytype transitions (due to crystal field splitting in the ground state in f elementcontaining compounds) profoundly influence the phase stability of compounds. A short description of the main characteristics of these transitions will be given below, together with references to more thorough treatments. The electronic heat capacity naturally has a pronounced effect on the energetics of insulator–metal transitions and the entropy of a firstorder transition between an insulating phase with g = 0 and a metallic phase with g = gmet at Ttrs is in the first approximation Dins–metSm = gmetTtrs. Differences in the Debye temperature, or in other words the vibrational character of the two phases, will modify the transitional entropy to some extent. Still, this entropy change is normally not large for transitions where the coordination number is preserved. Magnetic order–disorder transitions give rise to a heat capacity and entropy contribution of configurational nature. While the magnon heat capacity is complex, a very general expression is available for the maximum total order–disorder entropy. A particle with Nun unpaired electrons and total spin quantum number S = S 1 N un 2 has (2 S + 1) quantized orientations. While all spins have the same orientation at low temperatures for an ordered magnetic structure, all orientations are degenerate in the paramagnetic state. The entropy change corresponding to this disordering is thus kB ln(2 S + 1) per particle or DS = R ln(2 S + 1)
(8.49)
for one mole of atoms. For Fe3+ (d5) in its electronic ground state S = 5/2 and D S = R ln 6 = 14.89 J K–1 mol–1. If the disordering takes place through a secondorder transition, the entropy contribution at a given temperature may be estimated
8.4 Heat capacity contributions of electronic origin
257
200
C p,m / J K 1 mol 1
Fe 2O3 150
total Cp, m CV, m+ Cdil CV, m
100
50 Cp, m(magnetic) 0 200
400
600
800
1000
T /K
Figure 8.23 Heat capacity of Fe2O3 [18]. The heat capacity is deconvoluted to show the relative magnitude of the main contributions. Cdil = Cp,m â€“ CV,m = a2TV/kT.
from Landau theory (see Section 2.3). It should in this context be noted that a magnetic transition that takes place at high temperatures may give significant contributions to the entropy at temperatures far below TC, as evident from the deconvoluted heat capacity of Fe2O3 in Figure 8.23 [18]. Although the spinonly approximation has been shown to give reasonable estimates for iron oxides, for example, deviations from the spinonly entropy must in general be expected as for example shown for MnO [19]. An alternative approximation for the maximum magnetic entropy frequently used in thermodynamic representations of phase diagrams involves the saturation magnetization at 0 K instead of the spin quantum number [20]. Transitions with large entropy changes take place also in the paramagnetic state. Octahedrally coordinated transition metal ions having electronic configurations d4, d5, d6 or d7 can exist in the lowspin or highspin ground state depending on the strength of the ligand field. The same is the case for tetrahedrally coordinated transition metal ions with d3, d4, d5 or d6 configuration. Temperatureinduced spin transitions are expected in compounds where the ligand field splitting energy is comparable to the thermal energy and larger than the electron spinpairing energy. The ligand field splitting energy depends on the metal, its valence and the ligand, and for a given metal in a given oxidation state, the ligand determines the spin state. Some trivalent oxides of cobalt (for example Co2O3) are found to be in a highspin state at all temperatures, others are in a lowspin state (for example ZnCo2O4 and LiCoO2), while others show temperatureinduced spin transitions (for example Co3O4 and LaCoO3). The ligand field splitting is in general smaller for iron than for cobalt, and although Co3+ and Fe2+ have the same electronic configuration, all iron oxides are in a highspin state at ambient pressure. Reviews focusing on metalâ€“organic compounds by GĂźtlich et al. [21] and by Sorai [22] give more detailed accounts of the physics of spin transitions. Large entropy increments accompany the spin transitions. For Co3+ in an octahedral crystal field the highspin state has a degeneracy of 15 (the product of orbital
258
8 Heat capacity and entropy
C p,m / J K 1 mol 1
600
30 20
400
10 0 0
25
50
75
100
200 Co3O4 0
0
300
600
900
1200
T /K
Figure 8.24 Heat capacity of Co3O4 [23–25]. The insert shows the magnetic order–disorder transition at around 30 K [24] in detail.
and spin degeneracy), whereas the lowspin state is singly degenerate. A transition from the lowspin to the highspin ground state should thus give a configurational entropy increment of R ln 15 = 22.5 J◊K–1 mol–1 in the hightemperature limit and also substantial contributions to the heat capacity. The experimental heat capacity for Co3O4, which undergoes a temperatureinduced spin transition at high temperatures is shown in Figure 8.24 [23–25]. The normal spinel contains Co2+ at tetrahedral sites and lowspin Co3+ at octahedral sites. The heat capacity effect observed at T > 900K is in part a low to highspin transition of the Co 3+ ions and in part a partial transition from normal toward random distribution of Co3+ and Co2+ on the tetrahedral and octahedral sites of the spinel structure. The entropy change connected with the spin change is by far the largest contribution to the transitional entropy. The insert to the figure shows the magnetic order–disorder transition of Co3O4 at around 30 K. The magnetic entropies are large and indicate the need for thermodynamic models, atomistic or purely mathematical, that can handle these effects. Although spin transitions in principle may be simple twolevel transitions, they may also be affected by spin–orbit coupling (frequently observed for cobalt ions), magnetic ordering, and associated changes in the crystal structure. Since the spin transition affects the bonding in the crystal and thus the vibrational frequencies, an associated change in the Debye temperature of the compound must be expected. The size of this effect is limited for inorganic compounds. For organometallic compounds, on the other hand, the entropy connected with this lattice effect often is larger than the entropy of the spin state transition itself [22]. A lowspin to highspin transition relates to the crystal field splitting of the dorbitals in an octahedral or tetrahedral crystal field. However, even in cases where the energy difference between two spin states is much larger, electronic transitions are observed. An atom with total spin quantum number S has (2 S + 1) orientations. In a magnetic field the atom will have a number of discrete energy levels with
8.4 Heat capacity contributions of electronic origin
259
energy spacing dependent on the strength of the magnetic field. Although the crystal field experienced by a metalatom in a crystal is small compared to what can be achieved by external magnets, the crystalfield typically induces splitting of the felectron levels in actinides, and the effects of this are visible in the heat capacity in large temperature regions at relatively high temperatures [26]. Similar heat capacity effects are observed also in hydrated paramagnetic salts used for magnetic cooling [27]. The spins on transition metals like Ni and Fe are here localized since they are diluted by the presence of nonmagnetic ions. This dilution gives welldefined localized energy levels and thus sharp heat capacity effects. The heat capacity of transitions of this type is given by the energy level splitting in an electrostatic field and by the degeneracy of the energy levels. Let us for simplicity assume that we have a system with two levels with energy spacing e/kB. For T<< e/kB the upper level is occupied to a negligible extent only. For T >> e/kB both levels will be approximately equally occupied. Using Boltzmann statistics the heat capacity is
C sch
æ e = R çç è k BT
2
ö ÷÷ ø
æ g0 çç è g1
ù exp(e / k BT ) öé ÷÷ ê ú 2 ø êë{1 + (g 0 /g1 ) exp(e / k BT )} úû
(8.50)
where g0 and g1 are the degeneracies of the ground level and the excited level, respectively. Experimental Schottkytype heat capacities for Nd2S3 [28] and ErFeO3 [29] are shown in Figure 8.25. While the transition in the sulfide is spread over a large temperature range, the ErFeO3 transition is at low temperatures and occurs over a narrow range. A large number of experimental studies by Westrum and coworkers have shown that the energies of the different energy levels can be derived from accurate heat capacity data [26]. In these analyses, the number of energy levels and their corresponding degeneracies are derived based on the symmetry of the lanthanide cations in the particular compounds by crystal field theory.
12 Nd2S3
8
C p,m / J K 1 mol 1
CSchottky / J K 1 mol 1
10
ErFeO3
5
0
0
10
20
30
4
0
0
100
200 T/K
300
Figure 8.25 The Schottkytype heat capacity of Nd2S3 [28]. The insert shows the total heat capacity of ErFeO3 [29].
260
8 Heat capacity and entropy
Table 8.4 Energy levels of Nd2S3 [28]. E / cm–1 Level
Degeneracy
Spectroscopy
Calorimetry
0 1 2 3 4
2 2 2 2 2
0 76 140 180 358
0 80 140 180 340
The derived energy levels are shown to correspond closely to those obtained by spectroscopy [26]. Calorimetrically and spectroscopically obtained energy levels for Nd2S3 are given as an example in Table 8.4 [28].
8.5 Heat capacity of disordered systems Crystal defects Real crystals contain lattice defects and other extended defects at temperatures above absolute zero (see e.g. Wollenberger, Further reading). The creation of an intrinsic defect is always an endothermic process. However, as the temperature is raised the increased entropy associated with the large number of possible positions for the defect becomes important. Thus the counteracting effects of the entropy and enthalpy of defect formation determine the variation of the Gibbs energy with concentration of defects, which will have a minimum for a given defect concentration at a specific temperature. For a stoichiometric compound the temperatureinduced intrinsic disorder may be due to the formation of Frenkel or Schottky defects. This defect formation gives rise to a heat capacity contribution given by the molar entropy and enthalpy of formation of the defects, which for the Schottky defect case is given by C V ,m =
1 RT
2
é æ D vac S m 2 êD vac H m exp ç R è ë
æ D H ö öù ÷ú exp ç  vac m ÷ RT ø è øû
(8.51)
Here D vac S and D vac H are the molar entropy and enthalpy of formation of the defects. Using a pure metal like aluminium as an example, the fractional number of defects, heat capacity and enthalpy due to defect formation close to the fusion temperature are 5◊10–4, 0.3 J K–1 mol–1 and 30 J mol–1 [30]. In other cases more complex disordering mechanisms are observed. Nonstoichiometric oxides in which the oxygen vacancies are ordered at low temperatures illustrate convergent disordering. The oxygen atoms and oxygen vacancies are here distributed at the same sublattice at high temperatures. An example is
8.5 Heat capacity of disordered systems
261
Sr2Fe2O5 in which the entropy of the firstorder disordering reaction suggests that the oxygen atoms are far from randomly distributed at high temperatures [31]. Computer simulations described in Section 11.1 suggest that the disorder may be described in terms of a mixture of different structural entities: FeO4 tetrahedra, FeO5 square pyramids and FeO6 octahedra [32]. Cation disorder by what is termed nonconvergent disordering takes place in other systems, e.g. in spinels. Here the cations occupy two different sublattices, which also remain distinct in the disordered hightemperature state. This will be discussed further in Section 9.2. Fast ion conductors, liquids and glasses Fast ion conductors have many physical properties, typical of solids, while others are to some extent similar to those of liquids. For some fast ionic conductors, for example AgI, the high ionic conductivity is associated with a firstorder phase transition where the sublattice associated with the mobile Ag ion becomes almost completely disordered. The other sublattice remains unaffected and constitutes a structural frame, which gives the substance the expected mechanical properties of a solid. In some cases, the entropy of the order窶電isorder transition forming the fast ion conductor is larger than the entropy of the subsequent melting of the disordered fast ion conductor [33]. The large degree of disorder on the sublattice of the mobile species results in a high configurational entropy. This is a characteristic property of liquids as well. Another similarity between liquids and some fast ion conductors is a decreasing heat capacity with increasing temperature. This is observed for many liquids and also for some fast ion conductors like Cu2S [34] and Ag2S [35]. In contrast to crystalline solids characterized by translational symmetry, the vibrational properties of liquid or amorphous materials are not easily described. There is no firm theoretical interpretation of the heat capacity of liquids and glasses since these noncrystalline states lack a periodic lattice. While this lack of longrange order distinguishes liquids from solids, shortrange order, on the other hand, distinguishes a liquid from a gas. Overall, the vibrational density of state of a liquid or a glass is more diffuse, but is still expected to show the main characteristics of the vibrational density of states of a crystalline compound. The most characteristic feature of liquids relative to crystalline solids is the configurational entropy associated with the large degree of disorder in the liquid state. The high configurational entropy allows for fast motion by rotation or diffusion, and liquids are usually nonviscous in the stable region above the freezing point. The viscous properties of SiO2 and some other glassforming liquids are rare exceptions, but in this case the configurational entropy associated with the melting transition is unusually low [36]. The heat capacity of liquids at constant pressure appears in general to go through a broad minimum as a function of temperature. A classic example is Se, for which the heat capacity is given in Figure 5.1. The heat capacity is expected to decrease at high temperatures, where the intermolecular bonding becomes weaker and vibrational degrees of freedom may be lost when the shortrange order is gradually
262
8 Heat capacity and entropy 3
C p,m T –3 / J K–4 mol–1
Se (quenched glass) Se (annealed glass) 2
1 B2O3 (glass) B2O3 (s) 0
0
50
100
T/K
Figure 8.26 Heat capacity of glassy and crystalline B2O3 [42–44] and glassy Se [41] plotted as Cp,m◊T–3 versus T.
destroyed. Finally, it is worth noting that the heat capacity of inorganic and metallic liquids is not that well established experimentally and considerable spread is present even in the data reported for pure metallic elements like Cd [37] and Zn [38]. Two aspects of the thermodynamics of supercooled liquids have generated considerable interest: the nonequilibrium transition to the glassy state at the glass transition [39] as well as the heat capacity of the glass close to the absolute zero of temperature. As already discussed, the vibrational density of states of glasses resembles that of the stable crystalline compound. This is especially true for the vibratio